Handbook for Ironmongers
Handbook for Ironmongers
Ferrous Metallurgy Terms
Hand Tools in History Series
Volume 6: Steel- and Toolmaking Strategies and Techniques before 1870
Volume 7: Art of the Edge Tool: The Ferrous Metallurgy of New England
Shipsmiths and Toolmakers 1607 to 1882
Volume 8: The Classic Period of American Toolmaking, 1827-1930
Volume 9: An Archaeology of Tools: The Tool Collections of the Davistown
Volume 10: Registry of Maine Toolmakers
Volume 11: Handbook for Ironmongers: A Glossary of Ferrous Metallurgy Terms:
A Voyage through the Labyrinth of Steel- and Toolmaking Strategies and
Techniques 2000 BC to 1950
Volume 13: Tools Teach: An Iconography of American Hand Tools
Handbook for Ironmongers
Ferrous Metallurgy Terms
A Voyage through the Labyrinth of Steel- and
Toolmaking Strategies and Techniques
2000 BC to 2000 AD
and the Cascading Industrial Revolutions they Engendered
H. G. Brack, Editor
Museum Publication Series Volume 11
© Davistown Museum 2013
Copyright © 2013 by Harold G. Brack
Front cover illustrations: Clockwise starting at the top left
Small hand adz from the collection of the Davistown Museum ID: TBW1010. Forged
iron and wood, c. 1740 – 1780, 4 ¼” long with a 4 ¾” handle and 1” wide blade.
Basket-making knife from the collection of the Davistown Museum ID: 011006T1.
Blister steel, circa 1700, 6 7/8” long and ½” wide. This is a rare variation of the crooked
knife and was solely used for splitting the wood for baskets of ash or other woods.
Grub hoe from the collection of the Davistown Museum ID: TAB1011. Forged iron, 17th
or 18th century, 4” wide and 6” high.
Fishing spear from the collection of the Davistown Museum ID: TAB1015A. Forged
iron, mid-17th century or earlier, 6 ½” long. Probably a French trade item.
Belt hatchet from the collection of the Davistown Museum ID: 111206T1. Iron and weld
steel with a wood handle, c. 1680-1750, 8” long head, 2 ¼” wide cutting edge, 16 ¼”
long handle. A tomahawk with traditional weld steel forging and a more recent handle.
Frontispiece illustration: Peen adz from the collection of the Davistown Museum ID:
020807T1. 10” long, 4 1/8” wide adz head, 2 ¼” long and ¾” diameter beveled peen, and
28” long handle. Signed by J. F. Ames, who made edge tools in Richmond, Maine, c.
1855. He is listed in the 1855 Maine Business Directory as an edge toolmaker.
Cover design by Cory R. Courtois, Pages Plus (www.pagesplusme.com)
This publication was made possible by a donation from Barker Steel LLC.
P.O. Box 144
Hulls Cove, ME 04644
Davistown Museum Hand Tools in History
One of the primary missions of the Davistown Museum is the recovery, preservation,
interpretation, and display of the hand tools of the maritime culture of Maine and New
England (1607-1900). The Hand Tools in History series, sponsored by the museum’s
Center for the Study of Early Tools, plays a vital role in achieving the museum mission
by documenting and interpreting the history, science, and art of toolmaking. The
Davistown Museum combines the Hand Tools in History publication series, its exhibition
of hand tools, and bibliographic, library, and website resources to construct an historical
overview of steel- and toolmaking strategies and techniques used by the edge toolmakers
of New England’s wooden age. Included in this overview are the roots of these strategies
and techniques in the early Iron Age, their relationship with modern steelmaking
technologies, and their culmination in the florescence of American hand tool
manufacturing in the last half of the 19th century.
During over 40 years of searching for New England’s old woodworking tools for his
Jonesport Wood Company stores, curator and series author H. G. Skip Brack collected a
wide variety of different tool forms with numerous variations in metallurgical
composition, many signed by their makers. The recurrent discovery of forge welded tools
made in the 18th and 19th centuries provided the impetus for founding the museum and
then researching and writing the Hand Tools in History publications. In studying the tools
in the museum collection, Brack found that, in many cases, the tools seemed to contradict
the popularly held belief that all shipwrights’ tools and other edge tools used before the
Civil War originated from Sheffield and other English tool-producing centers. In many
cases, the tools that he recovered from New England tool chests and collections dating
from before 1860 appeared to be American-made rather than imported from English toolproducing centers. Brack’s observations and the questions that arose from them led him
to research the topic and then to share his findings in the Hand Tools in History series.
Hand Tools in History Publications
Volume 6: Steel- and Toolmaking Strategies and Techniques before 1870 explores
ancient and early modern steel- and toolmaking strategies and techniques, including
those of early Iron Age, Roman, medieval, and Renaissance metallurgists and
toolmakers. Also reviewed are the technological innovations of the Industrial
Revolution, the contributions of the English industrial revolutionaries to the evolution
of the factory system of mass production with interchangeable parts, and the
development of bulk steelmaking processes and alloy steel technologies in the latter
half of the 19th century. Many of these technologies play a role in the florescence of
American ironmongers and toolmakers in the 18th and 19th centuries. Author H. G.
Skip Brack cites archaeometallurgists such as Barraclough, Tylecote, Tweedle, Smith,
Wertime, Wayman, and many others as useful guides for a journey through the
pyrotechnics of ancient and modern metallurgy. Volume 6 includes an extensive
bibliography of resources pertaining to steel- and toolmaking techniques from the
early Bronze Age to the beginning of bulk-processed steel production after 1870.
Volume 7: Art of the Edge Tool: The Ferrous Metallurgy of New England Shipsmiths
and Toolmakers explores the evolution of tool- and steelmaking techniques by New
England’s shipsmiths and edge toolmakers from 1607-1882. This volume uses the
construction of Maine’s first ship, the pinnace Virginia, at Fort St. George on the
Kennebec River in Maine (1607-1608), as the iconic beginning of a critically
important component of colonial and early American history. While there were
hundreds of small shallops and pinnaces built in North and South America by French,
English, Spanish, and other explorers before 1607, the construction of the Virginia
symbolizes the very beginning of New England’s three centuries of wooden
shipbuilding. This volume explores the links between the construction of the Virginia
and the later flowering of the colonial iron industry; the relationship of 17th, 18th, and
19th century edge toolmaking techniques to the steelmaking strategies of the
Renaissance; and the roots of America’s indigenous iron industry in the bog iron
deposits of southeastern Massachusetts and the many forges and furnaces that were
built there in the early colonial period. It explores and explains this milieu, which
forms the context for the productivity of New England’s many shipsmiths and edge
toolmakers, including the final flowering of shipbuilding in Maine in the 19th century.
Also included is a bibliography of sources cited in the text.
Volume 8: The Classic Period of American Toolmaking 1827-1930 considers the wide
variety of toolmaking industries that arose after the colonial period and its robust
tradition of edge toolmaking. It discusses the origins of the florescence of American
toolmaking not only in English and continental traditions, which produced gorgeous
hand tools in the 18th and 19th centuries, but also in the poorly documented and often
unacknowledged work of New England shipsmiths, blacksmiths, and toolmakers. This
volume explicates the success of the innovative American factory system, illustrated
by an ever-expanding repertoire of iron- and steelmaking strategies and the widening
variety of tools produced by this factory system. It traces the vigorous growth of an
American hand toolmaking industry that was based on a rapidly expanding economy,
the rich natural resources of North America, and continuous westward expansion until
the late 19th century. It also includes a company by company synopsis of America’s
most important edge toolmakers working before 1900, an extensive bibliography of
sources that deal with the Industrial Revolution in America, special topic
bibliographies on a variety of trades, and a time line of the most important
developments in this toolmaking florescence.
Volume 9: An Archaeology of Tools contains the ever-expanding list of tools in the
Davistown Museum collection, which includes important tools from many sources.
The tools in the museum exhibition and school loan program that are listed in Volume
9 serve as a primary resource for information about the diversity of tool- and
steelmaking strategies and techniques and the locations of manufacturers of the tools
used by American artisans from the colonial period until the late 19th century.
Volume 10: Registry of Maine Toolmakers fulfills an important part of the mission of
the Center for the Study of Early Tools, i.e. the documentation of the Maine
toolmakers and planemakers working in Maine. It includes an introductory essay on
the history and social context of toolmaking in Maine; an annotated list of Maine
toolmakers; a bibliography of sources of information on Maine toolmakers; and
appendices on shipbuilding in Maine, the metallurgy of edge tools in the museum
collection, woodworking tools of the 17th and 18th centuries, and a listing of important
New England and Canadian edge toolmakers working outside of Maine. This registry
is available on the Davistown Museum website and can be accessed by those wishing
to research the history of Maine tools in their possession. The author greatly
appreciates receiving information about as yet undocumented Maine toolmakers
working before 1900.
Volume 11: Handbook for Ironmongers: A Glossary of Ferrous Metallurgy Terms
provides definitions pertinent to the survey of the history of ferrous metallurgy in the
preceding five volumes of the Hand Tools in History series. The glossary defines
terminology relevant to the origins and history of ferrous metallurgy, ranging from
ancient metallurgical techniques to the later developments in iron and steel production
in America. It also contains definitions of modern steelmaking techniques and recent
research on topics such as powdered metallurgy, high resolution electron microscopy,
and superplasticity. It also defines terms pertaining to the growth and uncontrolled
emissions of a pyrotechnic society that manufactured the hand tools that built the
machines that now produce biomass-derived consumer products and their toxic
chemical byproducts. It is followed by relevant appendices, a bibliography listing
sources used to compile this glossary, and a general bibliography on metallurgy. The
author also acknowledges and discusses issues of language and the interpretation of
terminology used by ironworkers over a period of centuries. A compilation of the
many definitions related to iron and steel and their changing meanings is an important
component of our survey of the history of the steel- and toolmaking strategies and
techniques and the relationship of these traditions to the accomplishments of New
England shipsmiths and their offspring, the edge toolmakers who made shipbuilding
Volume 13 in the Hand Tools in History series explores the iconography (imagery) of
early American hand tools as they evolve into the Industrial Revolution’s increased
diversity of tool forms. The hand tools illustrated in this volume were selected from
the Davistown Museum collection, most of which are cataloged in An Archaeology of
Tools (Volume 9 in Hand Tools in History), and from those acquired and often sold
by Liberty Tool Company and affiliated stores, collected during 40+ years of “tool
picking.” Also included are important tools from the private collections of Liberty
Tool Company customers and Davistown Museum supporters. Beginning with tools
as simple machines, reviews are provided of the metallurgy and tools used by the
multitasking blacksmith, shipsmith, and other early American artisans of the Wooden
Age. The development of machine-made tools and the wide variety of tool forms that
characterize the American factory system of tool production are also explored. The
text includes over 800 photographs and illustrations and an appendix of the tool forms
depicted in Diderot’s Encyclopedia. This survey provides a guide to the hand tools
and trades that played a key role in America’s industrial renaissance. The iconography
of American hand tools narrates the story of a cascading series of Industrial
Revolutions that culminate in the Age of Information Technology.
The Hand Tools in History series is an ongoing project; new information, citations, and
definitions are constantly being added as they are discovered or brought to the author’s
attention. These updates are posted weekly on the museum website and will appear in
future editions. All volumes in the Hand Tools in History series are available as bound
soft cover editions for sale at the Davistown Museum, Liberty Tool Co., local bookstores
and museums, or by order from www.davistownmuseum.org/publications.html,
Amazon.com, Amazon.co.uk, CreateSpace.com, Abebooks.com, and Albris.com.
Table of Contents
Preface .................................................................................................................................. i Introduction.......................................................................................................................... 1 Language & Interpretation............................................................................................... 1 Early Techniques ......................................................................................................... 1 Secrecy ......................................................................................................................... 2 The Changing Meaning of Technical Vocabulary ...................................................... 2 Modern Science and Technology ................................................................................ 3 Shortcomings of Modern Analytical Chemistry.......................................................... 3 On Ironmongers ............................................................................................................... 4 Time Line............................................................................................................................. 6 Handbook for Ironmongers: A Glossary of Ferrous Metallurgy Terms ........................... 11 Appendix I: A Guide to the Metallurgy of the Edge Tools at the Davistown Museum.. 171 Appendix II: Art of the Edge Tool .................................................................................. 173 Appendix III: Classification for Metals and Alloys ........................................................ 175 Appendix IV: Compositions of AISI-SAE Standard Carbon Steels ............................... 177 Appendix V: Classification for Carbon and Alloy Steels ............................................... 181 Appendix VI: Classification of Tool Steels..................................................................... 183 Appendix VII: Iron-Carbon Diagrams ............................................................................ 185 Schematic iron-carbon diagram ............................................................................... 185 Iron-carbon phase diagram ...................................................................................... 186 Iron-carbon constitutional diagram 1 ...................................................................... 187 Cooling curve of pure iron diagram ........................................................................ 188 Solidus-liquidus diagram ......................................................................................... 189 Iron-ironcarbide diagram ......................................................................................... 190 Critical temperature: heating versus cooling diagram ............................................. 191 Alpha-gamma-cementite eutectoid diagram............................................................ 192 Iron-carbon constitutional diagram 2 ...................................................................... 193 Transformation time diagram .................................................................................. 194 Appendix VIII: Popular Knife-Makers’ Steels, c. 1973 .................................................. 195 Appendix IX: Principal Bibliographic Sources ............................................................... 197 Appendix X: Metallurgy and Metalworking Bibliography ............................................. 207 v
Handbook for Ironmongers: A Glossary of Ferrous Metallurgy Terms is published by
The Davistown Museum as part of its Hand Tools in History publication series. This
glossary is an outgrowth of the research done during the investigation of the metallurgy
and metallography of many of the earlier (pre-1860) tools in the museum collection. The
many questions raised by the survival of these tools led to the review and reevaluation of
the art of edge toolmaking and the steel- and toolmaking strategies and techniques upon
which it was based. Also prompting the publication of this glossary as a separate
component of the museum publication series is the contemporary interest in the revival of
older techniques of making iron, steel, and hand tools and the relevance of this
information at the dawn of the era of the creative economy. The urgent need to maintain
or reestablish sustainable environments and lifestyles in the coming age of biocatastrophe
provides additional impetus for the compilation of this glossary.
Language & Interpretation
Many of the definitions and descriptions in this glossary and other Hand Tools in History
publications involve attempts to recreate, retrieve, and uncover older meanings, many of
which pertain to technologies that no longer exist. The editor’s journey through the
labyrinths of ancient metallurgical traditions, especially edge toolmaking, resulted in the
compilation of this glossary, which combines modern scientific knowledge about ferrous
metallurgy with necessarily subjective interpretations of what artisans and edge
toolmakers thought and knew centuries ago, when rule of thumb and intuition dominated
steel- and toolmaking strategies and techniques. Early traditions and techniques are
defined by using a combination of the concepts and terminology of modern ferrous
metallurgy, the writings of contemporary archaeometallurgists, and the fragmentary
descriptions of the past to explain the metallurgical constituents of tools that survive from
early times without any written records to describe how they were made. In compiling
this glossary and attempting to explain early steel- and toolmaking strategies and
techniques, the editor encountered the following concerns that impact our current
understanding and interpretation of ferrous metallurgy terms.
Before the evolution of modern science and the consequent development of an analytical
understanding of the chemistry of ferrous metallurgy and the microstructures of iron and
steel (metallography), the knowledge of successful steel- and toolmaking strategies and
techniques was based on the repetitive, intuitive, empirical methodologies of smelting,
carburizing (or decarburizing,) quenching, tempering, and annealing. These
methodologies often produced iron and steel, including tools, of a surprisingly high
quality. Early techniques were not based on theoretical or scientific conceptions but on
trial and error methods and are frequently referred to as “rule of thumb” techniques
(Brearley 1933, Barraclough 1984a). Intuition, ritual, and generations of empirical
experience played an important role in the art of the ironmonger, hence our inclusion of
“kan of the ironmonger,” a term which describes the kind of knowledge necessary for the
successful steel- and toolmaking that predates the era of bulk steel production (>1870). A
Japanese word and concept, the swordsmith’s “kan” was a combination of ritual and
empirical experience, a methodology of swordsmithing that was beyond words or written
language. The primary evidence for the technical finesse of early toolmakers is the tools
they made, which are the legacy of their uncanny ability to forge hot iron into steeled
Before the age of modern science, intuitive and rule of thumb knowledge of steelmaking
techniques involved implementation of steelmaking strategies that were often
unarticulated, closely guarded secrets manifested in fiery rituals of forging that
sometimes verged on magic. Metallurgists, such as sword cutters and knife-makers, edge
toolmakers, and forge masters who specialized in raw steel production, did not share the
knowledge of their craft traditions in an open society characterized by free exchange of
information. An important objective of any community or culture with an ability to make
superior weapons, tools, iron, or steel would have been to prevent competing cultures and
artisans from acquiring their skills. Until the 19th century, few attempted to systemize and
record knowledge of steel- and toolmaking strategies and techniques. When such writing
did begin to appear (Biringuccio  1990), it was of little use to practicing
blacksmiths, swordsmiths, or edge toolmakers, who operated in a closed society that was
based on mystery, secrecy, and conjuration, i.e. the production of magical effects
(steeling) by natural empirical means (the carburizing or decarburizing of iron).
The Changing Meaning of Technical Vocabulary
The meaning of words pertaining to the history of steel- and toolmaking strategies and
techniques varies from one cultural community to another and also changes over time.
Even today, the terms “German steel,” “wrought iron,” “malleable iron,” and “low carbon
steel” have a variety of meanings no longer consistent with earlier terminology. In many
cases, contemporary writers differ as to the meaning of these words, often not even
attempting to define a generic term such as “malleable iron,” which, it can be argued, has
no specific meaning at all. Many of the terms used in this glossary are no longer relevant
to modern ferrous metallurgists and their bulk process steelmaking techniques.
In his history of the development of iron-making in 17th and 18th century England and
Wales, Hayman (2005), provides relevant commentary on the problem of technical
vocabulary and the language of workmen.
The arcane glossary of terms to define aspects of furnace and forge was part of the
industry mystique and helped to foster a conservative, inward-looking culture. The
use of technical vocabulary in contemporary documentary sources is always at one
remove from its source, since these documents were written by managers and
ironmasters. Moreover, as an oral culture, the language was never definitively
codified. For these reasons the use of terms can seem idiosyncratic and not always
susceptible to definitive interpretation. Meanings also changed over time and so a
term must be interpreted within its specific context. (Hayman 2005, 59)
Modern Science and Technology
The understanding of ancient steel- and toolmaking techniques is significantly enhanced
by our ever-growing knowledge of the chemistry of modern ferrous metallurgy. No
ancient smelters or edge toolmakers had any knowledge of the role of carbon in making
steel or of the atomic structure of the world in which they lived. And yet, underlying our
21st century analytical understanding of chemistry and metallurgy are medieval and
Renaissance technologies based on long established craft traditions. Our interpretation of
early techniques and technologies derives from the projection of our contemporary
knowledge of modern chemistry and the microstructure of ferrous metals on these earlier
traditions. The growing diversity and complexity of alloy steels, recent advances in
powdered metallurgy, an increasing understanding of superplasticity in metals, and the
vast expansion of our understanding of the chemistry and kinetics of modern ferrous
metallurgy assist us in reevaluating the older steel- and toolmaking strategies and
techniques. The modern sciences of metallurgy and metallography thus serve as bridges
connecting two continents; one is made up of lost or obsolete techniques and
terminology, and the other consists of the vast amounts of information now available
through modern information and communications technologies.
Shortcomings of Modern Analytical Chemistry
Modern science has yet to unravel and explain in rational scientific language many of the
complexities of both ancient and modern ferrous metallurgical techniques and the phase
transformation kinetics upon which they are based. Contemporary iron-carbon diagrams
are sufficient only for simple schema. Modern science falls well short of being able to
explain adequately the art of edge tool production, given the wide variety of microconstituents as alloys (deliberately added) or micro-contaminants (accidentally present),
wide variations in the time and temperature of thermal and mechanical treatment
processes, and multiple strategies used in attempts to forge edge tools. In particular, the
complexity of the microstructure of the many varieties of iron and steel have not yet been
fully deciphered, despite the growing capacity of nanotechnology to penetrate this maze.
For example, there is no modern text that adequately explains the techniques and
scientific basis for the ancient production of Damascus steel swords. In this context,
words, including glossary definitions, are inadequate to explain the marriage of art, tools,
Given the challenges of interpreting the long history of steel- and toolmaking strategies
and techniques, the author reviewed numerous antiquarian and contemporary sources to
compile accurate and complete definitions of terms pertaining to the history of ferrous
metallurgy. The revised second edition also includes many new definitions and
descriptions of modern carbon, alloy, tool, and stainless steels, as well as a number of
riffs on the challenges faced by born-again ironmongers as contemporary tool wielders in
the context of an increasingly dysfunctional contemporary consumer society now
entering the early stages of post-Fukushima Daiichi, post-Sandy age of biocatastrophe.
Please contact the author with corrections, suggested revisions, comments, or additional
definitions at [email protected]
The Oxford English Dictionary has the following definition of “monger”:
In formations dating from the middle of the sixteenth century onward monger nearly
always implies one who carries on a contemptible or discreditable “trade” or “traffic”
in what is denoted by the first element of the compound, as in fishmonger…
In European communities before the settlement of North America and in colonial
America and the early republic, ironmongers were ironworkers following the trades of
the bloomsmith, forge master, founder, shipsmith, edge toolmaker, farrier, or community
blacksmith. Ironmongers usually worked in darkened environments, often at night, where
the lack of sunlight allowed them to make the critical judgment of whether the iron
implements and steel tools they were forging or repairing were ready for quenching and
tempering or other heat treatments, as shown by the cherry red color of steels heated to
the proper temperature for forging (1375° F). Before the science of metallurgy and the
chemistry of steel as an iron carbon alloy were known, ironmongers were considered to
be alchemists who somehow possessed the fiery secrets of forging the iron and steel tools
essential to the survival of every maritime and horticultural community. In the age before
the appearance of Lava soap, ironmongers were dirty and sooty, often too sooty, in fact,
to attend Sunday church services. Their odd hours, habits, and alchemical finesse
reinforced the perception of their peculiarity as metallurgical magicians, who were often
so suspiciously regarded that, in African communities at least, they were required to live
in homes located outside of the villages in which they worked.
When the first North American colonial integrated ironworks was established at Saugus,
MA, in 1646, Joseph Jenks and other toolmakers who worked at this facility were
emblematic of the commencement of a vigorous colonial iron industry that would play a
major role in the success of the American Revolution. The finesse of colonial
bloomsmiths, shipsmiths, and edge toolmakers was, in turn, based on two millennia of
Celtic ferrous metallurgy. This glossary is an attempt to retrieve and recapitulate
information about the forgotten steel- and toolmaking strategies and techniques of these
earlier centuries and their legacy to the modern science of ferrous metallurgy.
Table 1. The following time line provides a brief summary of the chronology of
important events pertaining to the steel- and toolmaking strategies of New England’s
shipsmiths and edge toolmakers. Descriptions with an * are excerpted from Barraclough
First production of high quality steel edge tools by the Chalybeans
from the high quality iron sands of the south shore of the Black Sea.
Steel is probably being produced by the bloomery process.*
Carburizing and quenching are being practiced in the Near East.*
Celtic metallurgists begin making natural steel in central and eastern
Widespread trading throughout Europe of iron currency bars, often
containing a significant percentage of raw steel
Tempered tools and evidence for the ‘steeling’ of iron from the Near
The earliest documented use of crucibles for steel production was the
smelting of Wootz steel in Muslim communities (Sherby 1995a).
Celtic metallurgists begin supplying the Roman Republic with swords
made from manganese-laced iron ores mined in Austria (Ancient
Julius Caesar invades Britain
Ancient Noricum is the main center of Roman Empire ironworks.
Important iron producing centers are also located in the Black
Mountains of France and southern Spain.
43-410 AD Romans control Britain.
Steel is made in China by ‘co-fusion’.*
High quality pattern-welded swords being produced in the upper Rhine
River watershed forges by Merovingian swordsmiths from currency
bars smelted in Austria and transported down the Iron Road to the
First documented forge used by the Vikings at L’Anse aux Meadows
First appearance of blast furnaces in central and northern Europe
First appearance of blast furnaces in the Forest of Dean (England)
[Natural] steel made in the Weald [Sussex, England] by fining cast
First record of the cementation process, in Nuremberg*
First shipsmith forge in the American colonies used at Fort St. George,
Cementation process is patented in England.*
The great pandemic sweeps through the indigenous communities of the
New England coast east of Narragansett Bay.
First Maine shipsmith, James Phipps, working at Pemaquid
The great migration of Puritans from England brings hundreds of
trained shipwrights, shipsmiths, and ironworkers to New England.
First colonial blast furnaces and integrated ironworks are established at
Quincy and Saugus, Massachusetts.
James Leonard establishes the first of a series of southeastern
Massachusetts colonial era bog iron forges on Two Mile River at
King Philip’s War in southern Massachusetts and Rhode Island
The great diaspora (scattering) of Maine residents living east of Wells
follows the King Philip’s War
First documented use of the cementation process in England
The war of the League of Augsburg
The war of Spanish Succession
Joseph Moxon ( 1989) publishes Mechanick Exercises or the
Doctrine of Handy-Works.
Abraham Darby discovers how to use coke instead of coal to fuel a
First appearance of clandestine steel cementation furnaces in the
First of the Carver, Massachusetts blast furnaces established at Popes
William Bertram invents manufacture of ‘shear steel’ on Tyneside.*
René de Réaumur (1722) provides the first detailed European account
of malleableizing cast iron.
Benjamin Huntsman adapts the ancient process of crucible steelproduction for his watch spring business in Sheffield, England.
The Seven Years War, the last of the French and Indian wars
John Wilkinson begins the production of engine cylinders made with
the use of his recently invented boring machine.
The defeat of the French at Quebec by the English signals the end of
the struggle for control of eastern North America.
The Treaty of Paris, which opened up eastern Maine for settlement by
James Watt designs and patents an improved version of the Newcomb
atmospheric engine, i.e. the steam engine.
John Wilkinson begins the mass production of engine cylinders used in
Watt’s steam engine pressure vessels.
Matthew Boulton and James Watt begin mass production of steam
The approximate date when Josiah Underhill began making edge tools
in Chester, NH. The Underhill clan continued making edge tools in
NH and MA until 1890
James Watt improves the efficiency of the steam engine with
introduction of the double-acting engine.
Henry Cort introduces his redesigned reverbatory puddling furnace,
allowing the decarburization of cast iron to produce wrought and
malleable iron without contact with sulfur containing mineral fuels.
Henry Cort invents and patents grooved rolling mills for producing bar
stock and iron rod from wrought and malleable iron.
Era of great prosperity for New England merchants due to the neutral
Samuel Slater first began making textiles
Henry Maudslay invents and produces 45 different types of machines
for mass production of ship’s blocks for the British Navy.
Samuel Lucas of Sheffield invents the process of rendering articles of
cast iron malleable.
Jesse Underhill is first recorded as making edge tools in Manchester,
The factory system of using interchangeable parts for clock and gun
production begins making its appearance in the United States.
Thomas Blanchard designs a lathe for turning irregular gunstocks.
Steam-powered saw mills come into use near Bath, Maine, shipyards.
Adoption of the hot air blast improves blast furnaces
Seth Boyden of Newark, NJ, first produced malleable cast iron
commercially in the US.
D. A. Barton begins making axes and edge tools in Rochester, NY.
Joseph Whitworth introduces innovations in precision measurement
techniques and a standardized decimal screw thread measuring system.
Malleableized cast iron is first produced in the United States.
Steel is first made by the puddling process in Germany.*
The first railroad is established between Boston and Worcester,
The Collins Axe Company in Collinsville, Connecticut, begins the
production of drop-forged axes.
In England, Joseph Nasmyth introduced the steam-powered rotary
William Vickers of Sheffield invented the direct conversion method of
making steel without using a converting furnace.
Joseph Nasmyth patents his steam hammer, facilitating the industrial
production of heavy equipment, such as railroad locomotives.
Thomas Witherby begins the manufacture of chisels and drawknives in
Joseph Dixon invented the graphite crucible used in a steel production.
John, Charles, and Richard T. Buck form the Buck Brothers Company
in Rochester, NY, after emigrating from England and working for D.
A. Barton. They later move to Worcester, MA in 1856 and Millbury,
MA in 1864.
Gasoline is first distilled at Watertown, Massachusetts.
Bessemer announces his invention of a new bulk process steelproduction technique at Cheltenham, England.*
The panic and depression of 1857 signals the end of the great era of
wooden shipbuilding in coastal New England.
First successful work on the Siemens open-hearth process*
Significant production of cast steel now ongoing at Pittsburg,
R. F. Mushet invents ‘Self-hard,’the first commercial alloy steel.*
1870-1885 Era of maximum production of Downeasters in Penobscot Bay (large
four-masted bulk cargo carriers)
Tilting band saw is introduced and revolutionizes shipbuilding at
Sidney Gilchrist Thomas invents basic steelmaking.*
The first electric-arc furnace is installed in Sheffield.*
Brearley invents stainless steel.*
The first high-frequency induction furnace in Sheffield*
*(Barraclough 1984a, 13-4).
Handbook for Ironmongers: A Glossary of
Ferrous Metallurgy Terms
The definitions in this text derive from a wide variety of contemporary and antiquarian
sources pertaining to the art of the bloomsmith, forge master, blacksmith, edge
toolmaker, shipsmith, founder, and other artisans of ferrous metallurgy. A bibliography
of sources used in the compilation of this glossary follows the other appendices and is
followed by a general bibliography on metallurgy. More comprehensive bibliographies
pertaining to steel- and toolmaking strategies and techniques before 1870, the evolution
of iron-smelting and toolmaking in colonial New England, and the florescence of
American toolmakers are included in each volume of the Hand Tools in History series.
All bibliographies are reprinted in Davistown Museum publication 48: Davistown
Museum: The Complete Bibliographies. This handbook also includes a variety of
definitions and notes pertaining to our contemporary (2013) social, political, economic,
and environmental milieu and the challenges faced by tool wielding artisans and
craftspersons (born-again ironmongers) as the tragedy of our round world commons
Acicular: An adjective describing interlocking needle-like formations that characterize
the crystal structure of ferrous metals under a variety of cooling conditions. Slowly
cooled pearlite, formed during the production of blister steel, has acicular characteristics
in the form of acicular ferrite. The rapid cooling of austenite results in the instantaneous
formation of martensite, another allotropic form of iron characterized by an acicular
crystal structure (Bain 1939). See allotropic forms of iron, blister steel, crystal structure,
ferrite, and pearlite.
Acicular ferrite: A common component of pearlite, ferrite that has acicular crystal
structures characterized by “tough and strong microstructures” (Sinha 2003, 9.24).
Acicular mode of transformation: Rapid quenching of austenite (eutectoid carbon steel)
during a time period of two minutes or less to slightly above or near room temperature
(200º F) results in transformation of austenitic microstructures by shearing mechanisms
that produce martensitic structures. In contrast, slow cooling rates are characterized by
carbon diffusion, which produces ferrite and cementite matrixes, i.e. pearlite. The
crystallographic planes of martensite have an acicular structure as a result of their near
instantaneous transformation; any remaining austenite also suffers deformation (Bain
1939). See acicular.
Acid process: Production of steel using furnaces lined by a siliceous refractory, such as
sand or clay, suitable for low phosphorous ores only. Until 1877, the acid process was the
primary means of bulk process steel production. Introduction of the basic process after
1877 allowed smelting of ores with a high phosphorous content. See basic process and
Acid steel: Steel melted under a slag that has an acid reaction and in a furnace with an
acid bottom or lining (Shrager 1949).
Acier fondu: The French term for cast steel.
Acier forge: The French term for fined (decarburized) pig iron. See pig iron.
Adz (adze): A common woodworking tool used for smoothing wood both across and
with the grain. The most ancient and important of all forms of woodworking tools, adzes
differ from axes in that the adz head is aligned with the haft, like a hoe. Primitive forms
of stone adzes were used as early as the beginning of the Stone Age. Cold hammered
bronze adzes were the most important shipbuilding tool in the Bronze Age. The oldest
known “steeled” adz is a malleable cast iron adz with a heat-treated steeled cutting edge
made in China, c. 950 BC (Barraclough 1984a). Iron, natural steel, and steeled iron adzes
were commonplace throughout the Iron Age and well documented in Roman
archeological sites (Manning 1985). Goodman (1964) has excellent illustrations of both
the socket and shaft hole adz forms. The most famous of all adzes is the unique New
England “Yankee Pattern” ship carpenter's lipped adz, which was first made sometime in
the 18th century and probably designed by some Gulf of Maine shipsmith whose identity
has been lost. Also called a dubbing adz, this tool was used for shaping the frames and
ribs of ships.
Age hardening: Changes in the physical properties of low carbon steels and other
nonferrous metals at or slightly above room temperature over a period of time where
unstable crystal structures gradually return to more stable forms.
Age of Bioengineering: See bioengineering, age of.
Air blast heat exchangers: In direct process Catalan forges, air blast heat exchanges
facilitated the transfer of heat from the furnace directly to the air blast by the use of
horizontal iron pipes that were exposed to furnace exhaust and connected to vertical iron
pipes that lead into the tuyère. Various designs of air blast heat exchangers characterize
all modern blast and cupola furnaces.
Air furnace: A furnace used to melt cast iron and to refine other metals. The fuel, which
is usually coal or coke, and the flame that passes over the bath holding the melted metal,
do not come in contact with the metal, and, thus, the carbon content of iron can be
carefully controlled. The term air furnace is synonymous with reverbatory furnace. See
AISI: See American Iron and Steel Institute.
Albedo: the reflection of sunlight from polar ice and snow cover; also the reflection of
high frequency ultraviolet light from the sun by the stratospheric ozone layer. Decreasing
surface albedo is an important cause of global warming. A decrease in the earth’s
stratospheric ozone layer as a result of chlorofluorocarbon emissions increases the risk to
human health from ultraviolet light.
Allotropic/Allotropy: Property of having changing physical characteristics, e.g. crystal
structure, while retaining elemental chemical identity, i.e. an iron carbon alloy. Allotropy
is expressed as the multiple forms of a space lattice in an element, i.e. its microstructure.
See allotropic forms of iron, allotropic transformation, crystal structure, phase
transformation, and space lattice.
Allotropic forms of iron: Iron has three allotropic forms. Alpha iron, also called ferrite,
the low temperature form of iron up to 1670° F (910° C), has a body-centered cubic
structure (BCC) and is soft, ductile, and magnetic. Gamma iron, also called austenite,
with a face-centered cubic form (FCC), is nonmagnetic in a temperature range from
1670° F to 2540° F (1393° C) and is more compact and dense than alpha iron due to its
carbon content being in a solid solution. In its pure iron form, austenite is also soft and
ductile (Sinha 2003, 1.1). Delta iron, with a body-centered lattice structure (BCC)
between 2240° F and 2793° F (1538° C), exhibits magnetism above its threshold
temperature of 2240°F. The space lattice structure of iron breaks down above 2793° F
(1538° C) as iron enters the liquid state. Temperature determines the crystal structure of
ferrite-iron carbide combinations. Variations in carbon and alloy content, quenching,
tempering, and cooling rates further influence the allotropic and microstructural forms of
iron, steel, and cast iron. See the iron carbon diagrams in Appendix VI.
Allotropic transformation: Spontaneous and reversible changes in the microstructure of
steel made by changing the temperature of the metal.
Alloy: Metallic substance fused with either another metal or a non-metallic element, e.g.
steel is an alloy made of iron and carbon. The metals most commonly alloyed with iron
are nickel, silicon, manganese, tungsten, chromium, cobalt, vanadium, and molybdenum.
See brass and bronze.
Alloy steels and alloy cast irons: Steel and iron containing other elements in addition to
carbon. Strength, durability, toughness, hardness, corrosion resistance, fracture, and
carbon distribution are among the many properties determined by metals alloyed with
iron and steel. Some alloying elements serve to increase the formation of martensite at
slower rates of cooling or at lower temperatures, therefore increasing hardenability. In the
AISI-SAE classification system, alloy steels are defined as any steel exceeding element
limits of carbon steels, e.g. manganese 1.65%, silicon 0.9%, and copper 0.6%. See
carburize, decarburization, and martensite.
Alpha iron: Another term for ferrite (pure iron); an iron with the face-centered cubic
(FCC) form at temperatures below 1414º F (768º C). The allotropic form of iron begins
changing to BCC at 1414º F, and the transition to Gamma iron is completed at 1670º F
(910º C). Alpha iron has a carbon content ≤ 0.03% and is the softest component in the
microstructure of steel. See carbon content of steels, ferrite, and wrought iron.
American felling ax: A distinctive form of American ax developed in the 18th century in
response to the need for a felling ax with a heavier poll than those on traditional English
felling axes. Such felling axes were usually forged out of two slabs of iron, which were
steeled with an inserted bit after being folded and welded (Kauffman 1972).
American Iron and Steel Institute (AISI): An association of North American steel
producers. They, along with the Society for Automobile Engineers (SAE) created the
modern classifications of standard steel, alloy steel, stainless steel, and tool steel. See
Appendix IV, carbon steel classifications, and classification system for steel.
American Society for Testing and Materials (ASTM): Recently renamed ASTM
International. Established in 1898 by the Pennsylvania railroad, the ASTM now
promulgates the standards for materials, including steel and iron used in industrial
processes. See Appendix IV.
American system of manufacturing: Developed after 1830, the American system is
characterized by the waterpower-driven production of tools and firearms with machinemade, interchangeable parts. The lower Connecticut River Valley was America's first
center of manufacturing utilizing interchangeable parts. Eli Terry (clockmaker), Elisha
Root (axes), Eli Whitney (firearms manufacturing), and John Hall (firearms
manufacturing) are some of the major figures in the evolution of the American factory
system. See the Tool Manufacturing Chronology online at
Amisenian: Synonymous with Chalybean, the Anatolian community that produced high
quality nickel steel from Black sea sands using chloanthite as a flux during the Bronze
Age (1900 BC). See Chalybean steel.
Anchorsmith: Blacksmith who specialized in making anchors. Before 1800, anchors
were often made from forged wrought iron produced by a bloomsmith at a direct process
bloomery. From the early Iron Age until the 18th century, many shipsmiths were also
anchorsmiths as well as edge toolmakers. After 1800, puddled iron gradually replaced
direct process bog iron for anchor production, and trade specialization resulted in the
separation of these crafts into individual professions. See blacksmith, bloomsmith, and
Ancony: Short thick wrought or malleable iron bar stock produced in a finery from
shingled iron before being sent to the chafery for shaping into special sizes suitable for
North American colonial era production of iron tools and artifacts. Anconies were two to
three feet long with knobbed or square ends (Gordon 1996). See chafery, finery,
malleable iron, and wrought iron.
Ångström: A non-SI (International System of Units) unit of measurement denoted by the
symbol Å which is equal to 1/10,000,000,000th of a meter (1×10−10 m).
Anisotropic: An adjective used to describe materials having different properties
determined by variations in the directional arrangement of their crystallographic patterns.
Directional dependency is also expressed by the related root word anisotropy. See crystal
structure, grain, isotropic, and microstructure.
Anneal: To heat steel to a temperature, which is usually, but not always, below its critical
temperature, followed by slow cooling to toughen it by altering its microstructure, which
allows the uniform distribution of particles of cementite within the crystal structure of the
annealed steel. Since, in many cases, annealed steel has not been quenched and tempered,
annealing can be considered an alternative method of softening steel or otherwise
relieving strain hardening. The variants of time, temperature, carbon, and alloy content
allow an immense variety of annealing techniques. “...to relieve internal strains and
improve strength, elasticity and ductility to meet the stresses to which it is subjected in
service. It is usually done by heating and holding at a certain temperature followed by
slow cooling” (Salaman 1975, 246). Annealing changes the diffraction patterns of the
crystal structure of the metal being annealed. During the annealing of white cast iron,
which typically takes 60 hours or longer, all the chemically combined carbon is reduced
to free carbon or graphitic carbon surrounded by pure iron. Iron oxide or millscale packed
with the white cast iron facilitates malleable cast iron production by assisting in the
freeing of the carbon from its chemical bond within the iron. Many variations of the
annealing process produce a wide variety of forms of malleable cast iron. Partially
decarburized, annealed cast iron can be reheated and suddenly cooled, giving a steely
fracture. In many cases, the specific procedures and techniques used to produce malleable
and grey cast iron artifacts, such as Griswold cast iron cookware, were highly guarded
trade secrets. In plain carbon steels, annealing usually results in the production of ferritepearlite microstructures. See full annealing, crystal structure, fracture, malleable cast
iron, martensite, temper, and white cast iron.
Annealed eutectoid steel: Pearlite, the transformation product of austenite containing
0.83% carbon content, after slow annealing. Variations in the temperature and rate of
annealing result in variations in the microstructure of the pearlite being formed as
annealed eutectoid steel. The rapid cooling of austenite produces martensite. See
annealing, austenite, eutectoid, martensite, and pearlite.
Annealed hypereutectoid steel: A pearlite-cementite matrix, the transformation product
of austenite containing more than 0.83% carbon content after slow cooling. Variations in
the temperature and rate of annealing result in variations in the microstructure of the
pearlite-cementite matrix being formed as annealed hypereutectoid steel.
Annealed hypoeutectoid steel: A pearlite-ferrite matrix, the transformation product of
austenite containing less than 0.83% carbon content after slow cooling. Variations in the
temperature and rate of annealing result in variations in the microstructure of the pearliteferrite matrix being formed as annealed hypoeutectoid steel. The rapid cooling of
austenite, followed by the termination of cooling between 800º F and 400º F and holding
of the temperature for a variable time period, usually hours (austempering), creates
microstructures known as bainite, the intermediary between ferrite-pearlite (uninterrupted
slow cooling) and martensite (fast cooling, as with quenching). A scientific
understanding of the microstructures of ferrous metals including eutectoid steels was not
clearly elucidated until Edgar C. Bain (1939) published his classic text Functions of the
Alloying Elements in Steel. See bainite.
Annealing pots: Cast iron pots utilized to enclose and protect steel being annealed from
the formation of iron oxide scale; used especially for annealing wire.
Annealing, purpose of: One of the most important strategies for producing a wide
variety of modern steels. There are now dozens of annealing techniques used for the basic
heat treatment of many special purpose alloy steels. Shrager (1949) has these comments
on annealing steel:
Annealing may be performed by one of several methods, depending upon the results
desired. The purpose of annealing may be: (1) to remove stresses that have occurred
during casting or as a result of work done on steel; (2) to soften steel for greater ease
in machining, or to meet stated specifications; (3) to increase ductility in order to
make steel suitable for drawing operations; (4) to refine the grain structure and make
the steel homogenous; (5) to produce a desired microstructure. (Shrager 1949, 154)
All of Shrager’s comments also pertain to the annealing of white and/or grey cast iron to
produce the many forms of malleable cast iron. See grey cast iron, malleable cast iron,
microstructure, stress, and white cast iron.
Antrim patent: Patent granted for welding steel straps onto the front band of shovels;
used at Ames Shovel Works to produce the best quality shovels.
Anvil: “A heavy iron block with a hardened or applied steel topped face suitable for use
by a blacksmith in working hot metal” (Sellens 1990, 5). In his Dictionary of American
Hand Tools, Sellens lists 36 different types of anvils, many of which had a wide variety
of forms, such as dengel stocks (scythe anvil). Most anvils had a flat work surface, in
contrast to mandrels and other tools with curved work surfaces. Anvils were made from
both wrought iron and cast iron and generally had a steel plate welded to the top. In the
late 19th century, some makers produced solid cast steel anvils.
Apocalypse: The revelation of biocatastrophe; the disclosure, understanding, and
experience of the synergistic components of biocatastrophe by the communities impacted
by the disruptions of cataclysmic climate change, the hemispheric transport of ecotoxins
and their bioaccumulation in pathways to human consumption, pandemics, and the
infrastructure collapse that results as a consequence of the growth and demise of a nonsustainable pyrotechnic industrial society.
Archaeometallurgy: Study of ancient and antiquarian strategies and techniques for
smelting, casting, and/or forging metals (copper, brass, bronze, lead, silver, iron, and
steel) into hand tools and other artifacts; the study of the microstructure of metals
produced by these techniques.
Archimedean screw: Hollow, inclined screw, usually in the form of a spiral pipe with an
inclined axis. When used as a water pump, the lower end of the screw gathers in water,
which is then discharged at the upper end; one of the first forms of the simple machine
known as the screw. It was named after its Egyptian inventor, Archimedes (260 BC).
Arms race: Competition between cultures/countries to produce superior weapons. The
first arms race occurred when the use of the blast furnace became widespread in northern
Europe sometime during the late 14th and early 15th centuries. Its principal function was
the production of cast iron cannon, which, along with bronze cannon, were used to arm
the growing fleets of England, France, Spain, and The Netherlands. The growth of
English merchant shipping and the Royal Navy were accompanied by the expansion of
cannon and ordnance casting, and the proliferation of wrought iron handguns, such as the
matchlock and then the flintlock. The arms race that began with the construction of the
first blast furnace has continued unabated into the 21st century. All advances in ferrous
metallurgy had and have as their primary social function the objective of improving
weapons production. Successful exploration, conquest, and settlement of the New World
were closely linked to innovations and improvements in the production of firearms.
Arquebus: The most common form of firearms at the time of Native American –
European contact. The arquebus was always made of wrought iron and was brought to
North America by French traders in exchange for furs, forever changing the lifestyles of
the indigenous communities impacted by its availability. See matchlock.
ASTM: See American Society for Testing and Materials.
Atomic planes: Planes within a crystal, along which the atoms of a particular lattice
structure are arranged.
Austemper: To produce bainite by the interrupted quenching of austenite in a bath of
molten salt held at a temperature of 450º F - 800º F until bainite formation is completed.
See bainite, martensite, and quench.
Austenite: Iron carbon alloy (steel), in which carbon is dissolved in iron as a stable solid
carbon solution at a temperature range of 723º C (1400º F). Unstable at room
temperature, austenite has a face-centered cubic (FCC) lattice structure, creating more
space for a higher proportion of carbon to be held in interstitial solution than in the bodycentered cubic (BCC) lattice structure of ferrite. If cooled slowly, granules of pearlite will
appear in the austenite matrix, creating steel of inferior quality. If cooled rapidly, hard
and brittle martensite will be produced, which, if then tempered (slowly heated and
cooled), will be slightly softened and made less brittle by the homogenous redistribution
of tiny spheroids of cementite, creating steel with a uniform carbon content (cc). See
cementite and microstructure.
Austenite formation: Use of thermal treatments (heating) to change the microstructure
and, thus, the allotropic form of a wide variety of ferrite-pearlite-cementite
microstructures to austenite (gamma iron). Austenite formation occurs in two stages in
low carbon steels: 1) pearlite transformation to austenite occurs at temperatures greater
than 800º C; 2) ferrite to austenite transformation occurs at 910º C. If the latter
temperature is not reached, “the second stage of further nucleation does not occur, and
the process is complicated by the growth of the remaining austenite particles within the
ferrite matrix” (Sinha 2003, 10.6).
Austenite nucleation sites: Since austenite is formed with pearlitic microstructures, three
favorable nucleation sites are “ the ferrite/cementite interface,  the line of
intersection between platelets and surfaces of the pearlite colony, and  the points of
intersection between platelets and the edge of the pearlite colony” (Sinha 2003, 10.2).
Austenitic steels: Alloy steels containing chromium, nickel, or manganese that retain
austenite at atmospheric temperatures.
Austenize: To create steel by heating iron above 723º C (1400º F) (the minimum
austenizing temperature) and holding that temperature to allow the microstructural
formation of austenite. The rate of cooling that follows determines the microstructural
qualities of steel (Wayman 2000). Rapid cooling produces martensite; slow cooling
allows austenite to return to ferrite and pearlite. See austenite, ferrite, martensite, pearlite,
quench, and temper.
Austenizing temperature: In modern alloy steel production, the temperature between
1400º F (723º C) and 1900º F (1040º C), depending on carbon content (Pollack 1977). A
more recent commentator notes austenite formation from various initial microstructures
as starting at 735º C and being contingent upon various holding times (Sinha 2003, 10.1.2). See austenize.
Ax (Axe): A common woodworking tool, on which the cutting edge, and, thus, the
cutting angle, is in the same plane as the sweep of the implement in contrast to the adz,
on which the cutting edge is perpendicular to the plane of the sweep.
Ax-Adz: Earliest metal form (copper) of a woodworking tool, dating to c. 4000 BC, 2100
years before the age of Chalybean steel. The cold hammered copper ax-adz was only
slightly less dull than a stone ax. The cutting edges of the ax and the adz were
perpendicular to each other as in a modern variation of this tool, one form of the
Ax bar: Bar stock that is 1” x 3” and often provided in 12’ lengths. A standard
commodity of the 19th century, ax bar stock ranged from malleable bar iron suitable for
steeling to German or blister steel suitable for additional steeling or forging. See Collins
& Co., ax, ax-making techniques, eyepin, and overcoat method.
Ax-making techniques: Before the era of the one piece cast steel ax, three strategies for
steeling an ax were used in most ax-making factories. The oldest method of steeling an
ax, used since the early Iron Age, was to insert a piece of carbon steel between a folded
slab of iron and then weld them together. A more modern form of steeling is the overcoat
method, in which a piece of high carbon steel is wrapped or folded over the iron or low
carbon steel ax body prior to welding. The third strategy for ax manufacturing is called
the scarf-joint method and was primarily used on the Canada pattern broad ax. “The iron
body was feathered to an edge and then the steel bit was scarfed onto the blade” (Lee
1995, 170). The modern method of drop-forging an ax involves cutting steel billets,
typically into three pieces, and then heating them to a temperature of 2350° F prior to
drop-forging and quenching in brine (Kauffman 1972, Klenman 1998). See ax, cast steel,
steeling, billets, drop-forging, eyepin, and iron cored.
Babbitt: Alloy used to make bearings. In its original form, babbitt is 89% tin, 3.5%
copper, 7.5% antimony, but it is also made with varying quantities of lead.
Bainite: Mixture of ferrite and cementite with a microstructure that forms during the
rapid cooling of austenite to a temperature of 800° F, after which it is held for a long
period of time at a temperature above 400° F, but less than 800° F. This quenching
method is known as austempering. Bainite is an intermediary between ferrite-pearlite
(slow cooling) and martensite (fast cooling, as with quenching) and is more ductile than
pearlite but less brittle than martensite. The transformation of austenite to bainite results
in a wide variety of microstructure formations and is contingent upon alloy content and
cooling strategies, the latter of which may vary in duration, temperature, and cooling
mediums, such as water, air, oil, or salt baths. Bainite is shown as ledeburite on some iron
carbon diagrams. See annealed hypoeutectoid steel, austemper, austenite, cementite,
ferrite, martensite, and pearlite.
Balkan Copper Age: The earliest pyrotechnic society, c. 6000 BC, the Balkan Copper
Age culture evolved from the Neolithic Vinča culture, which was located along the
shores of the Danube and flourished prior to the Copper Age in the Aegean. Early Iron
Age smelting techniques and furnace designs can be traced back to this culture. Its most
famous archeological site is Catul Huyuk (Çatalhöyük). See Renfrew (1973).
Ball vise: The principal vise used to hold die blanks for shaping drop-forged dies; also
used by silversmiths and pewter spinners for securing die-sinking patterns for flatware,
Britannia Ware, and pewter.
Bar mill: Mill in which billets of iron or steel are reduced in thickness and width by
Basic oxygen furnace: Modern furnace used to make steel by melting scrap steel using
oxygen produced in an oxygen plant as the fuel.
Basic oxygen process (BOP): One of the two most widely used steelmaking processes in
the 20th century. The basic oxygen process is an offshoot of the Bessemer process,
utilizing pure oxygen for the rapid decarburization of cast iron, with significantly less
pollution produced as an unwanted byproduct. The basic oxygen steelmaking process was
introduced in the US in 1955 and quickly supplanted open hearth furnace steel
production, reaching almost 65% of total US steel production by 1980. Furnace design
and the charges utilized, pig iron high in manganese content and low in phosphorous, are
similar to the now obsolete Bessemer furnace. Oxygen steelmaking processes are
subdivided into the top-blown oxygen process and the bottom blown process, with the
recent evolution of numerous special subtypes, including some suitable for processing the
high phosphorous ores that dominate European rock ore production. No tool steels are
produced by basic oxygen processes.
Basic steelmaking process: Process of making steel in steel furnaces with linings of
limestone and other basic elements. This process revolutionized bulk steel production
processes by allowing the smelting of ores high in phosphorous, which had not been
possible in furnaces with acid linings such as sand and clay. Invented by Sidney Gilchrist
Thomas in the 1870s and patented in 1879, this process was particularly useful for the
open-hearth and Bessemer process and furnaces in continental Europe, especially
Germany, located near high phosphorous ore deposits.
BDTT: Brittle-ductile transition temperature.
Beak iron: Tools with various designs of horns, points, or beaks, which could be inserted
into swage blocks and anvil hardy holes for the purpose of shaping iron and steel,
especially sheet iron. Many European and American specimens were collected in Europe
and brought to America by Kenneth Lynch (2007) and are illustrated in the publication
The Armourer and his Tools :The Kenneth Lynch Tool Collection. Historically important
variations of beak iron, all derived from European prototypes, include the blow horn and
ball-top, flat-top, and other stakes, which were also first produced in the U.S. by the
North Brothers in Connecticut.
Bears: Ferruginous furnace bottoms produced by the smelting of copper during the
Copper and Bronze Ages, when iron oxide (Fe2O3) was used as a flux; also called
salamanders. During the Iron Age, many of these bears, rich in iron oxide, were resmelted to produce iron tools and weapons.
Beating out: Shaping of the curved futtocks and other components of the ship’s frame
with the use of the broad ax either in woods at the timber harvesting site or at the
shipyard. The Yankee pattern broad ax is the generic ax used by New England
shipwrights for this purpose. See shipsmith and broad ax.
Bed charge: The pig iron placed on the coke bed prior to firing a cupola furnace.
Belgian iron: Soft wrought iron preferred by gun makers in Europe and Britain during
the Renaissance (1450-1650); more easily forged and welded than other irons and steels
used in gun barrel forging (Greener 1910).
Bell metal bronze: 75-80% carbon, 20-25% tin. Tin serves as a hardener.
Bergman, Tobern: Swedish chemist who was among the first researchers to identify
carbon as the critical component of steel in 1791.
Bessemer, Henry: (1813-1898). Inventor of the process of manufacturing low carbon
steel by oxidizing liquid pig iron with an air blast, thereby burning out silicon and other
constituents. Bessemer issued his famous paper The manufacture of malleable iron
without fuel in England in 1856. Due to the problem of phosphorus in the ores used to
make the pig iron, Bessemer was initially unsuccessful in producing a useful malleable
iron or low carbon steel product due to over oxidation. Robert F. Mushet soon suggested
the addition of spiegeleisen, an iron-carbon-manganese alloy, and after establishing a
steelworks in Sheffield in 1858, Bessemer gradually perfected the art of the mass
production of steel. See Mushet, Robert F.
Bessemer process: Conversion of pig iron to steel in one step; first described by Henry
Bessemer in 1856. A hot air blast produces Bessemer steel in a closed converter by rapid
oxidation of the impurities in the pig iron, including silicon and most carbon.
When Bessemer and open-hearth steels made their appearance in the market, an
attempt was made to use them instead of wrought iron as the base for high-grade
crucible steels. Though seemingly pure enough, apparently purer even than wrought
iron, these metals were not able to compete with wrought iron for this purpose. For
some reason, not yet satisfactorily explained, these new materials, which are made in
15, 35 and 50-ton batches, when used as a base, do not give as high quality tool steel
as puddled wrought iron, which is slowly and laboriously made in 500-pound lots.
(Spring 1917, 121-122)
The Bessemer process, which gave a brilliant fireworks display, was a rapid one,
taking less than half an hour. For this reason, it was not easy to control the process, so
the steel varied more than was thought proper. (Abell 1948, 148)
Until the addition of spiegeleisen to strengthen it, Bessemer steel was unsuitable for
many of its later uses. See crucible steel, manganese, open-hearth process, silicon,
spiegeleisen, and wrought iron.
Bickern: “A smaller, TANGED version of the ANVIL that was particularly useful for
small, rounded objects that were too small to be worked on the large anvil horn” (Light
Billets: Wrought or malleable iron bars forged by a blacksmith from an iron bloom. In
the early Iron Age, billets were made from smelters’ currency bars after the removal of
slag and consolidation of iron. After the development of bulk process steel, billets are
defined as semi-finished squares of iron and steel made from red-hot ingots prior to
further mechanical (rolling and forging) and thermal treatment. Roman billets were
typically 5 – 10 kg (Tylecote 1987).
Bimetallic tools: Axes with iron or steel cutting edges attached to bronze heads; axes
with iron cores covered with bronze (1300 – 1000 BC) (Wertime 1982).
Bimetallism: In early polymetalic societies, the production of tools and weapons using
more than one metal, e.g. pattern-welded bronze and iron knives (rare) or the use of
bronze rivets in iron shafts for sword production.
Biocatastrophe: The simultaneous degradation of the earth’s principal biomes and the
consequential decline of the capacity of biome ecosystems to produce sufficient supplies
of fresh water, affordable food, (including fresh and salt water fish), renewable biomass
fuels, and other biome-derived natural resources to furnish the needs of billions of people
dependent on the complex infrastructure grids of industrial society. Biocatastrophe is the
future consequence of the synergistic interaction of overpopulation, cataclysmic climate
and sea level change, oceanic pollution and fisheries depletion, deforestation, soil
erosion, depletion of non-renewable energy sources, reduced biodiversity, fresh water
depletion and contamination, regional and/or world wide pandemics, and the
accumulation of biologically significant chemical fallout and other ecotoxins in pathways
to human consumption. Political paralysis, social unrest, and entrenched income disparity
will characterize a collapsing global consumer society where public needs far outstrip
public resources. Iron-smelting, steel forging, and other pyrotechnic activities of
industrial society and its transportation systems will continue to play a principal role in
ecosystems degradation as important source points of biologically significant chemical
effluents, increased CO2 emissions, and non-renewable biomass fuel depletion. See
mercury and infrastructure collapse.
Biocatastrophe in a nutshell: The synergistic impact of a lot of bad things happening all
at once, i.e. the tragedy of the commons in a biosphere with finite natural resources.
Bioengineering, Age of: An optimist’s name for the Age of Biocatastrophe.
Biologically significant chemical fallout (BSCF): Liquid, gaseous, and particulate
emissions produced by the pyrotechnical activities of industrial society that have a
deleterious impact on living organisms, including humans, and which play a hidden, but
major, role in the ongoing decline of the biodiversity of most ecosystems. The
proliferation of gene altering hormone disrupting chemicals (HDC) in domestic
environments and consumer products (e.g. BPA) appears to be correlated with increases
in autism spectrum disorders, birth defects, asthma, and possibly obesity. Methylmercury,
dioxin, chlorinated hydrocarbons, perchlorates (rocket fuel), brominated fire retartants,
and other persistent organic pollutants (POP) are among the ubiquitous byproducts of
biomass fuels and their processing into thousands of chemicals used by industrial society
or in its consumer products. Long-lived anthropogenic radioisotopes are the primary form
of biologically significant chemical fallout produced by nuclear-powered heat engines
(steam turbines). Contamination of ecosystems with biologically significant chemicals
can take forms as diverse as stratospheric fallout (radioisotopes), tropospheric fallout (all
forms of chemical fallout derived from evaporated or biogeochemically mobilized
toxins), and liquid and/or particulate toxins emitted from terrestrial industrial and
domestic environments and consumer products. Most forms of BSCF bioaccumulate in
pathways to human consumption. See biocatastrophe, infrastructure collapse, mercury,
Biomass fuels: Wood, peat, coal, coke, gas, and oil utilized as fuels for the heat engines
of industrial society. Biomass fuels, most of which are nonrenewable, are a metaphorical
bank account that, once depleted, cannot be replenished. See biocatastrophe, furnace
types, and smelting.
Biosphere as bank account: Hundreds of millions of years of carbon cycling and
photosynthesis created most of the biomass fuels used by industrial society to smelt and
forge the earth’s abundant iron resources into the infrastructure grids (e.g. cities and
transportation systems, etc.) of contemporary global consumer society. Implicit in the
depletion of the earth’s biomass as bank account is the contraction and then collapse of
growth-based, consumer-product-centered, industrial society.
Biosphere as industrial effluent cesspool: Worldwide iron-deposit-derived steel
production is now rapidly passing 100 million tons per month. Exploitation of natural
resources, such as iron, coal, oil, and gas, occurs in conjunction with the use of the
biosphere as an industrial effluents cesspool. The rapid increase in industrial production
is accompanied by a concurrent reduction in biodiversity and natural resource
availability. Combustion gasses, including CO2 emissions and biologically significant
chemical fallout from industrial infrastructure activities, including consumer product
production, have as their probable outcome the synergistic interaction of the multiple
components of biocatastrophe, resulting in infrastructure collapse as the legacy of
pyrotechnic industrial society.
Biscayne ax: Ax produced in the Biscayne area in Spain (Catalonia), the principal
location of the manufacture of trade axes in the 15th and 16th centuries. These axes were
brought to the Carolinas and Florida by the Spanish and also transported over the
Pyrenees to be sold to the French. The French also brought them to North America,
especially to the St. Lawrence River region and traded them to indigenous communities
for furs, hence the name “trade ax.” See Russell (1967) and Kauffman (1972).
Bit: Steel cutting edge of an ax. See ax-making techniques and over-coating.
Black-heart: Form of malleable iron annealed only for a short time, with the result that
its fracture has a white rim with a black center. Most American-made malleable iron
takes this form (Spring 1917). See malleable cast iron and white-heart.
Blacksmith: Artisan who forms hot iron into tools and hardware. In some cases,
especially in the early Iron Age and as recently as the 19th century, blacksmiths smelted
their own blooms of iron and forged tools and weapons out of their loup of hot iron by
the various tricks of their trade, which included hammering, quenching, tempering,
annealing, piling, reforging, pattern-welding, casting, burnishing, etc. From the early Iron
Age to the modern era, most working blacksmiths obtained the iron they were forging
from the bloomsmith, then, later, from the blast furnace via the finery, and, today, from
bulk process steel furnaces.
Blacksmith trades: Ideally, the blacksmith, in a New England shipbuilding community,
for example, was a multi-tasking ironmonger forging or repairing horticultural tools,
oxen shoes, knives, ironware for shipbuilding, edge tools, and guns. In reality, most
blacksmiths forging their hot iron had specialized trades: edge toolmaker, shipsmith,
gunsmith, farrier, shovel maker, and general purpose village blacksmith.
Bladesmith: A contemporary term for knife-makers, among the most ancient of all
Blast: Machine that pumps air to the tuyères of the blast furnace. See blowing tubs and
Blast furnace: High shaft furnace developed in Europe after 1350 to smelt iron ore in the
reducing atmosphere of the partial oxidation of charcoal (and after 1750, of coke). The
liquid iron produced was cast into cannons, other utensils, or “pigs” for further
refinement (decarburization) into wrought and natural iron and steel. In modern smelting
processes, a flux of limestone is used to combine with and remove silicate and other
contaminants as slag. The blast furnace was a significant improvement over the smaller
direct process bloomery furnace because it more efficiently reduced the ore to its metallic
state with a higher carbon content and lower melting temperature than bloomery iron.
Larger quantities of iron were produced with significantly less iron oxide lost as slag,
therefore allowing smelting of lower quality ores. A series of improvements (including
the use of the steam engine to enhance [cold] air blast , furnace design changes
[1784)], and the adoption of the hot air blast ) increased operating temperatures,
furnace capacity and efficiency, and the control of carbon content. New England’s first
blast furnace began operation at Saugus, Massachusetts, in 1646. See bloomery, arms
race, cupola furnace, foundry, molding, Saugus Ironworks, slag, and carbon content of
Blister steel: Steel produced in a cementation furnace, whose design protected the iron
bar stock being carburized from oxidation caused by the burning fuel. Bars of wrought or
malleable iron were stacked in the sandstone furnace with layers of charcoal dust or other
carboniferous materials and fired for a period of five to twelve days. The resulting steel
bar stock had a heterogeneous carbon content (cc) with less carbon in the inner layers, a
higher carbon content in the outer layers, and blisters on the steel surface that were due to
gas formation from the chemical reaction between the carbon and impurities in the slag.
The slow cooling inherent in blister steel production resulted in the formation of ferritepearlite microstructures, including acicular ferrite. These microstructures required
reheating and reforging followed by tempering for the formation of the more desirable
allotropic forms of steel such as martensite-bainite, martensite-ferrite-bainite, and
martensite-ferrite-pearlite-bainite matrixes, which are temperature- and transformationtime-dependent microstructures. (See the transformation time diagram in Appendix VI).
Common 18th century and early 19th century names for these forms of reprocessed blister
steel included designations such as spring, shear, and double shear.
Benjamin Huntsman’s innovative introduction of easily hot-rolled cast steel (1742)
revolutionized edge tool manufacturing by producing steel with uniform carbon content,
which gave it characteristics of superplasticity at high temperatures and enhanced
plasticity at room temperature, hence its durability and ease of sharpening. Blister steel
bar stock was broken into pieces and re-melted in crucibles at high temperatures. The
addition of carboniferous material (e. g. powdered charcoal) resulted in a chemical
reaction that produced small quantities (5 - 50 kg) of cast steel with a highly homogenous
distribution of carbon.
Blister steel was often used as a “weld” steel in the manufacturing of edge tools and was
the principal form of steel produced in England from 1686 to 1850. Bars of blister steel
were frequently piled (bundled) and reforged into higher quality, special purpose steel
such as shear steel, double shear steel, and spring steel for saws. The edge toolmaker’s
act of forge welding a steel cutting edge to an iron pole or shaft also served the function
of altering the microstructure of the steel, producing a more ductile or a harder steel
cutting edge depending on the choice of mechanical and thermal treatments.
After 1750, despite the appearance of crucible steel, which was only produced in small
quantities, blister steel, along with German steel, continued to dominate the world steel
market until the development of bulk process steel (1870). See Bessemer steel, carbon
content, cast steel, cementation furnace, German steel, open-hearth furnace, sap, shear
steel, Sheffield classification of blister steel, spring steel, superplasticity, and wrought
Bloom: 1) (1870 definition) Partially melted, pasty mass of iron and slag resulting from
the smelting of iron ore. Some bloomery-produced iron was nearly pure ferrite with a
very low carbon content +/- 0.03% cc, but not more than 0.08% cc; slight changes in the
fuel-ore ratio, tuyère location, and smelting temperature could produce iron with a
variable carbon content ranging from that of malleable iron, with a range of carbon
content from 0.08 - 0.5%, to raw steel, with a carbon content between 0.5 - 1.5%.
Unwanted inclusions of pins and globules of steel would reduce the malleability and
ductility of wrought and malleable iron. They often characterized the heterogeneous
bloom produced in the direct process smelting furnace. These steel inclusions in the iron
bloom may have also assisted blacksmiths in forging natural steel tools in early direct
process open-hearth furnaces by encouraging experiments with furnace design and
smelting processes; otherwise, steel nodules were considered to lower the quality and
workability of wrought and malleable iron. 2) (Modern definition) Hot-rolled, semifinished billets, bars, and slabs of iron and steel produced in rolling mills. See carbon
content of iron, direct process, ferrite, loup, tuyère, and wrought iron.
Bloom size: Early Iron Age blooms (Halstadt, La Téne, Noricum) were two to ten
kilograms in size; medieval and late medieval bloomeries with water-powered trip
hammers made larger blooms, 25 – 50 kg (Tylecote 1987).
Bloom smelting: Production of a loup of wrought or malleable iron from the reduction of
iron ore (iron oxide) by the bloomsmith, whose success depended on accurate control of
furnace temperature and the intuitive control of the gas ratio, i.e. CO/CO2 (as in C + CO2
= 2CO). Excess production of carbon monoxide during the smelting process would tend
to recarburize the bloom of wrought or malleable iron, either accidentally or deliberately,
producing higher carbon malleable iron, natural steel or unwanted cast iron.
Bloomery: Charcoal-fired shaft or bowl furnace used for the direct reduction of iron ore
to produce wrought and malleable iron and natural steel. Bloomeries were the primary
facility used to produce iron or, in some cases, raw steel before the appearance of the
blast furnace (1350). They were in wide use in the United States until the Civil War and
continued in use until the late 19th century in the United States and in some sections of
Europe, such as Catalonia, despite the proliferation of blast furnaces after 1600.
Bloomery iron: “‘Bloomery iron’ was essentially similar to ‘wrought iron’ in being
virtually carbon free, but with entrained slag” (Barraclough 1984a, 11). Implicit in
Barraclough's definition is a difference between the relatively slag-free wrought iron
produced in the puddling furnace and the high slag content iron produced in the bloomery
furnace. In New England, implements made from direct process bloomery-smelted bog
iron ores have higher slag content than the wrought or malleable iron produced by
decarburizing cast iron in the puddling furnace and are characterized by highly visible
linear filaments of iron silicate. See bloomsmithing, malleable iron, silicon, wrought iron,
and natural steel.
Bloomery steel: Steel produced either deliberately or accidentally by bloomsmiths
operating a direct process furnace. Bloomery steel could appear as nodules of steel in the
form of irritating contaminants in wrought or malleable iron bar stock or be deliberately
produced by early Iron Age bloomsmiths, whose specific function was to make natural
steel for swordsmiths and/or edge toolmakers. Bloomery steel was often beaten into thin
sheets and piled in alternating layers with sheet wrought iron by swordsmiths, who made
the ubiquitous pattern-welded swords from the early Iron Age to the late Renaissance.
See natural steel.
Blooming mill: Modern term for rolling mills consisting of two high continuously
reversing electrically driven rollers, which reduce steel slabs into appropriately-sized
sheets, strips, and plates. Three high rolling mills require no reversing. In 1784, Henry
Cort designed and built the modern form of the grooved rolling mill to shape puddled
iron. See rolling mill.
Bloomsmith: Traditional name of the operator of a direct process bloomery from the
early Iron Age until the late 19th century. The bloomsmith smelted iron ore, making the
loup of wrought or malleable iron that would then be shaped by hand hammering, or,
after 1350, by use of a water-powered helve hammer to expel the slag and other
contaminants. In the early Iron Age, the bloomsmith would produce currency bars that
were widely traded. After 1350, the use of the helve hammer allowed the bloomsmith to
shape wrought or malleable iron bar stock. Both forms were then supplied to blacksmiths,
shipsmiths, and swordmakers as the raw material used in their often bellows-driven
forges. See currency bar.
Bloomsmithing: Direct process production of wrought and malleable iron by the
hammering of the bloom at red heat to remove slag. It was an inefficient process due to
the loss of +/- 50% of the iron content in the slag. In the early Iron Age, the first iron
furnaces were run by bloomsmiths, who also functioned as blacksmiths, forge welding
the first iron and steel tools. Historically, the bloomery process was the only practical
way to obtain wrought and malleable iron until the widespread production of cast iron
required strategies for decarburizing the cast iron. In the North American colonial period,
bloomsmiths used bog iron, widely available along the coastal plains of the colonies, for
the production of wrought and malleable iron. Successful bloomsmithing required a
temperature of at least 1200º C to liquefy the slag that acts as a protective covering for
the loup of iron being smelted. See carbon content of iron, bloomery, direct process,
bloom, bloomsmith, bloom smelting, and natural steel.
Blow hole: Defect caused by trapped gas within molten metal; an ongoing problem in
crucible steel production until the invention of the dozzle and also a continuing challenge
of modern steelmaking techniques. See crucible steel and dozzle.
Blowing devices: Instruments used to provide the air flow or blast in bloomery and blast
furnaces. The earliest blowing devices were leather bag bellows and fan bellows used in
Asia. These later evolved into piston bellows. The trompe is a form of hydraulic bellows
commonly used in Europe. The steam-powered blower was the universal blowing device
used after 1775 to provide the air blast for modern blast furnaces before the advent of gas
and electric motors. See blast furnace, blowing tubs, and trompe.
Blowing engine: Steam-powered rotary blowing engine, which was first introduced by
Joseph Nasmyth in England in 1837 and greatly increased the operating temperature and
efficiency of the blast furnace. One of a series of important innovations in blast furnace
operation, it was quickly adopted by American ironmongers. See blast furnace and
Blowing tubs: Wooden cylinders containing leather edged wooden pistons driven by
water-powered piston rods (Gordon, 1996) of various and gradually improved designs
based on piston-valve-cylinder combinations. Blowing tubs replaced bellows in the late
18th century, creating a stronger air blast in both bloomeries and blast furnaces. Smaller
blacksmith and shipsmith forges continued to obtain air blast from the use of handpowered accordion bellows until the end of the 19th century. See blast, blast furnace, and
Bluing: The color of surface oxide on steel resulting from low temperature heat treatment
(+/- 300º C).
Body-centered cubic structure (BCC): Low temperature (< 910° C / 1670° F)
crystalline form of (alpha) iron in which atomic centers are located at the corners and
center of sets of cubic cells; one of the three most common forms of crystal structures in
most metals. After heating beyond the eutectoid temperature (723° C), the lattice
structure of iron deforms into a face-centered cubic structure (FCC), as in gamma iron;
this transformation is completed at a temperature of 910º C. At a temperature of (2552° F
/ 1400° C), gamma iron reverts to a BCC structure. The third form of cubic space lattice
is the close packed hexagonal (CPH), characteristic of such non-ferrous metals as cobalt,
magnesium, and titanium. Metals in this last group lack plasticity (Shrager 1949, 5-6).
See lattice structure.
Bog iron: Iron precipitated in upwelling waters by contact with oxygen and organic
material. In bogs and swamps, the constant process of bog iron formation can be seen by
the characteristic brown scum on the top of the water formed by bacteria precipitating the
iron from the water, which then falls to the bottom of the pond or swamp forming bog
iron deposits. Limonite and goethite are the most commonly encountered hydrated iron
ores in the North American coastal plain. Because both are combined with water, they are
called hydrated iron ores. In the North American colonial era, bog iron was the most
important local source of iron until the exploitation of mined terrestrial ores occurred
around Salisbury, CT, in the early eighteenth century, as well as in Pennsylvania, New
York, Maryland, and elsewhere. Pennsylvania soon became colonial America’s most
important source of terrestrial ore. High in phosphorous, bog iron, unless extensively
refined, was smelted and forged into tools with highly visible slag inclusions. See
bloomsmithing, bloomery, wrought iron, limonite, goethite, and hydrated.
Bombard: Earliest form of firearms utilizing gunpowder. The production of bombards in
Europe after 1350 greatly increased the demand for wrought iron, which, in turn,
facilitated the development of the blast furnace because it could produce large quantities
of pig iron to be easily refined into wrought iron. See arms race, blast furnace, pig iron,
wrought iron, and gunsmithing.
Born-again ironmonger: Individual who executes the convivial use of hand tools while
at the same time resurrecting the knowledge of the ancient traditions of the ironmonger
and the history of technology and its cascading Industrial Revolutions; the basis for the
successful functioning of the skilled artisans and craftspersons essential for the viability
of sustainable economies in the unfolding Age of Biocatastrophe.
Bosh: Tapered combustion zone of a blast furnace, located just above the hearth.
Botting: Plugging of the tap hole in a cupola furnace after removal of molten iron prior to
the accumulation of the next batch of melted cast iron.
Bottom swage: Lower die placed into the hardy hole of an anvil for the purpose of
shaping iron bar stock.
Bowl furnace: Most ancient form of an open-hearth furnace. The first bowl furnace was
probably a campfire in which copper ore was accidentally melted. See furnace types.
Brass: Copper-zinc alloy with +/- 2.0% zinc content and lead as a micro-constituent.
Brazing: The process of joining of two pieces of metal by fusing a layer of brazing solder
alloy (copper-zinc, copper-zinc-silver, or nickel-silver) between adjoining surfaces with
two different melting points.
Breakdown furnace: Another name for a non-slag-tapping furnace where, at the end of
the smelt, the furnace walls must be broken down in order to remove the bloom of iron or
raw steel. Among the first forms of furnace design in the early Iron Age, open-hearth
breakdown furnaces are still used in the early 21st century for production of raw steel for
Brescian steel: Ancient North Italian process for producing steel from carburized
wrought iron soaked in molten cast iron; one of several steel producing technologies of
the Italian city states during the Renaissance; later used in Europe and possibly in the
United States before the introduction of crucible steel. The cast iron was broken into
pieces and mixed with saline marble as a flux and then melted. Billets of wrought iron
were then placed in the molten cast iron for +/- 5 hours, removed, forged, and quenched,
producing a high slag content steel with a variable carbon content. A similar procedure
was also used to make steel in China, at least as early as 700 BC and probably earlier
(Needham 1958, Barraclough 1984a). See Chinese steel.
Brine quenching: Expedition of uniform cooling by the chemical action of salt crystals;
most preferred quenching medium of many early edge toolmakers.
Brinell hardness: Older method of determining hardness by measuring the diameter of
an impression made by a ball of a given diameter under a specific load.
Britannia metal: Combination of tin, copper, and antimony to imitate pewter; invented
in Sheffield, England, by James Vickers in the late 18th century (Tweedale 1986). Also
called Britannia Ware.
British thermal unit (BTU): Amount of heat necessary to raise the temperature of one
pound of pure water by one degree Fahrenheit starting at its maximum density
temperature -39.1° F.
Brittle cleavage: Nearly instantaneous slip of the crystalline lattice structure of a metal.
Brittle-ductile transition temperature (BDTT): “...temperature at which iron upon
cooling; suddenly becomes brittle. The transition temperature is sensitive to the purity of
the metal” (Gordon 1996); also, the temperature at which iron and steel undergo a loss of
toughness, usually below room temperature. Phosphorous raises BDTT above room
temperature in the presence of carbon (Kauffman 1972). The most notable example of
brittle-ductile transition temperature is the rapid cooling of austenite to form martensite.
See cold short.
Brittleness: Tendency of a metal to suddenly fracture under low stress without
Broad ax: Form of ax with a wide blade (in excess of five inches); made in numerous
styles ranging from the bearded broad ax of German origin to the wide Pennsylvania style
broad ax. The “New England” style broad ax and the English pattern mast ax are the two
most common forms of broad ax found in New England shipyards. The former was
particularly important for use in the woods to “beat out” the white oak futtocks and keel
components for New England shipwrights.
Bronze: Copper-tin alloy; +/- 10% tin.
Bronze edge tools: Most common form of woodworking tools before the Iron Age.
Hammering flattened the cutting edge of a bronze tool, while, at the same time, hardening
it. Bronze celts were often secured in knee bent hafts, later followed by enclosed hafts
and socket cores. Bronze axes were frequently cast in molds with the aid of eyepins
(Tylecote 1976). See cold hardened, celts, eyepin, and shaft hole vs. socket hole.
Bulat: Russian name for Wootz steel sword blades.
Bulk carburization: Production of steel in the order of magnitude of tons; first made
possible by the design and use of the cementation furnace >1600. See basic steelmaking
process, converting furnace, blister steel, Bessemer process, and Siemens-Martins
Butt riveting: Riveting of two plates of low carbon steel or iron together by the use of a
covering plate that overlaps the two plates; one of two methods for building iron and steel
ships. See lap riveting.
CAD: See computer-aided design and CNC technology.
Calcining: Roasting of ore to remove impurities and moisture. The resultant product was
called ironstone, which was then smelted and reduced to loups (blooms) in a bloomery
furnace. See bloomery.
Calescent: Characterized by increasing temperature, i.e. glowing with heat.
Cannon metal: Alloy of copper and tin, also called gun metal. See alloy and gunmetal
Carbide: Compound of carbon with one or more elements, i.e. iron carbide, Fe3C; by
definition, the added element(s) must be characterized by a lesser electro-negativity. See
carbide forming metals.
Carbide banding: Patterns of aligned bands of cementite produced by the thermal and
mechanical treatment of steel.
Carbide forming metals: Metals, which, when present at 20 – 100 parts per million as
micro-segregated components of the interdendritic regions of iron carbide
microstructures, facilitate the formation of cementite bands in the form of nanowires and
nanotubes during, for example, the forging of Damascus and samurai sword blades.
Vanadium, chromium, titanium, molybdenum, niobium, and manganese are carbide
forming metals. These metals, as alloys in steel, have a wide range of applications, from
edge tool and knife-forging to manufacturing hardened steel cutting tools and shockresistant turbine blades. See alloys, cementite, Damascus sword, nanotubes, nanowires,
Carbide lamellae dimensions: “In the clusters of lamellae the films of hard carbide may
be as thin as half of one millionth of an inch or perhaps as thick as 0.00008. In the case of
spheroidal particle size the range is from what might be called molecular size to
spheroids perhaps nearly 0.001 inch in diameter” (Bain 1939, 22-3). All size dimensions
are controlled by the cooling and reheating of the steel, i.e. heat treatment cooling rates.
Carbon: Most important element in the creation of steel or cast iron from pure iron. The
amount of carbon added to iron and its pattern of distribution as an alloy determines the
microstructure and mechanical properties of steel or cast iron. With respect to the ferrous
metallurgy of woodworker's edge tools, carbon is the key element differentiating iron
from steel. Various forms of steel contain an intermediate level of carbon. Vandermonde,
Berthollet, and Monge first identified carbon as a component of steel in 1786 (Partington
1961). Also see Bergman (1781).
Carbon content of ferrous metals: Sources vary widely in defining the minimum carbon
content of steel, which ranges from 0.1 to 0.5% carbon. Please note the caveats that
follow the definitions.*
Wrought iron: 0.01 – 0.08% carbon content (cc); soft, malleable, ductile, corrosionresistant, and containing significant amounts of siliceous slag in bloomery produced
wrought iron, with less slag in blast-furnace-derived, puddled wrought iron. Wrought
iron is often noted as having ≤ 0.03% carbon content.
Malleable iron 1): 0.08 – 0.2% carbon content (cc); malleable and ductile, but harder
and more durable than wrought iron; also containing significant amounts of siliceous
slag in bloomery produced malleable iron, with less slag in blast furnace derived,
puddled malleable iron.
Malleable iron 2): > 0.2 – 0.5% carbon content (cc). Prior to the advent of bulkprocessed low carbon steel (1870), iron containing the same amount of carbon as
today’s “low carbon steel” (see below) was called “malleable iron.” Its siliceous slag
content gave it toughness and ductility, qualities not present in modern low carbon
steel, hence its name. Before 1870, a wide variety of common hand and garden tools
and hardware were made from malleable iron with a significantly higher carbon
content than wrought iron.
Natural steel: 0.2% carbon content or greater. Natural steel containing less than 0.5%
cc is synonymous with the term malleable iron. Natural steel is produced only by
direct process bloomery smelting and was the only form of steel produced in Europe
from the early Iron Age to the appearance of the blast furnace (1350). Small quantities
of natural steel continued to be produced by bloomsmiths, especially in the bog iron
furnaces of colonial New England until the late 19th century.
German steel: 0.2% carbon content or greater. Steel made from the decarburizing of
cast iron in finery furnaces, as, for example, at the Saugus Ironworks after 1646. The
strategy of making German steel dominated European steel production between 1400
and the advent of bulk process steel technologies, hence the term “continental
method” as an alternative name for this type of steel production.
Wrought steel: 0.2 – 0.5% carbon content (cc); another name for malleable iron.
Wrought steel was made from iron bar stock and was deliberately carburized during
the fining process to make steel tools that are still commonplace today, such as the
ubiquitous blacksmith’s leg vise.
Low carbon steel: 0.2 – 0.5% carbon content (cc). Less malleable and ductile than
wrought and malleable iron due to its lack of ferrosilicate, low carbon steel is harder
and more durable than either and can be only slightly hardened by quenching. Some
recent authors (Sherby 1995a) define low carbon steel as having 0.1% cc. Produced
after 1870 as bulk process steel (e.g. by the Bessemer process), low carbon steel has
all its siliceous slag content removed by oxidation. Before the advent of bulk process
steel production, there was no such term as “low carbon steel.” All iron that could not
be hardened by quenching (< 0.5% cc) was known as “malleable” iron, more recently
often referred to as “wrought” iron.
Tool steel: As with many forms of iron and steel, the term “tool steel” has multiple
meanings. Tool steel has traditionally been known as steel with 0.5 – 2.0% carbon
content (cc). Tool steel has the unique characteristic that it can be hardened by
quenching, which then requires tempering to alleviate its brittleness. Increasing
carbon content decreases the malleability of steel. If containing >1.5% carbon content,
steel is not malleable, and, thus, not forgeable, at any temperature. Such steel is now
called ultra high carbon steel (UHCS). Palmer, in Tool Steel Simplified, provides this
generic description of tool steel: “Any steel that is used for the working parts of tools”
(Palmer 1937, 10). The modern definition (post 1950) of tool steel is any steel
containing more than 4% of one or more alloys. For a more in depth description of
tool steel see Appendix V.
Ultra high carbon steel (UHCS): 1.5 – 2.5% carbon content (cc); a modern form of
hardened steel characterized by superplasticity at high temperatures and used in
industrial applications, such as jet engine turbine manufacturing, where extreme
strength, durability, and exact alloy content are necessary. Powdered metallurgy
technology is frequently used to make UHCS.
Cast iron: 2.0 – 4.5% carbon content (cc); hard and brittle; not machinable unless
annealed to produce malleable cast iron. For a more detailed description of the many
varieties of cast iron see cast iron.
*Caveats to carbon content of ferrous metals
Both modern and antiquarian sources vary widely in their definitions of wrought
iron, malleable iron, and steel. Modern sources variously define steel and/or low
carbon steel as iron having a carbon content greater than 0.08%, 0.1%, 0.2%, and
Before the advent of bulk process steel industries (1870), which produced huge
quantities of low carbon steel that could have a carbon content in the range of 0.08
– 0.5%, iron having a carbon content of < 0.5% cc was called malleable iron.
Other generic terms for iron that could not be hardened by quenching (> 0.5% cc)
were bar iron, wrought iron, and merchant bar.
The 1911 edition of the Encyclopedia Britannica defines wrought iron as
containing less than 0.3% carbon, cast iron as having 2.2% or more carbon content
and steel as having an intermediate carbon content > 0.3% and < 2.2%.
Gordon (1996) defines steel as having a carbon content > 0.2%. This cutoff point
is probably the most appropriate to use in defining steel, but also poses a problem
since most sources define wrought iron as having < 0.08% cc; therefore, leading to
the confusion of iron with a carbon content > 0.08% but < 0.2% as being either
wrought iron, low carbon steel or an orphan form of undefined iron.
In view of the long tradition of the use of the term malleable iron, this glossary
resurrects the use of that term to cover this gray area of the carbon content of
Carbon content (cc): The percentage of carbon in an object. Historically, carbon content
was determined by a visual examination of the visible microstructure of a broken sample
of iron or steel. Modern techniques include examination of a broken sample of steel cast
in a mold using rapid spectrographic analysis.
Carbon cycle: Cycle in which living organisms incorporate carbon from the carbon
dioxide in air or dissolved in water through the process of photosynthesis. Carbon
combined with oxygen (CO2) is released by respiration, decay, and oxidation, as with the
burning of biomass fuels. Human activity, including the smelting of metal and the use of
the internal combustion engine, is rapidly increasing the amount of free CO2 in the
Carbon diffusion: Diffusion that occurs mechanically as a result of hammering or
thermal treatments, such as annealing, but more efficiently initiated as a chemical
reaction during crucible steel production. The gaseous diffusion of carbon into wrought
iron, malleable iron, and low carbon steel cannot occur at a temperature less than 850° C.
See carburize and case hardening.
Carbon dioxide (CO2): Gas formed as a component of the carbon cycle when, after
carbon is incorporated in living matter by photosynthesis, it combines with oxygen and is
released by respiration, decay, or combustion. As a key component of the carbon cycle,
carbon dioxide is produced by all biotic organisms during respiration and by the
combustion of biomass fuels as occurs during the smelting of iron ore to produce iron.
Carbon dioxide is also produced during the smelting process when carbon monoxide
comes into contact with air and burns with a blue flame (2CO + O2 = CO2). It is
reabsorbed by plants (trees, crops, grasses) during the photosynthesis process, which
produces oxygen as a waste product. As a gas, the 2007 average global concentration of
carbon dioxide was 383 ppm by volume in the earth’s atmosphere and the rate of increase
was 2.14 ppm per year. By 2012, the concentrations had risen to 394.25 ppm
(http://www.esrl.noaa.gov/gmd/ccgg/trends/). Human activities are now increasing
greenhouse gas levels (water vapor, CO2, methane, ozone, chlorofluorocarbons, etc.)
more quickly than in the past. As a result of this increase in the atmospheric level of
greenhouse gases, more long wave radiation is being reflected downward to the earth’s
surface from these gases, resulting in rising worldwide temperatures and global climate
change. See carbon, carbon monoxide, cataclysmic climate change, and biomass.
Carbon elimination: The decarburization of ferrous metals, such as the fining of
malleable iron to make wrought iron, or pig iron to make German steel. Carbon
elimination is the result of the oxidation of carbon to carbon monoxide (CO) and carbon
Carbon family structures: Bain (1939) classifies three principal families of carbon steel
structures: 1) pearlitic lamellar structures formed by the slow cooling of austenite below a
temperature of 1000º F, 2) martensitic structures characterized by spheroidal structures
formed by rapid cooling at 200º F, requiring tempering for hardness mitigation, and 3)
bainite structures formed at an intermediate range of transformation temperatures (800º F
- 200º F) and having different mechanical properties than lamellar pearlite or tempered
martensite, i.e. enhanced toughness for the same hardness as tempered martensite. During
the bainite formation phase, austenite does not disappear entirely and may be retained
during constant temperature transformation up to 25% of its original content. See
annealing, austenite, bainite, martensite, pearlite, and transformation kinetics.
Carbon footprint: “Measure of the impact human activities have on the environment in
terms of the amount of green house gases produced, measured in units of carbon dioxide”
Carbon gradation: Pattern of carbon distribution that results from the cementation or
case hardening processes. The heating of the iron bar stock in the cementation furnace or
of tools packed for case hardening gradually moves carbon atoms from the surface to the
interior, resulting in gradation patterns expressed as changes in the crystal structure.
Natural steel produced in direct process smelting furnaces lacks carbon gradations due to
the erratic and heterogeneous distribution of carbon during the smelting process. See
cementation furnace, blister steel, natural steel, and case hardening.
Carbon monoxide (CO): Gas formed from the combustion of oxygen and carbon in the
reduction of iron ore in the direct process bloomery, which, when burned in the smelting
(reduction) process, also produces CO2. Hot carbon monoxide serves as the reducing
agent (electron donor) in the three-stage removal of oxygen from ferric oxide, first
creating Fe3O4 then FeO. In the final stage, carbon monoxide removes the last oxygen
molecule from the ferric oxide (FeO), creating pure iron (ferrite) and oxygen (O2). In
addition to CO2 being emitted during the combustion of furnace fuels, emissions also
occur when carbon monoxide is brought into contact with air and burns with a blue
flame, producing carbon dioxide (2CO + O2 = 2CO2).
Carbon movement: “The average carbon atom moves 0.06 inches in about eight hours
during carburizing” (Shrager 1949, 176). This slow movement makes the carburizing of
edge tools by forge welding a very tedious process. All blacksmiths know it is much
easier to make a tool out of low carbon steel bar stock than to carburize wrought iron into
a low carbon steel tool.
Carbon nanotube: Cylinder-shaped graphitic layers with diameters measured in
nanometers but with lengths up to a millimeter. Discovered in 1996 as a product of
fullerene research by 1996 Nobel Prize laureates Robert F. Curl, Harold W. Kroto, and
Richard E. Smalley, carbon nanotubes allow the production of a wide variety of
sophisticated products ranging from highly flexible tennis rackets to bullet-proof
clothing, sophisticated microtransistors, pharmaceutical drug delivery systems, computer
and cell phone applications, and production of sophisticated superplastic metals. A major
issue with carbon nanotube production is the wide variety of toxic off-gasses and other
contaminants that are associated with the cultivation of carbon nanotubes. Implicit in the
anticipated huge increase in carbon nanotube applications and production is the
concomitant increase in volatile persistent organic pollutants, which accompany the
evolution of this new industry. While the discovery of the molecular structure and
potential technological usefulness of carbon nanotubes dates to the mid-1990s, the actual
inadvertent usefulness of carbon nanotubes dates to the production of the Damascus
sword. See graphene, nanotube, nanowires, and superplasticity.
Carbon and slag solubility: The tendency of carbon and slag to become more soluble
with increasing temperature. In the smelting process, carbon and slag solubility are
temperature-dependent and increase with increasing temperature. The higher
temperatures achieved by blast furnaces (after 1350) were the critical factor in facilitating
carbon and slag solubility and, thus, the efficient production of cast iron.
Carbon steel: If no alloys are added, all steel is a solid solution of iron (ferrite) and
carbon. Pure low carbon steel (> 0.5% carbon content) is a form of malleable iron with no
slag impurities, the mass production of which was made possible by the implementation
of the Bessemer pneumatic process and other bulk steel production methods that oxidized
all slag constituents. Due to its lack of siliceous slag, carbon steel is not corrosion
resistant, nor is it as malleable or ductile as wrought iron, but more malleable than tool
steel. Low carbon steel is very useful for manufacturing drop-forged tools, especially if
mixed with alloys, but not appropriate for the manufacture of edge tools. The low carbon
steel produced by the Bessemer process had limited useful applications until manganesecontaining spiegeleisen was added in the smelting process. Carbon steel produced by
early direct and indirect process as well as in most other modern steel production
processes contain varying amounts of naturally-occurring manganese < 1.65%, silicon <
0.90%, phosphorus < 0.15%, copper < 0.6%, and sulfur < 0.05%. Carbon steels not
exceeding these naturally-occurring alloy limits are called “standard carbon steels”. See
carbon steel classification, alloy steel, Bessemer process, carbon content of ferrous
metals, manganese, and spiegeleisen.
Carbon steel classifications: Modern carbon steel is now classified by the AISI into the
following categories of standard steels based on the carbon content (cc) with the
limitations noted above for maximum naturally-occurring alloys.
Low carbon steel: < 0.2% cc
Medium carbon steel: 0.2 to 0.45% cc
High carbon steel: 0.45 to 1.5% cc
Steel used to make most hand tools is noted as having 0.5 to 0.62% cc
Alloy steels: carbon steels containing < 3.99% chromium or other alloys
Stainless steels: a type of standard carbon steel containing 4% to 30% chromium.
See stainless steel.
Tool steel: not included in the category of standard carbon steels, tool steel is
defined as steels containing more than 4% of one or more of a variety of alloys.
See tool steel, Appendix V.
Carbon steels are further classified as:
Nonresulfurized with a manganese content < 1.0%
Nonresulfurized with a manganese content > 1.0%
Resulfurized free machinery carbon steel
Resulfurized and rephosphorized free machinery carbon steel
Carbon tax: The taxation of the industrial, commercial, and petrochemical (e.g. coal,
automobiles, aircraft, etc.) production of climate-altering carbon dioxide (CO2).
Carboniferous materials: Carbon-bearing materials used in a cementation furnace to
make steel as biomass fuels or as a source of carbon for the case hardening of low carbon
steel tools, e.g. charcoal dust, charred bone, bone meal, wood, charcoal, coal, pigskin,
hides, et al.
Carbonless steel: Modern form of steel, made without carbon using elements, such as
manganese and titanium, which produce an alloy with microstructural characteristics
similar to an iron-carbon alloy (steel). Wertime (1962) is an early commentator on the
mid-20th century development of this oxymoronic form of steel.
Carburize: To diffuse carbon into wrought iron or steel at temperatures above 850º C –
910º C but below the melting point of the iron or steel artifact being carburized in a
carbon rich environment of charcoal, coke, or coal. Carburizing sheet iron into sheet steel
by submergence in a charcoal fire (case hardening) was an ancient steelmaking tradition
of desert swordsmiths and medina-dwelling cutlers. Partially enclosing an iron tool
within a charcoal fire for a period of 12 to 36 hours was another variation of the
carburization process for making an edge tool. However, the iron shaft of the tool being
carburized had to be enclosed in clay or some other covering to protect it from the
oxidizing effect of the fire.
Cascading Industrial Revolutions:
First Proto-Industrial Revolution (1300-1739): The age of the blast furnace,
printing press, round world exploration using wooden ships built by the edge tools
First Industrial Revolution (1740-1839): Age of Coke, cast steel, reverbatory
furnace; the steam engine as prime mover.
Second Industrial Revolution (1840-1874): Age of iron, factory system of mass
production, perfection of the production of malleable cast iron and grey cast iron;
the railroad as prime mover.
Third Industrial Revolution (1875-1899): Age of steel, perfection of Bessemer’s
bulk process, Siemens’ open heart and Mushet’s alloy steel production;
introduction of structural steel to build cities, use of the telegraph, telephone, and
electric lights; electricity as prime mover.
Fourth Industrial Revolution (1900-1944): Age of petrochemical-electrical man,
automobile, radio, diesel engine, age of global warfare; the gasoline engine as
Fifth Industrial Revolution (1945-1985): Age of petrochemical-electrical-nuclear
man, atomic bomb, TV, suburbia, leaded gasoline, industrial agriculture,
pesticides, chemical fallout; petrochemicals as prime mover.
Sixth Industrial Revolution (1986-2010): Age of information and communications
technology, Chernobyl, microchips, microprocessors, internet, fiber optics,
Windows, hyper-connectivity; digital technology as prime mover.
Seventh Industrial Revolution (2011f.): Age of biocatastrophe, round world impact
of cascading Industrial Revolutions, Fukushima Daiichi, Arab Spring, world water
crisis, cataclysmic climate change, antibiotic resistant bacteria and viral infections,
bioterrorism, ascendency of the klepto-plutocracy and its shadow banking
network, declining public resources, increasing public needs, political paralysis,
growing income disparity, assault rifle as an icon of human freedom; shadow
banking network as prime mover.
Case carburization: Ancient, as well as modern, toolmaking technique of carburizing
tools in charcoal pits, ideally at a temperature at or above 850º C - 910° C, where the
increased solubility of carbon results in the production of layers of ferrite and cementite
(pearlite). The various crystalline patterns of pearlite that result are dependent on the
relative abundance and grain size of microstructural formations of ferrite and cementite
created during the carburizing process, which, in turn, are dependent on carbon content,
cooling rates, additional thermal treatments, and tempering. See carburize and case
Case depth: Depth of carburization, which is time, temperature, and carbon content
Case hardening: Process of creating a hardened and long-wearing thin outer edge of
steel on forge welded tools. The inner component of the tool remained soft and ductile.
During case hardening, selected tools were placed in a protective enclosure with
carboniferous material and heated to harden the outside surface. The development of the
cementation furnace (after 1650), which protected the enclosed wrought iron from the
oxidizing effects of the fire, was simply case hardening on a grand scale. The interior
bundles of wrought iron in the cementation furnace always had a lower carbon content
than the hardened exterior bundles. In the 19th century, case hardening became widely
utilized on malleable cast iron and drop-forged carbon steel tools after they had been
shaped and machined by annealing or slowly reheating and cooling the tool. The notation
“case hardened” is often found on L. S. Starrett and other precision tools, such as
combination squares. See carburize and case carburization.
Cassiterite: Alluvial tin, found in Cornwall, England, Thailand, Malaysia, and desert
areas of Egypt. It was essential for the production of tin-bronze tools, which replaced
arsenic-bronze tools in the early Bronze Age. Interruption of tin trade routes may have
played a role in the rapid substitution of iron for bronze in the late second millennium BC
(+/- 1200 BC), first in Cyprus and then in Crete and the Peloponnesus region of Greece.
Cast iron: Carbide of iron, i.e. iron with such a high carbon content (2.0% - 5.0%) that it
is not malleable at any temperature. Cast iron was originally a waste product of early
shaft furnaces that ran too hot and, later, the principal product of blast furnaces.
Traditionally cast into pigs before being remelted in special function furnaces, cast iron
was also often cast directly into cannons and hollowware prior to the era of bulkprocessed steel produced from liquid cast iron. After the widespread appearance of the
cupola furnace, most cast iron was reheated and refined to further remove impurities and
excess carbon before being cast into specific forms, e.g. wheel axles, agricultural
equipment, boilers, etc. It was also reworked as wrought or malleable iron, carbon steel,
or crucible steel. According to Edward Knight, “The new production, instead of
remaining a spongy mass in the midst of the coal and slag, to be hauled thence by tongs
and be subjected to the hammer to clear it of foreign matter and condense it, ran down
like a fluid to the bottom hearth, and found its way out of a hole, running into a form
according to the shape of the hollow in the ground which received it. By this means the
smelter found he could withdraw the iron, without tearing out the front of his furnace for
each bloom” (Knight 1877, 1378). Knight’s Victorian era description of the production of
cast iron as a new innovation, even though it was not, is evidence of the continuing
widespread use of direct process bloomery smelting in mid-19th century American iron
production facilities. See malleable cast iron, white cast iron, and grey cast iron.
Cast irons: Cast iron comes in many forms, the following of which are the most
Graphite % Combined
(Free Carbon) Carbon %
White cast iron
Annealed malleable iron
Cast iron for chilled castings
Grey cast iron
Soft grey cast iron
Graphite % Combined
(Free Carbon) Carbon %
Table 2. (Spring 1917, 180)
Modern Machinery’s Handbook (Oberg  1996) defines ductile cast iron as
characterized by graphite in ball-like forms instead of in flakes as is in grey cast iron, and
as having high castability, machinability, and corrosion resistance. This is the
contemporary term for malleable cast iron, which Spring (1917) notes as annealed
Cast steel: 1) Term specifically referring to the steel used in the late 18th and 19th century
for the forging of edge tools for shipwrights, woodworkers, and other trades (e.g. scythe
blades, watch springs). [Not to be confused with the more modern use of the term with
respect to Bessemer's single process steel production (1865).] Listed by Moxon (
1989) in 1677 as one of the principal forms of steel available to blacksmiths at that time,
Smith (1960, 24) notes that Robert Hooke's 1675 diary also references cast steel,
suggesting that “cast steel was commonly known in England long before the time of
Robert (sic Benjamin) Huntsman.” Both writers were almost certainly referring to Wootz
steel imported from Persia. Cast steel became better known after Benjamin Huntsman
adapted the crucible steel process (1742) to make pure steel for his watch spring business.
Edge toolmakers soon recognized the higher quality of crucible steel and marked their
edge tools “cast steel” to advertise the superiority of the products over the less
homogeneous blister steel and its derivatives, shear and spring steel, previously used for
edge tool production, especially as weld steel. The words “cast steel” continued to be
stamped on English and American made edge tools into the early years of the 20th
century. The use of the electric furnace and the introduction of a wide variety of high
speed and special purpose alloy tool steels beginning in the early 20th century coincided
with the decline and end of crucible steel production. After 1930, the one piece cast steel
edge tools produced by Collins and other companies were not made from crucible cast
steel, but from steel produced in the electric arc furnace. 2) (Modern definition) Term
referring to steel made in modern bulk process furnaces, where the steel is poured
directly into molds that create the shape of the final product being manufactured. Cast
steel made in crucibles for the production of edge tools (see 1.) was made in batches of
10 to 50 kg; modern “cast steel” is made in batches that can range up to 50 tons, usually
in the form of “low carbon steel” (0.2 – 0.5% carbon content). Most bulk process modern
steel, if not rolled into sheets, is cast into one form or another. See Bessemer process,
crucible steel, furnace types, ingot, and Siemens-Martin process.
Cast steel microstructure: Characterized by coarse grained austenite with coarse
pearlitic inclusions and a uniform carbon content due to slow cooling in crucibles.
Casting: The pouring of liquid metals into molds to achieve a particular shape or form;
also, the shape thus obtained.
Cataclysmic climate change: Climate change characterized by unanticipated
accelerating rates of global warming and sea level change due to the synergistic effects of
increasing greenhouse gas emissions, methane releases from permafrost melting,
decrease in albedo from melting polar ice, deforestation caused by urban and suburban
development and biofuels production, and rapid melting of glaciers due to increasing
temperatures and water-flow-induced slippage.
Catalan furnace: Bowl type “low bloomery” direct process furnace developed in
Catalonia (Spain) after 1200 AD and still utilized as recently as the early 20th century for
the production of wrought and malleable iron; a precursor of the more efficient American
bloomery furnace. Depending on the fuel to ore ratio, open-hearth Catalan furnaces
operated by knowledgeable forge masters could be and were used to produce small
quantities of raw steel, which could be reforged into edge tools and weapons. See natural
steel and Biscayne ax.
Caulking: The process of inserting oakum between ship planking by the use of caulking
irons and caulking mallets to prevent leakage. During ship repair, the seam would first be
opened by a reefing hook to remove old oakum. A clearing iron, also called a reefing
iron, was used for further cleaning of the seam prior to re-caulking. Common caulking
tools include: the boot, spike, butt, making (common caulking), crooked (bent), and deck
irons (Sellens 1990), as well as special purpose long-handled horsing irons. Before 1800,
caulking irons were a common product of the shipsmith. In North American colonial era
shipyards, hemp and pitch-soaked cotton were sometimes used instead of oakum (Story
1995). America’s most famous producer of cast steel caulking irons was Christopher
Prince Drew of Kingston, Massachusetts (1815 - 1907). Numerous examples of caulking
tools and mallets are on exhibit at the Davistown Museum in Liberty, Maine.
Cavitation: Formation of voids and cavities within ferrous metal microstructures, which
inhibit plasticity by interfering with the uniform distribution of carbon in high quality
Celtic metallurgy: Knowledge of ferrous metallurgy, including a wide variety of steeland toolmaking strategies and techniques brought to central Europe by migrating Celtic
communities moving westward through Europe from the western steppes of Russia.
Celtic metallurgists were responsible for the flowering of the early Iron Age at Halstadt
and La Téne, respectively, beginning about 800 BC. The source of their knowledge of
ferrous metallurgy is unknown, but they were responsible for forging the swords, knives,
and edge tools in ancient Noricum that first led to the success of the Roman Republic and
the Roman Empire and then led to the defeat of the Roman Empire at the battle of
Adrianople (400 AD) by Goths supplied with Celtic-made, doubled-edged, patternwelded broad swords. Celtic metallurgists were already working in Britain when Caesar
invaded in 54 AD. See Halstadt, La Téne, gladius, spathas, natural steel, and manganese.
Celt: Earliest form of stone tool that was attached to a handle of antler or wood, often
secured by leather thongs.
Cementation: The process of introducing elements, including carbon, into the outer layer
of a metal (e.g. iron) by means of high temperature diffusion. See case hardening.
Cementation furnace: Enclosed stone or firebrick box containing alternate layers of a
carboniferous material, such as charcoal dust and the iron bar stock to be converted into
blister steel. With the fire located in an open-hearth below the box, which keeps the fuel
separate from the iron bar stock being carburized, the airtight furnace is fired for periods
ranging from 8 to 12 days and has a capacity up to 10 tons. First noted in 1574 (Wayman
2000), its first documented use was in Nuremberg in 1607; its first documented use in
England was in 1686. The use of the cementation furnace to make blister steel was the
principal means of producing steel in Britain (1700-1850). Less widely adopted in
continental Europe, it was supplemented by the crucible steel process after 1750 and was
gradually replaced by modern steelmaking technologies after 1865. Blister steel is used
for both shear (sheaf) steel and crucible steel production. The cementation steel furnace
represents an industrial scale application of the case hardening principle. Steel bar stock
with a widely varying carbon content could be produced depending on exposure time to
carboniferous materials, such as charcoal dust, in the cementation furnace. Steel with a
more uniform carbon content could be produced with lengthy firings (8-14 days). Blister
steel was often piled and welded into special steels, such as shear steel for cutlers and
edge tools, before cast steel became widely available (1750-1775). See blister steel, shear
steel, spring steel, cast steel, and converting furnace.
Cementation steel: Steel created by heating wrought iron in powdered charcoal in a
cementation furnace, which keeps the fuel separate from the iron bar stock being
carburized; also called blister steel. Because of the long cooling time for most blister
steel, ferrite-cementite matrices were its predominant microstructural constituents.
Sheffield, England steel makers have been very successful in the manufacture of
cementation steel. Their usual method is to pack flat strips of the best Swedish
Walloon iron in charcoal inside rectangular stone boxes about four feet wide, three
feet high and fourteen feet long. Alternate layers of small-sized charcoal and thin iron
bars are piled in these boxes until they are filled, the bars not being allowed to touch
one another. When full, top slabs are luted on to the boxes to make them airtight. Fire
is kindled in the firebox below and the heat gradually raised until furnace and boxes
are cherry-red in color. This heat is maintained for seven to eleven or more days,
depending upon the hardness desired, i.e., the amount of carbon they desired
absorbed. The furnace is closed and allowed to cool slowly, which requires another
seven or more days. Upon unpacking the furnace, the bars are found to be brittle and
of a steely fracture instead of the soft malleable material that was put in; they have
become high carbon steel. Expert workmen are able to judge very closely the
hardness of the steel by looking at the fracture and they sort the bars in this way,
piling bars of similar hardness together. Bars thus made show many blisters on the
surface and the steel became known as “blister steel” on this account. (Spring 1917,
See blister steel and cementation furnace.
Cementation temperature: Temperature required for the efficient diffusion of carbon
during the cementation process, from 1050º to 1100º C.
Cementite: “Iron carbide (Fe3C) in the microstructure of steel and cast iron” (Gordon
1996, 308). Cementite is the most common iron carbide and is hard and brittle. The
carbon content of cementite is all in the chemically combined form, with no free graphite
flakes. The carbon content of pure cementite is 6.67% (Pollack 1977). Cementite is often
fully dissolved in austenite with proper heat treatment, or, otherwise, partially dissolved
in steel and iron in various grain sizes and patterns, giving mechanical properties to steel
and iron products (strength, hardness, brittleness, etc). As carbon steel, cementite forms
directly from the melt in the case of white cast iron. As a component of carbon steel, it
either forms from austenite during cooling or from martensite during tempering. It mixes
with ferrite, the other product of the cooling of austenite, to form lamellar structures
called pearlite and bainite. Uniformly dispersed particles of cementite, usually with an
acicular microstructure, are an essential component of martensite. The uniform
homogeneous distribution of small cementite spheroids differentiates cast steel from
other forms of steel, such as blister and natural steel, which are characterized by a more
heterogeneous distribution of cementite. See austenite, cast steel, lamellar family of
structures, martensite, pearlite, and white cast iron.
Cementite plates: Characteristic of the microstructure of steel with a carbon content of
1.0 to 2.0%. Cementite plates result in high hardness and low ductility requiring
reprocessing by tempering to produce fine grained (usually spheroidal) microstructures,
sometimes in the form of nanotubes and nanowires, that are no longer brittle, i.e. their
superplasticity at high temperatures is demonstrated by plasticity and a lack of brittleness
at room temperature. See cementite, nanotubes, nanowires, and superplasticity.
Chafery: Forge for the further reworking of anconies of wrought or malleable iron by retempering and reshaping or slitting the metal into forms compatible with the production
of specific tools and iron products, e.g. nails, rolled sheet iron, wrought iron hardware,
and malleable iron agricultural tools. See ancony, bloomery, direct process, and muck
Chalybean or Chalibean steel: High nickel content steel smelted from the self-fluxing
iron sands of the Black Sea c. 1900 BC, at the height of the Bronze Age; often mistaken
for meteorite-derived steel (Piaskowski 1982); described in Greek literature by Aeschylus
and Strabo. The use of iron sands by Chalybean bloomsmiths or samurai swordsmiths as
the highest quality special purpose iron ore available was a prelude to the late 20th
century development of powdered metallurgy, the essential ingredient of which is a very
fine grained iron oxide powder. See samurai sword and Tamahagane.
Charcoal: The principal fuel used to make wrought iron and cast iron from the early Iron
Age until the mid-18th century, when coke became available as a blast furnace fuel in
England. Charcoal continued as the main source of fuel in heavily wooded environments,
such as the US and Sweden, for a century or longer than in forest-depleted England. The
very low sulfur content of charcoal iron made it ideal for edge tool production, in contrast
to coke and coal fired blast furnace iron, which was high in sulfur and ash. Swedish
charcoal iron, also low in phosphorous, was the key ingredient for blister steel production
in converting furnaces and was then used by Sheffield crucible steel manufacturers for
the final smelting of cast steel. Swedish charcoal iron was also imported in large
quantities to New Bedford (and many other U.S. ports), 1815 - 1850, presumably for use
by New Bedford whale crafters and edge toolmakers (Lytle 1984). Charcoal wrought iron
was produced by American direct process bloomeries for the Pittsburgh crucible steel
industry from its inception in 1860 until the end of the 19th century.
Charcoal hearth iron: Iron produced using charcoal as a fuel; also called charcoaled
Charcoal iron: Highly refined variation of iron made by alternating layers of pig iron
and charcoal in a finery furnace. After being partially melted, most of the silicon and part
of the phosphorus was eliminated. After solidification, the mass of iron was broken up
and reheated in a second furnace with alternate layers of charcoal, which removed most
of the remaining carbon, but some slag remained entrained within the bloom. Charcoal
iron produced by this method contained a higher carbon content than wrought iron but
contained less slag, most of which was in the form of iron silicate. Charcoal iron is, thus,
a form of malleable iron containing 1% or less of silicon slag content yet is more ductile
than wrought iron due to the extensive additional mechanical treatment to which it has
been subjected (e.g. rolling), especially in the direction opposite from its fibrous slag
layers (Aston 1939). Some Swedish bar iron produced in the late 18th and 19th centuries
may have been refined by this alternative method of iron production and utilized for edge
tool production via cementation furnaces. See bloom, cementation steel, malleable iron,
Chasing: Sinking of ornamental designs onto the surface of malleable sheet metals by
using a jeweler’s hammer and cast steel chasing tools, resulting in the formation of
grooves, indentations, and furrows in the metal surface; used especially in jewelry design
and manufacture. See repoussé.
Chemistry of carburization: Absorption of carbon by iron and steel from carbon
monoxide, which is formed by the reaction of the oxygen in the enclosed environment of,
for example, the cementation furnace, with the carbonaceous material inserted with the
iron bar stock. Iron carbide (cementite) and carbon dioxide are the resultant products. The
carbon dioxide is reconverted to carbon monoxide by reacting with more carbon to
extend the cycle of carbide formation:
3Fe +2CO = Fe3C + CO2
CO2 + C = 2CO
Chill: To use cold metal inserts within mold cavities in the production of cast iron
artifacts to facilitate rapid cooling and produce castings with hard surfaces but soft
Chilled cast iron: Cast iron that retains carbon in its chemically combined form if
insufficient cooling time is allowed for the precipitation of graphite flakes, as occurs
when the iron is cooled rapidly in iron molds rather than slowly in sand molds. “Cast iron
with a low silicon content cooled rapidly enough to form cementite rather than graphite in
its microstructure. Molders placed chills in molds to get white iron at places in a casting
where extra hardness was desired, as on the rim of a railroad-car wheel” (Gordon 1996,
308). The characteristics of chilled cast iron are a function of the thickness of the chill
(iron mold) and the carbon, silicon, sulfur, and other alloy content of the molten cast iron.
See white cast iron and combined carbon.
Chinese steel: Steel made by the Chinese utilizing multiple methods including:
immersing bars of wrought iron in a crucible containing melted cast iron (similar to
Brescian steel production); making steel from “. . . charcoal refining of pig iron, probably
a process not dissimilar to the Styrian process 1500 years later” (Barraclough 1984a, 2933); and malleableizing white cast iron and steeling the edges of woodworking tools
made from the cast. Barraclough (1984a) describes an adz c. 500 BC as follows: “The
fascinating feature of this implement is that the cutting edge has been sufficiently
decarburized to produce a steel-like structure; this is quite uniform and would appear to
be intentional . . . The methods of ‘malleableizing’ cast iron castings were obviously well
understood at this period since agricultural implements cast to shape and then fully
malleableized were fairly widespread during the Menchius era of the 4th century BC . . .
this was the process rediscovered by Réaumur some 2000 years later; in China it had
gone out of use in about the 7th century AD, after 1000 years of use.” Barraclough
(1984a) also notes several modifications to the Brescian style co-fusion process,
including a solid diffusion method, whereby coils of wrought iron were entwined with
insertions of cast iron to produce lump or raw steel. See Needham (1958), malleable cast
iron, white cast iron, and Brescian steel.
Chloanthite: Nickel arsenide compound composed of iron, nickel, cobalt, arsenic, and
sulfur added to the iron sand smelting process to produce the famed nickel steel made by
the Chalybeans of northern Anatolia, c. 1900 BC, at the height of the Bronze Age, a
process noted by Aeschylus and Strabo. See Amisenian, Chalybean, iron sand smelting
processes, Wertime (1980), and Piaskowski (1982).
Chrome steel: High grade alloy tool steel produced in the electric furnace and used for
applications requiring great hardness, such as ball bearings. Variations include chrome
vanadium steel used in automobile frame and knife and tool production and nickel
chromium steel used for automobile gears, axles, armor plates, projectiles, and airplane
parts. See alloy, alloy steel, stainless steel, and tool steel.
Chromium: Key alloy in the smelting of stainless steel. Chromium “is a strong carbide
former and stabilizer when present in small amounts (~ 0.5%). Chromium increases
hardenability, corrosion, heat, and oxidation resistance; improves high temperature
strength (in conjunction with Mo)… Chromium carbides are hard and wear resistant and
increase edge holding quality [italics added]” (Sinha 2003, 1.23). Chromium is often
present in alloy steels (> 4%), tool steels (4-10%), and stainless steels (>10%). See alloy
steel, stainless steel, and tool steel.
Cire Perdu: Lost wax method of making castings by using wax to make a pattern of the
object being cast. After being set in plaster, the wax is melted out of the mold; the
resulting mold often has great detail. This method was used for casting bronze objects in
antiquity and has been recently revived by contemporary artists. See embossing sequence
Classification system for steel: The American Iron and Steel Institute (AISI) and the
Society for Automotive Engineers (SAE) have developed a system for designating carbon
and alloy steels. The AISI has included additional classifications for tool steels with alloy
contents above 4% and stainless steels with chromium content above 10%. This system
begins with a designation of 10xx for carbon steels, the xx being the carbon content.
Eleven classifications of alloy steels include 66 types; AISI tool steels include 64 types.
Stainless steels include 4 classifications. See Appendix IV for the AISI-SAE system of
designating carbon and alloy steels.
Clay ironstone: Common form of iron ore and the principal form of iron ore in the
Weald (Sussex), England’s most important iron-producing region of the 16th century. It
occurred in the form of siderite as a hard gray rock within the clays, silts, and sandstones
of the Wealdean beds. This ironstone contained magnesium carbonate (MgCO3) and
manganese carbonate (MnCO3), which, as with the manganese in the Austrian ores of
Noricum, played an important role as a flux, enhancing carbon uptake in the production
of raw steel (Cleere 1985). See natural steel, Weald of Sussex, and manganese.
Cleavage plane: Smooth fracture occurring parallel to one or more crystallographic
planes. See deformation and lattice structure.
Close-packed hexagonal structure (CPH): Lattice structure characteristic of metals that
lack plasticity or lose plasticity during cold forming, including antimony, beryllium,
cadmium, cobalt, magnesium, titanium, and zinc (Shrager, 1949). See body-centered
cubic unit and face-centered cubic unit.
CNC technology: Computer numerical calculation (CNC) technology references the
ongoing tsunami of computerized manufacturing processes and industrial product
management using computer assisted design (CAD) programs. These programs, the
progeny of the information technology revolution, have vastly increased the efficiency
and productivity of both small and large corporations of every description, including our
rapidly expanding shadow banking network (SBN) and its numerous parasitic hedge fund
and derivative marketing entities. Its downside is the concomitant growth in structural
unemployment whereby large components of the middle class, formerly employed in
manufacturing or now computerized service industries, become members of an
underclass of unemployed, underemployed, or obsolete workers. The techno-elite who
make and operate the computers that drive the Age of Information Technology represent
a tiny percentage of a workforce whose main function is to serve as consumers in a now
globalized market economy. Invisible underground communities of self sufficient artisans
and craftspersons, including ironmongers, will inevitably utilize and benefit from CNC
technologies despite the gross income inequality generated by a global klepto-plutocracy.
The complex electrical power grid that is the prime mover of CNC technologies is
particularly vulnerable to geomagnetic (solar) storms. Recent Homeland Security, NRC,
and Oak Ridge National Laboratory reports postulate possible geomagnetic induced
current (GIC) disruptions of US electrical power grids ranging up to two years or more
(http://www.davistownmuseum.org/solarflares.html). See geomagnetic induced current,
geomagnetic storms, klepto-plutocracy, and shadow banking network.
Coal: Mineral fuel with two common forms: 1) bituminous (with a long flame and
containing 70 - 90% carbon) and 2) anthracite (with a short flame but containing 90 95% carbon.) Both forms contain significant quantities of mercuric sulfide, which is
released to the environment during combustion in the form of particulates subject to
tropospheric transport mechanisms, followed by conversion to toxic methylmercury by
bacterial action. Coal was used as fuel in blast and reverbatory (puddling) furnaces but
was unsuitable for bloomery and finery furnaces due to high sulfur content (+/- 2.0%).
See methylmercury, biocatastrophe, and biomass fuels.
Coalbrookdale: Important 17th and 18th century iron-producing center located on the
headwaters of the Severn River, in the Midlands of England, just west of Birmingham.
Coalbrookdale was the location of Abraham Darby's first coke-fired blast furnace and
also the location of the famous Ironbridge, England’s first cast iron bridge. It may also
have been the site of one of England’s first cementation furnaces, constructed by Sir
Basil Brooke (1636?) (Barraclough 1984a).
Cobalt: Important alloy in modern steel production. Cobalt decreases hardenability when
alloyed with other elements but increases red hardness when alloyed with vanadium,
chromium, or tungsten. In the forging of the Wootz steel Damascus sword, cobalt as a
micro-constituent of carbide nanotubes, especially if in the presence of chromium as
another micro-constituent, increases the distortion of unit cell patterns, thereby increasing
strain hardening and helping to give the Damascus sword its famed hardness and cutting
ability. Cobalt is often used in modern high speed drill bits. See alloy, Damascus sword,
nanotubes, nanowires, red hardness, and Wootz steel.
Co-fusion: Variation of the Brescian process for producing steel, whereby wrought iron
was dissolved in molten cast iron. One of the most ancient steel producing technologies,
co-fusion was a variant of crucible steel production methods used in India and Asia, was
later patented in England by Vickers (1839), and thousands of tons were produced
annually (Barraclough 1984). Similar combinations of ore were fired in the first Siemens46
Martin open-hearth furnace (+/- 1870). See Brescian steel and Chinese steel.
Cogging: Hammering, rolling, or pressing a red-hot tool steel ingot to convert it to a
Coke: “Porous, cohesive carbon made by expelling the volatile constituents from
bituminous coal” (Gordon 1996, 308). A product of the partial combustion of coal,
usually in large brick ovens, coke was invented by Abraham Darby in England in 1709,
and first produced commercially in 1735. Its use in blast furnaces resulted in the
production of iron with a high sulfur content, requiring a calcium bearing flux (lime) for
slag removal, as well as higher firing temperatures. The availability of coke as a fuel
stimulated the invention of the steam-driven piston bellows, which was needed to provide
a more powerful air blast for the smelting process. After 1785, the efficient use of coke
stimulated production of larger quantities of higher quality cast iron for reprocessing as
wrought and malleable iron in the newly invented reverbatory puddling furnace. See
reverbatory furnace and puddling furnace.
Coke smelting: Use of coke, instead of charcoal, as a fuel to smelt iron; became widely
used in England after the middle of the 18th century due to the depletion of English
forests by charcoal production. Coke smelting didn’t become widespread in the United
States until the 19th century due to the extensive availability of wood from which to make
Cold blast/hot blast: The switch from using a cold air blast to a hot air blast after
Nielson’s 1828 innovation of using waste gases to preheat the blast greatly increased the
efficiency of 19th century English, American, and European blast furnaces.
Cold drawing: Reshaping of iron or steel bar stock by drawing it through dies, resulting
in its permanent deformation.
Cold forging: Ancient tradition of hammering cold, malleable iron into tools and armor.
Bloomery-smelted charcoal iron with slag impurities, especially silicon, lent itself to
toolmaking because it welds easily, does not split, and is malleable to mold with a
hammer and anvil even at low temperatures. Modern low carbon steel made in blast
furnaces with mineral fuel, gas, or electricity lacks the silicon inclusions that facilitated
the creative cold hand-forging of Swedish and American charcoal irons (Bealer 1976,
36). See charcoal iron.
Cold short: Wrought iron containing phosphorous, thus brittle if worked or hammered at
Cold working: Rolling or forging steel at temperatures below 400° C to avoid recrystallization. Cold working increases strength and decreases ductility and toughness of
steel. If high in phosphorus, cold worked wrought iron can reach a hardness level as great
as 300 HV, above that of non-heat-treated carburized steel (Shrager 1961). See
phosphorous and carburize.
Collier: 1) Producer of charcoal for bloomeries, fineries, and charcoal-fired blast
furnaces. The activity of collier resulted in the deforestation of large areas of Europe and
the Mediterranean before 1800, and eastern North America until the Civil War. 2) Coal
miner. 3) A ship that transports coal.
Combined carbon: Carbon chemically combined in iron and steel alloys and, therefore,
not existing as free graphite flakes. As contained in rapidly cooled white cast iron, the
transformation of combined carbon into free carbon is the key step in the successful
production of malleable cast iron, which is thus more machinable. See malleable cast
iron, and white cast iron.
Combustion gasses: Gasses produced in smelting and fining furnaces and forges that
oxidize carbon and prevent carburization. The most important combustion gas is carbon
monoxide (CO), which is formed, in part, during combustion due to lack of oxygen;
otherwise, nonflammable CO2 (carbon dioxide) would be produced. During the reduction
process, if sufficient oxygen becomes available, CO will burn with a blue flame,
producing CO2. CO as a fuel is the most significant combustion gas due to its ability to
react with steel surfaces by oxidation. Such combustion of CO produces iron oxide
(FeO), which is then sometimes reused (reduced) in the smelting process to produce pure
iron, illustrating the complex dynamic of combustion/reduction processes. See carbon,
carbon dioxide, carbon monoxide, iron oxide, and reduction.
Compressive strength: Relative ability of a metal to avoid failure when pressed or
Computer-aided design (CAD): Also known as computer-aided drafting, it is the use of
computer systems to assist in the creation, modification, analysis, or optimization of a
design. These computer programs are the prime movers of CNC technologies in the Age
of Hyper-digital Technocracies.
Computer numerical calculations: See CNC technology.
Contaminant pulse: Presence of ecotoxins in abiotic and biotic media. The appearance
of global contaminant pulses is a result of the advent of bulk steel production (1870), the
widespread use of the internal combustion engine (> 1910), and the development of
petrochemical industries producing pesticides, sophisticated arms and explosives, and
globally traded consumer products and electronic equipment (> 1940). Global and
regional contaminant pulses of biologically significant chemical fallout (BSCF) including
persistent organic pollutants (POPs) and other ecotoxins can be tracked and monitored as
contaminant signals in abiotic and biotic media, often measured in parts per billion or
parts per trillion. Many forms of BSCF bioaccumulate in pathways to human
consumption. Concentration factors from water to consumers at the highest trophic levels
(e.g. predatory birds, humans) maybe as high as six orders of magnitude. See
biocatastrophe, biologically significant chemical fallout, petrochemical-electrical man,
and tragedy of the world commons.
Continental method: Generic name for steel produced by decarburizing cast iron
(German steel), so called because it was the principal method of producing steel in
continental Europe even after the cementation furnace dominated steel production in
England (1700). See German steel.
Converting furnace: Airtight furnace, also called a cementation furnace, usually of a
rectangular design and used to convert iron bar stock to blister steel after being packed in
charcoal. The first converting furnaces to make steel appeared in Nuremburg in 1607
(Barraclough 1984a), in England in 1686, and in the United States by 1713. The
converting furnace prevented contact between the fuel and the bar stock, allowing
production of steel in larger quantities and of a more uniform quality than that made by
fining cast iron lacking the manganese content of the ores used to make German steel.
See blister steel, cementation furnace, and cementation steel.
Convivial tools: Instruments of manual operation used to harvest and/or to create art and
artifact out of renewable resources (e.g. the woodworking hand tools of the shipwright)
or to recycle, rework, or reforge industrial salvage. In the broader sense of the term,
convivial tools are those which offer the pleasurable experience of using one’s hands to
create unique forms or execute significant repairs in comparison to the more impersonal
experience of operating machinery to do work. See born-again ironmonger.
Cooling rate: Speed of cooling. Along with carbon and alloy content, the cooling rate of
steel or cast iron after forging, melting, or austenizing plays a major role in determining
the allotropic form of the ferrous metal being produced. See phase transformation
Cooling rate of austenite: The cooling rate of austenite determines the microstructure of
ferrite and cementite and their mode of distribution in formations, such as pearlite and
bainite, after austenite is cooled below the critical temperature (723º C / 1300º F). Rapid
cooling of austenite to a temperature of 220º F creates martensite. The halting of the
cooling of austenite above the temperature at which martensite is formed, and its
maintenance in a temperature range between 1300 and 220º F (typically +/-800º F) for
variable periods of time creates the wide variety of microstructures characteristic of
bainite. Differences in the alloy content of austenite provide additional bases for
variations in microstructural formations, which may have specific industrial or
commercial applications, such as enhancing strength, hardness, or durability. See
austempering, bainite, critical temperature, critical cooling rate, and martensite.
Cope: Top half of a foundry mold. See drag and foundry.
Copper alloys: The two most important copper alloys are brass (an alloy of copper and
zinc) and bronze (an alloy of copper and tin). Usually both contain small amounts of lead.
Coppice: Wood harvested from the undergrowth of a wide variety of trees and used to
make charcoal. In England, small-sized wood, including branch tops with a diameter of 6
cm. or less (2.26 in.), were used to make charcoal; larger wood sizes produced friable
charcoal that transport or weight of the charge in the bloomery or blast furnace would
reduce to dust. The small diameter of the wood used to make charcoal meant that
regenerative coppicing renewed charcoal sources on the estates of the landed gentry, who
supplied much of the furnace fuel in England before the age of coke (1709). See Weald
of Sussex, charcoal, and collier.
Core box: Wooden molds used to form sand cores, which replicate holes, cavities, and
pockets in foundry castings. See pattern molding and foundry.
Core maker: One who designed and constructed the wooden molds used for foundry
work, along with a patternmaker. Sometimes, the core maker and the patternmaker were
the same person; at larger foundries, these functions were often two separate trades. See
Coring: A procedure for cutting or shaping the opening in the middle of an ax or adz for
hafting of the handle.
Coronal mass ejection (CME) event: The ejection by the sun of a blast of plasma
composed of electrons, protons, and highly excited gas at hundreds to thousands of
kilometers per second. A CME event is the source of most, but not all, geomagnetic
induced currents (GIC). For more information about geomagnetic storms and their
potential impact on the power grid go to
http://www.davistownmuseum.org/solarflares.html. The impact of solar storms should be
of interest to all contemporary metalworkers and born-again ironmongers in that the
worst case scenario for electric grid failure is an outage lasting four to ten years. Nonelectric powered hand tools will be an essential component of the long term response to
electronic infrastructure collapse.
Corrosion resistance: Prevention of rusting provided by the addition of nickel, copper,
or aluminum, as in stainless steels.
CPM S30V: “A martensitic (hardened) powder-made (sintered) wear and corrosion
resistant stainless steel developed by Dick Barber of Crucible Materials Corporation in
collaboration with knife-maker Chris Reeve.” It is composed of carbon: 1.45%,
chromium: 14.00%, vanadium: 4.00%, and molybdenum: 2.00% (Erin Casson 2013,
Creative economy: Ability of self-sufficient, post-apocalypse, off-the-grid communities
using convivial tools and renewable resources to maintain viable market, trading, and/or
barter economies in a biosphere with limited biomass fuel, minerals, fresh water, and
natural food resources. Ironmongers, as well as toolmakers and artisans, will be an
essential component of the creative economy of post-apocalypse society. See convivial
tools, biocatastrophe, and biosphere as bank account.
Creep: Slow, impermanent deformation of material under steady force that is below the
elastic limit of the material being deformed, occurring over a long period of time. See
Critical cooling rate: Lowest rate of austenite cooling at which martensite will form.
The critical cooling rate is dependent on the carbon content of the steel being heat treated.
If the cooling rate is lower than the critical cooling rate, pearlite will be formed instead of
martensite. “The rate of cooling which just prevents the reaction [of austenite to pearlite]
in the vicinity of 1000 degrees Fahr. and results in the lower temperature reaction is
called the ‘critical cooling rate’ or critical quenching rate. The former transformation and
its temperature is spoken of as Ar’ and the second as Ar’A; the critical rate is the cooling
rate separating the two. Many steels, however, cooled at about the critical rate, transform
in part by one mode and in part by the other, even in the same grain” (Bain 1939, 29).
“The critical cooling rate for hardening is decreased by an increase in austenite grain
diameter” (Bain 1939, 51). See austenite, martensite, and pearlite.
Critical point: Lowest temperature at which tool steel will harden when quenched, or at
which changes in the crystal structure of a metal will take place. See critical temperature,
quench, and quenching threshold.
Critical temperature: Temperature (Tc, 1341º F / 723º C) at which ferrite and pearlite (alpha
iron) are transformed into austenite (gamma iron). During this transformation, the
microstructure of the iron crystals is changed, and the amount of carbon dissolved into
this microstructure increases. As a component of heat treatment processes (e.g. sword and
edge tool tempering) slow cooling will allow the austenite to return to microstructures
characteristic of ferrite or pearlite. Rapid cooling changes the crystalline content of
austenite to the hard and brittle microstructure of martensite and requires further
tempering prior to the final forging of an edge tool or sword. See austenizing
temperature, crystallography of ferrous metals, microstructure, yaki-ire, and yakimodoshi.
Critical temperature range: Temperature difference between A1, the eutectoid
temperature, (723º C) and A3, the alpha-iron gamma-iron transformation temperature for
pure iron (910º C) expressed on contemporary phase transformation (iron-carbon)
diagrams as Acm. See Appendix VI.
Crucible: High-temperature-resistant earthenware vessel used for melting, fusing, or
casting metals. Clay crucibles have been used since the early Iron Age for the smelting of
small quantities of steel. The earliest documented use of crucibles for steel production
was the smelting of Wootz steel in Muslim communities c. 300 BC (Sherby 1995a).
Beginning in 1742, Benjamin Huntsman produced Sheffield cast steel in small clay
crucibles. During the height of Sheffield crucible cast steel production in the 19th century,
cast steel was produced in rows of crucibles with a +/-50 kg capacity. The lack of high
temperature resistant clays delayed cast steel production in the United States until the
mid-19th century, when Joseph Dixon’s invention of the graphite crucible provided an
alternative to Stourbridge clays for crucible production. See crucible steel, Stourbridge
clay, and Wootz steel.
Crucible furnace: Furnace composed of two firebrick boxes used to manufacture cast
steel for specialized purposes, such as watch springs and edge tools. The fire was in the
lower box, and the upper box held the crucibles. Other forms of crucible furnaces had
only a single firebox. Wasteful of heat and expensive to operate, crucible furnaces were
made obsolete by the invention of the electric arc furnace. See cast steel and crucible
Crucible holes: Slang term for the openings in a crucible furnace, into which the crucible
itself was inserted during the production of cast steel.
Crucible steel: Steel created by melting together pieces of blister or shear steel in a clay
crucible containing carboniferous material. The resulting chemical reaction equalized the
uniformity of carbon distribution. In the mid-19th century, crucible steel was also
produced from a combination of puddled wrought iron and steel scrap. High quality cast
steel has a microstructure of small carbide spheroids and qualities of plasticity, or near
superplasticity, at temperatures above its melting point, which allow it to be shaped and
rolled easily. Crucible steel was the first choice of English and American toolmakers for
the manufacture of high quality edge tools, often advertised by edge toolmakers as
“warranted cast steel.” Crucible steel was made in and imported from England after 1742
by Benjamin Huntsman and not manufactured in the United States until about 1860.
Spring (1917) makes the following observation:
For a century crucibles were made from clay molded to form, slowly dried and very
carefully burned. Usually each steel maker made his own crucibles. They could be
used but three times, becoming so thin and tender after use for three batches of steel
that they were not safe for a fourth. Graphite crucibles are now very largely used.
They withstand the severe heat much better and can be used five or six times. The
expense item for either clay or graphite crucibles is a large one. After filling with
small pieces of blister or shear steel the crucibles are entirely surrounded by coal or
coke in the furnace pit. The fire is so regulated that the steel is not too quickly melted.
Fresh coal or coke must be put in around the crucibles two or even three times. When
he thinks the steel should be molten, the expert attendant known as the “melter”
quickly removes the tight fitting cover of the crucible and with an iron rod determines
whether any un-melted pieces remain. After complete melting the steel must be
“killed,” else it will boil up in the mold upon pouring and leave a spongy or
insufficiently solid “ingot” or block of steel. This “killing” of steel is a rather peculiar
phenomenon. It is accomplished by allowing the steel to remain quiet in the furnace
for another half hour or so. Undoubtedly the quieting is the result of the escape of the
gases or impurities, which are contained in the charge, and absorption of the chemical
element, silicon, from the walls of the crucible. ...When the steel has been properly
melted and killed it is ready to pour. An assistant lifts the cover from the melting
hole; the “puller out” seizes the crucible just below the bulge with circular tongs and
pulls it from the coke, which surrounds it. The slag is skimmed off the top and the
steel poured into iron molds forming small “ingots,” usually from 2 to 4 inches square
and two feet or more long. Every part of the process, even the pouring, must be done
with extreme skill and care or the product suffers. After liberation from their molds,
the ingots are heated and either rolled or hammered down to the sizes desired for
tools, etc. (Spring 1917, 118-120)
Crucible steel should not be confused with the “cast steel” ingots of the Bessemer
process. See cast steel 1) and 2).
Crypto-fascism: Concealed agendas and hidden languages of a global consumer society
that glorifies growth and consumption at the expense of stable self-sufficient
communities using renewable resources in sustainable ecosystems. Crypto-fascist
pyrotechnical transnational industrial society uses military policy (e.g. oil wars) to
control and horde nonrenewable energy resources based on religious belief in divine right
and intelligent design for privileged social classes or sects (e.g. the klepto-plutocracy,
shadow banking network, Tea Party Taliban, and Christian fascists.) Crypto-fascist
consumer society utilizes mass media in lieu of secret police to control social and
economic activities, influence consumer habits, encourage non-sustainable growth, and
marginalize opposition to the frenzied consumption of nonrenewable resources. See
klepto-plutocracy, shadow banking network, and Tea Party Taliban.
Crystal: Geometric structure with a homogeneous distribution of atoms in patterns
characteristic of the specific elements or compounds in that structure.
Crystal structure: As used in ferrous metallurgy, the atomic structure characterizing
each phase of iron-cementite transformation.
Crystallography of ferrous metals: Study of the variations in the space lattice
formations (cubic structure) of the crystal structures of iron that result from various
thermal and mechanical treatments. Such structures are also dependent on the carbon
and/or other alloy content of the iron. See lattice structure and space lattice.
Cubic structure: Space lattice forms of unit cells within the crystal structures of metals.
In ferrous metallurgy, two forms of cubic structure characterize iron, i.e. the FCC (facecentered cubic) and the BCC (body-centered cubic). A third form of cubic space lattice is
the close-packed hexagonal (CPH), characteristic of such non-ferrous metals as cobalt,
magnesium, and titanium. Metals in this latter group lack plasticity (Shrager 1949, 5-6).
See crystal, space lattice, and unit cell.
Cupola furnace: Nineteenth century form of blast furnace used for re-melting cast iron;
a simple, fuel efficient shaft furnace usually using coke as a fuel, one of the principal
means for melting cast iron for foundries. The iron is melted in contact with the fuel.
Only gray cast iron is produced in the cupola furnace. Instead of the stone pyramid form
of the traditional blast furnace, cupola furnaces are constructed of sheet iron shells
culminating in a narrow top with adjacent elevators and a bridge to bring fuel and ore to
the top of the furnace. See blast, blast furnace, cast iron, foundry, and grey cast iron.
Curie temperature: Temperature at which magnetic transformation takes place, as in the
transformation of alpha iron to gamma iron (910º C).
Currency bar: Primary form of iron as a trade item in the early Iron Age, later replaced
by iron bar stock after the invention of rolling equipment in the 17th century. A currency
bar is a bloom of wrought iron, malleable iron, low carbon steel, or raw steel derived
from a direct-process smelting furnace. A blacksmith would take this bloom, often of
heterogeneous carbon content, hammer it to expel the slag and form bars of iron or raw
steel of various shapes and sizes, usually with handled ends, for easy transport from
smelting sites, such as those in Austria, to iron working and swordmaking centers, such
as those on the lower Rhine. Metallographic analysis indicates that these bars had a
widely varying carbon content, ranging from wrought iron to raw steel. Currency bars
were traded throughout Europe beginning in the early Iron Age. See bloomery, Iron
Road, Merovingian swords, and natural steel.
Cutler: Knife- or swordmaker. Boston swordsmiths were called “sword cutlers” c. 1800.
Cyaniding: Producing thin, exterior, high carbon layers in tool steel by applying liquid
cyanide; a modern process for case hardening. See case hardening.
Cybernetics: The science of communication and automatic control systems.
Cyberterrorism: The use of internet-based attacks by cyber-terrorists. The cyberterrorists of the future may be supplemented and even co-opted by geomagnetic storms to
give a whole new meaning to the term “infrastructure collapse.”
Cyrogenic: The specialized heat treatment of tool steels, including woodworking edge
tools, by freezing to increase durability and hardness, by soaking at a temperature of -320
ºF for up to 20 hours followed by double tempering. Cyrogenically treated steel is now
being used by contemporary toolmakers such as Lie Nielsen, Hock Tools, Bridge City
Tool, and Knight Toolworks.
Damascene: “a. to ornament (metal work esp. steel) with designs inlaid in the surface
and filled in with gold and silver. b. to ornament (steel) with a watered pattern, as in
Damascus blades” (Oxford English Dictionary 1971, 641). Stone (1999) defines
damascening as the process of inlay where the design is chiseled onto the surface of the
item and the precious metal (gold or silver) is hammered into the cavity and is disclosed
on the surface of the sword as either a flush or relief pattern. Stone notes the process of
false damascening in the English tradition, which an anonymous contemporary source
has described as: “Steel that has been overlaid with designs of precious metal anchored in
a cross hatched pattern that has been pricked in the surface of the steel (as opposed to
inlayed)” (personal communication 2008). Smith (1960) defines damascene as the
treatment of a pattern-welded iron and steel sword by a reagent for the purpose of
disclosing the crystalline pattern of the microstructure of the sword, which results from
the forge welding of the iron and steel and is dependent upon the unique combination of
iron and steel constituents and the lattice structure of the material being forged.
Damascened steel: Steel, especially steel swords, ornamented by designs inlaid in the
surface and filled in with precious metals or treated with a reagent to disclose
microstructural patterns. In the case of Japanese swords, makers can often be identified
by their characteristic patterns, which appear after treatment with the acid reagent and
express their forge welding techniques. In the 18th and 19th centuries, Englishmen
collected damascened gun barrels. The patterns disclosed by the use of the reagent
illustrated the artful forging technique of the gunsmith or swordsmith. The art of
damascening by inlay requires no reagent. Damascened steel is not the same as Damascus
steel. See Smith (1960) for commentary on damascened versus Damascus steel.
Damascus steel: Specialized form of crucible steel made for producing pattern-welded
wrought iron and steel sword blades; made in India (Wootz steel) and Asia (Asian
crucible steel), usually in very small batches of 2-3 kilograms per firing and then
transported as a trade item to Near East Asian communities, such as Damascus, for
reforging into swords; possibly one of the earliest forms of steel. As Wootz steel, it was
known in Europe after 1500 but was not widely utilized due to the difficulty of reaching a
temperature sufficient to relieve its hard, brittle, crystal structure by reforging. See Wootz
steel, Stourbridge clay, Moxon, Damascus blade, and cast steel.
Damascus sword: Term used to describe Persian, Indian, and Indo-Persian swords,
daggers, and scimitars, examples of which survive from the 16th to the 19th century and
are characterized by a diversity of patterns based on alternating layers of high and low
carbon steel but dissimilar to the traditional pattern-welded Merovingian sword.
Damascus blades (swords) were made out of Wootz steel. According to Smith (1960)
“Attempts to duplicate Wootz and watered steels generally led to James Stodart’s work in
France early in the nineteenth century, most of which was based on the erroneous belief
that the texture arose from forging. Many workers described the production of fancy
surface patterns by welding, twisting, and forging together variously shaped pieces of
iron and steel. The results were both decoratively and mechanically inferior to the
Oriental product and, in fact, were merely a return to sword-making of a technique
descendent from that of the Merovingian smiths which had meanwhile been extensively
used in the Near East and India for making so-called ‘Damascus’ gun barrels, which had
nothing but name in common with the sword.” Recent research (Levin 2005, etc.)
indicates that the Wootz steel used in Damascus swords has a high but heterogeneous
carbon content (1.5 - 2.0% cc), may contain micro-constituents such as cobalt, vanadium,
and chromium, and was probably forged at temperatures below the critical temperature,
creating carbon nanotubes, which provide Damascus swords with their characteristic
superplasticity. One probable reason why the production of Damascus swords cannot be
replicated is the depletion of the ores of continental India, from which they were derived.
See superplasticity and Wootz steel.
Damask: Etched pattern. When present on the surface of Merovingian and other patternwelded swords, the damask expresses the crystal structure of the pattern-welded iron and
steel in the sword. See damascened steel.
Damping: The capacity of a metal to absorb vibrations, reduce noise, and lower stress by
converting mechanical energy into heat. Grey cast iron has an elevated damping capacity
due to the presence of flake graphite in its microstructure.
Dapping block: A small rectangular steel block characterized by indented circles of
various diameters and depths used by a silversmith to shape silver. Often 4” x 4” x 4”, the
dapping block is a miniature version of a swage block but without its rectangular slots.
See swage block.
Debt: The totality of mortgage debt, college loan debt, credit card debt, consumer debt,
corporate debt, bond debt, pension fund debt, US government debt, banking debt,
sovereign government debt, including foreign debt. Total global debt in 2012 exceeded
190 trillion dollars. In contrast, total world gross productivity was about 80 trillion
dollars. The shadow banking network makes huge profits selling and trading debt as an
asset, often in the form of collateralized debt obligations. Its shadow banking network
debts as assets now exceed the total amount of both gross world productivity and gross
world debt. The Age of Biocatastrophe is also the Age of Klepto-plutocracy based on the
predatory but profitable trading in debt as an asset. Nearly invisible communities of tool
wielders, artisans, artists, craftspersons, born-again ironmongers, and a minority of the
elite technicians of our hyper-digital milieu have the challenge of formulating sustainable
lifestyles in the context of the unfolding tragedy of a world commons characterized by
debt as the primary asset of the klepto-plutocracy and its shadow banking network.
Decarburization: Removal of carbon from cast iron during fining or puddling or from
steel during heat treatment by oxidation, the latter of which produces surface
decarburization. Decarburization occurs either directly in an oxidizing atmosphere or
indirectly with iron oxide as an intermediary, producing carbon monoxide or carbon
dioxide gas. “Loss of carbon from the surface of heated steel. Decarburization prevents
steel from being properly hardened” (Gordon 1996). The decarburization of cast iron to
produce steel was the principal steelmaking strategy of the Renaissance and was not
replaced by the alternative method of carburizing wrought iron to make blister steel until
after 1690, and then primarily in England. See German steel, blister steel, and puddling
Decalescence point: The lowest temperature at which a change of structure occurs in
steel (1341° F), at which time the body-centered cubic unit cell of gamma iron changes to
the face-centered cubic unit cell characteristic of alpha iron accompanied by the
absorption of heat. See austenizing temperature.
Deep hardening: Creating modern cutting tools, dies, and lathe centers that retain
hardness at high temperatures and have a high resistance to wear and abrasion as a result
of the addition of tungsten, chromium, vanadium, and cobalt (T type alloy steels). In M
type alloy steels, molybdenum is substituted for tungsten and then combined with
chromium or vanadium.
The typical molybdenum high speed tool steel contains about 4 to 8.5 per cent of
molybdenum, 4 per cent chromium, 1.5 to 6 per cent tungsten, and about 2 per cent
vanadium. Since this material is very susceptible to oxidation, these tool steels must
be heated in a fused salt bath or coated with borax. They must be pre-heated to
approximately 1400 F and then heated quickly to 2200 F. They are quenched in air,
oil, or fused salts, depending on the type of steel used. They also have a strong
tendency to decarburize. These steels may be tempered at 1050 F. (Pollack 1977, 219)
Deforestation: The systematic removal of the mature forests of terrestrial ecosystems for
the purpose of agricultural or industrial activities or for the construction of human
habitations. Deforestation was the fate of large areas of North American forest after the
arrival of colliers producing charcoal fuel for bloomsmiths, blast furnaces, foundries, and
other ironmongers. Deforestation also occurred in Mediterranean, Near Eastern, and
European forested areas in the early Iron Age, and is currently occurring in tropical
forests in the twilight years of the pyrotechnic society and its systematic exploitation of
the earth’s natural resources. The recent global demand for biofuels is now increasing
both the rate of deforestation and the annual atmospheric levels of CO2 and other
greenhouse gasses that cause global warming. See collier.
Deformation: Changes in form produced by external forces and/or temperature change
acting on the non-rigid microstructures of metals, including ferrous metals. See creep,
lattice structure, microstructure, and stress.
Deformation bands: New grain boundaries that result from the rotation of the lattice
structure of metals during slip events, which may occur during cooling, tempering,
annealing, forging, or cold hammering. See creep, lattice structure, microstructure, and
Deformation history: Record of mechanical and heat treatment retained in a piece of
metal, exhibited by shapes of grain and slag particles. For example, cold working by
hammering leaves telltale Neumann bands in ferrite grains. See lattice structure,
microstructure, and stress.
Deformation twinning: The fractural movement of the atomic planes of crystal lattice
structures over each other, in contrast to the whole number increments of slip
deformation, during the microstructural deformation processes caused by the thermal
treatment of austenized steel (Pollack 1977, 73-75). It is a common mechanism of plastic
deformation in pearlitic steels. See twinning.
Dendrites: Branching forms characteristic of crystal growth patterns in metallurgy. See
crystal structure and crystallography of ferrous metal.
Deoxidation: The removal of oxygen by the addition of elements with a high oxygen
affinity, e.g. carbonaceous materials, as in the smelting of iron oxide ore and its reduction
to alpha iron or in crucible steel production to suppress formation of gas porosity during
the solidification of the liquid steel.
Deoxidizing agent: Elements used to remove oxygen or oxides from metals being
smelted, e.g. silicon or aluminum.
Depth of case: Depth of hardness penetration sought or achieved during the case
hardening of steel tools. See case hardening and case carburization.
Diderot’s Encyclopedia ([1751-75] 1959): Widely circulated multi-volume encyclopedia
illustrating important French trades, such as carriage making. The Diderot Encyclopedia
is particularly detailed in its depiction of the blast furnace, anchor and cannon forging,
casting of statutes, mining and smelting of metals, and manufacture of ornamental iron
work, which was a specialty of the French. The encyclopedia provides vivid pictorial
evidence of the longevity and the continental European origins of many of the tools that
reappear in New England workshops from the colonial period to the mid-19th century,
including the leg vise, anvil, and other related tools that would have been used by
toolmakers making their own hand tools. First published in the 18th century, the
encyclopedia is currently available in multiple reprinted versions. Sixty four plates of
hand tool illustrations from the Encyclopedia are reprinted in Tools Teach: An
Iconography of American Hand Tools (Brack 2013). See leg vise and pattern books.
Die casting: Shaping of molten metal by the use of external pressure, as in drop-forging.
Die driving: Hammering, heating, and tempering of dies prior to final casting, dropforging, or embossing of die-struck patterns or models. During hardening and tempering,
all dies must be shielded from the oxidizing effects of the fire by charcoal or a sheet iron
Die-sinking: The art of creating the patterns for drop-forged tools, which are hammered
or hydraulically forged out of hot carbon steel, tempered, annealed, and sometimes
subjected to additional mechanical and thermal treatments, including re-tempering to
restore hardness. Drop-forged dies are created by taking a pair of forged crucible blanks,
annealing them for softening, and shaping them by filing, chipping, and machining
(boring, slotting, and milling). The machining of the exactly matched die patterns
provides a surface that can be finished by polishing and further machining the edges. The
matched dies are re-dropped (reheated for tempering), pickled to remove scale, and
annealed again at low temperatures before being surface hardened for the fluid diecasting of drop-forged tools and other artifacts. During the die-sinking or shaping phase,
dies are often inserted into cast iron die holders. The best die steel alloy (c. 1910),
superior to carbon steel, was vanadium steel (Woodworth 1911). Occasionally, especially
in the 19th century, cast iron dies were used for some forgings. See die driving, dropforging, and drop press.
Die-sinking machine: Machine that replaced the hand work of the die-sinker and
enhanced production uniformity of interchangeable dies.
Direct conversion method: Method that allowed the direct conversion of Swedish
charcoaled bar and pig iron, in combination with quantities of scrap iron, into crucible
steel without the use of the converting (cementation) furnace; invented by William
Vickers in Sheffield in 1839. By 1880, most use of converting furnaces to produce blister
steel had ended. See blister steel.
Direct process: Single stage production of wrought and malleable iron from iron ore in
bowl and low shaft bloomery furnaces; also, an appropriate description for the single
stage production of hot-forged natural steel edge tools by a blacksmith directly from the
bloom, rather than from iron bar stock. Direct process iron is often high in slag. See
bloomery, wrought iron, malleable iron, and blast furnace.
Displacement: Slip or creep of the crystal lattice structure of metals during their plastic
deformation. See slip, creep, plastic deformation, and lattice structure.
Double-acting steam engine: A steam engine designed to allow steam to be admitted
alternately to each side of the piston while the other is exhausting due to the design
improvements of valve-controlled steam flow and the use of inlet and exhaust ports at
either end of the cylinder. Designed and produced in and after 1783, James Watts’
double-acting steam engine, soon called the reciprocating steam engine, represented a
major improvement in the efficiency of his first steam engines, which now could be
mounted at any angle and operated with increased speed and smoothness of
reciprocation. The reciprocating steam engine became widely used in the English textile
industry after 1785.
Double-process quenching and tempering: Modern, more complicated form of heat
treatment associated with relatively easy to melt high carbon steels; particularly useful for
the manufacture of super-hardened alloy steel composites.
Dozzle: Clay cone invented by R.F. Mushet in 1861 to contain a reserve of liquid steel to
alleviate the pipe in crucible steel ingots. The dozzle was inserted into the top of the ingot
near the end of the pour (Gordon 1996). See pipe, crucible steel, and cast steel.
Drag: Bottom half of a foundry mold. See cope.
Drawing furnace: Furnace used for tempering axes after hardening. Typically an ax is
heated to the color “pigeon blue”. Rapid cooling fixes the temper of the ax (Kauffman
1972). See temper.
Drawing temper: Heating of hardened steel to a specific temperature, followed by its
quenching to obtain a lesser degree of hardness.
Draw plate: “A plate of hardened steel, furnished with a series of tapered holes of
gradually diminishing diameters through which metals are drawn out into wires” (Audel
Drop-forging: Use of top and bottom dies to hammer a heated bar into the shape of a die
sunk pattern. Hydraulic forging performs the same function by pressing heated metal into
die sunk patterns. The drop-forging of hand tools began with the adaptation by the
Collins Axe Co. of some of the inventions of the English Industrial Revolutionaries for
ax and other tool production in the 1830s. The perfection of the production of malleable
cast iron and grey cast iron in the 1850s and the production of tempered alloy steels after
1870 provided the basis for the widespread use of drop-forging technology in the
American factory system of the mass production of tools and equipment of every
description. Modern CNC technologies continue to use drop-forging equipment. Dropforging techniques have their origin in the Bronze Age and early Iron Age where
individual axes and knives were forged in molds with hammers before being heat treated
and/or steeled by ancient ironmongers. See die-sinking and die driving.
Drop press: Machine for punching, shaping or embossing metals; originally hand or foot
operated utilizing a vertically guided weight; later, water or steam powered; fundamental
machine used for drop-forging tools. The most modern form of the drop press is the
hydraulic press. See drop-forging, die-sinking, and die driving.
Dross: Slag-like, metallic oxides that rise to the surface of the bath during the oxidation
process, as in the reduction of iron ore in the blast furnace.
Dry puddling: Direct production of wrought iron by the conversion of white pig iron in a
reverbatory furnace. Conversion of grey cast iron to puddled wrought iron required
preliminary refining due to its free carbon and low silicon content. See puddling furnace
and wrought iron.
Dry sand molding: Casting with a flask and a baked sand pattern, facilitating moisture
removal and providing a hard clean surface for detailed casts. See cope and drag.
Dubbing: Shaping and smoothing of frames and timbers with an adz during the
construction of a wooden ship.
Ductile cast iron: A cast iron characterized by a microstructure with graphite in ball-like
forms in contrast to the flakes of ordinary grey cast iron. Using special processing and
magnesium and/or cerium containing alloys results in increased strength and ductility due
to the nodulizing of the graphite. Widely used by the automotive industry, it is a modern
variant of malleable cast iron.
Ductile steel: “Sir Joseph Whitworth’s last contribution to mechanical engineering was
his discovery that guns made from ductile steel would wear by losing their shape whereas
hard steel guns tended to explode when they were unsound. The problem was in casting
ductile steel into ingots without creating air pockets, which made the metal unsound. Sir
Joseph Whitworth’s solution was an adaptation of Bessemer’s principle of hydraulic
pressure casting.” (The Whitworth Society
Ductility: Capacity of a metal to permanently deform without fracture when cold
Dunnage: Iron fragments, scrap, and faggots used as a shim, as well as ballast, in the
bottom of a wooden ship to raise the cargo above the bilge water level to prevent damage.
Duplexing process: Refinement of cupola-produced cast iron in an accurately controlled
electric furnace for the purpose of producing special purpose, high quality, structural cast
Early steel: Typically, natural steel produced in ancient and medieval times directly from
the bloom. The carbon iron microstructure of early steel always contains elongated or
fragmented silicon slag inclusions. See bloomery, Catalan furnace, ferrosilicate, and
Ecotoxin: Naturally occurring and anthropomorphic chemical toxins, such as
methylmercury and persistent organic pollutants (POPs), which originate at specific point
sources and are then subject to regional and hemispheric transport by the biogeochemical
cycles of the chemosphere. Many ecotoxins, such as biologically significant chemical
fallout, bioaccumulate in pathways to human consumption. Iron and steel production
facilities make a modest contribution to global ecotoxin contaminant pulses in the form
of polycyclic aromatic hydrocarbons (PAH) and mercuric sulfide emissions from
coal/coke fuel. See biocatastrophe, biologically significant chemical fallout, and global
Edge carburization: Alternative process for the carburization of iron, used by both early
and modern steelmakers from the early Iron Age to the modern era. Prior to the advent of
the mass production of edge tools, an iron tool would be enclosed by clay or another
protective covering and submerged in a charcoal fire to allow diffusion of carbon to steel
the cutting edge of the tool. Modern forging strategies subject the bit of an ax to
additional mechanical and thermal treatments, including grinding, tempering, and
annealing to increase the hardness and ductility of the cutting edge. See case hardening
Edge tool forging: Creation of steel edge tools by the heating of iron-carbon matrixes
(FeC, Fe3C) into the austenite phase followed by rapid quenching, which creates
martensite (iron with homogenous carbon distribution), which is then tempered to relieve
brittleness and then shaped by hammering, rolling, or casting into appropriate forms.
Properties of edge tools can vary widely, depending on carbon content, carbon
distribution patterns, mechanical processing (splitting, folding, piling, hammering, and
rolling), thermal treatments, (including duration of quenching, tempering, and annealing),
alloy content, if any, and slag inclusions and distribution. The key to successful edge tool
production is the rapid quench, which forms martensite instead of pearlite, the latter of
which is formed by slow cooling. This is followed by the slow tempering of the steel tool
over a longer time and at a much lower temperature (+/- 600º C) to alter the acicular
cementite microstructure of martensite to more finely and homogeneously distributed
cementite spherical formations, which soften it and increase its ductility. As an alloy,
silicon also functions as a softening agent, enhancing the ductility of the steel being
forged. Edge tools of a more inferior quality could also be made by forge welding
unquenched, slowly cooled austenite, but a sophisticated knowledge of the necessity of
the thermal treatment of forged steel to make knives, swords, and woodworking edge
tools dates to the early Iron Age (Barraclough 1984a).
Edge tools: Hand tools used by woodworkers to cut and shape wood, especially carving
tools, chisels, gouges, slicks, adzes, axes, and plane blades. In the broader context of the
history of hand tools, edge tools also include knives, swords, and cutlery. See convivial
Elastic deformation: Less than permanent deformation, which is remedied by the
removal of the stress or load causing the initial deformation.
Elastic limit: Point at which a metal becomes permanently deformed under stress; also
defined as yield strength.
Electric arc furnace: Furnace in which the heat needed to smelt metals is produced by
an electric arc between carbon or graphite electrodes and the furnace charge; also called a
low frequency induction furnace. One of the two most important 20th century steelproducing strategies, made possible by an electric power grid, the prime mover of which
was biomass-fueled steam turbines or water-powered turbines. Its special advantage is
that, in the production of high grade tool steels, the oxidation of alloys, such as chromium
or nickel, are avoided. The great majority of the hundreds of varieties of useful high
grade alloy tool steels produced in the 20th century were manufactured in this furnace. Its
appearance was significant for edge toolmakers because the steel produced in the electric
arc furnace gradually replaced the crucible steel production process after 1900. By 1940,
the disappearance of both the puddled iron process and the crucible steel process seems to
coincide with the diminishing quality of edge tools. The electric arc furnace can be built
in any size and utilizes scrap iron and steel efficiently. The first electric arc furnace was
constructed by Sir Charles William Siemens in 1878 but was used for melting only. The
first smelting of iron ore occurred in 1898. In 1927, the first high frequency electric
furnace was constructed. Modern electric arc furnaces produce almost all steel used for
contemporary toolmaking. Induction, consumable-electrode melting, and electro slag
furnaces are three modern subtypes of the electric arc furnace. The induction furnace,
which now has many variants, is a primary source of tool steels. The consumableelectrode furnace and electro slag re-melting furnace are used for production of special
alloy steels and ultra high strength missile and aircraft steel. By 1980, electric arc
furnaces were producing about 28% of all US steel. The uniformity and the high quality
of alloy steels produced in the electric furnace is illustrated in the wide variety of
sophisticated products of an atomic age, which was and is characterized by a diminished
capacity for mass production of high quality edge tools. See basic oxygen process and
Electro fusion: Modern form of steel production, which uses an electric current to melt
the charge of ore and flux, c. 1898. In the early years of the electric arc furnace, edge
tools made by this process were sometimes marked “electro fusion.”
Electron microscope: Type of microscope that uses electrons to illuminate and create an
image of a specimen. The electron microscope has much higher magnification and
resolving power than a light microscope, with magnifications up to about two million
times compared to a light microscope’s about two thousand, allowing it to see smaller
objects and greater detail in these objects. Unlike a light microscope, which uses glass
lenses to focus light, the electron microscope uses electrostatic and electromagnetic
lenses to control the illumination and imaging of the specimen. The three types of
electron microscope are: the transmission electron microscope (TEM), the reflection
electron microscope (REM), and the scanning electron microscope (SEM). See REM,
SEM, TEM, and HRTEM.
Elongation: Permanent extension of the microstructure of a metal by mechanical
processes, such as hammering or rolling, especially effective at high temperatures. In
alloy steels, elongation is due to grain boundary sliding of alloys in tension, which then
provide qualities of plasticity and superplasticity. See deformation bands, superplasticity,
Embossing: Ornamental designs executed by stamping or hammering on the reverse side
of a metal to form a relief. See chasing.
Embossing sequence: The first step in the embossing sequence is the creation of a
plaster or wax casting of the pattern to be embossed, e.g. a medallion. A cast iron pattern
is made from the plaster or wax pattern and is driven into the die to form a die-sunk
casting. This casting of the original pattern then recreates the original design. See die
casting, cire perdu, and die scaling.
Embrittlement: In ferrous metallurgy, a common result of sudden cooling, as in the
formation of martensite; usually due to the formation of acicular cementite
microstructures at grain boundaries, in contrast to spheroidization of cementite, which
characterizes microstructures with more ductility and plasticity.
Enclosure: Ancient practice of protecting forged iron tools being carburized from the
oxidizing influence of combustion gasses by covering the iron with a layer of organic
materials (pig fat, goat skins, clay, etc.). For the production of sheet steel from sheet iron,
the layer of charcoal served as the enclosure; for the production of Brescian steel, the
liquid cast iron provided enclosure. Various methods of case hardening necessitate
strategies of closure, e.g. the production of blister steel is based on the enclosure of iron
bar stock in the protective layers of the sandstone converting furnace. See case hardening,
carburize, and cementation furnace.
Energizers: Carbonates, which hasten case hardening and steel cementation, including
the carbonates of calcium, barium, and sodium in commercial carburizing compounds. In
early cementation furnaces, naturally occurring energizers in charcoal dust, bone, skins,
and hide inserted between iron bar stock facilitated carburization. See case hardening and
Engine: Compound machine that uses any power source (water, wind, biomass fuels,
heat, electricity, etc.) to do work. See prime mover.
Eoliths: First tools used by humans; un-hafted, un-knapped, found stones.
Erzberg: Name of the ore-bearing mountain in the Styrian section of Austria that was an
important source of manganese-laced siderite iron ores used from the early Iron Age to
the early modern period. The manganese content of these ores facilitated production of
natural steel in early shaft furnaces, which was then traded throughout central Europe as
currency bars. The manganese content also facilitated the production of high quality
German steel by assisting in the removal of sulfur during the decarburization of cast iron
made with Erzberg ore. See natural steel, Styrian steel, iron road, and currency bars.
Etching: Application of a liquid reagent to the polished surfaces of metals for the
purpose of revealing their microstructures. This method was widely used after 1885,
instead of visual analysis of a fracture, for the evaluation of the structural properties of
ferrous metals. See microstructure and lattice structure.
Eutectic: Minimum melting temperature of an alloy, i.e. the temperature at which the
crystalline becomes molten and the molten becomes crystalline but always involving a
mixture of two or more components. In ferrous metallurgy, the most important eutectic
point is the melting temperature of austenite at 723º C (1341 ºF). Steel and cast iron are
mixtures of austenite and cementite, which, if cooled below this temperature, become
mixtures of ferrite and cementite. If, however, austenite is suddenly cooled in water from
a red heat, martensite, (steel with uniform carbon content,) is produced. Hard and brittle,
martensite is softened and made more ductile by tempering, which causes the dispersion
of fine particles of cementite within the austenite. Another definition of eutectic with
respect to cast iron is: “a thermodynamic equilibrium of two different solid phases with a
liquid solution, e.g. an iron carbon mix with 4.3% carbon content (the eutectic
composition) at 1150º C (the eutectic temperature) where liquid iron carbon is in
equilibrium with austenite and cementite” (Wayman 2000). See ice cream, austenite,
carbon content, and cementite.
Eutectic composition: In ferrous metallurgy, “…a thermodynamic equilibrium of two
different solid phases with a liquid solution” (Wayman 2000).
Eutectic point: Minimum melting temperature of an alloy.
Eutectoid: The thermodynamic point equivalent to a eutectic point but with all three
phases solid, i.e. one solid solution and two solid phases, as in the iron/carbon system at
723º C (the eutectoid temperature) and 0.8% carbon (the eutectoid composition), where
austenite is in equilibrium with ferrite and cementite (Wayman 2000). Tool steels with a
carbon content of 0.6% or greater are examples of solid compositions, which have
undergone a eutectoid transformation, also called the martensitic transformation. In the
eutectoid transformation, the slow cooling of austenite produces ferrite and cementite
(iron carbide), which often exhibit lamellar structures, including bainite and pearlite. See
lamellar and eutectic.
Eutectoid composition: “…the composition which transforms wholly to austenite at the
lowest possible heating temperature” (Bain 1939, 31).
Eutectoid steel: Steel that contains 0.83% carbon is known as eutectoid steel, i.e.
austenite (Shrager 1949). Austenite with a carbon content of >0.83% is hypereutectoid; if
containing < 0.83% cc, it is hypoeutectoid steel. See hypereutectoid and hypoeutectoid
Eutectoid transformation temperature: The eutectoid transformation temperature
varies with carbon content. The lowest eutectoid transformation temperature or eutectic
point is 723º C (1340º F), at which mixtures of ferrite and cementite with a carbon
content of 0.83% undergo phase transformation to austenite. Mixtures with both higher
and lower carbon content undergo phase transformation to pure austenite at higher
Explosive compaction: In powdered metallurgy, the high pressure compaction of
metallic powders, composites, and ceramic and super-hard materials, including
nanocrystalline aggregates, by the use of shock waves. See powdered metallurgy.
Eyepin: Insert used as the core around which two pieces of mild steel are wrapped in axmaking. A high carbon steel insert is then welded into the fold to form a steel ax. In 19th
century ax-making factories, the hands of the grinder held the eyepin during finishing of
the ax prior to the introduction of automatic grinding machines. “No ax grinder ever died
from old age” (Kauffman 1972). See ax-making techniques.
Face-centered cubic structure (FCC): Location of atoms in a crystal structure at the
corners and in the middle of a cubic cell, as in austenized steel. At a temperature of 723°
C, the body lattice structure of alpha iron (BCC) begins deforming into the face-centered
cubic (FCC) structure of gamma iron (austenite). The change is completed at 910°
C/1670° F, when the lattice structure of the iron becomes a face-centered lattice structure.
Upon further heating, the FCC structure of gamma iron reverts to the BCC lattice
structure (delta iron) at a temperature of 2552° F/1400° C. See lattice structure, space
lattice, and cubic units.
Facings: Graphite, sea coal, or other material applied to or mixed with the sand mold into
which a metal is to be poured to provide a smooth surface for the casting. For steel
castings, silica flour mixed with molasses water was used c. 1910.
Faggoting: Bundling of iron rods or rolling of puddled iron and steel plates into bar stock
prior to further heat treatment and/or forge welding. See piling and billet.
Farga: Spanish word for the technology of the reduction of iron ore in direct process
Catalan furnaces. This technology was known and used in Germany at least as early as
the 16th century and was transported to Pennsylvania by German immigrants during the
18th century. Bloomsmiths in colonial New England may have been influenced by
German immigrants, who brought their knowledge and interpretation of direct process
Catalan bloomeries to England in the 16th and 17th centuries, after which it was
transferred to New England in the great migration.
Fargue: Spanish name for direct process Catalan bowl furnace.
Farrier: Blacksmith who specializes in the shoeing of oxen and horses.
Fast cooling rate: Rapid cooling of austenite that prevents excess carbon from
precipitating in the form of cementite. Iron atoms are rearranged to form an acicular
crystal structure that traps carbon in a diffusion-less solid state transformation
(martensite), in which no movement of microstructural dislocations is possible, thus
producing a hard and brittle microstructure.
Fatigue: Progressive loss of resistance of a metal to fracture, usually occurring at
ordinary temperatures, due to the application of force on a flaw that forms a crack that
spreads under repeated stress. See plastic deformation and lattice structure.
Fayalite: Form of iron silicate formed as fluid slag in the smelting process by the mixture
of silicate and iron oxide. Direct process bloomeries wasted significant quantities of iron
ore as fayalite before the role of lime as a flux, which reduced the loss of iron oxide, was
known. See acid process, basic steelmaking process, flux, and slag.
Feedback mechanism: Unintended adverse consequences of cascading Industrial
Revolutions, e.g. the impact of the combustion of fossil fuels by pyrotechnic industrial
society produces CO2 as a greenhouse gas, which warms the atmosphere, melting
permafrost, which releases large quantities of methane, another greenhouse gas, all of
which cause sea level rise by melting glacier ice. Can born-again ironmongers using
nanotechnologies invent some substance that could be used to build 40 foot high seawalls
around vulnerable cities to reduce the impact of cataclysmic climate change (e.g.
Feeders and risers: Fittings utilized during the solidification of cast metals in foundry
work to offset shrinkage by allowing the addition of molten metal during the casting
Female die: Lower die used in press working of jewelry, silverware, and toolmaking;
also known as embossing die. See die-sinking.
Ferdoux: French term for wrought iron produced by decarburizing cast iron. See acier
fondu, acier forge, ferfort, and wrought iron.
Ferfort: French name for malleable iron produced by decarburizing cast steel. Ferfort has
the same carbon content as modern “low carbon steel,” thus differentiating it from
wrought iron, which the French call ferdoux. Ferfort was frequently used in the
manufacture of horticultural tools (Barraclough 1984a). See ferdoux, German steel, low
carbon steel, malleable iron, and wrought iron.
Ferrite: “Low-temperature form of pure iron” (Gordon 1996). Ferrite is a solid solution
of carbon in iron up to 0.03% (alpha iron) stable below 723º C, as in wrought iron. “It is
the softest component in steel and is very ductile” (Pollack 1977, 124-5). Ferrite contains
trace amounts of iron silicide (FeSi) and iron phosphide (Fe3P). It is strongly magnetic,
soft, and ductile and has a tensile strength of between 40 and 50 psi and a Brinell
hardness of +/- 80. See austenite, cementite, and wrought iron.
Ferrite-carbide aggregate: The mixture of pure iron (ferrite) and iron carbide
(cementite) that is characteristic of many forms of carbon steel. The iron carbide content
is dispersed in a ferrite matrix. The proportion of cementite in steel or cast iron depends
on carbon content. The wide variety of microstructural forms of ferrite-carbide
aggregates in pure carbon steel is a function of heating and cooling rates and variation in
thermo-mechanical treatments: hammering, tempering, annealing, etc. See austenite,
bainite, carbide, cementite, ferrite, lattice structure, and pearlite.
Ferrite-cementite phase: Eutectoidal mixture of alternating lamellae of ferrite and
cementite, commonly called pearlite.
Ferrite-cementite-martensite complex: Specific carbide microstructure common to
many steels and also associated with superplasticity in steels. X-ray diffraction analysis
of the lateral face of a Wootz steel Damascus sword blade indicates a microstructure of αFe (ferrite) (73.8% wt), Fe3C (cementite), and Fe1XCX (martensite), without the presence
of either austenite or pearlite. The blade face also contained 2.4% wt carbon content in
the form of graphite (Levin 2005).
Ferrite-Pearlite (FP) Structural Steel: The most industrially significant form of modern
structural steel characterized by small ferrite and austenite grain size in the 5-6μ (micron)
range. The appropriate heat treatment of ferrite-pearlite steels creates a matrix with
virtually no undissolved carbides. The refinement of the ferrite and austenite grain size
creates a resistance to impulsive loading stresses (Paxton 1967, 3).
Ferritic malleable cast iron: Malleableized cast iron with a ferrite matrix imbedded with
particles of temper carbon.
Ferromanganese: Alloy of iron and manganese containing 80% manganese, 12% iron,
6.5% carbon, and 1.5% silicon, which is added to the steel during the smelting process to
increase its carbon and manganese content. Ferromanganese played a key role in
upgrading the strength and durability of Bessemer's bulk process low carbon steel to
make it suitable for uses such as steel rails. Ferromanganese also serves as a deoxidizer.
See Bessemer process and manganese.
Ferrosilicate: Siliceous (silicon bearing) flux formed from unreduced ferrous oxide and
fusible silicate slag that occurs in bloomery furnaces during smelting. Ferrosilicate
encourages oxidation of carbon at the end of the heat in early furnaces and thus assisted
in the production of wrought iron, preventing carbon uptake that would create unwanted
liquid cast iron (Schubert 1957, Wertime 1962, 45).
Ferrous bainite: “All nonlamellar aggregates of ferrite in carbide (irrespective of ferrite
morphology) as well as divorced pearlite” (Sinha 2003, 9.3).
Ferrous materials: Iron and iron alloy combinations within the iron carbon system.
Ferrous metals: Any metal containing iron. Most ferrous metals are iron-carbon alloys.
Many other metals may be deliberately added as alloys to iron-carbon formulations.
Numerous other chemicals such as phosphorus, sulfur, and silicon are inevitably present
as micro-contaminants. See alloys, silicon, manganese, chromium, and rebar.
Ferrous metallurgy: Art and science of smelting iron from iron-bearing ores and the
consequent use of hot iron by multi-tasking blacksmiths to forge iron and steel tools,
weapons, and other implements.
Ferrum Noricum: Iron products produced in the ancient Roman province of Noricum,
now southern Austria.
Fettling: Millscale (iron oxide) used to line a puddling furnace.
File-making: To create a file. Before the era of machine-made files, the process of
making a file involved the cutting and cropping of “strings” of steel into “moods.” File
steel “moods” were forged into triangular or half-round blanks and then softened before
surface scale was removed by filing. The cutting of the file edge with hammer and chisel
was followed by hardening by quenching, cleaning, and oiling. File-making is thus
anomalous, in that softening preceded hardening (Dane 1973).
Filing: Traditional method of shaping metal prior to the introduction of grinding
machines (c. 1875). For example, the hand file was used to make parts that would fit a
particular firearm before the factory system signaled the beginning of the mass
production of interchangeable tool and machine components. The telltale marks of hand
filing can be seen on many hand forged tools, which received their final shaping from
hand filing by individual toolmakers.
Fin: Surplus iron or steel at the parting line of a two piece die from any forging, which is
later trimmed off.
Fine grain: Uniform pattern of grain distribution in the lattice structure of iron-carbon
alloys resulting from simultaneous crystallization of the lattice structure nuclei in contrast
to random crystallization, which produces more deformed and irregular crystal structures.
Finery: Facility used for the decarburizing of pig iron to produce wrought iron using
charcoal fuel; a hearth used to further refine bloomery-derived wrought or malleable iron.
Products of the finery were often sent to a chafery for further thermal and mechanical
treatment, including shaping into bar stock. Finery-produced bar stock from direct
process bloomeries or the integrated iron works of a blast furnace complex was an
important cargo in the coasting trade and the main source of iron for blacksmiths in the
manufacture of hand tools. The finery was common before 1830 but was gradually
replaced by the puddling furnace and specialized chafery pit-type furnaces for hot
working or rolling malleable into semi-finished products such as slabs, billets, and
blooms, the latter not to be confused with the blooms of the direct process of iron and
steel production before the era of bulk steel production. See bloomery, malleable iron,
puddling furnace, rolling mills, and wrought iron.
Fining: Process of purification by removal of contaminants, as in a fining furnace.
Fining hearth: 1) Walloon and other open-hearth style furnaces used to decarburize cast
iron into wrought and malleable iron at an integrated iron works. An increase in the fuel
to ore ratio was sometimes used to produce malleable iron or raw steel instead of wrought
iron, i.e. the decarburization of the cast iron was halted before all the carbon was
eliminated from the pig iron being refined. In many cases, the iron being produced was
malleable iron 0.08 – 0.2% cc or a malleable iron with a higher carbon content equivalent
to that in modern (>1870) low carbon steel (0.2 – 0.5% cc). However, finery iron differed
from modern low carbon steel in that it has a variable siliceous slag content, hence the
term malleable iron. 2) A secondary hearth for refining the wrought or malleable iron
loup produced by the bloomsmith. Water powered North American colonial era smelting
furnaces often had multiple hearths for further hammering and thermal treatment of iron
bar stock. See cast steel 2), malleable iron, and Walloon process.
Firearm: Mechanical device that ejects a missile by the explosion of gun powder. The
largest firearms were cannons, initially made from bronze, and, later, from cast iron.
Smaller firearms, such as the Arquebus and the flintlock, were usually made of soft,
folded, and welded sheet wrought iron. In the post-Reaganomics era, high powered
assault rifles have become an icon of freedom as the influence of crypto-fascism has
Flame hardening: Localized heat treatment of a steel surface to be hardened by the
heating of the surface above the critical temperature (1300º F) to 1550º F.
Flange iron: Soft, ductile wrought iron used in applications subject to heavy stress.
Flash: Waste metal that remains on drop-forged tools after steam hammering.
Flask: Foundry molding box, consisting of the cope (top) and drag (bottom), often with a
core as part of the pattern, into which sand is rammed and packed.
Flat world: A term coined by Thomas Friedman and used as a title in The World is Flat:
A Brief History of the Twenty-first Century. Flat world refers to the capturing of the
attention of a large percentage of our population, including students, workers,
entrepreneurs, the educated elite, etc. by two dimensional Information Age technology,
including computers, iPhones, iPads, and a growing repertoire of other electronic devices.
Unfortunately, Friedman failed to reference, at least until later publications, the ongoing
escalation of the three dimensional round world crises that characterize the evolving age
of biocatastrophe: the world under crisis, catastrophic climate change, chemical fallout
and its human health impact, growing debt and income disparities, declining public
resources for infrastructure, education, and innovative research and development,
political polarization and paralysis, and the social unrest these engender.
Flatting mill: Small hand-cranked set of iron rollers with an inset cut into the rollers to
produce silver molding patterns, used by silversmiths on teapots and other wares in lieu
of hand-stamped chased molding. Flatting mills appeared +/-1720 and were a miniature
predecessor of later die-forging machinery of the factory system of tool manufacturing
>1830. The moldings produced by the flatting mill are also called die-rolled moldings.
Flintlock: Dominant form of small firearms from the reign of William III (1650) until
1840 (Greener 1910). Developed in the 1620s and of Spanish or Dutch origin, the
flintlock was much easier to fire than the matchlock. See matchlock, Arquebus,
wheellock, gun barrel iron, and gunsmithing.
Flow-strain rate response: Measurement of flow stress (MPa) over strain rate (s-1); “A
strain rate sensitivity … exponent of 0.5 is often considered the optimum one for
achieving superplasticity in fine-grained, metallic alloys” (Sherby 1995, 14).
Flow termination: Termination of plastic deformation in the crystal structure of metals
that result from either brittle cleavage or ductile fracture.
Fluid carburization: Modern process for the hardening of steel by its heating above the
critical temperature in a retort furnace in the presence of CO2, ethane, methane, propane,
natural gas, or liquid cyanide, any of which facilitate carbon penetration into the steel.
Fluidity of microstructures: Gestalt of diffusing, sliding, slipping, encompassing,
encroaching, straining, elongating, shearing, and/or proliferating microstructures
characteristic of the phase transformation kinetics of ferrous metals.
Fluidized bed process: Modern process for producing sponge iron that uses the heat
from the partial combustion of preheated air and natural gas for the reducing reactions.
“The reducing gas is composed of about 21 per cent carbon monoxide, 38 per cent
nitrogen, and 41% hydrogen. The reduced iron is pressed into briquettes and stored or
shipped” (Pollack 1977, 7). See sponge iron.
Flux: Additive in the smelting process, e.g. lime, which has the purpose of taking up and
absorbing the melted impurities in the iron ore, creating slag. The slag is then drained off
separately from the molten ore produced by direct process smelting or indirect process
blast furnaces, usually through an opening above the container of the molten iron.
Clamshells were the flux of choice in the bog iron forges and blast furnaces of
southeastern Massachusetts. In modern steelmaking and ironworking, fluxes are used for
bronzing to remove or prevent the formation of oxides and promote the free flow of filler
material. They may have the form of pastes, powders, gasses, or other coatings and
include borates, fluorides, chlorides, acids, and wetting agents. See brazing.
For-profit mental illness: Thorazine, Iproniazid, Prozac, Effexor, Paxil, Serzone,
Celexa, Zoloft, Risperdal, Seroquel, Zyprexa: pharmaceuticals made by pharmaceutical
companies are the prime movers of an epidemic in mental illness (Angell 2011). The
convivial tool wielding lifestyles of round world born-again ironmongers provide an
alternative to the flat world enhanced necessity of addictive but profitable pharmaceutical
Forest of Dean: Area just north of Bristol and the River Severn on the west coast of
England, where low phosphorus brown hematite iron ore of nearly equal quality to
Swedish ores was smelted in the 16th and early 17th century before being depleted. Along
with iron smelted from ores located to the east in the Weald of Sussex, iron produced in
the Forest of Dean may have played an important role in the manufacture of tools for the
early colonial settlements in North America before the manufacture of blister steel
became widespread (1700). The first blast furnaces in England were larger than those in
the Weald and may have been located in the Forest of Dean (Cleere 1985).
Forge: (noun) See furnace/forge.
Forge: (verb) To shape steel and iron into various forms by hot working, including
hammering, rolling, slitting, and bending. Until the early 19th century, forge welding by
hand was the primary means of shaping iron and steel tools. Henry Cort’s redesign of the
rolling mill (1784) represented a radical improvement in the efficiency of the forging of
hot iron. Beginning in the mid-19th century, most shaping or hot working of steel and iron
was done by machinery that forced hot metal into dies and rolling machines. In the case
of the manufacturing of hand tools, the patterns cut into the dies formed the tools being
shaped. See drop-forging, die-sinking, and steeling.
Forge train: “The set of heavy rolls between which the shingle bloom of puddled iron is
rolled into puddled bar (muck bar) The rolls are grooved in a diminishing series so as to
reduce the bloom to a manageable bar, and are made reversing if two high, or nonreversing if three high” (Audel 1942, 246). See rolling mill.
Forge welding: Bonding of pieces of steel or iron by hammering at high temperatures,
often in the presence of flux. See steeling.
Forging mill: Facility for producing finished steel by hammering and rolling. These mills
were particularly efficient when run by a water-powered hammer, which had even strokes
and more controllability than early steam-powered hammers, i.e. before the invention of
reciprocating steam engines with double acting pistons and smooth even strokes. See trip
Foundry: Workshop or factory for casting metals, including grey cast iron, malleable
cast iron, and nonferrous metals into cannons, hollowware, tools, hardware, and other
equipment. Sometimes the foundry was attached directly to a blast furnace, and, thus, no
re-melting of the metals was required. Foundries were often associated with cupola
Fracture: Characteristic crystalline pattern (grain) exhibited after accidentally or
deliberately induced cleavage altered or exposed the microstructure of the steel being
thermo-mechanically processed. A fracture by brittle cleavage produces a flat, smooth
surface. A shearing fracture produces a “rougher surface, usually slightly inclined to the
slip plane….When this type of fracture brings ductile elongation to an end, it is found
that the fracture occurs at a definite value of the resolved shear stress along the slip
plane” (Barrett 1943, 321). See Sheffield classification of blister steel, grain, cleavage,
crystal structure, and sap.
Fracture toughness: Ductility in iron and steel, characterized by the capacity to flex
without breaking. See fracture, ductile iron, and ductility.
Free oxygen: Oxygen that in a furnace causes iron to burn; one of the hazards for a
foundry master in situations where slag is not protecting the molten iron from oxidation.
Freezing point of iron: The freezing (or melting) point of iron is dependent on its carbon
content (cc). Pure iron freezes and melts at 1535° C. As the carbon content of iron, steel,
and cast iron increases, the melting and freezing point declines. Cast iron with a 4.3% cc
freezes and melts at a temperature of 1130° C, the eutectic temperature of this alloy
composition. Below the freezing/melting temperature, the iron or steel changes from a
liquid (the liquidus) to a mushy combination of liquid and solid until the temperature falls
sufficiently for the alloy to pass the solidus, or temperature at which it becomes
completely solid. See ice cream and solidus.
French iron and steel: France utilized the traditional Continental technique of making
“German” steel by decarburizing cast iron, sorting the results into three categories,
ferdoux (wrought iron), ferfort (malleable iron), and acier fondu (quenchable steel that
could be martinized, the highest quality of which is cast steel) (Barraclough 1984a). See
acier forge and German steel.
Friction welding: Modern welding technique involving the joining, by spinning and
jamming, of two pieces of metal in tubular applications. The high temperatures needed
for welding result from the rapid spinning (30,000 – 40,000 rpm) of the metal being
Fuel to ore ratio: Key consideration of early direct process smelting strategies.
Differences in the fuel to ore ratio could result in the production of a low carbon wrought
iron (< 0.08% cc), malleable iron with a carbon content (0.08% - 0.2% cc), malleable iron
with a carbon content equivalent to modern (1870) “low carbon steel” (0.2 - 0.5% cc), or
raw steel (> 0.5% cc). In the heterogeneous bloom of iron being smelted, increasing the
fuel to ore ratio tended to increase the probability of raw steel production. See natural
steel, carbon content of ferrous metals, and fining hearth.
Full annealing: Heating of iron alloys above their critical temperature for an appropriate
time period, followed by slow cooling, either in a furnace or in a thermally insulated
environment for the purpose of altering the crystal structure and, thus, the properties of
the metal being annealed. See annealing.
Full welding heat: Temperature necessary to weld two pieces of iron or one piece of
steel and a piece of iron together (2400° F / 1365° C). The iron will have a white color
and will emit visible sparks due to the oxidation of the iron.
Fullerene: “Any molecule composed entirely of carbon, in the form of a hollow sphere,
ellipsoid or tube… Fullerenes are similar in structure to graphite, which is composed of
stacked graphene sheets of linked hexagonal rings; but they may also contain pentagonal
(or sometimes heptagonal) rings… The discovery of fullerenes greatly expanded the
number of known carbon allotropes, which until recently were limited to graphite,
diamond, and amorphous carbon such as soot and charcoal” (Wikipedia 2013).
Fullering: Shaping of wrought or malleable iron by the use of a creaser (the fuller),
which may be placed in a hardy hole to shape the iron or may be struck by a hammer to
spread the iron by the formation of a series of indentations.
Furnace/Forge: Furnaces, including blast furnaces, are used for smelting ore or the
melting of pig iron (cupola furnace); forges are used to reprocess the product of the
bloomery or blast furnace by the mechanical and thermal treatment of metal after
smelting. In some cases, especially before 1900, small forges also served as a furnace for
reducing ore prior to the production of tools and ironware by the blacksmith or shipsmith.
In town histories and historical writings, “forge” is a term often mistakenly used to refer
to the furnace of a bloomsmith. The loups or blooms produced by the bloomsmith in his
furnace were often shaped into bar stock in chafery or finery forges and transported to the
forge of a blacksmith or shipsmith for further processing. See blast furnace, bloomery,
chafery, ferrous metallurgy, finery, and fining.
Furnace bottom: Slag that formed at the base of a non-slag tapping bowl furnace.
Furnace types (before 1870): Three basic types of furnaces characterize iron and steel
production from the early Iron Age to the beginning of bulk process steel production
(1870), the crucible, bowl, and shaft furnace (Tylecote 1987, Wertime 1962). Later
Stucköfen and blast furnaces are larger forms of the shaft furnace. Cementation,
reverbatory, and cupola furnaces are further adaptations of this form.
Crucible-shaped furnace: Among the earliest furnace designs was a simple crucible,
especially common in northern Asia and used for both cast iron and Wootz steel
production. Multiple crucibles with as little as 1 kg capacity were used for Wootz
steel production as early as 300 BC. Cast iron production in larger crucibles in China
can be dated at least as early as 800 BC. The crucible-shaped furnace evolved into the
cupola furnace commonly used in the 19th century to re-melt blast-furnace-derived
Bowl furnace: Earliest form of furnace. The charge of ore was often located in back
of the fuel and reduction occurred via a current of carbon monoxide formed by the
burning charcoal, assisted by a directed flow of air from a tuyère. The Catalan furnace
of northeastern Spain is the most well known form of the bowl furnace. Most earlier
bowl furnaces were slag pit types. The rectangular open-hearth breakdown furnace
used to smelt raw steel for Japanese swordsmiths is one of many variations of the
bowl furnace form.
Shaft furnace: Most common form of furnace throughout the Iron Age. Ore and fuel
are mixed together in a four sided shaft. The resultant bloom of wrought or malleable
iron is extracted from a hole at the bottom of the furnace. Combustion is also aided by
the use of the tuyère, powered by varying types of blowing devices.
Shaft furnace types are further subdivided as being slag pit types and slag-tapped
Slag pit furnace: Furnace in which the slag accumulates in situ at the bottom
of the furnace until the furnace is moved to an adjacent slag-free location.
Slag-tapped furnace: The slag-tapped furnace was more practical and
efficient than the slag pit furnace, where the slag from the smelting process
was withdrawn through a tap hole to an adjacent cavity or hollow in the
Stucköfen furnace: Low shaft (1 to 2 meters in height) slag-tapped furnaces
characterized most Roman era ironworks. Low shaft furnaces gradually grew in
height, capacity, and efficiency to become the high shaft Stucköfen of the German
Renaissance, the immediate predecessor of the blast furnace.
Blast furnace: A form of high shaft furnace designed specifically to operate at high
temperatures, thus carburizing iron ore to produce liquid cast iron. Blast furnaces
gradually increased in size from the high shaft Stuckofen furnace to the modern
furnaces with a capacity for converting up to 50 tons of cast iron to low carbon steel.
Two variations of the shaft furnace appeared during and after the 17th century, which
were characterized by furnaces designed to prevent fuel-ore contact. Along with the
modern blast furnace, these two furnace types dominated blister steel and puddled,
wrought, and malleable iron production until the appearance of modern bulk steel
furnaces. Both facilitated greatly increased quality control and quantity of steel and iron
Cementation furnace: Sandstone furnaces, in which iron bar stock was enclosed to
be carburized into blister steel, also called “steel furnace,” especially in the United
States in the colonial period. First noted in Nuremburg in 1601, such furnaces
protected the steel being smelted from the oxidizing influence of the burning fuel. The
cementation furnace should not be confused with the many modern forms of steel
furnaces developed after 1860.
Reverbatory furnace: A furnace form with a fire pit located underneath the hearth
that facilitated the decarburization of large quantities of pig iron by heat reflected
from the metal roof of the furnace, preventing fuel to ore contact. Primitive forms of
the reverbatory (refractory) furnace, also known as the puddling furnace, were
improved by Henry Cort into the modern form of the reverbatory furnace in 1785,
allowing production of large quantities of high quality wrought iron.
See blast furnace, blowing devices, bowl furnace, shaft furnace, and tuyère. For modern
furnace forms, see basic oxygen process, Bessemer process, electric arc furnace, openhearth furnace, and Siemens-Martins.
Futtock: Four or five separate pieces of timber comprising the ribs of a ship, usually held
together by iron bolts made by a shipsmith.
Galvanize: To coat the surface of iron and steel with tin or zinc, usually to prevent
Ganister: Furnace linings made of refractory rocks, such as sandstone. See acid process.
Gangue: Contaminants in iron ore removed as slag, e.g. quartz and oxides of aluminum
and silicon, often found in clay-like materials associated with the iron ore. The most
common component of gangue is silicon. See ferrosilicate, slag, flux, and reduction.
Generosity of the 1%: The majority of the one percent in America, several million wage
earners, doctors, actors, musicians, and successful entrepreneurs, are not members of the
klepto-elite but rather fund charities and nonprofits that are a viable alternative to the
stock and bond market casinos and tax loopholes of the American klepto-plutocracy.
Geoengineer: A person who measures and models the earth for applications using civil
engineering technologies to combat, for example, the impact of climate change by
producing temperature lowering atmospheric smog. Will innovative geoengineering
concoct some creative solution to the looming disaster of increasing greenhouse gas
emissions, cataclysmic climate change, and rapidly rising sea levels?
Geomagnetic induced current (GIC): Disruptions in the earth’s magnetosphere and
ionosphere caused by coronal mass ejection (CME) events, which cause voltage surges in
power lines, transformers, pipelines, satellites, and other information technology
Geomagnetic storm: A temporary disturbance of the Earth’s magnetosphere caused by a
solar wind shock wave and/or cloud of magnetic field which interacts with the Earth’s
magnetic field. The increase in the solar wind pressure initially compresses the
magnetosphere and the solar wind’s magnetic field interacts with the Earth’s magnetic
field and transfers increased energy into the magnetosphere. Both interactions cause an
increase in movement of plasma through the magnetosphere (driven by increased electric
fields inside the magnetosphere) and an increase in electric current in the magnetosphere
and ionosphere. During the main phase of a geomagnetic storm, electric current in the
magnetosphere creates a magnetic force which pushes out the boundary between the
magnetosphere and the solar wind. The disturbance in the interplanetary medium which
drives the geomagnetic storm may be due to a solar coronal mass ejection (CME) or a
high speed stream (co-rotating interaction region or CIR) of the solar wind originating
from a region of weak magnetic field on the Sun’s surface. The frequency of
geomagnetic storms increases and decreases with the sunspot cycle. CME driven storms
are more common during the maximum of the solar cycle and CIR driven storms are
more common during the minimum of the solar cycle (Wikipedia 2013).
German silver: Alloy of nickel and copper and sometimes zinc; also called nickel silver.
German steel: Steel made by the predominant steelmaking strategy in the Renaissance,
both in England and on the European continent. German steel was made by decarburizing
blast furnace pig iron in a separate finery type furnace (1400-1650). The resulting
steel/iron mix was further refined into bar stock, bundled, reheated, quenched, broken up
into fragments, reheated, annealed for +/- 45 minutes, and re-hammered as billets of steel
(German steel). German steel was also produced in England after the establishment of the
first blast furnaces in the mid-15th century until the cementation furnace became widely
used after the mid-17th century. The roots of German steel production lie in the
manganese rich ore of Styria and Carinthia (Austria), which facilitated the first iron
production at Halstadt. Used by the Romans to produce steel weapons (Noricum), the
possibly accidental production of natural steel in early bloomeries became the deliberate
production of German steel in Stucköfen (shaft) furnaces, which could produce pig iron,
steel, malleable iron, or wrought iron, depending on the fuel to ore ratio and smelting
temperatures. Production of steel from decarburized cast iron in separate fineries was an
outgrowth of the appearance of blast furnaces producing large quantities of pig iron in
continental Europe after 1315. “Steel made from the seventeenth century onward in
Styria and Carinthia by fining manganese rich pig iron. It contained alternating bands of
high- and low-carbon content and was considered a superior material for cutlery”
(Gordon 1996). Of great importance during the florescence of Nuremburg and Augsburg
watch-making and armor manufacturing, +/- 1500 AD, numerous fine examples of hand
tools made between 1500 and 1750 from German steel are on display at the National
Museum in Nuremburg, Germany. Having the appearance of cast steel (Manganese in
smelted iron ore results in a sheen, similar to that of cast steel.) and probably containing
some martensite, these low carbon steel tools (+/- 0.5% carbon) are labeled as “eisen”
(iron) by the National Museum. Their manganese content is the probable cause of their
visual similarity to the crucible steel tools produced in Sheffield after 1750. In the
broader context of tool production, between 1400 and 1800, German steel had a wide
range of carbon content depending on its intended use. Many edge tools made after the
appearance of the blast furnace, such as trade (e.g. Biscayne ax) and felling axes are
composed of one piece of steel with no steel-iron interface, as in later “steeled” axes. See
Biscayne ax, spiegeleisen, spathic ore, natural steel, and Styrian steel.
Gladius: Roman short sword made of wrought iron and low carbon steel, occasionally
pattern-welded. The gladius was often cold work-hardened (not heat-treated) or surface
carburized at its steeled edge. See spathas.
Glide plane: Points in the lattice structure that combine rotation on the screw axis with
movement along a translation parallel, e.g. axial or diagonal length, of the lattice
structure. Plastic deformation of the lattice structure of iron, for example, occurs along
the crystallographic glide plane, also called the slip plane (Barrett 1943, 288).
Global contaminant pulse: The global transport of ecotoxins derived from industrial
activities, transportation system and agricultural petrochemicals, and the electronic and
pharmaceutical products of global consumer society. Global contaminant pulse transport
occurs in the context of a biosphere composed of interconnected ecosystems where
ecotoxins are detected as contaminant signals in abiotic and biotic media. These
ecotoxins tend to biomagnify in pathways to human consumption and in human blood,
tissues, and breast milk. See biocatastrophe, cascading Industrial Revolutions, ecotoxin,
and tragedy of the world commons.
Goethite: “Ore mineral composed of hydrated iron oxide” (Gordon 1996).
Googolplex of microstructures: The endless variations in the microstructures of ferrous
metals. If one “googol” is greater than the number of elementary particles in the known
universe, then, given the variables of carbon content, alloy content, innumerable
mechanical and thermal treatments, and invisible microconstituents, the forging of iron or
steel produces a googolplex of microstructures, no two of which are alike. See kan of the
Gossans: Oxidized iron pyrite in the form of outcrops of decomposed rocks; a source of
iron for early smelting furnaces.
Grain: In ferrous metallurgy, the consistent alignment of microstructural crystals, the
patterns of which allow a blacksmith to judge the mechanical properties and quality of
iron and steel. For example, grain size in cast iron is determined by the rate of cooling of
the iron in molds, as well as its silicon content. High silicon content (2 - 3%) produces
large graphite flakes and a coarse grain structure. See fracture, combined carbon, and
Grain boundary kinetics: Phase transformation by grain boundary diffusion, also called
diffusion creep, is a characteristic of non-superplasticity in metals, typified by the
formation of ferrite-pearlite structures during the slow cooling of blister steel. Grain
boundary sliding by dislocation creep is a characteristic of superplasticity in metals and is
facilitated by fine grain size and lack of cavitation.
Grain direction: Expresses the uniformity or lack of uniformity of the microstructure of
the iron or steel being forge welded. The ability of the smith to follow the strain patterns,
expressed as grain direction, of the metal and incorporate them in the design of the
implement to be manufactured is key to successful forge welding. “In a gun hammer, the
strain is along the nose, across the finger and down the body of the cock” (Greener 1910,
246). One of the primary objectives of the faggoting, piling, and reforging of wrought
iron into bar stock of the highest quality was the correct alignment of the grain direction
of the siliceous fibers remaining in the wrought iron.
Grain growth: Increase in the grain size of crystals within the lattice structure of iron
carbon alloys, which occurs when the metal is heated above the critical temperature and
held at that temperature for a time sufficient for adjacent crystals to absorb each other.
Grain size: Along with homogeneity of carbon distribution, grain size determines the
mechanical properties of steel, including the strength, toughness, and hardness of the
crystal structure of iron and steel. Coarse-grained austenite increases hardenability in
steel. In other cases, increasing grain size in polycrystalline structures decreases hardness.
Decreasing grain size increases hardness, as in the dispersion of fine cementite particles
during the formation of martensite. Austenite grain size coarsens with increasing heating
temperature and influences hardenability by slowing the cooling rate of the interior of a
piece of steel being quenched while the exterior becomes hard martensite. “Fine grained
martensite usually transforms to fine-grained ferrite, pearlite, bainite or martensite,
thereby providing increased strength and toughness” (Sinha 2003, 10.7).
Grain structure: Microstructural arrangements of the crystals in iron carbon alloys that
determine their properties, i.e. coarse grained, fine grained, stressed (slip plane
dislocations, as in martensite shearing). See stress fields, microstructure, lattice structure,
and grain direction.
Graphene: A one atom thick sheet of pure carbon characterized by high conductivity,
high electron mobility, and a free standing two dimensional crystal microstructure.
“Graphene nanoribbions may prove generally capable of replacing silicon as a
semiconductor in modern technology” (Wikipedia 2013). Graphene transistors are the
wave of the future for communications technology. The recent discovery of the existence
of graphene as a component of carbon nanotubes may unravel some mysteries about the
microstructure of Damascus steel swords.
Graphite crucibles: Crucibles for casting steel made from a combination of clay, lead,
and graphite. Developed by Joseph Dixon in 1850, the thermal efficiency of the lead
(plumbago) in American-made crucibles, which allowed casting at high temperatures,
played a role in the rise of American crucible steel production after 1860. See
Stourbridge clay and cast steel 1.
Graphite flakes: Randomly occurring, bent, wrinkled, crystal scales of graphitic carbon,
which weaken the structure of cast iron by creating spaces in its crystalline structure. See
crystalline structure, graphitic carbon, and grey cast iron.
Graphitic carbon: Free graphite flakes, as in wrought and cast iron. The relative
proportion of free graphitic carbon flakes and chemically combined carbon in cast iron
determines its structure and physical properties, i.e. whether the iron is brittle or durable.
The amount of the graphitic carbon is dependent on the cooling rate of the iron. The
slower the cooling rate, as in sand molds, the higher the free graphite content. Free
graphite weakens the iron but also increases its machinability. White cast iron is
characterized by the predominance of chemically combined carbon, which is produced by
rapid cooling, i.e. in iron molds. It is extremely durable but difficult to machine. See
malleable cast iron, white cast iron, grey cast iron, and cooling rate.
Great migration (1629-1643): Migration of tens of thousands of Puritan dissenters to the
Massachusetts Bay Colony, beginning with the Winthrop fleet of 1629, which transported
hundreds of knowledgeable blacksmiths, bloomsmiths, shipsmiths, and shipwrights to
colonial New England. This migration was the foundation for the rapidly expanding
ironworking and shipbuilding economy of New England that was well underway by
Green sand mold: Mold used for casting grey cast iron, malleable cast iron, and other
non-ferrous metals such as bronze, brass, and aluminum. Damp sand is rammed around a
pattern and, when the pattern is removed, the sand mold is filled with molten metal. See
casting and molder.
Grey cast iron: Cast iron containing free graphite in the form of graphite flakes as its
principal form of carbon and having its combined carbon content not in excess of the
eutectoid percentage. Slowly cooled cast iron is characterized by larger than normal
acicular graphite crystals, which are very weak, making cast iron that is very brittle.
Produced in its modern form in hotter, coke-fired blast furnaces, its higher silicon content
inhibits cementite formation and makes the grey cast iron more difficult to decarburize. It
can occur as a matrix of ferrite and pearlite or as a mixture of both and is the principal
industrial form of cast iron. It is also used to make malleable cast iron by chilling and
annealing. This process changes the large grey flakes of free graphite to a more finely
divided pattern of graphite distribution, promoting the formation of graphite-austenite
microstructures. Free graphite in grey cast iron that occurs as loose brittle flakes cuts
through and separates grains of iron and makes the cast iron brittle rather than malleable
resulting in low tensile strength and high thermal conductivity. The annealing of grey cast
iron restores malleability. Chemically combined carbon prevents malleability in white
cast iron, which is also annealed to make malleable cast iron. The addition of silicon and
graphite stabilizing elements enhances the fluidity and durability of annealed cast iron.
Modern grey cast iron is composed of approximately 4% carbon, 2% silicon, 1.5%
manganese, 1% phosphorous, and 0.05% sulfur. The addition of chromium and vanadium
facilitates the formation of carbides, producing fine grained, high strength cast iron
(Pollack 1977). For some grey cast irons, nickel in a range of 4 – 15% may be added to
control graphite flake size and enhance heat and corrosion resistance. Tool Talks (Stanley
Tools 1937, 15) describes grey cast iron for use in the manufacture of Stanley planes.
This entire article on grey iron casting is available on the Davistown Museum website as
a tool information file. See cast irons, ferrite, graphite, malleable cast iron, pearlite, and
white cast iron.
Grind: Removal of material by abrasive action; for edge tools, to wear down, polish, or
sharpen using friction. Grinding by motorized machinery using vitrified bond wheels
consisting of a mixture of emery and pottery slip clay replaced grinding utilizing
sandstone wheels and hand files for most toolmaking functions beginning in 1878 (Lee
1995, 34). The use of a sandstone wheel mounted in a wood or metal frame continued in
rural communities for sharpening axes until well into the 20th century.
Grindability index: A designation of the ability of a high speed tool steel cutting tool to
be re-sharpened or otherwise altered due to the presence of alloy related hard metallic
Grindstone: Traditional tool for sharpening axes. As used in the 19th century ax-making
industry prior to the invention of the vitrified bond wheel by Frank Norton of Worcester,
MA, grindstones were 6 to 12 inches thick, 4 to 8 feet in diameter, and weighed 2000 to
4000 pounds (Lee 1995, 34). Smaller versions of ax grindstones mounted in a wood or
metal frame are still commonly encountered in rural environments, in which stone
thickness is typically 3 to 4 inches and diameter range is 18 to 36 inches. Most
grindstones were traditionally water-cooled. Sandstone was the preferred material
because it was the only stone to release particles at a controlled rate during the grinding
process. See ax-making techniques and eyepin.
Gun barrel iron: Sheet wrought iron folded around a rod and then welded to form the
gun barrel. See gunsmithing and Belgian iron.
Gunmetal bronze: Alloy containing 90% copper and 10% tin.
Gunsmithing: Making of guns by a gunsmith. Prior to the advent of the all cast steel gun
barrel, gunsmithing usually involved the pattern-welding of piled soft iron and,
occasionally, strips of silver or shear steel (refined German or blister steel). Apparently,
soft wrought iron (<= 0.08% carbon content) was preferred to malleable iron (0.08 –
0.5% carbon content) due to its ductility and ease of workability. The exception to the
generic production of guns from wrought iron as welded iron and steel are the exquisite
all steel wheellock guns produced by German gunsmiths in the late 16th and early 17th
centuries for the nobility, professional military officers, and royalty, examples of which
are currently on display in the Arms and Armor section of New York’s Metropolitan
Museum of Art. The exacting techniques used to forge this high quality steel remain
unexplained in contemporary texts. See Belgian iron, pattern-welding, and wrought iron.
Gutterman: In the operation of a blast furnace, the person in charge of supervising
activity in the lower region of the blast furnace, especially the efficient drainage of liquid
cast iron from the bosh through the temp to the molds. In the case of blast furnaces
producing pig iron rather than hollowware, the gutterman would direct the melted iron
into the rows of sows, creating cast iron ingots with the appearance of pigs, hence the
name pig iron. Most pig iron was remelted in cupola or other special purpose furnaces for
its intended use. See temp, Bosch, blast furnace, cupola furnace, and molder.
H1 Stainless steel: A new stainless steel made in Japan that is “precipitation-hardened
and contains nitrogen instead of carbon as the primary alloying element.” Used for knifemaking, “the people who have used it claim it is completely impervious to oxidation.” It
is composed of carbon: 0.15%, chromium: 14.00-16.00%, manganese: 2.00%,
molybdenum: 0.50-1.50%, nickel: 6.00-8.00%, nitrogen: 0.10%, phosphorus: 0.04%,
silicon: 3.00-4.50%, and sulfur: 0.03% (Erin Casson 2013, personal communication).
HRTEM: High-resolution form of the transmission electron microscope used in the early
21st century for the analysis of the microstructure of metals. A HRTEM has the ability,
not previously available to archaeometallurgists, of analyzing structures of nanometer
dimensions (billionths of a meter, as in the nanowires of cementite in Damascus swords –
10 - 20 nm in diameter, 200 nm in length) (Levin 2005). See microstructure and
Haft: Helve or handle of an ax or adz set up in a shaft hole at a right angle to the major
axis of the tool. See eyepin.
Halstadt: First Iron Age culture in Europe, named after the salt-mining town in Austria,
where Celtic metallurgists switched from making bronze to iron tools c. 750 BC. See
Hand Tools in History Volume 6 and La Téne.
Hammersmith: Another name for the Saugus Ironworks (1646 to +/-1676), America’s
first integrated ironworks.
Hand tool: Instrument of manual operation.
Hard facing: The use of welding methods to add a coating, edge, or point on a metal,
especially an alloy, to resist impact, corrosion, abrasion, or heat.
Hardenability: Ability of steel to be hardened. The following factors determine
hardenability: carbon content, grain size, lattice structure, heating temperature, heating
and cooling rates, and prior thermal treatments. “The depth to which steel can be
hardened to martensite under stated conditions of cooling is called its hardenability”
(Shrager 1949, 145). “A mechanical and retrospective expression of the processes and
phenomena occurring in steel products on cooling from austenizing temperatures” (Cias
n.d., 3). “The capacity of steel to avoid transformation to soft products with a lower and
lower cooling rate regardless of just what maximum hardness it may achieve in the
martensitic state” (Bain 1939, 46).
Hardening: The process that occurs during the heating and forge welding of iron (alpha
iron) with a carbon content of 0.5% or greater due to sudden cooling (quenching) of the
metal from a temperature at 910° C or above, which freezes the lattice structure of
austenite (gamma iron) in a hard and brittle form, which is difficult to work unless
softened by tempering or annealing. Hardness is thus a function of tempering
temperature. Tempering relieves stress by allowing lattice rotation, changing the crystal
structure of the steel. “If steel contains less than four tenths of one percent of carbon it
has little or no hardening power under this treatment [sudden cooling]; but steel with six
tenths of one percent or more of the element, has the wonderful property of being slightly
malleable in the annealed state but extremely hard and brittle after this sudden cooling”
(Spring 1917, 109). See annealing, carbon content of ferrous metals, recovery, and
Hardness: “Resistance to plastic deformation by penetration, scratching or bending”
(Shrager 1949, 367). The sudden increase in hardness following hardening increases
tensile strength but reduces toughness and ductility, which are restored by tempering. See
Hardness formation effectiveness: Slowly cooling austenite to produce lamellar
structures of pearlite produces steel with different mechanical properties than the
production of spheroidized structures from quenched and tempered steel. The lamellar
formations of slowly cooled austenite have greater tensile strength than rapidly quenched
and tempered austenite, but the dispersion of the carbide spheroids of the quenched, then
tempered martensite provides greater elasticity (plastic flow) than the pearlitic
microstructures characteristic of slowly cooled blister steel (Bain 1939).
Hardness penetration: Depth of the hardened surface of quenched tool steel, often
increased by the addition of alloys (Palmer 1937). Hardness penetration is a prerequisite
for many modern machine designs, including aeronautical and aerospace applications and
is facilitated and enhanced by the use of combinations of alloying elements, the most
effective of which is molybdenum (Cias n.d.). See alloy steel and tool steel.
Hardness scale: Graphs of measurements made by pressing a steel ball (Brinel test), a
diamond (Vickers test), or a diamond cone (Rockwell test) against a metal surface. The
diameter of the resulting impression is expressed by the reporting unit of kg/mm2. See oil
temper and Rockwell hardness test.
Hearth: Area in the bottom of a furnace, in which the bloom of iron or molten pig iron is
contained until removed by tongs or drained by tapping; often accompanied by liquid
Heat engine: Machine that utilizes heat energy from biomass fuels, which is then
converted to forceful motion (work), as, for example, in the form of steam under
pressure. The internal combustion engine is another form of heat engine that uses
combustion gases to do work. Heat engines either use biomass as fuel or the heat
generated by nuclear energy to power steam turbines and other machinery. See
biocatastrophe, industrial infrastructure, and prime mover.
Heat engine fuel shortage: The fundamental challenge of modern industrial society is to
find alternative energy sources for its industrial heat engines. New age ironmongers will
be smelting iron with renewable resources to make functional artifacts and art for creative
economies in the post-apocalypse. See infrastructure collapse.
Heat treatment: Modern steelmaking techniques include five major forms of high
treatment, many the results of centuries of ironworking. Thermal processing of ferrous
materials includes hot forging, quenching, tempering, annealing, and a variety of
additional heat treatment processes including, normalizing, spheroidization, and stress
relieving, all of which change their microstructure and, therefore, their properties. Rapid
cooling of austenized steel creates martensite, a high strength, easily fractured material,
rather than ferrite, cementite, and/or pearlite microstructures. For edge tool production,
martensite must be tempered in a range of 200º C to 500º C, precipitating and uniformly
distributing iron carbide particles (cementite) to relieve brittleness. Quenching and
tempering may involve modified techniques using two or more quenching media, such as
oil, water, or brine, e.g. austempering and martempering. See annealing, austempering,
cubic structure, martempering, temper, and martensite.
Helveman: Hammer man at a puddling furnace or finery.
Helve hammer: Traditional tool used by the bloomsmith in a water-powered bloomery
forge to shape the loup of wrought iron and expel excess slag and other contaminants.
First developed in Europe in late medieval forges in conjunction with the appearance of
blast furnaces, the helve hammer was traditionally made of wood with an iron hammer
head and was a component of most direct process bloomery forges, including those
operated in the US from the early North American colonial period to the beginning of the
20th century. In the 19th century, lighter weight tilt hammers with smaller beams operating
at higher speeds (400 strokes per minute) evolved from the more primitive helve hammer
designs. See Gordon (1996, 93) for an excellent illustration of a helve hammer.
Hematite: “Ore mineral (Fe2O3) containing 70% iron” (Gordon 1996), i.e. ferric oxide,
the most commonly mined ore in the U.S. Hematite is a common deposit at the bottom of
marshy ponds in its hydrated form, i.e. limonite (bog iron), and is a common component
in bedrocks of all ages.
High frequency induction furnace: Modern form of the electric furnace, in which a
high frequency alternating current is induced via a water-cooled copper core, producing
the heat for smelting the charge. They are used especially for high alloy steels, including
high speed tool steel, and for specialty production, such as marine hardware. See furnace
High impact hardness: Resistance of steels to fracture and deformation.
High pressure non-condensing steam engine: Improved, more efficient version of
Watts’ steam engine. Invented in 1790 by the American, Oliver Evans (1755 – 1819), it
represented a major innovation in heat engine design and played an important role in the
rapid industrialization of western economies and the rise of the factory system.
High-resolution transmission electron microscope: See HRTEM.
High speed tool steel: Alloy steel formerly made by the crucible process and more
recently manufactured in electric furnaces. High speed tool steels are differentiated from
alloy steels in the AISI classification system for steel as having a minimum alloy content
above 4%. Commonly used alloys characterizing high speed tool steels include tungsten,
vanadium, cobalt, chromium, manganese, and molybdenum. High speed steel-cutting
tools retain their hardness when heated to a red heat, whereas carbon steel cutting tools
lose their temper with cutting speeds above 20 to 30 linear feet per minute. Oil-hardened
tungsten steel can cut up to 200 to 300 linear feet per minute on a milling machine or
lathe without losing its temper. There are now hundreds of varieties of high speed tool
steel alloys used in manufacturing processes. See alloy, Appendix V, and steel, types of.
High strength low alloy (HSLA): A descriptive term for a modern type of steel that
provides better mechanical properties or greater resistance to corrosion than carbon steel.
HSLA steels vary from other steels in that they are not made to meet a specific chemical
composition but rather to specific mechanical properties (Wikipedia; March 2013).
History of Woodworking Tools: Definitive survey of the history of woodworking tools
by W. L. Goodman (1964) first published in 1964 and reprinted several times. This text
contains information about early tool forms (e.g. socket hole vs. shaft hole). Goodman
discusses woodworking tools dating as early as 2540 BC Egypt and has important
information on Roman and medieval forms, as well as illustrations from Moxon. Citing a
Russian archaeometallurgist, Goodman, has this comment on 11th and 12th century
carpenters’ tools found in a Russian late medieval horde: “Of 22 axes tested, 7 had a steel
tip welded over the iron base; in 7 others, the steel was inserted between the folded iron
of the head. Seven others were solid steel and one of iron throughout. In most cases, there
were signs of subsequent tempering, confined of course to the cutting edge” (Goodman
1964, Kolchin 1953).
Hollowware: Artifacts other than ordnance made at blast furnaces or cupola furnaces by
casting pig iron directly into molds e.g. kettles, fire backs, stove plates, anvils, etc. The
slitting mill cylinders used by the nail makers of Wareham, MA, and elsewhere were cast
in situ at the blast furnaces of Carver (Murdock 1937). See grey cast iron and molders.
Hogging: Bulk material removed by high speed tool steel cutting tools.
Homogenous transformation: Phase change transformation in which precipitation
occurs uniformly throughout the entire matrix, usually characterized by continuous
enlargement of initially small fluctuations within the supersaturated or undercooled solid
solution (Sinha 2003).
Hoop iron: Thin strips of malleable iron used to hold the staves of the coopers’ cask in
place; often made by the shipsmith, as well as the village blacksmith, from the North
American Colonial Era to the mid-19th century.
Horimono: Decoration of Japanese swords by the addition of ornate carvings or grooves
prior to the final polishing of the sword. See tsuchioki, yaki-ire, and yaki-modoshi
Horse power: One horse power is the lifting of 33,000 lbs. to a height of one foot in one
minute. The maximum horse power achieved by the editor of this glossary in unloading
hand tools from his truck after a buying trip to southern New England is approximately
1/40 horse power.
Horsing irons: Long-handled caulking irons used to seal the deck butts and garboard
seams of wooden ships.
Hot- and warm-forging: Strategy used by early Iron Age blacksmiths to forge edge
tools and swords by alternating the temperature of the steel being forged; especially used
by Damascus swordmakers working with high carbon Wootz steel to produce the
discontinuous patterns of the damascened sword by repetitive hammering. No
metallurgical analysis is yet available to indicate if New England edge toolmakers of the
late 18th to mid-19th centuries did or did not use this technique.
Hot blast: Developed in 1828 by Nielsen in England, cold air for the blast furnace was
preheated in a separate oven already heated by the waste gasses of the furnace. The hot
blast increased blast furnace temperature, slag fluidity, overall furnace efficiency, and
reduced fuel consumption. In the United States, the development of the hot blast furnace
encouraged the substitution of coal and coke for charcoal as a fuel, stimulating the
construction of larger, more efficient blast furnaces. In England and continental Europe,
the hot blast increased the efficiency of furnaces already using coke as a fuel. See blast
furnace and coke.
Hot forge: To carburize raw iron in a carbon-rich environment. See carburize and
Hot molding capacity: Essential characteristic of superplastic metals at high
temperatures in order to form complex shapes, accurately replicating essential industrial
molds, such as aircraft turbine blades. See mold and superplasticity.
Hot press: Technique of using dies to form self-welded molded steel or ceramic artifacts
under high pressure and temperature from atomized powders of ore-alloy mixtures.
Hot set: Chisel with a handle used to cut iron bar stock when at a bright red-orange color.
Hot short: Disintegration of hot steel during forging due to its contamination with liquid
iron sulfides from ore or fuel-derived sulfur. Iron sulfides are preferentially removed as
slag constituents by manganese-containing flux, as occurs with the addition of
spiegeleisen to cast iron or the natural occurrence of manganese in rock ore, eliminating
brittleness in steel at high temperatures. “When [metal is] unworkable at a welding heat it
is [said to be] hot short” (Brewington 1962, 15). See sulfur, phosphorus, and ferrosilicate.
Hot strength toughness: Ability of alloy steels to resist wear, abrasion, and brittleness.
Hot, round, and crowded: Also polluted, infected, genetically modified, hormonally
disrupted, incontinent, feminized/masculinized, unemployed, uninsured, uninformed,
manipulated, marginalized, indebted, disenfranchised, powerless – and angry: The tale of
the unfortunate decline of western finance capitalism market economies in the decimated
round-world commons of our giant integrated ecosystem (Brack 2010). See flat world.
Hot white heat: Temperature at which the breakdown of spheroidized carbide molecules
in high carbon steel occurs (< 1200º C); also, the normal temperature for forging low
carbon steels and malleable iron due to their higher melting points. The dissolution of the
cementite phase at white heat results in the embrittlement and weakening of the steel
microstructure, which will then crumble upon hammering.
Hot-work die steels: Modern alloy steels containing chromium, tungsten, and
molybdenum. These alloys are resistant to cracking and thermal shock during use in high
temperature die-forging applications. Hot-work die steels may be further hardened by
heating to a temperature of 1850º F, air- or oil-quenched, and then tempered. See alloy,
deep hardening, quench, and temper.
Hot working range: Temperatures at which iron maintains plasticity at or above its
crystallization temperature (700 – 1250° C), allowing it to be reshaped into various tool
forms. During hot working, including rolling or forging, the lattice structure of the metal
is simultaneously deformed and reformed with a tendency to form more uniform grain
structures. See eutectic, eutectoid, lattice structure, and critical temperature.
Hurricane Sandy: A powerful hurricane that devastated parts of New York City and
New Jersey in late 2012. Cataclysmic climate change-derived infrastructure collapse
Hydrate: To become combined with water, as in bog iron, a hydrated form of limonite.
See bog iron and hematite.
Hydraulic press: Press now used for manufacturing most drop-forged tools. The
hydraulic press squeezes instead of hammers metal into shapes, e.g. hammer heads, ax
heads, etc., utilizing two-piece dies often made of high carbon steel. Originally used for
drop-forging heavier castings, e.g. railway car axles. See die casting, die driving, dropforging, and die-sinking.
Hydrofracking: The recently expanded technology of deep well vertical, and then
horizontal, drilling for gas and oil in underground geologic deposits such as the Marcellus
Shale of eastern North America. Hydrofracking utilizes a complex mixture of toxic
lubricants to facilitate extraction contaminates large volumes of water in underground
aquifers, exacerbating the world water crisis. The prospect of the combustion of ever
increasing amounts of greenhouse gas producing nonrenewable biomass fuels assures the
prospect of cataclysmic climate change by accelerating global warming.
Hypereutectoid steel: Steel with carbon content above 0.83%, e.g. pearlite, with an
excess of cementite at grain boundaries, which makes it harder and more brittle than
Hypoeutectoid steel: Steel having less than 0.83% carbon content, i.e. less than the
eutectoid composition, characterized by an excess of ferrite at grain boundaries, giving it
the soft and ductile qualities of low carbon steel and malleable iron.
Ice cream: The eutectic (melting) point of ice cream is 32°. In a sense, it is similar to
steel, an iron carbon alloy with a much higher melting temperature than ice cream. Steel,
however, has a much wider range of melting temperatures due to its carbon content and
also a wider range of temperature gradients between its solid and liquid form. In between
the two temperatures, steel is mushy. Mushy ice cream would have a smaller temperature
range between its solid and liquid forms. When frozen to 400° below zero, ice cream has
something in common with martensite steel: it is hard and brittle and cannot be spooned
easily and it needs to be tempered to soften it up a bit. Severely frozen ice cream does not
lend itself to annealing; its re-crystallized lattice structure makes it unpleasant to ingest.
A final observation on this unfortunate metaphor: Ben and Jerry’s Chunky Monkey and
Cherry Garcia are the equivalents of various tool steels to which alloys have been added,
i.e. tungsten (cherries), manganese (chocolate chunks). These compare with soft serve
Dairy Queen style ice cream, just the basics, as with low carbon steel produced by the
Bessemer process, where all the interesting contaminants, some of which help make
convivial edge tools, e.g. silicon, have been burned out of the steel (Illich, 1973). Soft
serve can be made more palatable. Just add the hot fudge (manganese). See critical point,
eutectic, liquidus, martenizing, and solidus.
2200 1200 Iconography of tools: Depiction of tool forms
throughout history including in art, catalogs, and
Light yellow 1975 1080
reference books. The illustration of tool forms on wall
1830 1000 drawings in Egyptian pyramids and shaft furnaces and
blacksmith tools on Greek vases are early examples of
the consistent tendency to illustrate tool forms in art,
particularly in printed books after 1350. Also the
photographic depiction of tools. See Phenomenology of
Bright cherry 1450 790
tools, Diderot’s Encyclopedia, Moxon, pattern books,
History of woodworking tools, and Tools Teach: An
Iconography of American Hand Tools (Brack 2013).
Impact strength: Measurement of the ability of a metal
to withstand fracture under shock.
Impingement: The engulfing of carbide particles by
growing austenite crystals after they have first been
nucleated by an austenite crystal during the formation
Table 3. Temperature colors
of austenite (Paxton 1967, 10-1).
(Palmer 1937, 129)
Incandescent temperature colors: The colors used to
judge the hardness and forge-ability of steel from the early Iron Age to the mid-19th
century, when instrumentation became available to measure high temperature in heated
metals by measuring their expansion, e.g. pyrometers. The key color for the blacksmith
quenching hot iron to make steel is the cherry red heat (1375° F/750° C), which is the
minimum quenching temperature, or critical point, of steel. See critical point, edge tools,
Income disparities: The rapid growth in income disparities is a component of the
evolution of a global market economy and its prime mover, the Information Technology
Revolution. The extreme accumulation of wealth by the klepto-plutocracy (the 0.01%),
the robust accumulation of wealth by the opulent (the famous 1%), and the modest but
now declining wealth of the semi-affluent beneficiaries (the 10%) of America’s now
withering free enterprise system will not be sufficient to offset social unrest of the other
89% who suffer the consequences of income disparities and lack of public resources as
the Age of Biocatastrophe unfolds.
India iron: Iron first produced in southern India circa 1100 BC, followed by the
production of Wootz steel at a later undetermined date, but no later than 300 BC
(Srinivasan n.d.). The origins of iron and steel production in India appear to derive from a
combination of pre-Islamic Hindu and Islamic Indian metallurgical traditions.
Induction furnace: Form of the electric arc furnace in which the primary current is
carried by a coil of copper tubing circling the shell of the furnace, which generates a
strong secondary current in the charge of ore and flux, which is quickly heated by the
resistance to the secondary current. In electric arc welding, the same principle is utilized,
i.e. secondary currents result in the electric fusion of two pieces of metal being welded.
After slag skimming, discreet quantities of alloys can be added to create a variety of alloy
Induction hardening: Process for surface and localized hardening produced by the
heating of steel placed in a high frequency field (9,000 – 300,000 Hz) in an electric arc
furnace, where resistance to the creation of magnetic fields by eddy currents heats the
work piece (Pollack 1977). See electro fusion and induction furnace.
Industrial infrastructure: Interwoven technological grids of pyrotechnic society in the
age of global climate change, which include telecommunications, mass transportation, the
electrical grid, energy production and distribution, industrial manufacturing, consumer
product manufacturing and distribution, water resources and availability, oceanic
fisheries, and terrestrial food production and distribution. Hyper-digital information and
communication technologies increase the efficiency and productivity of the global
industrial infrastructure but also make it more vulnerable to a predatory shadow banking
network, cyber-terrorism, and natural events such as geomagnetic storms (solar flares)
and extreme weather. See biocatastrophe.
Industrial metallurgy: With respect to ferrous metallurgy, the development of bulk
process steelmaking technologies after 1870 characterized by the successful
implementation of the Bessemer pneumatic and Siemens open-hearth processes.
Infrastructure collapse: Anomalous, unplanned, unpredictable consequences of the
synergistic interaction of natural events (hurricanes, fire, earthquake, drought, sea level
rise, cataclysmic climate change, antibiotic resistant and viral infections, and
geomagnetic storms), and human activity (warfare, greenhouse gas emissions, resource
and ecosystem depletion, overpopulation, and the global transport of ecotoxins) with the
interwoven technological grids of a pyrotechnic society. The worst-case scenario for
infrastructure collapse will result from the impact of global biocatastrophe on the
interwoven technological grids of pyrotechnic society. See biocatastrophe, deforestation,
and industrial infrastructure.
Ingot iron: Modern form of highly refined iron with a very low carbon content produced
in open-hearth furnaces operating at very high temperatures, e.g. Armco iron, which has a
carbon content of only 0.015% (Baumeister 1958, 612-3).
Ingot: Cooled steel and iron castings derived from a cast iron mold after smelting. After
solidification, these castings are subsequently reheated for further mechanical and
thermal treatment by forging, rolling, or other forms of processing. See iron ingot.
Integrated circuit: The prime mover of the Age of Information and Communication
Technologies. An integrated circuit consists of a set of electronic circuits on one small
plate now characterized by millions of photolithographic transistors per mm2 of
microchip. Digital nanotechnology produces huge gains in the efficiency and productivity
of global consumer society. It is also the basis of the high speed electronic computerized
trading systems of a predatory shadow banking network. Born-again ironmongers and
back-to-the-land activists can, nonetheless, harness these technologies for their own
sustainable economies, the risk of psychic numbing notwithstanding.
Integrated ironworks: Indirect process, multi-purpose ironworks including a blast
furnace, refinery, chafery, and the multiple hearths of blacksmith/shipsmith forges. The
Saugus Ironworks historic site is an excellent reconstruction of an early colonial
integrated iron works.
Interdendritic shrinkage: Tendency of crystals in the microstructure of ferrous metals
to freeze in irregular patterns, leaving interstitial spaces within the lattice structure of the
metals. “… an alloy will rarely freeze with a smooth surface and even a pure metal will
reveal partially formed crystals” (Smith 1960, 128). See alloy, crystal structure, lattice
structure, and microstructure.
Internal combustion engine: Biomass devouring heat engine, which produces
combustion gasses to propel private passenger cars, commercial trucks, aircraft, merchant
shipping, and most railroads and mass transportation systems. See carbon footprint.
Internal stress: Residual stress within the lattice structure of a metal that remains after
thermal and mechanical treatments; relieved by tempering or annealing.
Interrupted quenches: “An interrupted quench is one which is not carried through to the
temperature at which transformation of austenite to martensite commences, but is
interrupted at some higher temperature, in order to suppress transformation of austenite
into pearlite and at the same time avoid formation of martensite. The quenching bath is
kept at a stated temperature appropriate to the formation of the microstructure which is
desired for the steel being treated” (Shrager 1949, 169). See austenite, bainite, martensite,
pearlite, and temper.
Interstitial: Solid solutions of iron carbon alloys in which atoms (e.g. carbon) occurring
within the empty spaces of the crystal lattice structure (e.g. ferrite) distort the structure.
Intuition: A critical component of the art of edge tool forging and swordsmithing prior to
the understanding of the chemical basis of ferrous metallurgy. Based especially on the
color and feel of the steel being forged and centuries of the empirical experience of
swordsmithing, cutlery and edge toolmaking, the collective experience and secret
formulas derived from the intuitive working of hot iron were called “kan” by the
Japanese swordsmith (Miyairi). See kan of the ironmonger and rule of thumb.
Iron: “A heavy malleable ductile magnetic silver-white metallic element that readily
rusts in moist air, occurs native in meteorites and combined in most igneous rocks, is the
most used of metals, and is vital to biological processes” (Merriam-Webster Dictionary
online 2008). Iron is the fourth most common element composing about 5% of the earth’s
crust. Iron has a melting point of 2793° F (1538° C) and is difficult to smelt in its pure
form, but when carburized (combined with carbon), it undergoes microstructural changes,
which increase its hardness. Malleable iron (0.02 – 0.5 % cc) becomes steel when its
carbon content range is 0.5 – 2.0%. If its carbon content reaches a range of 2.0 – 4.0%, it
becomes cast iron with a lower melting temperature of 2075° F (1149° C). Cast iron has a
wide variety of forms depending on variations in heat treatment and alloy content. See
carbon content of iron and steel, cast iron, malleable iron, and steel.
Iron Act: Act passed in 1750 by the English Parliament that prohibited the manufacture
of iron and steel tools, hardware, and artifacts in the American colonies. In part, this act
was a response to the Swedish export tax (1750) on charcoal iron, which resulted in an
increase in the importing of bar iron from the colonies to England after 1750. This Act
was never successfully implemented, and a robust North American colonial era iron
industry had already been established at the end of Queen Anne’s War and the Treaty of
Utrecht in 1713 (Bining 1933). The Iron Act played a key role in stimulating colonial
resentment of British rule, helping to lay the foundation for the coming revolution. See
Iron carbide: Alloy of strongly bonded iron and carbon atoms with various patterns of
carbon distribution; also, specifically cementite (Fe3C). The homogeneity or
heterogeneity of the carbon distribution pattern in iron tools, for example, determines the
characteristics of the tools as cast iron, low carbon steel, wrought iron, or crucible steel.
Iron carbide is not brittle at high temperatures. Rolling and forging can successfully break
up iron carbide networks, especially in high carbon steel being worked at temperatures
between 650º and 750º C, at which point the network is transformed into coarse iron
carbide particles visible to the naked eye as layered structures, as exemplified by the
damascened patterns on pattern-welded Wootz steel swords. See carbon content, crucible
steel, cementite, cast iron, Damascus sword, Wootz steel, and wrought iron.
Iron carbide networks: Essential components of the microstructure of ferrous metals at
certain temperatures. The formation of brittle iron carbide networks in high carbon steels
> 0.8% cc as a result of undercooling (interrupted cooling) or quenching (rapid cooling to
room temperature) is responsible for their low ductility and fracture vulnerability at room
temperature, in contrast to the plasticity of carbide networks formed at high temperatures.
The rate of cooling and undercooling determines the grain size of the microstructures
formed by the iron carbide networks and thus influences the mechanical properties of the
steel being produced. See carbon content of iron, microstructure, and microstructure
Iron-carbon constitutional diagram: “A constitutional diagram each point of which
represents the composition of steel or cast iron that is in equilibrium and that contains
only iron and carbon” (Shrager 1949, 368). See Appendix VI.
Iron cored: One of three ax-making techniques, known as the overcoat method, where
steel strips are wrapped and welded around an iron core, then forged into the desired
shape. While not listed in Pleiner’s (1980) sketch of knife-making strategies, this
contemporary ax-making technique may represent an additional early Iron Age strategy
for making knives and possibly edge tools. See ax-making techniques.
Iron-fuel contact: A perennial problem in older furnace designs prior to the development
of the reverbatory furnace by Henry Cort in 1784, which eliminated fuel to ore contact.
Earlier furnaces decarburizing cast iron or bloomeries producing wrought or malleable
iron ran the risk of recarburizing their iron by oxidation, as well as of contamination of
the iron by contact with unwanted products in the fuel, such as sulfur. See ferrosilicate,
finery, oxidation, puddling furnace, and reverbatory furnace.
Iron ingot: Common form of reprocessed cast iron, often produced in cupola furnaces as
the raw material for foundries and other special purpose furnaces. See malleable cast iron
and foundry. See ingot.
Iron mill: Forges, often rolling mills, that reprocessed the iron ingots derived from blast
furnaces and iron muck bars (bar stock) from bloomeries and puddling furnaces for
special purpose applications. This term applies to iron production before the era of bulk
process steel. See blast furnace, bloomery, and ingot.
Iron ore: Ore containing any of the iron oxide minerals magnetite (Fe3O4), hematite
(Fe2O3), or siderite (FeCO3), sometimes in various combinations. Iron ore also occurs as
the hydrated iron oxides goethite and limonite, as in the bog iron deposits of southeastern
Iron oxide: There are 16 known forms of iron oxide. In the smelting process, the most
important is ferrous oxide, a highly volatile form of iron oxide that easily ignites and
provides the spectacular fireworks displays seen in bulk process steel production. Iron
oxide is produced by the oxidation of iron through natural processes, as well as by
smelting. Ferrous oxide plays a major role in the decarburization of cast iron by
facilitating the reduction process and the removal of carbon. Another important form of
iron oxide is the iron ore magnetite (Fe3O4), which is formed when iron corrodes after
contact with water. See carbon content, cast iron, decarburization, iron ore, oxidization,
Iron Road: Famous trading route used from the early Iron Age to the late medieval era,
via which currency bars smelted in Austria (Styria and Carinthia, also called Noricum)
were transported by wagon north to Linz on the Danube River and then upstream to
portages linking Austria with the forges and swordsmiths of the lower Rhine region. This
latter area was particularly active as the Merovingian swordmaking center of the early
Frankish empires of the region (650 – 750 AD) and later during the German Renaissance.
See Celtic metallurgy, Halstadt, La Téne, and Spathas.
Iron sand smelting process: Process which makes use of self-fluxing, black sands from
the south shore of the Black Sea to produce iron and nickel steel, c. 1900 BC. This was
the first documented industrial production of iron and steel tools, which, ironically,
occurred at the height of the Bronze Age (Wertime 1980). Iron sands are also the source
of iron smelted by Japanese samurai swordmakers. Finely granulated iron sands are a key
link between the intentional use of rock ores and the late 20th century development of
powdered ferrous metallurgy, an industry which is dependent upon the availability of
finely granulated powdered iron. See Chalybean steel, flux, samurai swords, satetsu, and
Iron silicate: Along with ferrite, the principal component of wrought iron. It occurs as
glass-like slag and is present in wrought iron in amounts that vary from 1 to 3% by
weight. It is distributed in the wrought iron as highly visible threads or fibers, which run
in the direction of rolling (mechanical processing). “In well made wrought iron there may
be 250,000 or more of these glass-like slag fibers to each cross-sectional square inch. The
slag content occupies a considerably greater volume than a percentage by weight would
indicate, because the specific gravity of the slag is much lower than that of the iron based
metal” (Aston 1939, 2-3). The iron silicate content of wrought iron provides unique
qualities, especially resistance to corrosion and fatigue. The iron silicate content of early
forge welded hand tools explains their resistance to rusting in comparison to modern
drop-forged low carbon steel tools, which rust quickly when exposed to moisture. See
drop-forging and ferrite.
Iron-smelting furnace: Direct process shaft or bowl furnace used by bloomsmiths from
the early Iron Age until 1900 to produce wrought and malleable iron. Most such iron was
reprocessed by fineries and shaped by chaferies and rolling mills into forms compatible
with its intended use. This term could also apply, in the generic sense, to blast furnaces,
in contrast to melting furnaces, such as the cupola or reverbatory furnace. See furnace
Ironmonger: Ironworkers following the trades of the bloomsmith, shipsmith, edge
toolmaker, cutler, farrier, or community blacksmith. Ironmongers usually worked in
darkened environments, often at night, where the lack of sunlight allowed them to make
the critical judgment of whether the iron or steel tools they were forging or repairing
were ready for quenching, tempering, or other thermo-mechanical treatment, as shown by
the cherry red (1375º F) or other colors of iron and steel heated to appropriate
temperatures. For further commentary on ironmongers, see the On Ironmongers preface.
See born-again ironmonger, incandescent temperature colors, and kan of the ironmonger.
Isometric crystal forms of iron: Temperature dependent allotropic forms of iron, which
include alpha iron (ferrite) < 1670º F (910º C), gamma iron (austenite) 1670 - 2540º F
(910 - 1393º C), and delta ferrite > 2540º F (1393º C). The addition of alloying elements
other than carbon can change the temperature range of phase transformation.
Isothermal transformation diagram: Time temperature transformation (ttt) curves in
the form of diagrams that graphically illustrate the changes that occur when steel is
cooled at various rates. The diagram for eutectoid steel (Shrager 1949, 143) illustrates the
phenomenon that, at relative low temperatures (+/- 1000º F), the transformation of
austenite into martensite can take place in a matter of seconds. The first isothermal
transformation diagrams were formulated by Davenport and Bain in 1930. See critical
temperature and Appendix VI.
Isotropic: Materials having identical properties in all crystallographic formations, i.e.
their elastic forms are alike in all directions. See anisotropic and crystal structure.
Japanese samurai swords: Japanese swords are traditionally pattern-welded matrixes of
layered iron and steel, re-piled and reforged in elaborate rituals that often result in
hundreds of thousands or millions of steel strata. The heyday of samurai sword
production was the Kamakura era (1185 - 1392). Japanese swords had two basic forms:
banded steel jackets around a softer steel core and hard steel inserted between softer steel
plates. Smith (1960) has an extended discussion of Japanese swordmaking techniques in
A History of Metallography. National Public Television’s NOVA (October 2007) had an
excellent program on direct process smelting of the steel used for the samurai sword,
including a vivid depiction of the use of a breakdown furnace to produce the bloom of
raw steel. See natural steel and breakdown furnace.
Jominy end quench test: Standard test for determining the hardness of alloy steels after
quenching. A piece of machined steel 1” in diameter by 3 7/8” long is heated to a
quenching temperature, which is held for 20 minutes. Gradients in the cooling rate of the
steel rod produce associated gradients of hardness. See hardenability and tool steel.
Juanita charcoal iron: Highest quality direct process smelted wrought and malleable
iron bar stock produced in Pennsylvania in the 19th century; highly valued by Pittsburgh
producers of cast steel. See cast iron.
Kan of the ironmonger: Combination of ritual and empirical experience of the Japanese
swordsmith; a methodology of swordsmithing that was beyond words or written
language. Swordsmiths had their own individual technique for the forging of the sword
and learned their art under the tutelage of older swordsmiths. This intuitive rule of thumb
understanding of the mysteries of forging hot iron was also the key to the successful
production of Damascus, Viking, and Merovingian swords. Intuition and empirical
experience were also the keys to the success of New England’s edge toolmakers and
sword cutlers in the decades before science provided its academic explanations of phase
transformation kinetics. The kan of the ironmonger was intuitive in nature, a series of
moments of epiphany, a technical finesse beyond written language learned by years of the
trials, errors, and observations of the apprentice ironmonger working under the tutelage
of master ironmongers, who themselves worked within the legacy of millennia of hot iron
forging. See yaki-ire and yaki-modoshi.
Kentledge: Hardened blocks of pig iron used as ballast in coasting vessels and then
sometimes sold to fineries and foundries for further processing. See iron ingots and pig
Kera: Raw steel bloom produced in breakdown furnaces and used in Japanese samurai
sword production. See furnace types and Japanese samurai sword.
Keyword index for cascading Industrial Revolutions: Terminology that summarizes
key components of the cascading Industrial Revolutions (IR) of pyrotechnic industrial
society— IRI: steam (>1750), IRII: machines (> 1840), IRIII: steel (>1875), IRIV:
petrochemicals (>1900), IRV: science (>1945), IRVI: fiberoptics (>1995). The Age of
Biocatastrophe (>2011): the struggle for survival in the context of gross income
inequality. See cascading Industrial Revolutions.
Kill: “To remove dissolved gas in liquid steel so that it will not boil while solidifying”
(Gordon 1996, 309); a key step in the successful production of high quality cast steel. See
Killed steel: Steel held in the crucible until no more gas is emitted and the surface
appears “quiet;” a process that prevents blow holes and other structural anomalies (Spring
1917). When the steel in the crucible solidifies, uneven cooling causes shrinkage, which
then produces a central pipe in the crucible casting. See dozzle and pipe.
Kiln reduction process: Modern process for the smelting of sponge iron in a gas-fired
rotating kiln furnace, which is typically 150 feet long, 7.5 feet in internal diameter with a
fire brick wall about 8 inches thick. In the kiln reduction process, the iron being smelted
is moved slowly through the kiln by a conveyor and then dropped into a cooling kiln
located below the main kiln. Large quantities of sponge or wrought iron can be produced
by this method (Pollack 1977).
Kinetics: Study of the motion of bodies and the forces acting on them; with respect to
ferrous metallurgy, the study of the changes in the allotropic forms and microstructural
characteristics of iron alloys due to mechanical and thermal treatments and events. See
phase and phase transformation.
Klepto-plutocracy: An elite class of the top world income earners who maintain
economic and political control of a globalized market economy. In the US, the one
hundredth of one percent includes a minority of plutocrats, such as Bill Gates, who
redistribute much of their wealth for worthwhile social causes. The majority of the 0.01%
are klepto-plutocrats who obtain their wealth by the manipulation of banking, stocks, and
investment funds (e.g. the shadow banking network) or by the accumulation of wealth by
utilizing tax loopholes (e.g. the carried interest rate) and off-shore tax havens. America’s
klepto-plutocracy is made possible by lobbyists who can subvert congressional efforts to
ameliorate the federal tax codes, redirect sectarian political factions, such as tea party
crypto-fascists, and an Information Technology Revolution that promotes computerized
trading, media propaganda, massive structural unemployment, and the psychic numbness
of flat world technology. The resulting rapidly increasing income disparities, political
polarization and paralysis, and social inequities and unrest provides the context of and
challenges for the sustainable economies and social networks of the future. In the Age of
Klepto-plutocracy, finesse in the use of hand tools by ironmongers and other artisans will
provide the basis for alternative lifestyles and sustainable economies. The dynamics of
the Age of Round World Biocatastrophe will also impact the lifestyles of the kleptoplutocracy and techno-elite whose innovations and ingenuity are the prime movers of
their wealth, as well as the one hope of mitigating the impact of the unfolding Age of
Biocatastrophe. See biocatastrophe, flat world, income disparities, and shadow banking
Knife forms: There are five basic forms of knives, as described by Tylecote (1987, 269
after Pleiner 1969), which are derived from his excavations of central European
archeological sites over a period of several decades. These knife forms existed more or
less simultaneously in eastern, western, central, and European sites from the beginning of
the early Iron Age (Halstadt +/- 700 BC) until the late medieval period (1000-1500 AD).
The forms are: all iron knives, knives with carburized cutting edges, raw or natural steel
knives, sandwich pattern knives (the iron components of the knife are folded over the
steel cutting edge, the earliest known variation of welded steel construction), and patternwelded knives, where alternating layers of steel and sheet iron are welded together. The
last appears to be the most common knife form in archeological sites. See history of
woodworking tools and pattern-welding.
Knife makers’ steels: Traditionally, most knives and swords were pattern-welded
combinations of steel and wrought iron. Until the mid-19th century the chemistry and
alloy content of knife makers’ steels were unknown. Appendix VII reproduces Latham’s
(1973) listing of popular knife makers’ steels. The carbon content of these steels
generally ranges from 0.85 to 1.5% cc. The wide variation in alloy content of these steels
illustrates the complexity and diversity of the alloy content of steels used by knife and
swordmakers, as well as edge toolmakers. The high chromium and molybdenum content
of many of these steels illustrates the important contemporary role of alloys as additives
to knife makers’ steels. For knife and sword makers working before 1850, the presence of
significant alloys, such as manganese and silicon, may have been known through
practical “rule of thumb” use of ores containing these compounds. After the development
of modern chemistry in the late 19th century, alloys with precise combinations of
additives were produced for specific types of knives, cutlery, and edge tools.
Knobbler: Bar maker at a finery who made anconies. The name derives from the fact
that most anconies had a knob at the end to facilitate ease of movement. See ancony.
Lamellae: With respect to the crystal structure of steel, the plate-like structures that
characterize pearlite. During the slow cooling of austenite, identical pairs of lamellae are
formed by the process of twinning, creating pearlite, a form of steel with a more distorted
crystal structure than that contained in tempered martensite. See austenite, bainite,
cementite, laminae, martensite, Neumann bands, pearlite, and twinning.
Lamellar family of structures: The unique lath-like microstructure formed by the slow
cooling of austenite. If heated to 1400º F (760º C), austenite with a carbon content
ranging from 0.7 - 0.9% consists of polyhedral grains, which, when slowly cooled, revert
to lamellar structures of ferrite and carbide (pearlite). Interrupted cooling results in the
wide variety of lamellar structures called bainite. Increasing the rates of cooling increases
the hardness of the steels formed while lowering the temperature of phase transformation
(Bain 1939, 25). A higher carbon content results in a change in the fine-grained lamellar
structure to increasing coarseness. During rapid cooling, lamellar transformations are
halted at 1000º F (550º C) until the temperature falls below 100º C (200º F), at which
time martensite is formed (Bain 1939, 25-8). See bainite and pearlite.
Lamellar pearlite: “Pearlite crystals covered by a thick layer of cementite” (Shrager
Laminae: With respect to gunsmithing and swordmaking, the patterns resulting from the
piling and forging of alternating layers of steel and iron strips and plates, which form the
composition of the pattern-welded gun barrel or sword. See damascene, gunsmithing,
piling, pattern-welding, and gun barrel iron.
Laminar cementite: Lath-like formation of slowly cooled cementite. Another variation
in what Bain (1939) called the “lamellar family of structures.” See Levin (2005).
Laminated structure: Alternate layers of different allotropic forms of iron, such as the
alternating layers of ferrite and cementite that constitute pearlite.
Laminating: Early Iron Age technique of knife-making characterized by pattern-welded
layers of sheet iron or sheet steel with varying carbon content, as exemplified by
Egyptian knives dating from 900 – 800 BC, as well as an adz from the same period.
Laminating is a frequently used technique for steeling edge tools by the lamination of
steel on the underside of the tool. See Wertime (1980, 120), knife forms, and patternwelding.
Lap riveting: Riveting of overlapped sheets of iron and steel in boiler-making and iron
and steel shipbuilding.
Lapping machine: Machine with cast iron disks having lapping compounds imbedded in
the disk; used especially for fine surface finishes on the back of edge tools prior to final
Lap weld: To weld pipe so that the skelped pipe edges are beveled, overlapped, and
welded together; a variation of scarf welding. See scarf weld and skelp.
La Téne: Village and ritual site on the edge of Lake Neuchâtel in Switzerland. The tools
uncovered at La Téne reflect both a western movement of Celtiberic metallurgists and the
evolution of a more war-like culture than Halstadt. Iron axles made their first appearance
in Europe in warrior burials at La Téne. See Halstadt and natural steel.
Lattice bending: Bending that results from the random application of stress on the lattice
structure of metals, producing distortion patterns that lack crystallographic regularity
(Barrett 1943, 307). See plastic deformation, cubic structure, and space lattice.
Lattice reorientation: Lattice reorientation of the crystal structure, of iron for example,
occurs by three processes: uniform rotation of the crystals, bending of the lattices
between planes of slip, and division of crystals into deformation bands “within which the
lattice rotates in different directions” (Barrett 1943, 347-48). Heating and cooling are the
principal causes of rapid lattice reorientation (slip); cold working is the principal cause of
slow lattice reorientation (creep). See plastic deformation, slip, and creep.
Lattice structure: Crystal structure of the unit cells of metals. See allotropic forms of
iron, crystallography of ferrous metals, cubic structure, unit cell, lattice reorientation,
plastic deformation, and space lattice.
Ledeburite: Cast iron containing 4.3% carbon in the form of the eutectic mixture of
austenite and cementite. The austenite in ledeburite may transform to ferrite and
cementite during cooling.
Leg vise: Special form of vise characterized by a 3” to 8” wide jaw taper mounted on an
iron leg with a bar spring mechanism. The presence of the leg vise, anvil, and associated
hand tools characterized blacksmith forges and farm workshops where toolmaking and
repair occurred. Leg vises can be traced back to Roman smithies and are illustrated in
Diderot’s Encyclopedia ([1751-75] 1959) and in English pattern books. Most leg vises
recovered from New England workshops appear to be domestically produced and are
often hand-forged, wrought steel, often one-of-a-kind creations of local workshops.
Leonard, James: An English ironmonger who migrated to the Massachusetts Bay
Colony during the great migration and worked briefly at the Braintree Ironworks
(Furnace Brook) before moving to Taunton, Massachusetts, and establishing his forge on
the Two Mile River in 1652. With his brother, Henry, his son, Nathan, and many other
members of his family, James was instrumental in establishing a vast network of bogiron-smelting furnaces and forges from Rowley in northeastern Massachusetts to New
Haven, Connecticut. Many of these forges were still operating in the first few decades of
the 19th century. The Leonard clan played a major role in supplying New England
shipsmiths and toolmakers with domestically produced direct process smelted iron bar
Lime as flux: Lime was used extensively to remove phosphorous from iron. By 1878,
Sidney Gilchrest Thomas had elucidated the chemical basis for its usefulness as a slag
constituent and as a furnace lining. See acid process, basic steel, flux, and limestone.
Lime boil: Violent reaction occurring during the basic open-hearth process when carbon
dioxide gas is released from the limestone on the hearth floor. See furnace types and
Limestone: Stone used as a flux in iron-smelting after 1600; used specifically as a flux
for high phosphorous iron ores after 1878. The calcium content of limestone greatly
reduced the iron content of blast furnace slag, allowing recovery of 90% or more of the
iron being smelted. See acid process, basic process, and lime as flux.
Limonite: Bog iron; also “all forms of hydrous sesqui-oxides of iron” (OED 1975, 1629).
“Impure form of goethite containing a variable amount of water” (Gordon 1996, 309).
Limonite is mined from bogs and heated to evaporate water, a principal source of iron for
bloomeries and blast furnaces in the American colonies, especially in southeastern
Massachusetts and the pine barrens of New Jersey. See bloomery and bog iron.
Liquidus: “The upper curve in a constitutional diagram, which is the locus of
temperatures at which each alloy starts to solidify” (Shrager 1949, 370). See
Barraclough’s constitutional diagram in Appendix VI.
London spring steel: A common trademark on Henry Disston’s highest quality hand
saws, London spring steel is cast steel rolled into sheets. Disston used English cast steel
to manufacture many of his saws until the 1880s, even though excellent cast steel was
being produced in Pittsburg, PA after 1850. See spring steel.
Lost wax process: Ancient method of casting that utilizes wax patterns for molds, which
are then destroyed by the casting process; particularly useful for precision casting, such
as in jewelry making. The use of the lost wax process has been widely adopted by
contemporary jewelers and artisans. See cire perdu.
Loup: Synonymous with “bloom,” as in the “bloom” or “loup” of iron produced in the
smelting process. See bloom, bloomery, direct process, and reduction.
Low carbon cast iron: Cast iron produced in air furnaces as white cast iron for the
manufacture of malleable cast iron; contains about 20% less carbon than grey cast iron.
See cast iron and grey cast iron.
Low ductility of high carbon steel: A characteristic of high carbon steel that has been
cooled from high temperatures to intermediate temperatures. Its low ductility is a result of
the formation of brittle iron carbide networks, as in the case of martensite shearing. At
room temperatures, such high carbon steel is subject to cracking due to embrittlement
before annealing or other thermal treatments reduce microstructural stresses. See carbon
content of iron, martensite, shear steel, and sheering stress.
Machinability: The ease with which alloy steel and malleableized cast iron may be
machined. Water-hardened alloy steels and malleableized cast iron have the best
Machine: Apparatus for applying mechanical power, consisting of a number of
mechanical parts, each having a definite function. Machines are often powered by heat
engines. See simple machines, turbine, and heat engine.
Machine steel: A modern form of “low carbon steel,” usually with 0.08 - 0.2% carbon
content but without the slag content of malleable iron; frequently drop-forged in dies to
be made into hand tools other than edge tools; often subject to additional carburization,
usually by case hardening. See carbon content of ferrous materials, low carbon steel,
malleable iron, and case hardening.
Macro-etch: To treat the surface of a sword, for example, by a reagent, for the purpose
of determining the quality of metal by analysis of the flow patterns that reveal the
structural differences characteristic of the iron and steel used to fabricate the sword by
pattern-welding. See Damascene, Japanese sword, and reagent.
Magdalenberg: Important early Iron Age metalworking site in Austria, located in
Carinthia, near Styria and Erzberg (Ore Mountain); the location of many shaft furnaces
and the probable production site of malleable iron and natural steel tools and weapons.
Magnetite: “Magnetic mineral (Fe3O4) containing 72% iron; the active ingredient in
‘lodestone’” (Gordon 1996, 310). While hematite (Fe2O3) is the world’s most common
form of iron ore, magnetite is the primary source of tool steel for edge tools and industrial
alloy steel products of all kinds. Among the world’s most important historic sources of
magnetite are the low-sulfur, low-phosphorus rock ores of northern Sweden, which were
used to supply the steel manufactories of Sheffield. Swedish magnetite-derived wrought
iron bar stock was an important transatlantic trade commodity and was imported to the
United States in large quantities throughout the 18th and 19th centuries for American edge
Mainspring: Apparatus that replaced weights as a method of powering clocks. They first
appeared in Germany in 1550 and became widely used in the florescence of German
clock-making from 1550 to 1634 and in England and Holland after 1650, when the
German industry began to decline. The search for higher quality steel for mainspring
production led Benjamin Huntsman to readapt crucible steel manufacturing techniques
for his Sheffield clock and watch spring business in 1742. See cast steel 1).
Male die: Upper die, also called a “force,” made of steel, cast iron, or copper by a drop
press in a machine shop or by a toolmaker, rather than by a die-sinker. A heated pattern
blank is used to shape the male die by the drop press. The die is then hardened and
tempered, making a reproduction of the pattern model. See female die.
Malignant tool dependency (MTD): Generally progressive condition ultimately linked
to universal acquisition disorder, familiarly known as the collector’s disease. As with
other degenerative obsessive-compulsive conditions, MTD can deepen to the extent that
the gathering of tools far exceeds need, either for use or profit. First state MTD can begin
before formal schooling and may lead to a morbid late stage that can create a broadly
negative presence in the subject’s life (hoarding). Symptoms are numerous and varied,
often well hidden behind an apparently rational barricade. Destructive patterns can
continue long after corrective resolutions are made. There is no permanent cure
(McLaughlin, David 2008, Liberty Salvage Co., personal communication).
Malleability: Relative ability of a material to be permanently deformed by rolling,
casting, forging, extruding, etc. without fracturing and without developing increased
resistance as it is deformed. Malleability usually increases when temperature increases.
Wrought iron, gold, silver, aluminum, copper, and magnesium are malleable metals. See
ductility, plastic deformation, and malleable iron.
Malleable casting: Malleable cast iron having some of the properties of wrought iron;
derived from annealed cast iron by a process that involves the cleaning of the cast iron by
pickling, followed by its stacking within the annealing oven after being covered with
millscale or other forms of iron oxide. Rapid heating is followed by very slow cooling,
which produces an iron that is resistant to damage by sudden shock and often
machinable. See annealing, casting, and malleable cast iron.
Malleable cast iron: Cast iron, characterized by the predominance of free carbon in the
form of graphite flakes made by the rapid cooling of white cast iron or from heat-treated
grey cast iron. The most common and commercially useful form of cast iron because it is
durable, strong, shock resistant, malleable, and machinable, its fracture and color express
its metallurgical composition. Malleable cast iron is made in two forms: whiteheart and
blackheart, which are differentiated by the processes used to anneal them and by their
chemical composition (Spring 1917). White cast iron containing chemically bound
graphite is unsuitable for making malleable cast iron until it is melted and annealed,
freeing the bound graphite in the form of temper carbon, which softens the microstructure
of the cast iron, allowing it to withstand distortion without breaking. Malleable cast iron
is also produced in cupola air furnaces as pearlitic malleable cast iron, particularly useful
for drop-forging hand tools, where shorter annealing times result in greater strength and
wear resistance. Knight (1877) provides this definition: “Iron cast from the pig into any
desired shape, and afterwards rendered malleable, or partially so, by annealing. A great
variety of articles such as bridle-bits, snuffers, parts of locks, various forms of builders’
and domestic hardware, some kinds of culinary and other vessels, pokers, tongs, and
numerous other things can thus be produced in a more economical and correct manner
than they could be by forging. Many of these are subsequently case hardened and
polished. The art of softening cast iron and working it, and afterward hardening it again.
[italics added] ...The inventor of the process of rendering articles of cast-iron malleable
was Samuel Lucas of Sheffield, by whom it was patented in 1804” (Knight 1877, 137677). First produced commercially in the United States by Seth Boyden in Newark, NJ, in
1831, with various alloy combinations and heat treatments, malleable cast iron has been
used to manufacture an endless variety of hardware and utensils. Writing in France in
1722, R.A.F. de Réaumur also describes this process. The widespread production of
malleable cast iron tools in the 3rd and 4th century BC in China has also been noted
(Needham 1958, Barraclough 1984). See annealing, grey cast iron, and temper carbon.
Malleable iron: Nineteenth century term for iron having a slightly higher carbon content
(0.08 - 0.5% carbon) than wrought iron (< 0.08% carbon content), now commonly
referred to as “low carbon steel.” However, unlike low carbon steel, malleable iron
contains variable amounts of silicon slag (more if smelted by a bloomsmith, less if
refined in a puddling furnace from decarburized cast iron), as well as manganese,
phosphorous, and sulfur. Silicon, manganese, and phosphorous can add beneficial
qualities in tools being produced from malleable iron. Silicon enhances the ductility and
durability of malleable iron, and manganese enhances strength. In small quantities,
phosphorous increases hardness and has a useful role in nail making. Sulfur has no useful
function in any metallurgical context. Malleable iron will harden slightly when suddenly
cooled. Siliceous slag-bearing malleable iron was produced as a “bloom” or “loup” in
direct process bloomeries. Iron with low slag content was produced in indirect process
puddling furnaces from pig iron. Malleable iron containing significant levels of silicon is
not suitable for production of tool steel alloys. The silicon content of malleable iron
played an important, but unrecognized, role in the forge welding of hand tools, including
edge tools, in the era preceding bulk process steel and machine drop-forging. The
confusion between very low carbon wrought iron and relatively low carbon malleable
iron continues, the latter being frequently referred to as wrought iron, while having the
same carbon content as modern “low carbon steel.” See carbon content of iron, Bessemer
process, mild steel, and low carbon steel.
Malleableizing: Annealing of white cast iron for the purpose of changing chemically
combined carbon to temper carbon, creating malleable cast iron that is less brittle, more
durable, and more machinable than gray or white cast irons. See malleable cast iron and
Manganese: Metallic element Mn, often appearing in its oxide form in ores. Manganese
is an important constituent in steel alloys (+/- 0.2%). It dissolves in ferrite, hardens and
toughens it, serves as a deoxidizer, increases elasticity, and causes carbon to stay in
combined forms as hardened steel. Manganese retards austenite transformation,
neutralizes phosphorous, and also makes iron non-magnetic. It makes tool steel easier to
hot roll or forge and increases the penetration of hardness during quenching. Water
quenching of manganese alloy steels tends to make them too brittle for most applications.
Historically, the manganese content of iron ore played an important role in natural steel
production by lowering the melting temperature of slag, thus facilitating carbon uptake in
a bloom of iron. The manganese would become part of the flux, preferentially combining
with contaminants such as sulfur and phosphorous, which were removed when the slag
was drained off of the bloom. As a constituent of cast iron, manganese played a similar
role in the production of German steel. When the cast iron was fined, the manganese
preferentially absorbed the sulfur, which was removed as slag. Uniformity of carbon
distribution was facilitated, but only in fined cast iron containing the manganese. In the
19th century, the chemical basis of the role of manganese became known, and the addition
of ferromanganese to the smelting process was the key to the success of Bessemer steel.
It is also used in the modern production of rifle barrels with tough hardened cores.
Siderite is the only naturally occurring iron ore containing manganese; notable siderite
deposits of historical importance were located in the Erzberg (Ore Mountain) section of
Austria (Noricum) and in the Weald (Sussex) and Weardale sections of England.
Manganese is also a constituent of bog iron. See German steel, Mushet, Robert F., Weald
of Sussex, Noricum, steel, and alloy steel.
Manganese oxide: Important replacement for iron oxide during the fining
(decarburization) of cast iron into steel, as in the puddling furnace. Manganese oxide has
a lower melting temperature than iron oxide as a slag constituent and facilitates uniform
carbon distribution during steel production (Barraclough, 1984b, 91-106). See
decarburization, manganese, and puddling furnace.
Manganese steel: In its modern form, an alloy steel containing 11 to 14% manganese
and 1.0% carbon. It is used for safes, steam shovels, and other applications requiring high
wear resistance. It cannot be machined or softened by annealing but is made somewhat
softer and less brittle by quenching, the very reverse of the usual steel treatment process.
See alloy steel, spathic ore, and spiegeleisen.
Manganiferous iron ores: Iron ores containing manganese.
Maraging steel: Modern carbon-free steel containing an iron-nickel martensite structure,
which becomes hard and tough with aging and/or heat treatment after initially being
ductile, malleable, and, thus, machinable. The high nickel content of maraging steels (18
– 25%) results in exceptional hardness and high resistance to stress corrosion (Pollack
Marriage of psychiatry with pharmaceuticals: Can ironmongers avoid ADHD, PTSD,
depression, anxiety, psychoses by wielding their instruments of manual operation?
Assault rifles anyone? See for-profit mental illness.
Martemper: To quench in molten salt at temperature slightly above the critical
temperature to produce a fully martensitic structure in a uniform nearly stress-free
Martenize: To form a hard, brittle, allotropic form of steel by the rapid cooling
(quenching) of austenite. Martensite formation begins at a temperature of 220º C and
below and contrasts with the formation of ferrite-pearlite microstructures from the slow
cooling of austenite, which begins at 1000º C, or the wide variety of microstructures
(bainite) formed by halting cooling and holding the metal alloy being cooled at
temperatures between 1000º C and 220º C for various time periods. See allotropic forms
of iron and austenite.
Martensite: “Martensite is considered to be a super saturated solid solution of carbon in
ferrite; it is the hardest, strongest, and least ductile form of steel” (Shrager 1949, 141).
Hard, brittle steel with various distorted microstructures determined by the range of
carbon content and distribution, martensite is formed by rapid displacive transformation,
rather than slower diffusive transformations. The microstructures are lath-like in low
carbon steels and plate-like in high carbon steels. Derived from the rapid cooling
(quenching) of austenite, tempering will alleviate brittleness and restore ductility and,
therefore, usefulness in edge tool production. Martensite forms at lower temperatures
than pearlite, which is prevented from forming by the rapid cooling of austenite. It has an
unstable body-centered tetragonal structure differing from austenite and ferrite only in its
axial ratio, which is determined by carbon content. Martensite is formed rapidly (0.002
seconds) when austenite is cooled below 240˚ C and has a needle-like crystallographic
structure, with no diffusion into particles of cementite. During the tempering of
martensite, carbon is diffused into finely dispersed particles of cementite by a decrease in
its crystal structure axial ratio. Martensite can be considered an intermediate step in the
transformation of austenite to ferrite (Barrett 1943, 478). See austenite, cementite,
martensite, microstructure, quench, and temper.
Martensite shearing: In contrast to the diffusion of carbon during the tempering of
martensite to produce malleable, ductile steel, martensite shearing is the result of a
combination of the presence of alloys such as cobalt, vanadium, manganese, silicon,
chromium, and tungsten and heat treatment processes. These processes result in
formation of tangential stresses that change the angle between the face and the length of
the diagonal of the microstructure of the alloy steel being heat treated, creating stressed
(super hard) microstructures. Martensite shearing is characteristic of the phase
transformation processes (kinetics), which result in the production of modern hardened
steels. See alloy, microstructure, stress, and temper.
Martensite tempering: At temperatures between 220 and 450º C, some of the carbon
leaves the martensite crystal structure and precipitates as carbides, leaving behind pure
alpha iron ferrite, which provides more ductility as a component of martensite-ferritebainite microstructures. The tempering time to produce the complex microstructures that
include bainite varies from ½ to 8 hours. After longer tempering times, pearlite structures
begin appearing and dominate the microstructure complex (Pollack 1977). See the phase
transformation diagrams in Appendix VI.
Martensitic transformation: “The coherent formation of one phase from another
without change in composition by a diffusionless, homogenous lattice shear” (Petty 1970,
Mass spectrometry: “…an analytical technique used to measure the mass-to-charge ratio
of ions. It is most generally used to find the composition of a physical sample by
generating a mass spectrum representing the masses of sample components. The mass
spectrum is measured by a mass spectrometer” (Wikipedia 2008). Mass spectrometry is
the characteristic measurement method used in all forms of electron microscopes. See
electron microscope, TEM, REM, SEM, and HRTEM.
Matchlock: Device used to ignite a firearm; term used to describe some early firearms.
The earliest form of a handgun was the arquebus using a simple serpentine matchlock
ignition system. Some early muskets also used matchlock ignition systems. Matchlocks
were unwieldy and unreliable and required a source of fire, such as a lit match, which
would reveal the position of the gunner to his adversaries prior to the firing of the
weapon. Nearly useless during rainstorms and inclement weather, the matchlock was
always made of folded and forged strips of wrought iron. The battle of Saco, Maine,
1607, is a landmark event in American history, during which Micmac Indians, supplied
by French traders, made first use of firearms in the form of matchlocks in a pitched battle
defeating the Abenaki community during the fur trade wars. See the Davistown Museum
publication Norumbega Reconsidered Appendices D and E (Brack 2006), arquebus,
flintlock, wheellock, gun barrel iron, and gunsmithing.
Maximum permissible forging temperature (MPFT): Ranging from 1300° C for low
carbon wrought iron, the MPFT declines with increasing carbon content, reaching
approximately 1100° C for steel containing 1.2% carbon. Steel containing more than
1.5% carbon is “virtually unforgeable” (Barraclough 1984a, 5). See forging, incandescent
temperature colors, steeling, and quenching threshold.
Mechanical properties of metals: Properties that determine the ability of a metal to
withstand force without tearing, bending, or fracturing. See compressive strength, tensile
strength, toughness, brittleness, malleability, ductility, impact strength, fatigue, elastic
limit, and creep.
Mechanical working: The shaping of metal by hammering, rolling, pressing, punching,
bending, or drawing to change its form. These processes may also change the metal’s
physical properties, i.e. its crystallographic structure. The fabrication of armor by a
combination of cold hammering and heat treatment is the classic example of medieval era
thermo-mechanical working of iron and steel. See lattice structure, cold forging, and cold
Melting furnace: Furnace used to re-melt smelted iron prior to its specific-purpose use.
Fineries, chaferies, and cupola and puddling furnaces are all examples of early modern
melting furnaces common before the advent of bulk process steel technology.
Melting points of iron and steel: See temperature range for melting iron and steel.
Merchant bar: High quality wrought iron bar stock re-processed in fineries by piling,
reheating, and re-rolling bloomery-derived bar stock or puddling-furnace-derived muck
bar. See ancony, bar stock, bloomery, chafery, finery, and muck bar.
Mercury: Chemical element in the periodic table with the atomic number 80 and the
symbol Hg. Mercury is one of five elements that are liquid at or near room temperature.
Mercury is among the most toxic of all forms of biologically significant chemical fallout
(BSCF). With respect to ferrous metallurgy, its importance lies in the large amount of
mercury released through the burning of coal, the smelting of iron, and the production of
steel. Harmless in its naturally occurring form (mercuric sulfide), it undergoes
transformation through bacterial action into highly toxic methylmercury, which is readily
absorbed by living organisms and is easily transported in pathways to human
consumption. Increasing rates of the cross placental transfer of methylmercury from
mother to child has been documented in the late 20th century. Widespread contamination
of fresh water and food products, including some farm-raised fish, may play a much more
important role in the rising rates of autism in children than methylmercury contamination
from specific source points, such as thimerosal, the antiseptic/antifungal once commonly
used in children’s vaccinations. Mercury is one of many skeletons in the closet of the
pyrotechnic society. See BSCF, pyrotechnology, biocatastrophe, and infrastructure
Merovingian swords: Swords produced by Celtic metallurgists for the Frankish
kingdoms preceding and during the reign of Charlemagne. Merovingian pattern-welded
swords were famed for the quality of their steel and their artistic beauty. Predecessors of
the later Viking all steel swords, Merovingian swords represent the high point of Celtic
metallurgy, which utilized the natural steel produced in Noricum and transported down
the Iron Road and then upstream on the Danube River to a portage west of Nuremberg.
This portage linked the smelting furnaces of ancient Noricum to the metal smithing
centers of the lower Rhine, supplying the famed swordsmiths of the Merovingian era.
Metal cutting technologies: Technologies for cutting metals developed on a parallel
track with welding methods, often using the same tools. Early cutting was done with
chisels, often on material hot from the forge, using a hot chisel or hot set, the sledge
hammer version of a hot chisel. Cold cutting with a cold chisel or cold set had endless
applications, often in tasks involving light gauge materials, such as in the manufacture of
armor. Armorers would have made good use of oxy-acetylene torches for both welding
and cutting, but they were not available until toward the end of the 19th century. So called
cutting torches and their heavier relative the oxygen lance use the principle of rapid
oxidation of ferrous material through the cut line, quite different than the removal of
chips in the path of a tool, such as in a lathe-based system or even with a hacksaw.
Handheld hacksaws were known to be used in medieval times, eventually leading to
horizontal and vertical band saws that use endless blades usually of bimetallic
construction. Tungsten carbide-tipped circular saw blades produce accurate cuts when
mounted on stationary and portable machines. These are distantly related to abrasive cutoff systems that use circular blades, which grind through material and are consumed in
the process. Other contemporary strategies involve an electric arc, as in the plasma arc
machines now common in many shops, and some do not, as in the abrasive waterjet
system, which will cut almost any material in addition to all metals (McLaughlin, David
2008, Liberty Salvage Co., personal communication).
Metallofullerene: A customizable metal-matrix composite consisting of self-replicating
homochiral chains that allow for superior flexibility and resilience, high strength and
durability, and an extremely low coefficient of friction. It also may be used in the realm
of microRNA, the next step in pharmaceuticals
Metallographic analyses: Analysis of metals to determine their microstructure,
including wrought iron, steel, and cast iron. The five principal techniques of
metallographic analysis are: etching of metal surfaces with potassium bi-chromate,
observation and photography of crystal structures by the optical microscope,
spectrographic analysis, x-ray diffraction analysis, and x-ray fluorescence analysis. See
Metallography: The study of the structure of metals and alloys and the properties that
derive from their thermal and mechanical processing. As a science, metallography lagged
several centuries behind the technological development of early modern steelmaking
techniques (blister steel, 1685; crucible steel, 1742). Henry Clifton Sorby’s pioneering
microscopic analysis of the structure of metals did not receive widespread attention until
1882. See blister steel, crucible steel, microscope, microstructure, and Sorby, Henry
Metalloids: Non-ferrous constituents of cast iron and steel up to 25% in volume, e.g.
carbon in cast iron in the range of 2.2% – 5.0%; also silicon, sulfur, phosphorous,
manganese, etc. Metalloid alloys in cast iron and tool steel, such as manganese,
chromium, nickel, and other metals, radically change the microstructure and, thus, the
appropriate function of the cast iron or tool steel being produced. See alloy, alloy steels
and alloy cast irons, cast iron, Chalibean steel, manganese, and silicon.
Metallurgy: “The art and science of extracting metals from their ores and other metalbearing products and adapting these metals for human utilization” (Shrager 1949, 371).
Metalworker: A modern generic term for ironmongers of all types: blacksmith,
bladesmith, gunsmith, founder, etc.
Metaphor: A figure of speech. Microstructural deformation, stress field, slip
interference, fracture, strain hardening, creep embrittlement, internal stress, interrupted
quenches, lattice bindings, martensite shearing, overheating, and grain displacement are
all metaphors for a global consumer society in crisis.
Metastable: Term describing any process that is characterized by rapid transformation,
as in the rapid transformation of austenite to martensite (nearly instantaneous, but within
a critical cooling rate of 80 seconds or less from 1000º C to +/- 200º C).
Methylmercury: Product of bacterial action on elemental mercury in the form of
mercuric sulfide after its release by coal and coke-fired blast and steel furnaces and
electric power plants. Methylmercury is one of the most potent and biologically
significant ecotoxins in the repertoire of the global contaminant pulse. It is the skeleton in
the closet of a pyrotechnic society that uses biomass to fuel its heat engines. See mercury,
biocatastrophe, infrastructure collapse, and post-apocalypse society.
Micrographs: Data produced by optical and electron microscopes during metallurgical
analysis, initially in the form of photomicrographs and, after the invention of electron
microscopes, by x-ray diffraction measurements of the microstructure of metals. See
electron microscope, TEM, HRTEM, REM, and SEM.
Microscope: A tool utilizing one or more glass lenses to view objects too small to be
seen by the naked eye. The invention of the microscope was the first technological
innovation allowing analysis of the crystal structure of metals. First developed in the
Netherlands in the early 17th century, microscopes were initially used to investigate the
structure of biological materials. Henry Clifton Sorby (b. 1826, d. 1908) inaugurated the
science of metallography with his etching and microscopic analysis of sectional slices of
various ferrous metals (wrought iron, cast iron, Bessemer steel, blister steel, decarburized
cast iron, spiegeleisen) (Smith 1960, 173). See electron microscope, HRTEM, optical
microscope, and Sorby, Henry Clifton.
Microstructures: In ferrous metallurgy, an almost infinite variety of the morphologies of
the crystal structures in the various phases of the carbon iron system, resulting from the
thermal and mechanical treatment of steel and iron. Microstructures can be observed by
optical and electron microscopes. Microstructure determines the forms and properties
and, ultimately, the uses of iron and steel. See annealing, austenite, crystal structure,
electron microscope, lattice structure, optical microscope, martensite, and unit cell.
Microstructure variables: The microstructure of various allotropic forms of steel is
contingent upon an almost unlimited number of variables with respect to thermal and
mechanical treatments. Generic variables include temperature, cooling rate, carbon
content, and alloy content. See bainite, crystal structure, googolplex of microstructure,
mechanical working, and thermal treatment.
Mild steel: Another name for bulk-process-produced low carbon steel (0.1% - 0.3% cc).
Before the era of bulk process steel (1870), malleable iron, characterized by the same
carbon content as mild or “low carbon steel” but including siliceous slag as a microconstituent, served many of the same functions (e.g. toolmaking) as “modern” mild steel.
See carbon content of iron and steel and low carbon steel.
Mill forge: To create directional grain structure by the action of rollers under great
pressure in modern rolling mills.
Millscale: The oxidizing agent, iron oxide. Millscale is initially formed from the
hammering and rolling of heated iron, the surface of which is oxidized to form magnetic
iron oxide. Millscale, along with lime and fluorspar, is often used as a flux in smelting,
and, as an oxidizing agent, greatly increases the efficiency of puddling furnaces. See flux,
oxidation, and reduction.
Minimum quenching temperature: Temperature below which rapid quenching will not
result in hardening; also called the critical point. See austenite, martensite, and
Miyairi: Japanese swordsmith.
Modern era: With respect to ferrous metallurgy, that period of time characterized by the
perfection of bulk process steel production (>1875); also that period of time beginning
after Benjamin Huntsman reinvented a method for producing crucible cast steel (1742).
With respect to the Industrial Revolution, the modern era is also denoted by the
widespread appearance of Watts’ steam engine (1775), which involved the innovation of
doing work by boiling water rather than harnessing the power of falling water. The
modern era is also denoted as the Age of the Factory System of Mass Production
(>1840), and lastly, as that historical era characterized by the development of the
electrical transmission grid and the automobile (>1890), i.e. the Era of Petro-Chemical
Electrical Man. See cascading Industrial Revolutions.
Modes of carbide dispersion: Upon the cooling of austenite, iron carbide may form “in
plates (lamellae), intergranular cells, or somewhat spherical particles, all over a vast
range of sizes. Nowhere in metallurgy is there a more complete representation of the
effects of the distribution of hard particles in a soft plastic matrix than in steel. The finer
the dispersion, the greater the hardness of the aggregate” (Bain 1939, 22).
Mohammed’s ladder: Special pattern of repeated vertical markings on Damascus steel
swords. These markings are a result of the distribution of ultra fine networks of iron
carbide during warm forging of the Wootz steel in Damascus swords. See Damascus
steel, nanowires, nanotubes, ultra fine microstructures, superplasticity, and Wootz steel.
Moiré Métallique: Intentional use of patterns resulting from crystal formation to produce
decorative effects on metals. Invented by Allard in 1814, etched tinned iron plate was
covered with a lacquer to produce lacquered tinware (Smith 1960).
Mokumé: Disclosure of the structural and chemical properties of pickled iron and steel in
the form of wood grain patterns for the purpose of decorating Japanese iron sword guards
(tsuba). Described and illustrated by Cyril Smith in his chapter on Japanese swords
(Smith 1960, 57-62).
Mold: Form that contains the cavity for the casting of metal objects from molten metals.
Molded malleable cast iron: Malleable cast iron, which, after annealing, is suddenly
chilled in iron molds, producing a steely cast iron with a very smooth surface, as in
Bailey plane bodies c. 1855. Malleable cast iron may have been subject to additional heat
treatments to become grey cast iron, which was used by the Stanley Tool Co. for
planemaking. An exact description of the heat treatment process used to manufacture
high quality Stanley iron bodied planes in the last four decades of the 19th century
Molder: In the operation of the blast furnace, the person in charge of making sand molds
out of wooden patterns, which formed the shape of the cast iron object being
manufactured, and then supervising the pouring of the melted cast iron into the mold. See
blast furnace, hollowware, and patternmaker.
Molder’s finishing tools: Small steel hand tools used for shaping, smoothing, and
finishing the surfaces of sand molds, e.g. slicks, corner slicks, trowels, and lifters.
Molybdenum: Most effective of all alloys in the hardening of steel by phase
transformation kinetics (Cias n.d.).
Mountain ore: Term used by Peter Oliver to refer to iron ore being imported, preferably
from Pennsylvania, to be used as a substitute for the rapidly disappearing bog iron
deposits of the Middleboro, MA, area. Oliver’s Forge on the Nemasket River in
Middleboro was then producing mortars, cannon, and howitzers for the Crown. In a letter
dated March 21, 1756, Oliver, a Tory, noted the superiority of “mountain ore” over bog
ore for heavy ordnance (Weston 1906).
Moxon: Joseph Moxon’s Mechanick Exercises or the Doctrine of Handy-Works [1703
(1989)] is the most comprehensive survey of blacksmithing, toolmaking, and crafts such
as joinery, house carpentry, turning, bricklaying, and mechanical drawing available at the
end of the 17th century. It contains important illustrations of basic tools, some of which,
such as the frame saw, bow saw, scribe, bevel, keyhole saw, chisels, and gouges, are still
found in old tool chests and collections, linking contemporary tool forms to English
prototypes used in the early North American colonial period.
Muck bar: Nineteenth century American term for puddling-furnace-derived,
unprocessed wrought iron produced by a single passage through a rolling machine. Muck
bar was usually subject to further refinement by additional shingling, rolling, or faggoting
and piling into higher quality wrought iron. Also used in this Glossary in reference to the
bar stock produced by the bloomsmith prior to refining.
Multiple alloys: Alloys that play a role in phase transition kinetics by enhancing or
mitigating mechanical properties such as hardness.
Multiple hearths: While North American colonial era forges and smelting furnaces often
had only one hearth, most integrated ironworks had multiple hearths, occasionally as
many as twenty or thirty. Ancony hearths, chaferies, blacksmith forges, and anchor forges
are examples of special use hearths used at integrated ironworks or colonial forge
complexes where the multiplicity of hearths differentiated these ironworks from the
community forges of individual shipsmiths, edge toolmakers, and blacksmiths.
Multiple transformation modes: Modes occurring within the critical cooling rate
temperature range (1000º F to 200º F) and resulting in the production of a wide variety of
morphologies, ranging from lamellar structures to structures that exhibit spheroidization
at grain boundaries. Alloying elements and the grain coarseness of the austenite being
cooled also influence the multiplicity of microstructures formed within the critical
cooling rate range. Bainite is the generic name for many of the microstructures formed
within this temperature range and is a testament to Edgar Bain (1939), who first
elucidated these phenomena.
Mumbra: Ancient African tribe that made cast iron using horn and quartz as flux
Mushet, Robert F.: (1812 - 1891). English metallurgist with a clandestine steelworks in
the Forest of Dean. Mushet was the first English ironmonger to commercially produce
spiegeleisen, an iron-carbon-manganese alloy, which he convinced Henry Bessemer to
use in his conversion process for the mass production of low carbon steel. Mushet later
played a major role in the development of alloy steels, inventing what he called selfhardening steel (1868). Initially made with high tungsten content, as well as manganese
and other alloys, “self-hard” was the principal form of tool steel used for the next three
decades. The metallurgists Taylor and White eventually discovered that manganese,
rather than tungsten, was the principal alloy providing hardness. See manganese, R.M.S.,
self-hard, spiegeleisen, Taylor-White, and tempered alloy steel.
Music wire: Fine steel wire used as strings in musical instruments, as well as for
precision measurement functions; produced by drawing annealed steel wire through a
draw plate. See draw plate.
Myth of wrought iron: Mistaken belief that “until the iron makers of Central Europe
developed a new type of furnace around 1350, wrought iron had been the only product
made from iron ore” (Aston 1939). This is incorrect. The wide variety of iron tools,
weapons, and currency bars recovered from early Iron Age Roman era and migration
period archaeology sites indicates that wrought iron production (0.02 - 0.04% carbon
content) in direct process bloomeries was rarely achieved. The great majority of artifacts
recovered from these sites contain widely varying carbon contents ranging from what
today would be called low carbon steel (> 0.08% cc) to heterogeneous raw steel with a
carbon content as high as 1.5%.
Naginata: Form of Japanese weapon; a wood shaft with a curved blade and a tsuba
(guard) between the blade and the shaft. Traditionally used by samurai warriors, the
naginata is the subject of the modern ritual of naginatajutsu, especially popular with
contemporary women in Japan.
Nanotechnology: Study of the microstructure of metals, ceramics, and other materials
utilizing the high resolution transmission electron microscope (HRTEM), which can
provide images of formations in the order of magnitude of billionths of a meter.
Nanotechnology is especially useful in the study of the crystal structure of forged and
heat-treated steels and the measurement of trace amounts of ecotoxins in pathways to
human consumption. It is also associated with semiconductor physics of microfabrication technologies and potentially significant environmental contamination, which
is the hidden downside of innovative nanotechnology. See nanotubes, nanowires, and
Nanotubes: With respect to ferrous metallurgy, the spheroid carbide (cementite)
microstructures containing nanowires created by forging high carbon Wootz and other
steels at temperatures below the eutectoid point. The carbide microstructure of nanotubes,
which can only be examined using the high resolution transmission electron microscope
(HRTEM), differs from the microstructure of pearlite, which has a lamellar morphology
composed of alternating plates of ferrite and cementite. In ferrous metals characterized by
the presence of nanotubes, the nanotubes, containing cementite nanowires, are often
adjacent to plates of pearlite and provide elements of superplasticity not present in steels
characterized by other microstructures. See carbon nanotube, nanowires, superplasticity,
and Wootz steel.
Nanowires: Characteristic linear arrangement of carbide (cementite) structures within the
nanotubes of superplastic steels, often in the form of parallel wires in areas outside of
cementite particles. The distribution of nanowires is not uniform and their “preferred
direction” can have local variations. “…there are obvious similarities between the
nanowires found here and the laminar cementite in pearlite” (Levin 2005, 913).
Nanowires may also contain other alloys, such as vanadium, cobalt, chromium or
manganese, as micro-constituents, which may play a role in facilitating superplasticity.
See nanotubes, spheroidization, and superplasticity.
Natural steel: “Steel made in a bloomery directly from iron ore. It contained slag
particles since it was a carburized form of wrought iron” (Gordon 1996, 310). Natural
steel production was dependent on higher than normal fuel to ore ratio, rapid air flow to
facilitate high furnace temperatures, high silica, high manganese, and low phosphorous
ore content (Barraclough 1984a, 17) and was the most common steel-producing strategy
before the appearance of the blast furnace and the consequent development of the
decarburization of cast iron to produce (German) steel. See bloomery, direct process,
ferrosilicate, German steel, and manganese.
Natural steel edge tools: Tools that are forge welded (hammered, quenched, and
tempered) by the blacksmith directly from the bloom of unrefined smelted iron. Starting
with malleable iron bar stock with at least a 0.2% carbon content, additional carburization
of the cutting edge of a tool results from its careful placement with a charcoal fire.
Knowledgeable blacksmiths could make high quality edge tools using this method but
only one or a few tools at a time. The best natural steel tools were made from manganesebearing spathic ores, first at Halstadt (Austria), then by the Romans in Austria (Noricum),
in Spain in the medieval period, and especially in southern Germany after 1400 AD.
Natural steel edge tools were also produced, but probably with greater difficulty, by
American blacksmiths utilizing manganese laced, bog iron-derived bar stock in situations
where German or blister steel bar stock was not available for “steeling” edge tools.
Natural steel was the most common constituent of forge welded edge tools from the early
Iron Age until the late medieval period. See forging, bloomery, direct process, natural
steel, and nest carburization.
Nest carburization: Steeling of groups of malleable iron chisels, caulking irons, or other
tools by their submergence in charcoal pits for periods of days (24 – 72 hours). In this
ancient variation of case hardening, nests of tools would often be enclosed by clay or
other non-combustible coverings, which would protect the iron components of tools
being steeled from deleterious effects of combustion gases. See carburize, case
hardening, and enclosure.
Neumann bands: Bands observed in the microstructure of steel that result from
mechanical treatments, such as hammering at room temperature or slow deformation at
lower temperatures. These bands are formed by twinning, i.e. the grouping of identical
lamellae in patterns characteristic of the crystal structure of a specific allotropic form of
an iron carbon alloy, e.g. pearlite. See Widmanstätten structure, deformation history,
plastic deformation, lamellae, lattice structure, bainite, and pearlite.
Newcastle: Principal steel-producing center of England between 1700 and 1775. Located
in the far northeast of England, Newcastle predated Sheffield's emergence as England's
late 18th and 19th century center of steel production. Newcastle emerged as an important
steel-producing center after iron and steel production activities ended in the Forest of
Dean and the Weald of Sussex. See Forest of Dean, Weald of Sussex, and Weardale.
Nickel: Important alloy in steel. Nickel helps retain austenite in high carbon steels except
in those with a high chromium content (Pollack 1977). See Chalibean steel, chloanthite,
and nickel steel.
Nickel-Silver: 50% copper, 25% zinc, 25% nickel; also called German silver; strong,
hard, and corrosion-resistant.
Nickel steel: Alloy steel containing nickel; nonmagnetic with high tensile strength.
Nickel “increases strength by strengthening ferrite without decreasing ductility” (Shrager
1949, 187). A typical nickel alloy steel is 3.5% nickel and 0.5% carbon and has several
thousand pounds per square inch more strength than pure steel. Steels with more than
22% nickel are nearly corrosion resistant; those with 25% to 46% nickel are used
specifically for watch parts and measuring instruments due to their failure to expand and
contract. Meteor iron often contains about 10% nickel, which greatly strengthens it.
Chalybean nickel steel has historically been misinterpreted as meteor-derived
(Piaskowski 1982). See Chalybean steel and German steel.
Niello: Black alloy of silver, lead, and sulfur used for filling in engraved designs in silver
and other metals. See alloy and chasing.
Nitriding: The modern process for surface (case) hardening selected alloy steels by
heating the steel in an atmosphere of nitrogen (ammonia gas) at approximately 950 ºF,
followed by slow cooling. Heat treatments, including annealing, are usually applied
before nit riding, which reduces distortion. Standard alloy steels containing chromium
and molybdenum and nonstandard alloy steels containing aluminum are the only steels
suitable for nitride formation. Iron nitriding is a recently developed process used to case
harden cutting tools utilizing ionized low pressure gas.
Nodular cast iron: Made from iron with a low sulfur content, with various alloys such as
sodium, magnesium, and cerium, in which carbon is present in spherical nodules, also
called ductile cast iron. A versatile modern form of cast iron available in a variety of
chemical configurations, characterized by high tensile strength and a significant capacity
for elongation, nodular cast iron is representative of the wide variety of iron carbon alloy
combinations developed in the 20th century. See cast iron.
Noric steel: Steel produced by Celtic metallurgists from the siderite ores of the Mount
Erzberg region of Austria and supplied to both the Roman Republic and the Roman
Empire for weapons production. Noricum was a Roman province, hence the name of the
natural steel produced there from the manganese-rich spathic ores. See natural steel,
German steel, Erzberg, Styrian steel, Celtic metallurgy, iron road, and spathas.
Noricum: Area of Austria called Styria and Carinthia including Mount Erzberg (Ore
Mountain) that was the Celtic center of Roman ferrous metallurgy.
Normalizing: A heat treatment for steel. Normalizing is the slow cooling of iron-based
alloys from temperatures above the critical point in an environment of still air and normal
Norwegian steel: Forged and laminated steel made out of high carbon hard tempered
steel and soft iron, having a Rockwell hardness of 63 – 64; used by knife makers and
capable of being bent in a vise (Latham 1973).
Nucleation: “The formation, through thermally activated fluctuation, of the smallest
stable particles of a new phase” (Sinha 2003, 6.1). Nucleation is characterized by
randomness, rapidity of transformation, and is essentially equivalent to freezing. See
freezing point of iron.
Nucleation capacity: Actual controlling factor in hardenability for a given composition;
correlated with the austenitic grain diameter and the presence of alloying elements, which
change the composition of austenite prior to hardening (Bain 1939, 54). See phase
transformation and kinetics.
Oakum: Shredded rope or hemp fiber often used for ship caulking, thus requiring the use
of caulking irons and mallets, standard tools of the working shipyard. See caulking iron.
Oil temper: In the forging of edge tools, temper obtained by the quenching of tool steel
in oil rather than brine or water. See hardness scale, Rockwell hardness test, temper,
martensite, and brine quenching.
Open-hearth furnace, early forms: The most common form of furnace used in
antiquity, the open-hearth furnace had two basic forms, bowl and shaft, both of which
exposed the ore being smelted to the direct impact of the oxidizing flame of the burning
fuel. The shaft furnace, which dates to the early Iron Age in central Europe, was later
developed into the high shaft German Stucköfen furnace, the predecessor of the blast
furnace. The bowl furnace, which later evolved into the Catalan furnace, was used in
southern Europe until the early 20th century. Both were used for direct process production
of iron blooms, and both forms occur as slag pit furnaces and slag-tapped furnaces. The
most primitive slag pit type furnaces were characterized by the accumulation of slag in
pits underlying the furnace, which required the movement of the furnace to adjacent slagfree locations. More practical and productive were furnaces designed with adjacent pits
for slag tapping, the residue of which was more easily moved to rubble piles in the form
of slag heaps. See furnace forms, shaft furnace, bowl furnace, slag pit furnace, slagtapped furnace, bloomery, and direct process.
Open-hearth furnace, modern forms: Another name for two modern (after 1865) forms
of the blast furnace, i.e. the Siemens-Martin process and the Siemens open-hearth
furnace, which are differentiated primarily by the type of material used in the charge. The
Siemens-Martin process used pig iron and scrap steel for the charge; the Siemens openhearth furnace used carefully measured additions of iron ore to the slag after the melt was
underway, increasing its iron oxide content. Both use waste gases to preheat the air blast
and are considered superior to the Bessemer blast furnace because they allow better
quality control of alloy steel production. The open-hearth furnace process is also less
wasteful than the Bessemer furnace, utilizing all ores and scrap, which were more slowly
heated to higher temperatures by indirect radiated heat from a regenerative gas furnace.
Modern open-hearth furnaces use gas, coke oven gas, natural gas, oil, and powdered
coals as possible fuels. In the Siemens open-hearth process, “molten pig iron is run onto a
hearth or bedcover, which gas flames play to maintain the heat and to burn up carbon and
other defects [contaminants]. This process took some eight hours, and in the result, was
able to produce an even nature throughout” (Abell 1948, 148). See basic process, acid
process, Siemens-Martin process, Siemens open-hearth furnace, and the Siemens
regenerative gas furnace.
Optical microscope: Microscope used by William Sorby (c. 1885) to investigate the
space lattice structure of ferrous metals. The optical microscope inaugurated the science
of metallography, i.e. the study of the microstructure of metals.
Ordnance: Military supplies and weapons. Bronze and cast iron cannons and artillery
were the most important product of foundries and ironworks producing ordnance in 16th
century England and Europe. For example, the casting of cannons for the coastal defenses
of England was the most important use for the products of the blast furnaces of the
Weald. The demand for ordnance, gun iron, shipsmith’s ironware, and edge tools resulted
in the expansion of the English iron industry from the Forest of Dean and the Weald
north to the midlands after 1600, to Newcastle after 1700, and to Sheffield after 1750.
Before 1635, the location of production of the finest early handguns by gunsmiths and
sword cutlers was southern Germany (Nuremburg, etc).
Ore boil: The violent frothing that occurs in the open-hearth process as a result of the
interaction between the iron ore and iron oxides in the slag and the carbon in pig iron.
The carbon monoxide thus formed causes the frothing. In the puddling furnace, the
termination of the boil signals the full decarburization of the pig iron and its conversion
to wrought iron. See puddling furnace.
Oriental crucible steel: Produced in high temperature resistant refractory clay crucibles
in small quantities (+/- 3 kilograms) in India, China, and Japan as early as 300 BC and
possibly earlier in India. Crucible steel was a trade item which may have reached the
Levant in the first millennium and was probably used by the Vikings in sword
production. Damascus steel is one variation of Oriental crucible steel. When Benjamin
Huntsman “discovered” crucible steel, he was readapting an already known, but obscure
and difficult, steelmaking process for his watch spring manufacturing business. See cast
steel, Wootz steel, and Venetian steel.
Osmund: A form of malleable iron or natural steel imported from Sweden and Spain
during the Medieval period and used for knitting chain mail, also used to make
arrowheads and fishhooks.
Over-coating: A modern method of ax-making; the overlaying of a piece of high carbon
steel (the ax bit) upon a folded iron or low carbon steel ax body prior to welding
(Kauffman 1972, Klenman 1998). See ax-making techniques and iron cored.
Overheating: Process that results in the surface decarburization of iron or steel, which
begins occurring at a temperature of 1200º C. Surface carbon is removed and the iron is
oxidized into an iron oxide scale. “No useful degree of carburization can be achieved
when iron is heated unprotected in a forge fire” (Barraclough 1984a, 31). Overheating in
direct process smelting had the ironic effect of promoting carbon uptake in the bloom,
facilitating the formation of liquid cast iron. Iron absorbs carbon more rapidly at high
temperatures; the increase in the carbon content of the bloom then lowers its melting
temperature. See enclosure, bloomery process, natural steel, cast iron, and carburization.
Overseas carrying trade: A term referring to the North American colonial era transport
of masts, spars, planks, and other timber products to English and continental shipyards.
Overshot water wheel: The most efficient form of the water wheel, which utilizes the
height and volume of falling water as the power source for the operation of the
blacksmith's trip hammer, the up and down mill saw, the grist mill, and belt-driven
machinery of every description. See undershot water wheel.
Oxidation: The combination of oxygen with an element to form an oxide or the
combination of an oxide with more oxygen to form a higher oxide (Shrager 1949).
During the smelting process, oxidation removes impurities from the higher iron oxides,
resulting in the production of a lower form of iron oxide, FeO, the precursor to the
formation of pure wrought iron (ferrite, Fe).
Oxidation reduction reaction: The simultaneous occurrence of the oxidation and
reduction of iron in the smelting process. Intermediate reducing agents remove oxygen
from the reductant, e.g. iron oxide, therefore oxidizing it. Carbon removes oxygen from
iron oxide and then is transformed into carbon monoxide: FeO + C = Fe + CO. Both
processes work ideally to produce the ferrite (Fe) sought by the bloomsmith. Entrained in
this ferrite is siliceous slag (ferrosilicate) and the combination of the two constitutes
wrought iron. With the exception of sulfur, oxidation results in the removal of most forms
of impurities as slag. See ferrosilicate, oxidation, reduction, and smelt.
Oxidizing reaction: In iron-smelting, the change in composition that occurs during the
making of wrought or malleable iron or steel from iron ore or pig iron. The carbon in the
fuel separates as a gas in the form of CO or CO2 and thus removes oxygen from iron
oxide, producing iron or steel. When ferromanganese and ferrosilicon are added to the
steelmaking charge, they serve to reduce the dissolved gases and the iron oxide in the
metal. The manganese and silicon form oxides, which collect as slag and encourage the
uniform distribution of carbon in iron to produce raw steel. See natural steel.
Oxygenation: The reaction of oxygen with hot metal (e.g. iron oxide) to produce CO and
Pack carburization: 1) The case hardening of stacked tools packed in a metal box
containing carboniferous material or in a pit containing charcoal. 2) The sealing of iron or
steel in a furnace or container in conjunction with carboniferous materials; an ancient
strategy for carburizing iron or low carbon steel that is still used in the modern era. The
release of carbon diffuses below the surface of the iron or steel to form carbides when the
steel is heated above the critical temperature. See case hardening, cementation steel, and
Packing: The compacting of fibers of wrought iron or carbon steel by hammering in
order to increase the density and, thus, the strength of the tool or implement being forged.
For example, packing is done with carbon steel when the metal is “sunrise red, barely
discernible in regular light… if the metal is too hot, it will not pack, if too cold it may
crystallize and break” (Bealer 1976a, 168).
Palimpsest: In a historical context, a historical palimpsest is a parchment written upon
once and then covered over again by subsequent narrations that obscure the original
inscriptions. In an archaeological context, the palimpsest is the accidental durable
remnants (ADR) used to interpret prehistoric cultures and consists of the multiple layers
of material cultural artifacts, the archaeologists’ excavation and study of which results in
the compilation of an account of these societies. The primary source of information about
prehistoric societies are the forms of tools and other artifacts used and discarded in layers
of cultural materials, now the subject of study by archaeometallurgists and
Pattern books: Toolmakers’ catalogs issued in England by manufacturers, such as
Wykes (watch making tools), Stubbs (files and hand vises), and Timmins (tools of the
trades), which often illustrated tool forms derived from Roman and near eastern sources.
Pattern books signal the rise of a market economy in the late 18th century when the
gentleman and his tool chest become equal, if not greater, in importance to the lowly
artisan, such as the file-maker, blacksmith, or shipsmith, all of whom used tools to make
other tools. See Diderot’s Encyclopedia, iconography of tools, and Moxon.
Patternmaker: The woodworker who crafts the wooden patterns that form the sand
molds for casting bronze, brass, aluminum, cast iron, and steel into the wide variety of
tools and equipment made in foundries. See cope, core box, and drag.
Patternmakers’ shrink rules: Rules that, by graduated variations in their increments,
make allowance for the changing (shrinking) dimensions of metals, which contract at
various rates during the cooling process from the freezing temperature of the hot metal to
room temperature. With as many as 12 variations of allowed shrinkage to the foot
ranging from 1/12” to 3/8” (Stanley 1984), such shrink rules provided for the fabrication
of larger patterns necessary to compensate for the tendency of metal to shrink upon
Pattern-welding: The ancient craft of knife and sword production based on welding
together strips of natural steel or case-hardened steel and strips of wrought iron, which
were forge welded, quenched, and tempered to produce the desired weapon; used as a
sword and knife-making technique from the early Iron Age to the modern era; made
famous by Merovingian, Viking, Muslim, and Japanese sword makers. See Damascene,
reagent, sword cutler, and steel smith.
Pearlite: A mixed layer structure of iron carbide (cementite) and ferrite; a microstructural
form of steel derived from the eutectoid transformation of austenite. Pearlite has a much
higher tensile strength (125,000 lbs/sq inch) than ferrite (50,000 lbs/sq inch). If the
lamellar morphology of alternating plates of ferrite and cementite containing 0.83%
carbon is cooled below 723º C, it then becomes pearlite (Wayman 2000). “Pearlite is in
fact the dominant microstructural form in medium to high carbon steels (0.4 – 0.8 percent
C)” (Sherby 1995, 11). See cementite, ferrite, lamellae, and microstructure.
Pearlite nodules: Nodules that contain multiple colonies of parallel lamellae
characterized by random arrangements, often as interwoven bicrystals of ferrite and
cementite; a common characteristic of pearlitic steels.
Pearlitic malleable cast iron: A cast iron, the manganese content of which allows its
pearlite matrix to retain carbon in the form of cementite.
Persistent organic pollutants (POP): Long-lived, synthetic, organic chemicals produced
by pyrotechnic societies in large quantities beginning in the middle of the 20th century.
Most biologically significant POPs are volatile and/or lipid soluble, bioaccumulate in
pathways to human consumption, and are globally transported by hemispheric transport
mechanisms, including the water and carbon cycles. See biocatastrophe and biologically
significant chemical fallout.
Pewter: An alloy of tin and lead or tin and copper. Bismuth and zinc are also sometimes
a constituent of pewter. While Roman pewter was high in lead, modern pewter, if
intended to be used as an eating utensil, is made without lead. See alloy.
Phase: With respect to ferrous metallurgy, a physical (allotropic) form of iron
characterized by specific microstructures. “Phase is a portion of a system whose
properties, composition and crystal structure are homogenous and which is separated
from the remainder by distinct boundary surfaces. …the phases present in Fe-Fe3C and
Fe-C diagrams are molten alloy, austenite, α-ferrite, δ-ferrite, cementite, and graphite”
(Sinha 2003, 1.3-4). See allotropic forms of iron, Appendix VI, phase transformation
kinetics, and phase transition.
Phase diagram: Diagram that expresses the relationship of carbon content to
temperature; also called an equilibrium diagram. Temperature is plotted vertically and
carbon content is plotted horizontally. See Appendix VI for a sampling of the wide variety
of phase diagrams and an illustration of the simple phase transformation kinetics of pure
Phase transformation kinetics: The study of the process of altering the microstructure
of ferrous metals through mechanical and thermal treatments and by the addition of
alloys; especially used in modern steelmaking strategies to create hardened steels.
Phase transition: The change in the microstructure of iron from one allotropic form (e.g.
austenite) to another allotropic form (e.g. pearlite) without a change in its chemical
constitution, usually due to thermal and/or mechanical treatments.
Phenomenology of tools: The sum total of all the ways in which we construct and
deconstruct our world with tools, i.e. the language of tools, including not only the making
and using of tools but also the construction of landscapes and cityscapes as an
iconography of tools at work.
The phenomenology of tools is the totality of the voices of tools in history, a large
extended family of function, skill, technique, necessity, history, obsolescence,
memory, expressed in a cacophony of images and artifacts, all squabbling to be used
or laid aside, remembered or forgotten. From eolith to atomic bomb, from artisans to
nation states, the craftsmanship and history-making of tools join with the archaeology
of tools to construct, deconstruct, and again reconstruct the stories of history. (Brack
The phenomenology of tools is, in essence, the writing of history by the wielding of tools,
as well as the inscription and incorporation of tools in and as art. In the 18th and 19th
centuries, huge areas of North American forest were cleared by timber harvesting,
charcoal production, and farming. Later in the 19th century, much of this landscape
became towns and then cities with paved roads. The transition from handmade hand tools
to machine-made hand tools to a global consumer society, where almost all artifacts are
machine-made, characterizes the evolution of industrial society. Implicit in this dynamic
of the phenomenology of tools are the lessons of pyrotechnic societies, i.e. the recurring
narrations of the deleterious environmental impact of carbon dioxide emissions (Gore
2005), biologically significant chemical fallout, or the looming possibility of nuclear
disaster, antibiotic resistant infection, biocatastrophe, and infrastructure collapse. What is
it, in fact, that we are constructing or have constructed with our tools? See
biocatastrophe, Brack (1984), infrastructure collapse, methylmercury, and post117
Phlogiston theory: A theory popular between the late 17th and late 18th century that
stated that combustion was due to the presence of phlogiston in the flammable materials,
the phlogiston having no mass, taste, odor, or color and being produced as ash by
combustion. It was assumed to occur in all flammable materials and to be released by the
combustion process. The discovery of carbon and its role in combustion put an end to the
Phosphorus: Inflammable, nonmetallic, chemical element (P) commonly found as a
naturally occurring contaminant in iron ore. When present in wrought iron (+/- 0.025%
cc), phosphorus increases hardness, making it useful for nail-making. It increases the
fluidity of cast iron and thus aids in the casting of hollowware. Otherwise, phosphorous is
not useful as a hardener when in the presence of carbon; the higher the carbon content of
malleable iron or steel, the more deleterious the phosphorous content. Phosphorous
content above (+/- 0.05%) causes brittleness at room temperature. See cold short.
Photomicrograph: A photograph of a microscopic or magnified object taken with a
microscope. The appearance of more powerful light microscopes in the late 19th and early
20th centuries allowed detailed analysis of the wide variety of the crystalline
microstructures characteristic of various allotropic forms of ferrous metals. Such
photomicrographs led to the discovery that pearlite was a form of steel composed of
alternating lamellae of ferrite and iron carbide (cementite). See allotropic, cementite,
electron microscope, ferrite, HRTEM, iron carbide, lamellae, microscope, optical
microscope, and pearlite.
Pickling: Use of a diluted acid bath to remove oxide scale from iron and steel surfaces
prior to mechanical treatments, such as cold rolling or wire drawing.
Picotechnology: The study of structures, including those of ferrous metals and ecotoxins,
in parts per trillion (sub-nanometer quantities), where measurement of single atoms or
molecules in metals and especially in abiotic and biotic media will provide additional
information about the microstructures of metals and, most importantly, the movements of
ecotoxins in pathways to human consumption. Picotechnology will be particularly useful
in documenting the presence of persistent organic pollutants (POPs) in environmental
media, which are currently below the limit of detection of most nanotechnological
analysis systems at lower trophic levels. Many ecotoxins are biomagnified at higher
trophic levels and bioaccumulate in living organisms, reaching their maximum level of
concentration and synergistic interaction in wildlife feeding at the highest trophic level
(e.g. bald eagles, humans).
Pig iron: The high carbon iron silicon alloy (2.0 - 5.0% carbon content) produced by the
hot temperatures of large shaft furnaces and, later, blast furnaces. The hotter the furnace
fire, the more rapid the absorption of carbon by the iron being smelted. Originally a waste
product of smaller bloomery and shaft furnaces, pig iron is the first stage product of the
indirect process of iron- and steelmaking. Because cast iron was produced in a liquid
form in the blast furnace, when it was drained off it was solidified in rows of sows.
Hence, the term “pig” iron was due to its appearance as cooled ingots. “Iron alloyed with
carbon and silicon produced in a blast furnace” (Gordon 1996, 310).
Pile: To bundle and reforge iron or steel bar stock.
Piled wrought iron: A term for refined wrought iron made by the repeated faggoting of
bars or plates of bloomery iron or puddled wrought iron, followed by shingling
(hammering) to remove additional carbon and slag constituents and further align the
silicon slag content into the fibrous patterns that provide its unique toughness and
ductility. The high quality Swedish iron bar stock used in England and America to
produce steel was highly refined, piled wrought iron, which was essential to the
production of the highest quality edge tools. See finery, loup, refined wrought iron,
shingling, and whalecrafters.
Piling: A technique used by knife- and swordmakers in all ages. Piling was the bundling
and then forging of alternate layers of wrought iron and steel. In the age of blister steel
(1686 – 1750) in England, piled blister steel was reforged into shear steel. The highest
quality steel was known as double shear steel made by re-piling and reforging shear steel
yet again (Barraclough 1984a). Piling also refers to the reheating of iron bar stock on clay
tiles prior to reforging and the reheating of stacks of bar iron in a balling furnace. Shear
steel production was gradually replaced by the crucible steel process, i.e. the production
of steel by a chemical reaction that required fewer steps and less labor and fuel and
offered more quality control of the slag and carbon content of the cast steel being
produced. See knife forms, pattern-welding, and swordmaking.
Piling and folding: A process used by sword cutlers and edge toolmakers to reduce the
heterogeneity of sheet steel and sheet iron during edge tool and sword production. Sheets
of steel and iron were forge welded into a more homogenous mixture by piling and
folding before reforging. The highest quality samurai and Damascus swords were piled
and folded hundreds of times before a final product was ready for exchange. See
Japanese sword, pattern-welding, and reagent.
Pin the boundaries: To form very fine grains of pure iron and iron carbide that prevent
growth of large carbide spheroids, allowing the unhindered boundary sliding necessary
for superplasticity in metals (Sherby 1995). See superplasticity.
Pins: Inclusions of unwanted natural steel in wrought iron not fully decarburized, making
the iron useless for many applications. Pins were the bane of furnaces making iron shafts
and blacksmiths making wrought iron hardware and implements. See natural steel.
Pipe: The shrinkage cavity within a cast steel ingot formed as a result of uneven cooling.
In crucible steelmaking, this cavity is eliminated by the teamer, who has an extra reserve
of liquid steel to put in a dozzle (clay cone) to fill the cavity. See cast steel, dozzle, and
Piston bellows: Bellows developed in place of accordion bellows after 1750 and used in
conjunction with steam engines. The higher efficiency of piston bellows allowed for the
construction of larger blast furnaces. Community blacksmiths and shipsmiths continued
to use accordion bellows to provide the air blast for their small forges until the late 19th
Pit vault molds: Molds set vertically in the ground to receive cast iron or bronze for
cannon casting. Pit vault molds were Henry the Eighth’s molder’s principal method of
casting cannon in the Weald for protecting the south coast of England from French
invaders, circa 1520 – 1545. The more advanced 18th century methods of cannon casting
are graphically illustrated in Diderot’s Encyclopedia ([1751-75] 1959).
Planish: Hammering of metal to smooth, harden, and strengthen it, as in late medieval
Plastic deformation: Deformation in metals that results from slippage, gliding, twinning,
cleavage, or creep and is accompanied by three modes of lattice reorientation. For
example, the propensity of the crystal structure of ferrite, when in the form of wrought
iron (<0.08% carbon content) to allow slippage, gives wrought iron its soft ductile
plasticity. Plastic deformation is the movement of crystal lamellae along slip planes in a
particular direction determined by the crystal structure of the lattice network. See lattice
Plasticity: In ferrous metallurgy, the propensity of heated crucible steel to be ductile; i.e.
to have high workability and to be easily rolled and shaped. No other form of steel has
the extreme plasticity of heated crucible steel. The same characterization applies to
wrought iron with a carbon content of 0.08% or less. Its silicon content enhances its
plasticity and workability. See superplasticity.
Plating mills: North American colonial era ironworks first established in the early 18th
century for making sheet iron to produce iron pans and utensils, as well as hoops for
coopers and tin plate for whitesmiths.
Polyhedral: A many-sided structure with three or more planes meeting at a point and
usually containing more than six plane faces.
Polymetalic societies: Pyrotechnic communities that smelted multiple types of metals,
including copper, silver, gold, bronze, and iron. Polymetalism is one of the characteristics
of industrial society.
Popham Colony: Location of the ill-fated attempt to establish the “North Virginia”
colony, which ended up at the mouth of Maine’s Kennebec River, 1607-1608, and the
location of New England’s first documented shipsmith forge. Archaeological
explorations by J. P. Brain located a forge site with associated slag. Also recovered were
a ships’ caulking iron and strips of wrought iron roves, which functioned as washers,
used in conjunction with iron rivets and/or spikes to fasten the planking of the pinnace
Virginia, the first ship documented as being built in Maine. The roves, spikes, and rivets
were almost certainly made on site. The caulking iron was probably a German steel tool
brought from England but conceivably could have been made on site from iron bar stock
brought by the Popham settlers as ballast.
Post-apocalypse: The unknowable future that will follow the end of the Age of
Biocatastrophe when much smaller human populations will have to cope with a radically
altered biosphere with dramatically diminished natural resources. Will the techno-elite
wave flat world magic wands to mitigate the tragedy of our round world commons?
Post-apocalypse society: A term appropriate for describing social conditions in
communities following biocatastrophe and the partial or complete collapse of the
industrial infrastructure and the health, social, and public services associated with modern
society. In the post-apocalypse, self-sufficient agrarian communities using sustainable
technologies will survive along with pockets of crypto-fascist, technologically elite,
fortified settlements with the capacity to hoard scarce resources and maintain
independent electronic grids. Communities that survive the impact of biocatastrophe on
the infrastructure of modern pyrotechnical, industrial society will face the challenge of a
decentralized, dysfunctional, post-industrial society unable to provide adequate supplies
of fresh water or healthy food or consistently maintain essential services for the majority
of survivors. In post-apocalypse society, renewable energy sources will only be sufficient
to provide the energy needs of a small component of the once rapidly expanding
populations of the world’s pyrotechnic global industrial economies. See apocalypse,
biocatastrophe, mercury, and infrastructure collapse.
Pouled Janherder: The Persian term for Wootz steel, called “bulat” (steel) in Russian.
See bulat and Wootz steel.
Powdered metallurgy: With respect to steel production, the modern technology of
utilizing finely powdered iron and selected alloys and molding them in hydraulic diepresses operating under high pressure at high temperatures and for long durations. The
end product is steel with a microstructural homogeneity equal to or greater than crucible
steel. Due to their alloy content, many powdered metallurgy steel products have
characteristics of super hardness and extreme durability. Powdered metallurgy
technology bypasses many messy solid/liquid phase transformation processes
characteristic of traditional smelting procedures by using whole body melting technology
in alloying operations. See superplasticity.
Precision casting: The precise casting and boring of cast iron steam engine cylinders,
which required the development of the steam engine in England in the 18th century to
become a principal source of power for mills and blast furnaces. First pioneered by John
Wilkinson as an improved method of boring cannon, Wilkinson’s precision ground
cylinders were quickly adapted by Bolton and Watt for production of steam engines. See
Pressed steel: Steel plate bent or pressed by means of dies into channel or other sectional
forms, giving great strength with a minimum weight of metal (Audel 1948, 419).
Prime mover: The fundamental power source for the operation of any tool or machine –
wind, water, human, animal, biomass, nuclear, or digital. The hand is the primordial
prime mover. The steam engine as a prime mover utilizes heat from the combustion of
biomass to do work. The utilization of biomass-powered steam engines in England in lieu
of water-powered machines was the key innovation that gave birth to an industrial society
of textile mills, machine-made fire arms and tools, and steam-powered railroads and
watercraft. Ironically, America’s extensive river resources allowed the growth of an
American factory system that initially relied on water power as its prime mover. The
current reliance on non-renewable biomass energy resources as the principal power
sources for the heat engines that power our pyrotechnic society is only possible because
of the frenzied increase in the consumption of coal, oil, and gas. Costly future sources of
nonrenewable biomass fuel resources can be expected to be available with the help of
high technology for generations to come. Prime movers can also be defined as sources of
technological and thus social change: blast furnaces, printing presses, steam engines,
railroads, gasoline, microchips, fiber optics, iPads, computerized high speed trading,
CNC technology. The current sudden widespread availability of hydrofracked gas and oil
has postponed the end of the Age of Nonrenewable Fossil Fuels but exacerbated the
inevitability of cataclysmic climate change and the world water crisis. See biomass fuels,
heat engine, Hunter (1979), and hydrofracking.
Principio: The largest integrated ironworks in the Mid-Atlantic colonies. Principio (est.
1731) was located at the head of Chesapeake Bay and was a focal point of the growth of
the American iron industry in the Pennsylvania/Maryland region after 1720 (Gordon
1996). Ship fittings produced at Principio and nearby furnaces “ironed” the famous
Baltimore clippers constructed in Chesapeake Bay in the century following the
establishment of this ironworks. See integrated ironworks and shipsmith.
Privilege: The granting of the right to use the water of a running stream or brook to
power a waterwheel for the operation of a trip hammer at a bloomery, finery, or
integrated iron works or for powering saw mills, grist mills or water-powered machinery.
Individual communities in colonial New England issued privileges from the early
colonial period until the middle of the 19th century. See overshot water wheel and trip
Proeutectiod: The designation for steel, in the form of austenite, formed by ferrite and
cementite above the eutectoid temperature of 723º C. When cooled slowly (below 723º
C) austenite becomes pearlite, the main microstructural component of cementation steel,
with a heterogeneous carbon distribution. If rapidly cooled, martensite is formed. See
bainite, hypereutectoid steel, and hypoeutectoid steel.
Proeutectoid cementite: Iron formed upon the cooling of austenite, when carbon in iron
is in excess of the eutectoid (0.83% cc). After the formation of pearlite, proeutectoid
cementite is deposited at the grain boundaries of pearlite. The microstructures of pearlite
and proeutectoid cementite are hypereutectoid (Pollack 1977, 126).
Proeutectoid ferrite: The free ferrite remaining after the formation of pearlite, after the
cooling of austenite below the eutectoid temperature. Proeutectoid ferrite is a mixture of
ferrite and cementite (0.83% carbon content). The resulting structures, pearlite and
proeutectoid ferrite, are hypoeutectoid (Pollack 1977, 126).
Proeutectoid ferrite reaction: “Of the several diffusional reactions by which Austenite
can decompose—Proeutectite Ferrite, Proeutectite Cementite, Pearlite and Bainite—the
Proeutectoid Ferrite is the most important. This is the first transformation to occur over
wide ranges of temperature and composition in most steels produced in large quantities.
The kinetics of this reaction thus determine the hardenability of these steels, and at lower
cooling rates play a major role in establishing their mechanical properties. The
Proeutectoid Ferrite reaction is also the simplest from the viewpoint of ascertaining the
effects of alloying elements upon the fundamental quantities determining the kinetics of a
diffusional transformation, namely the rates of nucleation and rates of growth” (Kinsman
Proeutectoid reaction: The response to the impact of cooling rates on the formation of
the lamellar structures of proeutectoid cementite and ferrite. “The higher the rate of
cooling, the smaller the amounts of proeutectoid ferrite or carbide to be found. The
proeutectoid reaction is essentially one of diffusion [and is a function of temperature].
The greater the degree of undercooling the less the size of the ferrite or carbide masses
formed” (Bain 1939, 31).
Profiler: A machine for cutting complex dies in the die-sinking process.
Progeny of ironmongers: In the 21st century, not only mechanics, machinists, plumbers,
and other tool wielders employed by the palisaded elite, but silversmiths, jewelers,
sculptors, printmakers, artists, and artisans of every description, not to mention a vibrant
community of blacksmiths, knife-makers, and edge toolmakers.
Psychic numbing: What happens to individuals whose attention is captured by flat world
hyper-digital technology, computers, iPods, flat screen TVs, Facebook, etc. Alternatives
to the psychic numbing of flat world technology include meditation, nurture, nature
(sustainable agriculture, environmental awareness), and the phenomenology of tools, i.e.
the marriage of tools, art, and history. The irony of psychic numbing is that flat world
technologies have the useful function of enlarging our understanding of our round world
biosphere and the finite resources that limit the boundaries of technological innovation
Puddled bar: The first bar rolled from a puddled bloom of wrought iron after shingling
in the decarburization of cast iron; also called a muck bar due to entrained impurities. The
puddled bar is often subject to further fining and processing. See finery, muck bar, and
Puddled steel: Steel manufactured by puddling by the premature halting of the
decarburizing process. “Carbon removal is slowed by adding manganese oxide instead of
iron oxide, stopping the boil of the puddled iron. Puddled steel is high in slag content and
became an important source of steel in Germany and England between 1855 and 1870”
(Barraclough 1984a). Barraclough also notes that the oxidation of the carbon was
retarded by the “smoky, reducing atmosphere in the furnace during the latter part of the
process” (Barraclough 1984b, 93-4). To some extent, puddled steel replaced the
traditional production of German steel, which was made by decarburizing cast iron in
shaft furnace refineries. In this sense, puddled steel is “German steel” produced in a
refractory (puddling) furnace. Barraclough (1984) also notes that “it provided for the
needs of industry for some time, in default of a better method, and was capable of
producing satisfactory steel from phosphoric pig iron, which is more than could be said
for either Bessemer or open-hearth steel up until 1880. It is strange that it has been
largely overlooked by almost all of the historians of the iron and steel industry”
(Barraclough, 1984b, 93-4). The extent of production in the United States is unknown,
but puddled steel may have been used for small scale edge tool production in New
England and elsewhere. Halting the decarburization of cast iron to produce malleable iron
or steel instead of wrought iron was very difficult due to the challenge of estimating the
carbon content of the malleable iron or steel being produced. Unknown is the extent to
which individual New England ironmongers mastered this technique and thus
supplemented the traditional process of using cementation furnaces to produce blister
steel, which then had to be piled and reforged to produce higher quality edge tool steels.
See puddling and puddling furnace.
Puddled wrought iron: Iron containing less siliceous slag than direct process bloomery
wrought iron and made in reverbatory (puddling) furnaces after 1785 by the indirect
process from decarburized cast iron. The development of the puddling or refractory
furnace allowed the more exacting production of large quantities of wrought iron with a
uniform carbon and slag content. The mass production of this high quality wrought iron
and growing production of cast iron produced the iron used in the rapid growth of
America’s industrial and transportation systems before bulk-processed low carbon steel
became available after 1875. Aston (1939) details the wide use of wrought iron, for
example, in 19th century bridge construction. Due to the disappearance of both the
bloomery and the puddling furnace by 1930, wrought iron was no longer produced by
these long established techniques in any significant quantities in the U.S. See furnace
types, puddled steel, puddling furnace, reverbatory furnace, and wrought iron.
Puddling: The process of decarburizing cast iron and oxidizing its slag constituents in a
reverbatory furnace. The resultant products include puddled steel, malleable iron, and
Puddling furnace: A redesigned version of older refractory furnaces, also called the
reverbatory furnace. The first of Henry Cort's puddling furnaces was built in 1784 and
was one of the most important advances in iron and steel production during the second
stage of the Industrial Revolution. The puddling furnace kept the fuel separated from the
ore to avoid recarburization and was used for producing relatively slag-free wrought iron
from pig iron, using coal or coke as a fuel. A secondary function of the puddling furnace
was the production of malleable iron and, after 1830, puddled steel. See furnace types
and refractory furnace.
Pyrotechnic pie chart: The legacy of the pyrotechnic society including its many
ironmongers and swordsmiths can be expressed as a pie chart of ecotoxins and
biologically significant chemical fallout (BSCF). CO2 emissions (the carbon footprint) is
only one small slice in a pie chart that includes methylmercury and other heavy metals,
dioxins, perfluorinated chemicals, and chlorinated hydrocarbons of all kinds
(organochlorides, polychlorinated biphenyls [PCBs], phthalates, polybrominated
diphenyl ethers [PBDEs], bisphenol-A, etc., many of which have dozens of congeners
[subspecies]). Anthropogenic radioactivity is also one slice of the pyrotechnic pie chart.
Every rain shower is a chemical fallout event. See biocatastrophe and tragedy of the
Pyrotechnological products: The glass, pottery, lime (cement), copper, bronze, iron,
steel, and tool steel alloy products produced by biomass-consuming polymetalic
pyrotechnic societies from the Copper Age to the contemporary era. Environmentally
significant byproducts of polymetalic industrial societies include carbon dioxide (CO2)
and biologically significant chemical fallout, including numerous persistent organic
pollutants (POPs), methylmercury, and long-lived radioisotopes. See apocalypse,
mercury, phenomenology of tools, post-apocalypse society, biocatastrophe, and
Pyrotechnology: The process of using fire to make glass, terra cotta (pottery), cement
(lime), iron, and other metals. Pyrotechnology is the primordial industrial basis for
civilized society. Given the environmental consequences of pyrotechnic societies,
(including climate change, resource depletion, and biologically significant chemical
fallout) after five millennia of the growth and evolution of pyrotechnology and 250 years
of the massive productivity and emissions of a full blown Industrial Revolution,
pyrotechnological consumer societies may be sailing close to the wind, i.e. approaching a
rubicon, after which biocatastrophe is inevitable. See biologically significant chemical
fallout and mercury.
Quants: Mathematical wizards, often with PhDs from Harvard, who operate the high
speed electronic trading system that makes the shadow banking network the most
profitable of all endeavors of our growing klepto-plutocracy.
Quench hardening: Making steel more homogenous by sudden cooling for the purpose
of hardening. Hardened steel edge tools were tempered (reheated to less than the forging
temperature and slowly cooled to relieve brittleness). See austenite, martensite, quench,
Quench: To cool steel rapidly in order to increase its strength and hardness. Quenching
also results in extreme brittleness of steel, requiring further heat treatment (tempering).
Brine, cold water, and oil are the fastest quenching mediums, respectively, for austenized
steel. Air is the slowest cooling medium. Ancient quenching techniques included the use
of urine and other assorted odd confabulations. See carbon content of iron and steel,
martensite, quenching threshold, and temper.
Quenching method: Method that determines hardness as a function of the rate of
cooling. Brine, water, oil, and air are the most common quenching mediums. Oil
hardened steels deform less than water quenched steels; air hardened steels deform the
Quenching temperature: Temperature required for the rapid cooling of steel. Higher
carbon content steel requires a lower temperature for efficient quenching; lower carbon
content steel requires a higher temperature.
Quenching threshold: The point at which iron containing less than 0.5% carbon cannot
be significantly hardened by quenching and, therefore, cannot be made into tool steel or
quality edge tools. A large percentage of modern steel is low carbon steel (0.2 - 0.5% cc),
which can only be slightly hardened by quenching.
Question for the reader: Will clever techno-elite entrepreneurs and bioengineers create
magical flat world solutions for the unfolding tragedy of the round world commons?
REM: Reflection electron microscope. Along with the transmission electron microscope
and scanning electron microscope, REMs are important tools used for the study of the
microstructure of metals. The HRTEM is the most advanced form of the resolution
electron microscope. See electron microscope, HRTEM, SEM, and TEM.
R. M. S. (Robert Mushet steel): Special self-hardening steel introduced by Robert
Mushet in 1868. The forerunner of high speed steel, R. M. S. contained 7% tungsten, 2%
manganese, and increased metal cutting speeds by 50% (Tweedale 1986). One important
advantage of R. M. S. was that it hardened upon being air-cooled, whereas, most steels
had to be quenched for hardening. Later, it was discovered that manganese along with
tungsten was responsible for its increased efficiency in comparison to high carbon tool
steel without alloy additions. See Mushet, Robert F. and Taylor-White.
Rabble: The tool used by the iron puddler in a reverbatory furnace to stir, form, and
remove the loup of wrought iron in the furnace.
Radanites: Jewish traders operating along the Silk Route, 500 AD - 1200 AD, who
brought Wootz steel from India to Persia for Damascus sword production.
Reaganomics: The radical philosophy promoting the crypto-fascist ideals of a selfindulgent unfettered free enterprise system manifested in the growing income disparities
of a flourishing klepto-plutocracy and its shadow banking network. The financial crisis of
2008 is a recent expression of a growing threat to sustainable economies by a philosophy
of greed, which ironically undermines our traditional free enterprise system by
empowering a few at the expense of a vast underclass of victims of financial exploitation.
Its antithesis is invisible sustainable economies where hand tools are the symbol of selfsufficiency and viable alternative lifestyles.
Reagent: With respect to Damascus steel, the acidic medium, such as lemon juice, used
to reveal the particular crystal structure that results from the forge welding of the sword
or gun barrel by a particular smith.
Rebar: Round steel bar stock commonly used for bridge and building construction. In
addition to its main constituent of pearlitic steel, a typical sample of rebar has the
following chemical composition: carbon +/- 0.45%, manganese 0.80 to 1.0%, silicon
0.2%, copper 0.3%, nickel 0.08%, chromium 0.1 to 0.2%, sulfur 0.04 to 0.05%,
molybdenum 0.04%, and phosphorus 0.01 to 0.02%. The complex chemical composition
of this commonplace steel product illustrates the ubiquitous presence of important alloys,
such as manganese, silicon, copper, nickel, and molybdenum as microconstituents in steel
products (NUCOR 2007).
Recalescence: The sudden reappearance of glowing light in metal being cooled, which
occurs during the transition of beta iron to alpha iron, which also gives off heat.
Recarburizer: Carbonaceous material, including pig iron, added to molten steel to
increase its carbon content. Recarburization is analogous to the ancient process of
submerging wrought iron in a bath of pig iron to produce Brescian steel.
Recovery: Loss of lattice dislocation through the elimination by diffusion of strain
hardening from thermal stress and the subsequent re-crystallization of the lattice structure
of a metal. Recovery can occur as a consequence of tempering but also may occur
gradually at room temperatures.
Re-crystallization: Process resulting from the use of heat treatment to form new crystal
lattice structures in deformed metals.
Recycled steel: The product of a common strategy for obtaining steel for hand tool
production before the era of bulk process steel production, such as the reuse of dull steel
files and rasps, which were commonly reforged into knives, turning tools, farrier’s tools,
and other implements requiring a high carbon content. This strategy for reclaiming steel,
commonly used by the blacksmith, was the precursor of the later use of steel scrap as part
of the charge used to make crucible and open hearth steels. See reforged steel.
Red brass: Brass consisting of 85% copper, 5% tin, 5% lead, and 5% zinc.
Red hardness: Term for the capacity of cutting tools to operate at temperatures above
Red heat: 650º - 850º C, the temperature at which the spheroidization of cementite by
mechanical treatments (hand forging, drop-forging, or rolling) can occur.
Red ocher: Finely ground hematite. The mineral iron oxide is the most valuable of all
iron ores (Fe2O3). Red ocher is perhaps best known for its ceremonial uses in indigenous
Native American burial sites.
Red short: “When impurities, such as sulphur arsenic, render the metal unworkable at a
red heat, it is said to be red short” (Spring 1917). The red short metal’s brittleness makes
it subject to shattering when hammered or forged.
Reduce: To transform an element by the removal of oxygen from a highly oxidized state
to a less oxidized state, as in the conversion of iron oxide to iron in the smelting process.
Reducing slag: Slag that facilitates the removal of oxygen. See slag.
Reductant: The reactant, e.g. carbon monoxide, which facilitates the chemical reduction
of iron oxide to iron, also producing carbon dioxide while removing the oxygen.
Reduction: The partial or complete removal of oxygen from an oxide. See oxidation
Refined iron: 1) In a generic sense, any rolled or hammered bar stock produced by a
direct process bloomery or a blast furnace finery, subject to additional mechanical or
thermal treatment (refining) in a finery to further remove slag, add or remove carbon, and
more closely align slag inclusions. Hence the terms “double refined” and “triple refined”
descriptions of refined iron that has undergone additional thermal and mechanical
treatment. See finery and refinery. 2) The result of an optional intermediate step in the
production of fine quality wrought iron in the puddling furnace, whereby pig iron is
partially decarburized in a run out (cupola) furnace in which multiple tuyères produce an
air blast that removes much of the silicon and carbon in the pig iron. The iron is then cast
in iron molds and cooled by water circulating in the hollow walls of the mold. The
resulting iron, in the form of plates or ingots, is then broken up and further decarburized
in the puddling furnace to produce high quality wrought iron. See cupola furnace.
Refinery: “Hearth used to remove silicon from pig iron preparatory to fining or puddling,
usually fired with coke” (Gordon 1996, 310); not to be confused with “finery,” an openhearth furnace used since ancient times to refine either bloomery iron or cast iron. The
refinery represented an additional step in the industrial process utilized to prepare the cast
iron for subsequent manufacturing processes, such as re-melting, rolling, or drop-forging,
especially in the 19th century. See finery.
Reflection electron microscope: See REM.
Reforged steel: A common source of tool steel prior to the era of bulk-processed steel <
1870. Typically, worn out steel rasps and files were reforged by heating and hammering
and thus recycled to make edge tools, farriers’ tools, and other steel implements.
Reforged rasps and files often exhibit vestigial traces of the teeth of the original tool. See
Refractory: In the modern era, any high temperature resistant material used to line
furnaces, i.e. “refractory” metals or ceramics. Refractory is another term for the crucible
used in cast steel production, circa 1800, which necessitated the use of special high
temperature resistant clays (+/-1500º C). The principal contribution of Benjamin
Huntsman's reintroduction of the crucible steel process (1742) was his use of high
temperature resistant Stourbridge clays to manufacture his crucibles. The unavailability
of such refractory clays in America postponed the advent of cast steel production until
1850 and the introduction of graphite crucibles. See Stourbridge clays and crucibles.
Refractory furnace: Another name for the cementation furnace, which operated through
the use of sealed refractory chambers to produce blister steel where there was no fuel to
ore contact. See blister steel, cementation furnace, puddling furnace, and puddled steel.
Regenerative gas furnace: A form of furnace that recycles and burns waste blast furnace
gases, further increasing blast furnace efficiency. The regenerative gas furnace was
introduced in America in 1857, shortly after Sir Carl Wilhelm Siemens developed it in
Regeneration: The use of waste heat and escaping gases to preheat incoming air in blast
and other furnaces.
Renewable energy resources: Energy sources that are both finite and continuously
available due to the biogeochemical cycles of the chemosphere, e.g. hydroelectric, solar,
geothermal, tidal, biomass, and wind. There are sufficient renewable energy resources to
sustain sophisticated industrial economies with a population of +/- two billion people,
who are supported by sustainable agrarian and ocean fishery communities of another +/one billion persons.
Rennwerk: The direct process reduction of iron ore to wrought iron, in which steel is
sometimes a byproduct. In Sweden, circa 1600, the production of natural steel as a
byproduct of Rennwerk was one of three options for making steel. The other two were
fining (decarburizing) cast iron (also called German steel) and carburizing wrought iron
in a steel furnace (blister steel). See German steel, blister steel, and puddled steel.
Repoussé: The formation of raised designs by hammering the reverse side of malleable
sheet metals being utilized for jewelry (etc.) design and manufacture. Combined with
chasing, the technique is utilized to create three-dimensional works of art. See chasing.
Resistance to decarburization: Property of iron being smelted to not lose carbon due to
furnace condition and slag content. Resistance to decarburization varies with the alloy
content of the steel (e.g. chromium).
Retained austenite: Austenite retained as a result of adding alloys to carbon steel, which
prevents the transformation of austenite to martensite, allowing as much as 35% of the
structure of steel to remain as non-magnetic austenite, e.g. as in stainless steels.
Tempering will eliminate most retained austenite (Shrager 1949).
Retort reduction process: A modern process for producing sponge iron by using
preheated natural gas injected into a furnace retort and forced through the furnace charge.
This process begins with charging and is followed by primary reduction, secondary
reduction, and cooling (Pollack 1977). See sponge iron.
Reverbatory furnace: “Furnace with a brick roof heated by flame. Metal on the hearth is
heated by reflection and radiation from the roof and does not come in contact with the
fuel” (Gordon 1996, 310). In the reverbatory furnace, both the hearth and the roof are
built from refractory brick, and the flame enters the furnace from the side. Henry Cort's
improved design of the reverbatory furnace in 1784 was a key event in the Industrial
Revolution, enabling the rapid production of larger quantities of wrought and malleable
iron for hand-forged hardware and tools. The reverbatory furnace was especially
important for the refining of cast iron into nearly pure wrought iron to be used in the
production of cementation steel, which was then utilized in producing pure crucible steel
(cast steel). See crucible and puddling furnace.
Riddle: A foundry sieve usually made of brass or galvanized iron cloth for removing
solid materials from molding sand.
Roasting oven: Oven commonly used before 1850 to preheat and dry iron ore before
smelting in either a bloomery or blast furnace. The roasting process was a variation of the
ore dressing process, which could also be done by manual crushing with a sledge and air
drying. The objective of these processes was to make the surface of the iron ore more
porous and, thus, susceptible to the effects of reducing gases in smelting processes.
Rockwell hardness test: “A method of determining the hardness of metals by indenting
them with a hard steel ball or a diamond cone under a specified load, measuring the depth
of penetration, and subtracting the latter from an arbitrary constant. Rockwell hardness
numbers are based on the difference between the depths of penetration at major and
minor load; the greater this difference, the less the hardness number” (Shrager 1949).
Rod mill: A mill utilized for rolling billets into semi-finished hot-rolled rods used for
wire drawing. See billet.
Rolling direction: The direction of rolling that determines the grain direction in steel or
iron bar stock. For knife and edge toolmakers cutting curves or patterns across the grain,
reforging the grain direction is necessary before a new directional pattern in the lattice
structure of the steel or forged iron tool can be created. See rolling mill.
Rolling mill: Mill used after the decarburization of cast iron in a finery or further
refinement of the anconies produced in a chafery to shape malleable iron bar stock into
useable forms, such as nail and wire rods and sheet iron, for forging into nails, tools,
utensils, and hardware by a blacksmith or shipsmith, or, later, into rails (1839) and Ibeams (> 1870). Rolling removed impurities and further strengthened the iron or steel
being rolled. In 1784, Henry Cort designed the basic form of the modern rolling mill,
adding groove rollers to rapidly shape the puddled iron produced by his recently
redesigned puddling furnace into the multiplicity of forms suitable for manufacturing
ironware of every description. Rolling mills that produced sheet iron and steel for
armorers appeared at least as early as the 16th century, during the height of the German
Renaissance, and were used by the mid-18th century to produce sheet silver for
silversmiths. Rolling mills are a ubiquitous component of all modern (>1870) bulk
process steel producing communities. Modern primary rolling mills, similar to or
synonymous with chaferies, use pit-type furnaces to soak steel ingots before hot rolling
into semi-finished products such as bar stock, slabs, billets, sheet iron, and blooms of
pure steel. A variety of secondary rolling mills further process them into finished
products. Steel ingots utilized in primary rolling mills often weigh in the range of 10 to
40 tons or higher. See cast iron, chafery, decarburization, finery, forge, furnace types,
malleable iron, bloomery, and puddling.
Round hearth: Innovative hearth design introduced in America in 1832 that increased
the efficiency of blast and bloomery furnaces.
Round world: The biosphere and its inventory of finite resources. The context for the
history of ironmongering ; the iconography of the tools thus produced tell us about the
history of technology: cascading Industrial Revolutions eventually evolve into to the Age
of Biocatastrophe as finite round world natural resources are depleted or contaminated.
Ruff, Drawn, Gadd, and Slick (steel): Early 18th century English terminology described
by Barraclough (1984a) pertaining to cementation steel (ruff) and its faggotted and
welded enhancements, i.e. spring (drawn), single shear (gadd), and double shear (slick).
German immigrants living in or near Newcastle (1680 through 1730) were instrumental
in introducing continental steel finishing strategies and applying them to the production
of improved varieties of cementation steel. See blister steel and cementation steel.
Rule of thumb: A term used to describe work patterns based on the empirical experience
of generations of ironmongers. Prior to the development of modern chemistry in the 19th
century, blacksmiths and edge toolmakers had no knowledge of the chemistry of steeland toolmaking strategies and techniques. The role of carbon in steelmaking was
unknown. Significant alloys such as manganese and silicon, which played such an
important role in determining the characteristics of iron and steel, were as yet
unidentified. Nonetheless, high quality edge tools were produced over long periods of
time from the early Iron Age to the early modern period by these repetitive, intuitive
work patterns (Barraclough 1984a). See kan of the ironmonger.
Russian iron: Sheet iron with a very hard and highly polished surface, made in Russia by
a secret process and used for steam engine boilers, etc.; also known as planished iron due
to its smooth surface. See planish.
SEM: Scanning electron microscope. Along with the reflection electron microscope
(REM) and the transmission electron microscope (TEM), SEMs are commonly used
analytical tools for analyzing the microstructure of metals by detecting low energy
secondary electrons emitted from metals due to excitation by a primary electron beam.
Detectors then map the data by noting beam position. See electron microscope, HRTEM,
TEM, and REM.
Sagger: Metal pot used to hold castings to be malleableized by annealing.
Salamander: Slab or bear of solidified cast iron produced by high shaft direct process
bloomery furnaces as unwanted waste products during the bloom smelting process. In
central Europe, these salamanders may have been the basis for recognizing the possibility
of decarburizing cast iron to produce German steel by altering the fuel to ore ratio in the
smelting process. Many salamanders were later recycled in blast furnaces due to their
high iron silicate content. See direct process, iron silicate, and slag.
Salt bath: Baths of molten chemical salts utilized for hardening and tempering a metal.
They provide uniformity of heat treatment as well as protection from oxidation.
Samurai sword: See Japanese samurai sword.
Samurai/Damascus sword surface pattern: Pattern produced by the hardening of
cementite grains during the forging process and shown as layers of bright areas in blade
cross sections after blade surface treatment by reagents. See damascene and Damascus
Sand mold: Mold made with wooden patterns that allowed precise shaping of cast iron
products, first used by Abraham Darby at his Bristol iron foundry in the early 18th
century. Sand molds replaced the earlier technique of molding with hay, clay, and loam
and could be utilized for multiple castings. Wooden patterns and sand molds paved the
way for the production of Newcomen steam engine cylinders by Abraham Darby II (c.
1722-1733). See cast iron, foundry, and molding.
Sandwich technique: One of several ancient strategies for making knives by which sheet
iron is wrapped around a steel core, which is then ground away to expose the cutting edge
Sap: Traditional term for the characteristic appearance of the fracture of blister steel
produced in cementation furnaces prior to any further thermal or mechanical treatments.
Changes in the appearance of sap express the changes in the crystal structure of iron in its
conversion from malleable iron to steel. The appearance of the fracture of blister steel
after smelting was the key to determining its carbon content. During the conversion of
bar iron to blister steel in the converting furnace, “sap” appeared to signify ongoing
changes in the crystal structure in the bar iron (“a rim of fine crystals around an unaltered
coarse central structure” [Day 1991, 270]). The sap, i.e. coarse crystals indicating blister
steel with a low carbon content (0.5 – 0.6% cc), was gradually changed into a fine
crystalline pattern and the percentage of the sap in the fracture became lower. According
to the Sheffield classification of blister steel, the sap entirely disappeared in steel having
a carbon content of 1.15% and was replaced by a pattern of fine crystals signifying fully
austenized steel. At a carbon content of 1.4 and above, coarse crystals began reappearing,
signaling increased cementite content (Barraclough 1984a, 44-5). See cementation
furnace, fracture, and Sheffield classification of blister steel.
Saugus Ironworks: America’s first integrated ironworks established on the Saugus River
in Saugus, MA, in 1646. This ironworks, which was also known as Hammersmith,
included a blast furnace, finery, chafery, and a blacksmith shop, which was used by
Joseph Jenks (later Jencks) for scythe and edge tool production. The flux used at this
blast furnace was a unique form of limestone called grabbo, brought by boat from nearby
Nahant. The Saugus Ironworks also functioned as one of New England’s first known
Satetsu: The iron sand used by samurai sword makers to produce a raw steel bloom
(kera) in a direct process open-hearth clay furnace (tatara) prior to the final forging of the
sword. See bloom, breakdown furnace, and tatara.
Scanning electron microscope: See SEM.
Scarf weld: An ancient technique for making knives and swords that involves the steel
being laid on cold iron and then wired, heated, and welded to create a steeled edge tool.
Also, see Bealer (1976) for a contemporary description of the blacksmith’s art of scarf
welding, i.e. the hammering and welding of two overlapped pieces of metal. See forging.
Secondary hardness: Phenomenon of the resumption of hardening that occurs during the
tempering of high alloy steel after the initial quench hardening.
Self-hard: The first commercial alloy steel, R. M. S., invented by R. F. Mushet in 1868
in his Forest of Dean ironworks. He added 8% tungsten to the molten steel, allowing it to
harden in the air with no rapid quenching in water. See Mushet, Robert F. and R. M. S.
Self-hardening steel: High carbon alloy steel, which hardens at room temperature
without oil or water quenching. Its alloy content slows the transformation of austenite to
Semi-steel: High-grade grey cast iron, which is made stronger by the addition of steel
scrap in the charge and contains lower silicon, phosphorous, and total carbon content than
grey cast irons (3.2% versus 3.4% for grey cast iron and 3.45% for soft grey cast iron). In
contrast, the carbon content of white cast iron and annealed malleable cast iron is 2.75%.
Many of the pieces of machinery on display at London’s Victoria and Albert Science and
Technology Museum made between 1800 and 1840 may be semi-steel. See carbon
content of iron and steel and cast iron.
Shadow banking network (SBN): Along with multinational corporations, the SBN is a
significant component of the klepto-plutocracy that dominates American economic
activity in the 21st century. Based on high speed trading, the sale of collateralized debt
obligations and credit default swaps, currency manipulations, and parasitic hedge funds,
the SBN is dependent on computerized mathematical formulas concocted by “quants”,
e.g. Harvard PhDs with a doctorate in math. While traditional banking institutions
provided essential services to local businesses and homeowners, the SBN utilizes
hundreds of trillions of dollars of debt as “bank assets,” which are constantly traded in a
world banking network “casino”. The resulting commissions and profits, which derive
from the manipulation of gross world assets, are collected by a tiny percentage of
individuals with extraordinary incomes, i.e. the klepto-plutocracy.
Shaft furnace: Common form of open-hearth furnace for smelting iron throughout the
early Iron Age, along with the bowl furnace. Shaft furnaces evolved into blast furnaces as
the length of the shaft grew in size. Early Iron Age shaft furnaces were difficult to control
and often produced iron with a heterogeneous carbon content, ranging from liquid cast
iron and natural steel to malleable iron, though low carbon wrought iron might have been
the goal of the smelt. The high shaft bloomery “Stucköfen” furnace of south Germany
was the final stage in direct process iron production (circa 1500 AD). The larger shaft
furnaces which followed were true blast furnaces producing cast iron that needed
refinement into wrought iron and/or steel. See bloomery, bowl furnace, German steel,
open-hearth furnace, slag pit furnace, and slag-tapping furnace.
Shaft hole vs. Socket hole: Two alternative methods of securing handles to adzes, axes,
and hammers. In Neolithic Europe, socket hole tool design was “the traditional method of
hafting the head to a knee-shaped, cleft handle. In the course of time, the shape of the
head was drastically modified, yet even when casting was adopted they still kept to the
old way of lashing the head to the shaft” (Goodman, 1964, 14). In the early Iron Age in
Europe, some socket holes were of square design; “It was about this time, between 500
and 200 B.C., that this traditional method was finally abandoned, and the ax assumed the
form familiar to us today, a heavy wedge-shaped forging, with the shaft-hole, usually
elliptical in cross-section, made by folding a rectangular billet of iron in the middle,
leaving the eye parallel to the cutting edge” (Goodman, 1964, 20). Goodman illustrates
shaft hole axes and adzes dating as early as 2900 BC, including Mesopotamian tools
utilizing this modern form. One of the mysteries of history is why primitive socket hole
tool forms continued to be used in Cis-Alpine Europe... “One of the most curious blind
alleys in the whole checkered history of human progress” (Goodman, 1964, 14). See
Goodman (1964), Childe (1925), and Brack (2008).
Shear steel (Sheaf steel): Steel resulting from the reworking of blister steel to increase
purity and homogeneity by taking cut bars of blister steel and piling, reheating, re-rolling,
re-hammering, and re-welding them; also called “spring” steel when rolled into sheets for
saw-makers. The mechanical working of bundled bars of blister steel more evenly
distributed its carbon content. It is called shear steel “because blades for shears for
cropping woolen cloth were always made this way” (Spring 1917, 117). The term shear
steel also derives from the simple process of shearing blister steel bar stock before it is
repiled and reforged into higher quality steel. Prior to the production of crucible steel,
shear or “sheaf” steel was the highest quality steel available. Implements marked “shear”
or “sheaf” were usually manufactured before 1784, after which the designation “cast
steel” became more commonplace. Many a shipwright’s tool was made from shear steel
by New England’s edge toolmakers and sword cutlers. Cutlers probably used it for
swordmaking due to its heterogeneous carbon content, in contrast to the homogenous
carbon content of pure cast steel.
Shear stress: The stress threshold for crystal flow (slip and creep). Shear stress in the
lattice structure of metals is temperature dependent, decreasing with increasing
temperature and reaching zero at the melting point.
Shearing movements: Rapidly occurring microstructural changes typified by the
acicular formation of martensite and the twining formations in the intermediate phases of
bainite. The slow rate of nucleation, as in the formation of pearlite, is the antithesis of
Shearing stress: Stress that changes the angles between the faces and the lengths of the
diagonals of microstructures, acting tangentially to the surface of contact without
changing the lengths of the sides of the structure undergoing stress. “Shearing stress
intensities are of equal magnitude on all four faces of an element” (Baumeister 1958, 523). The stress threshold for crystal flow (slip and creep) and shearing stress in the lattice
structure of metals is temperature-dependent, decreasing with increasing temperature and
reaching zero at the melting point. See stress fields, slip, creep, crystal structure of
metals, and martensite shearing.
Sheet iron: Iron sheets produced by plating mills beginning in the early 18th century for
use as hoops by coopers and tin plate by whitesmiths.
Double Shear Heat
Steel Through Heat
Fine crystals throughout
Coarse crystals throughout
Very coarse and facetted crystals
Table 4. (Barraclough 1991, 270) [sap: unaltered coarse central structure]
Sheffield classification of blister steel: The classification of the visual appearance of the
unaltered microstructures of the central portion of a piece of blister steel bar stock after
manual fracturing. The visual appearance of these microstructural formations was called
“sap” by 18th century English steelmakers and based upon the coarseness of the grain
structure as shown in Table 4.
Sheffield plate: Fused copper and silver, developed in the late 18th century as imitation
silver by Thomas Boulsover (Tweedale 1987). Sheffield plate is usually in the form of
sheet copper sandwiched between two thin layers of silver.
Shiage: The rough grinding and shaping of both sides of a sword blade to be tempered
using a two-handled drawknife made from a steel sword. Shiage is the first step in the
heat treatment of the Japanese sword. See Japanese samurai sword, naginata, tsuchioki,
yaki-ire, and yaki-modoshi.
Shingler: The manipulator of the puddled ball being hammered at a puddling furnace.
Shingle the loup: The first step in manufacturing wrought and malleable iron bar stock.
The forge master hammers the hot metal bloom of wrought iron to expel the impurities,
shape the bloom, and align the silicon fibers remaining in the bloom to enhance the
tensile strength of the metal. Shingling preceded the fining (reheating, re-hammering) of
wrought or malleable iron, which was then shaped into bars called anconies. See
merchant bar, piled wrought iron, puddled iron, refined iron, and rolling direction.
Shipsmith: A blacksmith with a specialty in making both the iron fittings and edge tools
needed to construct a sailing ship. Ubiquitous in England, northwestern Europe, and
colonial New England before 1800, shipsmiths sometimes also made anchors. Both the
North River and the Taunton River in the bog iron country of southeastern Massachusetts
were the location of the forges of numerous shipsmiths working between 1650 and 1750.
After 1800, trade specialization resulted in shipsmithing and edge toolmaking being
regarded as separate trades, as illustrated in the 1856 Maine Business Directory. The
shipsmiths and edge toolmakers listed in Maine directories lived in coastal shipbuilding
communities or nearby upstream towns with water power for trip hammers and easy
access to the Maine coast by river. See Art of the Edge Tool (Brack 2008), adz, broad ax,
Siemens-Martin process: Process that enabled the melting of any combination of cast
and wrought iron to make steel. This process combined the melting of pig iron in openhearth furnaces by the Siemens process with the addition of molten pig iron to the charge
utilized by the Martin process, which originated in France. In 1865, the Martin brothers
utilized the regenerative gas furnace designed by Siemens to develop one of the first bulk
steelmaking technologies, which was later perfected in 1877 with the introduction of
basic hearth linings. After 1877, the basic open-hearth process produced more tonnage of
steel than the acid open-hearth process, which could not utilize iron ores or pig iron high
in phosphorous. See open-hearth furnace and Siemens open-hearth furnace.
Siemens open-hearth furnace: Along with the Bessemer process, the most important
steel production furnace type from 1870 to the mid-20th century. The Siemens openhearth furnace replaced the Siemens-Martin pig and scrap furnace, providing better
quality control of the steel production process by the addition of carefully measured
amounts of iron-oxide-producing iron ore to the slag after the melt was underway. This
addition of iron ore during the melt caused spectacular boiling reactions at the slag/metal
interface, as a result of the burning of carbon monoxide, also differentiating the Siemens
open-hearth furnace from the Siemens-Martin furnace.
Siemens regenerative gas furnace: Gas furnace adapted for open-hearth furnaces as
well as for more efficient crucible steel production, both in England and America;
developed in 1857.
Silent majority: The well meaning, usually convivial, and often Christian majority of the
90% who are neither Tea Party Taliban nor crypto-fascists. They are an economic
underclass whose indirect computer drive exploitation is the source of the ever growing
power of the American klepto-plutocracy.
Siliceous slag: The slag or iron silicate content in wrought iron (1.0 - 3.0%). Its content
depends on the type and extent of mechanical treatment of iron by the smith with hammer
and anvil, water-powered trip hammers, or rolling mills. Most siliceous slag is removed
by the blast furnace in indirect iron and steel production but remains in wrought iron after
direct process bloomery smelting. After bloomery-smelted wrought iron is refined in a
finery furnace, variable amounts of slag remain in the iron, depending on the refining
techniques and objectives of the finer. These iron-silicate microconstituents play an
important role in enhancing the plasticity of edge tools forged from malleable iron and
give older edge tools their convivial “feel” and ease of sharpening in contrast to most
“hard” modern edge tools and plane blades. Trace quantities of silicon may also be added
to cast steel as the result of chemical reactions in the walls of the clay crucibles, which
shed tiny amounts of silicon-bearing material back into the crucible steel. The role of
silicon as a microconstituent in the production of fine edge tools has not yet been
scientifically documented. See carburize, forge, forge welding, and silicon as a softener.
Silicon: An important deoxidizer during the smelting of iron that softens cast iron and
increases its fluidity by facilitating the formation of graphite from carbon, strengthens
ferrite by making it more resistant to oxidation, strengthens the microstructure of pearlite
by the solid solution hardening of ferrite, decomposes other carbides, and enhances
graphite formation. When present in steel in concentrations up to 2%, silicon intensifies
the tendency of molybdenum, manganese, and chromium to increase hardenability and
enhance carbide formation. It may also soften edge tools, increasing their ductility. See
Silicon as a softener: The capacity of silicon to help precipitate chemically combined
carbon into free graphitic flakes. The higher the silicon content is the more combined
carbon becomes graphite. Silicon greatly increases the machinability of cast iron pieces,
such as iron valves and hollowware. Silicon also plays a role in making the old cast steel
plane blades and edge tools from Sheffield and Pittsburg superior to the tools drop-forged
from steel made in the modern electric furnace. Silicon as a microconstituent produces a
softer more congenial cutting edge, traditionally preferred by shipwrights, timber
framers, and case furniture makers. The silicon content of edge tools may also increase
durability by increasing the tensile strength of the cutting edge, relieving the brittleness
characteristic of many modern edge tools. See siliceous slag.
Silicon steel: An alloy steel containing silicon. If steel contains 1 to 2% silicon, it is very
tough and suitable for automobile springs. With 3 to 5% silicon, it has improved
magnetic properties and is often used in electrical appliances.
Silver steel: “A soft and ductile steel with a low carbon content. It is supplied ground to a
bright finish in small-diameter rods. It is useful for model makers and in laboratories. It
cannot be hardened owing to its low carbon content” (Salaman 1975, 247). Noted by
Cyril Smith as “the first alloy steel to become – undeservedly – popular” (Smith 1960,
141). Stodart and Faraday utilized it during their attempts to duplicate Damascus steel.
Also noted by Lee (1995) as follows “This mark is commonly found on old handsaws…
when it was discovered that adding a percentage of chromium to high carbon steel not
only increased the hardness and toughness but also gave the steel a bright silvery finish
that improved rust resistance, the alloy was quickly dubbed silver steel” (Lee 1995, 20).
Simple machine: “In physics, a machine is any device that can be used to transmit a
force and, in doing so, change its size or direction… simple machines include the inclined
plane, the lever, the screw, and the wheel and axle. All of these machines illustrate the
concept of work” (Maiklem 1998, 26). The pulley and block and tackle are simple
machines. See machine, Tools Teach: An Iconography of American Hand Tools (Brack
2013), turbine, and work.
Singer, Nimick & Co.: Established in 1849 in Pittsburgh, by 1853, Singer, Nimick &
Co. was the first reliable producer of cast steel in the US (Gordon 1996). It is unknown to
what extent this company supplied edge toolmakers, such as Timothy Witherby, the Buck
Brothers, and the Underhills, who manufactured cast steel woodworking tools during and
after this time.
Sinter: To produce hard solid metal or ceramic artifacts from atomized powders (e.g.
iron powder) using hydraulic dies operating at high temperatures and under high
pressure. See powdered metallurgy.
Skelp: Strips of mill steel used to produce lap-welded and/or butt-welded steel tubes by
drawing the strips through a bell-shaped pattern at welding temperature.
Skilled labor shortage: One of the ironies of the Age of Information Technology and the
early years of the Age of Biocatastrophe is a growing skilled labor shortage despite
intensifying structural unemployment caused by the IT revolution, CNC technologies,
and the increasing use of robots to execute industrial and manual functions. Artisans and
craftspersons skilled in the use of hand tools, born-again ironmongers as it were, are
increasingly in short supply for maintenance and repair of the infrastructure of a global
consumer society that still needs plumbers, carpenters, electricians, mechanics, and
communications systems specialists. The widespread deletion of vocational education, a
rapid decline in the quality of public education, and a failure to invest in technical
training of a contemporary workforce skilled in the use of hand tools engender this
Slack quenching: To quench at a rate too slow to produce martensite. When slowly
cooled, austenite instead forms pearlite, lamellae of ferrite, and cementite arranged by
twinning into Neumann bands. Slack quenching “worked best on a relatively low carbon
material. Damascus swords were quenched slowly in oil, or by a current of air” (Smith
1960, Footnote 24). See acid process, basic process, Damascus steel, Damascus sword,
ferrosilicate, flux, and manganese.
Slag: The non-metallic waste product of bloomery and blast furnaces, usually a silicate of
calcium, magnesium, and aluminum, which covers the molten metal in the smelting
process. Varying amounts of iron oxides, especially iron silicate, also characterize slag.
The slag of small bloomery and open-hearth furnaces contains more wasted iron in the
form of iron silicate than the slag of more efficient blast furnaces, especially if limestone
was used as the flux in the blast furnace. The slag is usually skimmed off of the molten
metal prior to tapping or pouring. See blast furnace, bloomery, salamander, and siliceous
Slag heap: The siliceous slag-bearing waste products of bloomeries and blast furnaces;
the tell-tale evidence of smelting activities. See slag.
Slag pit furnace: A common form of early bowl or shaft furnace. The slag accumulated
in pits dug underneath the furnace. High in iron oxide, many slag blocks were recycled in
blast furnaces, which more efficiently reduced their iron content. Slag pit furnaces were
often moved for re-firing when the slag built up under the firing chamber, resulting in the
accumulation of huge quantities of slag in early Iron Age smelting locations, such as the
Black Mountains of southern France.
Slag-tapping furnace: A furnace in which slag was tapped by draining liquid slag from
the furnace using a trench; the most common form of direct process furnace from the
Roman era to the late medieval period (Tylecote 1987).
Slag viscosity: “The viscosity of a fluid is a measure of its resistance to gradual
deformation” (Wikipedia 2013). Slag viscosity is increased by low iron oxide content, as
in efficient blast furnace operation, in contrast to the higher iron oxide content of
bloomery slag. The addition of lime or feldspar as slag fluidizers lowers slag viscosity,
increasing the efficiency of blast furnace operation.
Slater, Samuel: (1768-1835). Builder of America’s first automated textile mill on the
Blackstone River at Pawtucket, RI, in 1793. After emigrating from England, Slater was
able to copy the designs of the machinery invented by Richard Arkwright and used in
English textile mills. Unlike England’s coke-fired steam-powered textile mills, American
industry relied upon water power as its industrial prime mover well into the 19th century.
Slick (slice): 1) Long chisel for smoothing the planking of a wooden vessel; particularly
useful on surfaces not accessible to a lipped adz; also called a slice by many Downeast
shipwrights. 2) Small hand tool used by molders in a foundry to smooth and finish a sand
cast prior to the casting process. See core, drag, foundry, hollowware, molder, and sand
Slip: Grain displacement that occurs within the crystal lattice structure of metals during
deformation. See plastic deformation, space lattice, and stress fields, and unit cell.
Slip interference: The collision of crystals within the lattice structure of metals during
slip events, which causes internal stress and hardening of the metal. See stress fields and
Slip lines: The bands observed on stressed metals due to the deformation of their crystal
structure after cold working by any mechanical process. See slip interference.
Slip plane: That component of the lattice structure of a metal that undergoes plastic
deformation during mechanical or thermal treatments.
Slitting mill: A mill with machinery used to cut iron bar stock into rods for use in nail
making or wire drawing. Often associated with the chafery in integrated ironworks,
slitting is a further step in the refining of wrought iron. The first slitting mill was
established in the Kent district of England in 1590. Related technology for making wire
for wool cards was implemented in England in 1566. Slitting mills were first established
in New England in the late 17th century.
Smelt: To reduce a metal ore, e.g. iron, by a chemical reaction in a high temperature
furnace; “any metallurgical operation in which the metal sought is separated in a state of
fusion from the impurities with which it may be chemically combined or physically
mixed” (Shrager 1949, 377). The fundamental chemical process in the smelting of iron
ores involves the burning of a carboniferous fuel which reduces the iron oxide ore by
removing oxygen, ideally producing pure iron (ferrite) and CO2. The carbon in the CO2 is
derived from the burning fuel and the O2 from the reduced ore. Impurities in the iron ore
are removed by the addition of flux to the smelting process and are drained out of the
smelting furnace as slag. In the smelting of iron ore, the melted or partially melted
product is either cast iron produced in the indirect process after cooling/solidification or a
semi-pasty bloom of either wrought iron or malleable iron produced by direct process
reduction with variable carbon content, usually lower than 0.5%. In the smelting process,
the burning fuel removes oxygen from the iron oxide ore, providing iron with a range of
carbon content. Varying amounts of iron oxide are not reduced in the smelting process
and are transferred to slag as accidental waste products, usually in the form of iron
silicate or siliceous slag. See blast furnace, bloomery, furnace types, reduction, siliceous
slag, and slag.
Smelting furnace: A furnace used to reduce iron and other metals from their chemically
combined state, e.g. iron oxide, to a metallic state by dissolution (reduction) of the
chemical bonds of the iron oxides or other iron ores. The most common products of the
smelting furnace are wrought iron with < 0.08% carbon content, ranging as low as 0.02%
carbon (pure ferrite) and malleable iron with a carbon content ranging from 0.08 – 0.5%.
The lower the carbon content of the iron produced by the smelting furnace, the more
malleable and ductile is the wrought iron being produced. In the smelting furnace, the
iron bloom coalesces at 730º C as a plastic mass that is easy to shape by hammering. If
the smelting furnace reaches a temperature of 1150º C to 1200º C, the iron absorbs
carbon. At 3.5% carbon content, the eutectic (melting) point is reached, and liquid cast
iron is produced, due to the lower melting temperature of iron with a high carbon content.
Wertime (1962) notes the difficulty of controlling the smelting process in early shaft and
bowl furnaces as follows:
The small furnaces to be found in ancient China, medieval Europe or modern Africa
posses the capability to yield high-carbon cast iron. Any effort to avoid this result and
to produce low carbon wrought iron or steel, by means of a process involving only a
single step, became a matter of exquisite human and technical restraint. (Wertime
See bloomsmithing, furnace types (before 1870), natural steel, smelt, and wrought iron.
Smithing forge: Small forge used by blacksmiths, shipsmiths, farriers, cutlers, and other
tradesmen to make bolts, horticultural tools, ships’ hardware, ox and horse shoes, and
hunting knives and swords. The blast was often powered by accordion bellows. Smithing
forges were supplied with iron bar stock produced at direct process iron-smelting
furnaces or at integrated ironworks from cast iron that had been fined into iron bar stock
in fineries and chaferies. After the appearance of the reverbatory furnace and the
development of modern rolling mills (1784), wrought and malleable iron bar stock of
more uniform quality could be produced for use at a smithing forge. See blacksmith,
integrated ironworks, merchant bar stock, and iron-smelting furnace.
Smithy: A blacksmith’s workshop for light duty forge welding, in contrast to a larger
forge equipped with a trip hammer for heavy duty work. See trip hammer and waterpowered drop hammer.
Soaking pits: Modern underground furnaces used to heat steel ingots to a temperature of
2,200º F before rolling and milling.
Softening temperatures: The temperature range at which high carbon steel without
alloys softens. The softening temperature range is 600 – 800º F (Pollack 1977).
Solder: A combination of tin and lead used by tinsmiths for joining tin plate since the
mid 16th century; now commonly found in contemporary workshops and, recently, the
subject of concern due to the health threat from lead poisoning. An alloy of two or more
metals used for joining other metals by surface adhesion. See alloy.
Solidification range: The range of temperatures that culminate in the freezing or
solidification of a metal. See liquidus and solidus.
Solid solution: The dissolved composition of two metals within each other in their solid
Solid solution austenite: Austenite formed when carbon solubility suddenly increases at
the critical temperature (Bain 1939).
Solidus: The lower curve in a constitutional diagram, which is the locus of temperatures
at which each alloy has completed solidification. See Barraclough’s constitutional
diagram in Appendix VI.
Solingen: An important center in West Germany for the production of cutlery and
pattern-welded sword blades, bayonets, and knives; located in close proximity to Cologne
and other important steel-producing centers, such as Remscheid and the Rhine River.
Solingen was an important steel producing community as early as the Middle Ages;
Damascus steel production techniques and samples of Wootz steel may have been
brought to Solingen during the Crusades. Thousands of individual toolmakers and
swordsmiths used small forges to produce cutlery, swords, and edge tools from the early
Middle Ages to the late 19th century.
Sorby, Henry Clifton: The foremost of all English metallurgists; the first scientific
researcher to document the microstructure of pearlite and note re-crystallization as the
mechanism of recovery of crystalline polarity in ferrous metals (Smith 1960). Sorby, a
resident of Sheffield, England, produced the first photomicrograph studies of the
structure of iron and steel by polishing and then etching thin sectional slices of various
forms of ferrous metals with a dilute solution of nitric acid. He exhibited some of his
samples at the British Association in 1863 and wrote a paper on his research about the
relationship between the physical properties and microstructure of metals in 1864.
However, it was not until he gave a lecture at Firth College in Sheffield in 1882 that his
research on the microstructure of ferrous metals became widely known.
Sorinaoshi: The further heating and hammering of the Japanese sword after tempering
and the removal of the clay enclosure for the purpose of making fine adjustments.
Source points of biologically significant chemical fallout (BSCF): During the smelting
of iron and the production of steel, facilities that burn biomass fuels are source points for
biologically significant chemical fallout, including sulfur dioxide and, most especially,
methylmercury derived from the burning of coal. Carbon dioxide (CO2) produced by the
combustion of any biomass fuel can also be considered a form of BSCF due to its role in
cataclysmic climate change. After 1950, the rapid increases in the production of
ecotoxins, including persistent organic pollutants (POPs) derived from pesticide,
consumer product, and electronic equipment manufacturing, have dominated the
contaminant pulses of BSCF. Nuclear power and fuel and weapons production facilities
are source points of biologically significant anthropogenic radioactivity. See biologically
significant chemical fallout.
Space Lattice: “The orderly geometric form into which atoms tend to arrange themselves
during the process of crystallization” (Shrager 1949). “Every point of a space lattice has
identical surroundings… There are 14 space lattices. No more than 14 ways can be found
in which points can be
arranged in space so that
each point has identical
1943, 2-3). Space lattices
are expressed through
their system of axes, each
of which possesses
i.e. equality of angles and
links. The basic unit of a
Figure 1. Space lattice (Shrager 1961, 5)
space lattice is the unit
cell, which, in metallurgy, has three common forms: body-centered cubic (BCC), facecentered cubic (FCC), and close packed hexagonal (CPH). While there are a limited
number of forms of the space lattice, there are an unlimited number of crystal structure
patterns that can exist within those forms. When in the form of low carbon ferrite, iron is
characterized by the body-centered cubic form of the space lattice of its crystal structure,
which provides strength in comparison to the face-centered cubic form of ductile metals,
such as copper and gold. When heated beyond the temperature of 910º C, the allotropic
form, and, thus, the space lattice structure, change to the face-centered cubic form
(austenite). Metals that lack plasticity, such as cobalt and titanium, have a close packed
hexagonal crystal structure. See allotropic form, Barrett (1943), lattice reorientation,
plastic deformation, Shrager (1949), and unit cell.
Spalling: The surface cracking and flaking of metals resulting in the creation of small
particles of loose metal.
Spangle: The surface patterns on watered steel swords, derived from the crystal structure
of the steel. See Damascus steel, Damascened steel, and especially Cyril Smith (1960).
Spark test: A rule of thumb test often used in the 19th and early 20th century for quickly
identifying iron and steel types, also possibly useful in contemporary home workshop
situations. The following spark patterns are generated using a powered dry wheel for
grinding the item:
Long yellow streaks, becoming leaf like in shape before expiring
More variety in streak length, with smaller leaves and some sparking
Almost no leaf, some forking, great variety of streak length, sparking nearer the
No leaf, bushy spark pattern, forking and sparking starting very close to the wheel;
less bright than medium-carbon steel
Small leaf before streaks fork to form sparks
Faint red streaks forking at the tip
Bright yellow streaks with a small leaf end (Lee 1995, 22)
Spathas: Doubled-edged pattern-welded broad swords used by the Goths to defeat the
Romans at the battle of Adrianople (400 AD). In 53 BC, the Romans had defeated the
Gauls with the help of their superior swords, made by the same Celtic metallurgists
(swordsmiths) in Noricum, who now made the Spathas for the Goths to use against the
Romans (Gardner 1892). See Celtic metallurgy, Iron road, pattern-welding, and Styrian
Spathic ore: Another name for the manganese rich iron ore from the Styrian and
Carinthian section of Austria. See German steel, manganese, spiegeleisen, and Styrian
Spectrometry: The measurement of spectroscopic interactions. An instrument that
performs such measurements is a spectrometer or spectrograph. A plot of the interaction
is referred to as a spectrum. The primary form of modern spectrometer used to study
ferrous metals is the energy dispersive x-ray spectroscope (EDX), which uses x-rays to
generate the electro-magnetic waves that characterize each unique electronic structure.
Spectroscopy: The study of the interaction between radiation (electromagnetic radiation,
or light, as well as particle radiation) and matter.
Spheroidize: To soften high carbon steels by freeing ferrite from cementite, therefore
causing the cementite to assume a globular crystal structure, facilitating machinability.
Spheroidizing occurs after initial heating just above the transformation temperature,
followed by lengthy heating just below the critical point (annealing). See spheroidization
Spheroidization: Production of round-shaped cementite carbide microstructures, often in
veins (nanotubes), by repeated hammering and reheating, for example, samurai and
Wootz steel Damascus sword blades. “Forging at temperatures below the temperature of
cementite formation from austenite, Acm (Acm ≈ 850ºC) leads to the destruction of needlelike cementite and, after heat treatment, to spheroidization of Fe3C …Annealing above
Acm would made the cementite disappear” leading to the loss of properties characteristic
of high quality swords or edge tools, i.e. the combination of toughness (resistance to
fracture) and the retention of hardness on the cutting edge (Levin 2005, 905). “Small
additions of Mn, Si, P + S seem to enhance the breakup of cementite into spheroidized
agglomerates” (Levin 2005, 906). The recent development of the high resolution
transmission electron microscope (HRTEM) has allowed a more detailed examination of
carbide microstructures in forged steel, resulting in a better understanding of the
nanotubes and nanowires that are characteristic of the presence of superplasticity in steels
and other metals, including swords and edge tools. See nanotubes, nanowires,
spheroidize, and superplasticity.
Spiegeleisen: In its modern form, a pig iron containing 15 - 30% manganese and 4.5 –
5.0% carbon, added to steel both as a deoxidizing agent and to raise the manganese
content of the steel (Shrager 1949). Spiegeleisen also refers to cast iron derived from ores
containing naturally occurring manganese, which was used to produce “German” steel
(1400 to 1875 AD). This cast iron was produced in a blast furnace using manganese-rich
siderite iron ores (+/- 2.0% manganese), resulting in cast iron with a bright, mirror-like
appearance or “mirror iron,” a brittle fracture, and manganese content of 5.0 - 10.0% in
its final form. As a component of the flux manganese preferentially combined with sulfur
and phosphorus, and their elimination in and as slag allowed more homogeneous carbon
distribution within the austenitic iron after the slag formation (manganese oxidation)
process. On September 22, 1857, Robert Mushet patented the modern form of
spiegeleisen as an addition to Bessemer steel to relieve its “burnt out” quality (Fisher
1963) by enhancing its strength, durability, and hardness. The addition of spiegeleisen
was a key step in the successful adaptation of the Bessemer process to a wide variety of
industrial applications (e.g. production of steel rails and machinery). The widely varying
amounts of manganese in various forms of cast iron produced from 1350 to the present
time, and its presence in a wide variety of modern alloy and tool steels illustrates its
importance as an alloy of iron and steel. See alloy steel, German steel, manganese, Noric
steel, Styrian steel, and tool steel.
Sponge iron: A modern term for the bloom of wrought or malleable iron produced by
direct process smelting. See bloom, malleable iron, wrought iron, and direct process.
Spoon adz: Adz used by shipwrights for roughing out large mortises when framing a
wooden ship; also called the “gutter adz” in America. Finish work on such mortises was
completed with the use of the mortising chisel, lipped adz, and, in some cases, a slick.
Spring steel: Blister or weld steel that was reheated, re-hammered, and then rolled as
sheet saw steel to increase purity and homogeneity. Spring steel was the principal
constituent of high quality handsaws before the appearance of cast steel and was also
used for coach and other types of springs. Rolled cast saw steel was still labeled “spring
steel” on hand saws at least until the late 19th century, as were Henry Disston’s “London
spring steel” saws. The mechanical and thermal treatments used during these processes
served to increase the purity and hardness of the saw steel. Differing mixtures of alloys
were sometimes added as micro-constituents during the forging of spring steel. Such
formulations were often the subject of extreme secrecy on the part of the steel producers
and saw manufacturers, sometimes one and the same. See blister steel, cast steel
definition 1, piling, and shear steel.
Sprue: Representative test piece of cast iron, which shows its approximate composition
by its fracture. For example, a gray iron fracture indicates a high silicon content.
Spurrier: A smith who forged steel spurs and stirrups in the medieval era (Gardner
Stainless steel: Steel that contains 18% chromium and 8% nickel, has high tensile
strength, and resists abrasion and corrosion, developed by Harry Brearley in 1913 for
cutlery. The AISI classification system for steel defines stainless steel as having a
minimum of 10% chromium, with or without other alloys. In general, stainless steels are
defined as low carbon-high alloy steels. Stainless steels are further grouped according to
their heat treatment dependant microstructures: Austenitic – ferritic – martensitic.
Martensitic is hardenable by heat treatment; austenitic and ferritic stainless steels are not
hardenable by heat treatments. Many types of alloy steels and tool steels contain
chromium in lesser quantities. Stainless steel is one of the most important steels produced
in the modern electric arc furnace. Martensitic steel (AISI types) 414, 420, 420F, and
440F are often used for the drop-forging of a wide variety of stainless steel hand tools.
See the AISI-SAE classification system in Appendix IV.
Stamping: The process of manufacturing drop-forged tools or hardware (e.g. gun parts)
by forcing red-hot low carbon steel or malleable iron into dies. See drop-forging, low
carbon steel, and malleable iron.
Steam-driven tilting band saw: Unique form of power saw for framing out wooden
ships. Along with the water-powered circular saw, the appearance of the tilting band saw
(c. 1850) was an important step in the mechanization of shipbuilding activities, replacing
the pit, frame, and whip saws for many functions.
Steam engine: By 1669, Thomas Savage’s steam pump for recovering water from coal
mines to save England’s threatened forests was improved by the addition of Newcomb’s
use of pistons to power the pump. Radically improved in the 1760s by Watts’ use of
improved cylindrical engine pressure vessels, the steam engine became a prime mover of
the first Industrial Revolution. In the 1830s, Joseph Nasmyth designed a high pressure
steam engine, which was more powerful due to recycled waste steam and played a major
role in the development of railroads and, after 1840, the factory system of mass
production. In 1884, the development of steam turbines (rotary steam-powered motors)
paved the way, after 1900, for the ascendancy of petro-chemical electrical man, and then
after 1945, petro-chemical electrical nuclear man where steam engines were the prime
movers of nuclear power plants.
Steam turbine: A form of heat engine driven by the kinetic energy of steam in contrast
to the piston-driven steam engine, which is powered by the pressure of a volume of steam
on a piston. See heat engine and steam engine.
Steel: A thermodynamically stable alloy of iron containing from 0.2% to 2.0% carbon.
Steel often contains substantial quantities of manganese (±1%) and silicon (±0.6%), and
trace amounts of sulfur and phosphorous as microconstituents. In contrast, wrought iron,
a silicon slag-bearing iron alloy, is defined as containing <0.8% carbon content. Cast
iron, which is much more brittle than steel, is an iron alloy containing more than 2.0 2.2% carbon; most cast iron products contain 3 - 3.5% carbon. Note: the upper and lower
limits of carbon in steel vary among information sources. A recent source notes that most
steels contain levels of carbon from about 0.1 - 0.8%, depending upon the desired
properties and applications (Sherby 1995, 10-11). The advent of the modern open-hearth
electric furnace process allowed the manufacture of a wide variety of steel alloys,
therefore opening up the floodgates for tool and machinery production of every
description, i.e. the classic period of the Industrial Revolution. The magic of steel is its
range of properties. Steel is malleable at high temperatures. Its ductility, malleability, and
capacity for being welded decrease in proportion to its rising carbon content. Mechanical
and thermal processing determines its microstructure. If containing in excess of 0.5%
carbon (the quenching threshold of steel), steel has the unique quality of being greatly
hardened by sudden cooling (quenching), after which it is very brittle and fractures
easily, requiring further heat treatment by tempering to soften the martinized steel for
edge tool production and other uses. The most remarkable quality of steel is its capacity
for being tempered to many degrees of hardness, allowing the production of a wide
variety of tools and weapons from ancient to modern times. Quality edge tool
manufacturing is, in part, contingent on the amount of time spent by the edge toolmaker
on the repeated slow reheating, hammering, and slow re-cooling (annealing) of the steel
cutting surface of the edge tool. See alloy steel, annealing, bulk process steel, carbon
content of iron and steel, German steel, low carbon steel, martenize, microstructure,
natural steel, puddled steel, quench, stainless steel, tempered alloy steel, and tool steel.
Steel blooms: Steel produced as semi-solid or solid masses by the following processes:
natural, Brescian, German, blister (cementation), and puddling. Liquid steel, in contrast,
was produced in crucibles and by modern bulk steelmaking techniques, such as the
Steel furnace: Prior to the introduction of modern forms of steel furnaces, the term “steel
furnace” was synonymous with cementation furnace, which were sandstone furnaces that
kept the fire separated from the ore being smelted. Cementation furnaces for blister steel
production replaced shaft furnaces for producing German steel in England in the mid to
late 17th century and began appearing in America after 1720. See cementation furnace
and furnace types.
Steel microstructure: The principal allotropic forms of the microstructure of steel are
ferrite, austenite, and cementite. All other variations of the allotropic forms of steel, such
as martensite and bainite, are the result of various thermal treatments of steel during
quenching, tempering, and annealing. The addition or presence of alloys, such as silicon,
manganese, vanadium, molybdenum, etc., may alter the physical characteristics of steel
but not their basic microstructural allotropic forms.
Steel piling: Bundling and reforging of raw steel bar stock. The piled steel sword is the
characteristic sword of the Vikings, made from piled sheets or strips of steel, possibly
Wootz steel obtained during trading activities; piled steel swords are a variant form of the
earlier Merovingian swords +/- 700 AD, made from pattern-welded layers of steel and
wrought iron. See Merovingian sword, pattern-welding, Viking sword, Japanese samurai
sword, and Wootz steel.
Steel press: “A machine for compressing molten steel in casting, to improve the quality
of the product” (Audel, 1942, 544).
Steel production: In 1840, the combined steel production of the US, England, and
Western Europe was less than 200,000 tons. In 1948, US steel production was about 90
million tons. By 2006, US annual production had dropped to 67 million tons, but world
steel production had risen to over 120 million tons per month. In the early 21st century,
China is the world’s largest producer of steel and is building coal-fired methylmercuryproducing power plants at a rate of one per week to power its rapidly expanding
industrial infrastructure. See biologically significant chemical fallout and mercury.
Steeling: 1) The processes used by a blacksmith to convert red-hot wrought or malleable
iron to steel. These processes include repeated hammering to remove slag and other
impurities; reheating the iron allowing it to absorb sufficient carbon from a carburizing
fuel such as charcoal, for example, by case hardening; quenching (rapid cooling) to
achieve hardness; and tempering (slow reheating and cooling) for a final softening of the
steel. Prior to the era of modern chemical analysis (1885 f.), a blacksmith judged the
quality of his steel intuitively and subjectively, as well as objectively, by considering the
following observable properties of his product: appearance, texture, feel, color, fracture,
and grain. In essence, the job of blacksmiths was to evaluate the microstructural changes
when iron is converted to steel by making visual and tactile evaluations of the products.
They observed whether the desired steel product had tears, veins, spots, or fissures
indicating impurities or had the smooth look and feel of steel rather than the gray or white
grainy quality of cast iron or the fibrous ductile quality of wrought iron. In this context,
up until the late 19th century, the work of the blacksmith was an art, not a science. See
kan of the ironmonger, carburizing, case hardening, quench, and tempering. 2) The
creation of steel cutting edges on iron tools by scarf welding, or folding and welding steel
onto the iron tool, e.g. the creation of a welded steel-iron interface. In the case of knives,
steeling was also done by folding iron over steel and then quenching it. Salaman (1975)
provides two examples of how hardness required for edge tools is obtained by a working
blacksmith: “(a) carbonization: the edge was heated in a charcoal fire and then rapidly
quenched in cold water - a method known in pre-historic and Roman Britain, or (b) by
the equally old method of ‘steeling’, i.e. thin strips of good quality steel were let into the
edge of a wrought-iron blade and joined by forge-welding in the fire” (Salaman 1975,
247). See ax-making techniques, scarf weld, and weld steel.
Steelmaking c. 1950: Fisher (1949) provides the following concise riff on midnineteenth century steelmaking before the era of powdered metallurgy: ore mines,
limestone quarries ore vessels, coke ovens, coal chemical byproducts blast furnaces
steelmaking furnaces: open-hearth, Bessemer, electric ingot molds, ingot strippers,
ingot soaking pits semi-finishing mills (blooms, slabs, billets) finishing mills, rail
and structural products; plate, sheet, and strip mills; bar, rod, and wire mills; pipe and
tube mills. Fisher then lists approximately four dozen categories of products produced by
the finishing mills ranging from rails, bridges, automobiles, ships and aircraft to tools,
springs, farm machinery, and other consumer products (Fisher 1949, 60-61).
Steel scale: The flaking layer of iron oxide produced on steel surfaces as a result of
oxidation, also called fire scale. See iron oxide.
Steelsmith: A bloomsmith whose only function was to produce raw steel rather than
wrought iron. In the early Iron Age and prior to the evolution of the blast furnace and the
indirect process of producing wrought iron and steel, most steelsmiths would have been
associated with furnaces producing raw steel for sword makers. Contemporary Japanese
steelsmiths continue to smelt raw steel for samurai swordmakers in breakdown furnaces,
as depicted in a Nova episode on PBS. See bloom, bloomsmith, breakdown furnace,
natural steel, and pattern-welding.
Stock removal method: A modern knife-making technique involving sawing and then
grinding off excess steel from steel bar stock, in contrast to the forging of the knife blade
Stopped off: The covering over of parts of an iron tool, other than its working edge,
during the carburization of edge tools that occurs in forge welding. Clay was a common
media for enclosure during such procedures; the clay cover protected the iron from the
oxidizing impact of burning fuel. See carburize, enclosure, and forging.
Stour Valley: An important 18th century center of furnaces and forges in the Severn
River watershed in the Midlands of England. The ironworks in the Stour Valley supplied
many of the toolmakers of nearby Birmingham in the years before Sheffield became
England’s most important steelmaking center.
Stourbridge: An early steelmaking center in the Midlands of England, famous for its fine
heat-resisting clay, so important to Benjamin Huntsman's production of crucible cast steel
(1742). See cast steel, crucible, and Stourbridge clay.
Stourbridge clay: The high temperature resistant clays found near the Village of
Stourbridge in England and utilized by Benjamin Huntsman to make the crucibles used
for the production of the cast steel that he needed for his watch spring business. No such
high temperature resistant clays were available in the U.S. for production of cast steel
until the 1840s, when Joseph Dixon developed the graphite crucible. See cast steel
definition 1 and crucible.
Strain: Stress within the microstructure of ferrous metals caused by grain boundary
sliding and grain rotation.
Strain hardening: The deformation of the crystals in the lattice structure of metals,
which increases their hardness and yield strength prior to shear stress-induced slip. Strain
hardening decreases with rising temperature. Annealing is the recovery from the strain
hardening of the lattice structure of steel, for example, which is then softened and made
less brittle (under less strain) by slow temperature changes in the process. See annealing
Strain rate sensitivities: Sensitivities that increase with increasing temperature and with
decreasing grain size.
Stress: Internally distributed forces within the microstructure of metals in the form of the
mechanical reaction of the microstructure to deformation forces. “Stresses always occur
in pairs” and include compressive, tensile, and tangential stresses (shearing) (Baumeister
Stress fields: Fields that surround dislocations on slip planes. “Dislocations may be
generated at a flaw and follow each other along a slip plane until they encounter some
imperfection or a boundary where they become stuck. The stress field that they set up at
this point opposes the approach of additional dislocations and therefore hardens the
metal” (Barrett 1943, 338). Stress fields may also build up a super lattice of dislocations,
which serve to raise critical shearing stress through the phenomena by which similar
dislocations repel each other and dissimilar dislocations attract each other, creating a
checkerboard of stress fields throughout the crystal. See creep, plastic deformation,
martensite, slip, shearing movements, and work hardening.
Stress relief: Thermal treatments, such as tempering, that relieve the stresses in the
lattice structure of iron and steel alloys caused by cold working, quenching, and workrelated plastic deformation. See annealing, cleavage plane, creep, and space lattice.
Structural unemployment: A consequence of the revolutionary impact of the Age of
Information Technology. A vast underclass of workers is confined to low paying service
jobs instead of higher paying and now computerized manufacturing (etc.) positions.
Structural unemployment provides the context for future viability of an underground
economy of skilled craftspersons and artisans essential for the maintenance of the global
market economy infrastructure. Knowledge of the history of technology and an ability to
use hand tools will be key components of the viability of alternative economies, which
are not characterized by structural unemployment.
Stucköfen furnace: The high shaft furnace used in Austria and Germany during the
Renaissance that evolved out of earlier low shaft furnaces and was the immediate
predecessor of modern blast furnace forms. See furnace types.
Styrian ore: Iron ore with 1.0 - 2.0% manganese content found in the Styrian-Carinthian
area of Austria but otherwise not commonly encountered in the ores of Sweden and the
United States. This ore facilitated the direct process production of iron having steel-like
qualities (strength, durability, hardness), while still containing significant amounts of
siliceous slag inclusions. This ore also played a major role in the production of German
steel. The high manganese content of cast iron assisted in the removal of the unwanted
contaminants sulfur and phosphorous in the flux. See German steel, natural steel,
manganese, spiegeleisen, Styrian steel, Weald of Sussex, and Weardale.
Styrian process: The continental technique of refining (decarburizing) pig iron
containing manganese (spiegeleisen) by the use of charcoal fuel to produce wrought iron,
malleable iron, or German steel.
Styrian steel: Natural steel produced by the reduction of iron ores containing manganese
in direct process bloomeries, later produced by fining (decarburizing) blast-furnacederived spiegeleisen; also called German steel. The Styrian method, also called the
continental method, was the principal steel-producing process of Renaissance England
and Europe north of the Alps between 1350 and 1650. Carinthia and Styria, in Austria,
were the principal sources of manganese-containing iron ores from the early Iron Age
until the 19th century, thus the name of the process. Before 1600, manganese-laced ores
were also found in the Weald of Sussex (England). See continental method, German
steel, natural steel, and Noric steel.
Sulfur: Nonmetallic chemical element (S) that is a naturally occurring microconstituent
of most iron ores and a major contaminant in iron and steel production resulting from the
introduction of coke as a fuel. Sulfur limited the uses for cast iron and steel unless
neutralized by a high lime base slag at high temperatures, producing the phenomena of
“hot shortness” during forging, when steel contaminated with sulfur would disintegrate
upon impact when hammering. The introduction of steam-driven piston blowers, creating
higher temperatures that helped burn out the sulfur, allowed the successful use of coke as
a universal blast furnace fuel in the late 18th century (Tylecote 1976). Sulfur is also
neutralized in slag at lower melting temperatures by the presence of manganese in iron
ore in the smelting process. See hot short, manganese, and spathic ores.
Superplasticity: “Polycrystalline solids which have the ability to undergo large uniform
strains prior to failure” (Sherby 1995). Superplasticity is further defined as the capacity of
a metal or other polycrystalline solids in tension at high temperatures (above ½ of the
melting temperature or eutectic) to undergo deformation elongations above 200% prior to
failure (mse.mtu.edu). “The explanation of the superplasticity of the UHCS [ultra high
carbon steels] is that the typical microstructure can lead to a fine uniform distribution of
spheroidised cementite particles (0.1 mm diameter) in a fine grained lower carbon ferrite
matrix” (Srinivasan n.d., 59). In his classic Functions of the Alloying Elements in Steel,
Bain (1939) notes superplasticity results when “coarse networks of pro-eutectoid
cementite forms along grain boundaries of prior austenite producing a uniform
distribution of fine spheroidised cementite particles (.1 μ diameter) in a fine grained
ferrite matrix.” In ferrous metallurgy, the most notable historic example of a steel having
characteristics of superplasticity at high temperatures is the Damascus steel sword, famed
for its ability to bend while retaining a hard cutting edge. The probable source of the
superplasticity of such swords is cementite microstructures in the form of nanotubes
(spheroids) created by the forging of very high carbon steel (1.5 - 2.0% cc) that contains
significant micro-contaminants such as cobalt, vanadium, or manganese. Forging at
temperatures well below 850º C results in spheroidization of the needle-like structures of
cementite, creating cementite nanotubes with their characteristic nanowires. High
temperature superplasticity facilitates plasticity and toughness at normal temperatures in
Damascus and samurai swords, as well as in forge welded edge tools. The molding
capability of superplastic metals, i.e. their ability to exactly replicate the forms of CAD
(computer assisted design) industrial equipment patterns, makes them the most important
component of modern machinery production, e.g. aircraft engine turbines. The role of
alloys, such as vanadium and cobalt, as microconstituents of the cementite nanowires in
facilitating superplasticity has not yet been determined. See CAD, carbide forming
metals, cementite plates, Damascus sword, electron microscope, HRTEM, nanotubes,
nanowires, and patternmaker.
Surface carburizing: A difficult, tedious, and infrequently used method of steel
production prior to the era of modern steel production that required protecting the tool
being carburized from the combustion gasses, which would oxidize (decarburize) the iron
or steel surfaces of the tool being forged. In the case of the cementation process used to
produce steel (<1830), surface carburization was the first step in a process that would
continue for days or weeks. See carburize, case carburization, case hardening,
cementation process, enclosure, and nest carburization.
Surface decarburization: The propensity of the surface of some carbon steels to lose
carbon if heated above 1333º F. The hardness of such surfaces is drastically reduced
when quenched from elevated temperatures (Pollack 1977). See carburize and edge tool
Surface hardening: To impart to the surface of low carbon steel, by carburizing
(austenizing followed by slow cooling), a wear and abrasive resistant surface that retains
a ductile and tough interior composition; also called case hardening. This is a modern
steelmaking technique. See carburize, cementation furnace, and case hardening.
Surface oxidation: Result of exposure to oxygen in the atmosphere, which causes the
oxidization of carbon and scaling on the surface of the iron tool being worked. The higher
the forging temperature, the higher the rate of surface oxidation is. Surface oxidation is
the most significant challenge in the successful hot forging of iron implements or tools.
Swage: Tool used by blacksmiths for rounding bar stock. The swage has two
components. The bottom swage fits into the hole in an anvil or swage block. Top swages
are often handled and used to pound the metal into the desired shape on the bottom
Swage block: A large block of cast iron, semi-steel, or wrought steel with multiple holes
and rectangles of various sizes used for shaping hot bar stock by a blacksmith or
toolmaker. See dapping block.
Swedish iron: The high quality, low sulfur, nearly phosphorus-free, highly refined
wrought iron derived from charcoal-smelted cast iron and exported from Sweden to
England and America. English steelmakers preferred Swedish charcoal-smelted iron to
domestically produced mineral-fuel-smelted iron because of its superiority for blister and
crucible steel production. The success of the English steel industry (1750-1860) was
closely connected to the ready availability of Swedish iron. Despite international trade
restrictions, Swedish bar iron was imported to the colonies and to toolmaking centers,
such as New Bedford, in the early 19th century, possibly for use in steel furnaces for
blister steel and whaling tool production. See blister steel, charcoal, charcoal iron, finery,
Whalecrafters, and wrought iron.
TEM: Transmission electron microscope (TEM), which utilizes a high voltage electron
beam emitted by a tungsten filament cathode to produce an image of the inner structure
of the metal being studied, which is then magnified by a series of electro-magnetic lenses
and recorded on photographic plates, fluorescent screens, or light sensitive cameras. See
electron microscope, HRTEM, REM, and SEM.
TRIP: See transformation induced plasticity.
Tamahagane: The Japanese steel used for the production of samurai swords. It is
produced from locally available iron sand known as “satetsu,” which is smelted into raw
steel in the Japanese open-hearth clay breakdown furnaces known as “tataras.” See
Chalybean and Japanese swords.
Tap hole: The discharge opening for molten metals in a smelting furnace.
Tatara: The Japanese term for the furnace used by samurai sword makers for smelting
raw steel out of iron sand (satetsu). A form of breakdown furnace, the tatara is an openhearth clay furnace approximately four feet by twelve feet and is deconstructed after
every firing for the removal of the raw steel bloom. See breakdown furnace.
Taylor-White: Frederick W. Taylor and Maunsel White developed the modern improved
form of high speed steel by heating high quality alloy tool steels to a temperature just
below their melting temperature (1900). When these steels cooled, they were able to
maintain efficient cutting capabilities at much higher temperatures and much greater
speed than the older version of alloy steel, R. M. S. Widely used after 1910, the use of
Taylor-White steels required heavier machinery and, thus, the retooling of the many
industries who used high speed steels in the 20th century. Molybdenum became an
important addition to tungsten in alloy tool steel configurations. Taylor and White also
discovered, during their investigation of high speed steels, that a key ingredient along
with tungsten in Robert Mushet’s self-hardening steel (R. M. S.) was its 2.0 – 2.5%
manganese content (Tweedale 1986). See manganese, Mushet, Robert F., and R. M. S.
Tea Party Taliban: America’s answer to the rise of radical jihadists. Their highly
partisan radicalism is a reflection of the growing social stress characteristic of the
unfolding Age of Biocatastrophe and one of many challenges to the viability of
sustainable economies of the future. The Tea Party Taliban joins greed and hyper-digital
technology as the primary enablers of a klepto-plutocracy based on institutionalized
Techno-elite: Born-again ironmongers in a world of silicon chips. Where did the
manganese go? The techno-elite, skilled born-again ironmongers, are the primary
enablers of the efficient functioning of the complex infrastructure of modern global
consumer society. The success of modern information and communications technologies
is dependent upon their skills and ingenuity.
Teeming: To use a ladle to fill ingots with molten metal.
Temp: The trough, usually made of stone, that transported melted iron from the blast
furnace to the molds used for making hollowware. See blast furnace.
Temper: To reheat steel that has been hardened by quenching (martensite) to reduce the
hardness and especially the brittleness of edge and other tools, usually done at a
temperature range of 150º C to 650º C for periods ranging from 30 minutes to hours
(Barraclough 1984a); closely related to annealing. The variables of time and temperature
determine the microstructure of steel, as with martensite, where tempering precipitates
iron carbide (cementite), creating less brittle steel by encouraging the homogenization of
its carbon content. “To make steel less brittle and therefore tougher, to relieve internal
stress and either to stabilize the retained austenite or to cause it to transform into a
dimensionally stable structure” (Shrager 1949, 165). See austenite and martensite.
Temper carbon: The form of carbon found in grey cast iron and malleable cast iron in
the form of nodules of large gray flakes of free graphite; also called free carbon. Temper
or “free carbon” softens cast iron, weakening its structure, but also increasing its
machinability. Annealing of cast iron can restore durability, especially in cast iron
containing silicon, manganese, and other alloy micro-constituents. The annealing of grey
cast iron and its temper carbon content were key components of the successful production
of iron-bodied hand planes by Leonard Bailey & Co. and later Stanley Rule and Level
Co. (1850 to 1870f.). See combined carbon, free graphite, grey cast iron, malleable cast
iron, and white cast iron.
Temperature control: The key to successful forging techniques for the earliest edge tool
and edged weapon makers, as well as for the most modern knife, edge tool, and tool steel
manufacturers. Loss of accurate temperature control during the forging process results in
an inferior product. The same observation can be made about hardening alloy steels or
austenizing and annealing any form of steel or cast iron.
Temperature range for melting iron and steel: Pure wrought iron (cc < 0.03%) melts
at a temperature of 2793° F / 1538º C. Increasing carbon content results in the lowering
of the melting temperature such that cast iron (cc > 3.5%) has a melting temperature of
Tempered alloy steel: A now obsolete term that came into widespread usage after
Robert Mushet invented his “self hard” tungsten-manganese alloy steel in 1868.
Toolmakers after this date combined new discoveries about the efficacy of tempering and
annealing techniques with the adaptation of alloy steel in hand tool production, especially
for machinists’ tools. After Taylor and White developed a wide variety of new tool steels
and Harry Brearley perfected the production of stainless steels in 1913, production of
tempered alloy steels became so widespread that this designation disappeared from tool
markings just as the designation “cast steel” was no longer used to mark edge tools. See
alloy steel, drop-forging, Mushet, Robert F., stainless steel, and Taylor-White.
Tempered martensite: In fully tempered steels, the change from the martensite matrix to
homogenous distribution of carbon is a result of the uniform distribution of fine particles
of cementite within the martensite, stabilizing its lattice structure by relieving its
brittleness (i.e. its strain hardening). Acicular carbide units of martensite grow in size,
decrease in number, and become more spherical, increasing plasticity. See austenite,
cementite, critical point, superplasticity, and temper.
Tensile elongation: The tensile elongation capacity of steel at room temperatures
decreases as carbon content increases. Low carbon steel (< 0.05% cc) shows significantly
larger percentages of elongation, up to 30% on an 8” test specimen than higher carbon
steels, which approach 0% tensile elongations in steels with a carbon content of 1.3%.
Crucible steel has the highest elongation plasticity among test steels (Howe 1890).
Tensile strength: A measurement of the maximum load that a material can withstand
without being pulled apart; also known as maximum strength or ultimate strength.
Tensile strength is measured in units of force per unit area. The non-metric units are
pounds-force per square inch (lbf/in² or psi). Soft grey cast iron has the lowest tensile
strength at 23,000 lbf/in² or psi. Tensile strength is highest in high carbon tool steels used
for lathe tools, chisels, files, and saws (steel with a 1.25% carbon content has a tensile
strength of 135,000 psi); wrought iron has an intermediate tensile strength of 52,000 psi.
Tetragonality of martensite: The formation of the anomalous atomic arrangement of the
microstructure of martensite due to the failure of carbon atoms to form carbides at lower
temperatures. As a result, the formation of asymmetrical, tetragonal, ferrite-cementite
acicular, plate-like microstructures gives hardness and brittleness to low carbon
martensite. Martensite can be uniformly softened by reheating (annealing), which
modifies its acicular plate-like microstructures. See bainite, lattice structure, and
Thermal fluctuations: Changes in temperature that affect the stress fields of the crystal
lattice structures of metals and that thus generate lattice dislocation. See annealing, lattice
reorientation, and tempering.
Thermal hysteresis: The lag time during heat treatment, characteristic of either cooling
(r) [refroidissement] or heating (c) [chauffage]. Minor variations in heating and cooling
rates can play a major role in the phase transformation kinetics of alloy steel production,
especially for hardened steels used in applications where superplasticity is essential. See
critical temperature range and transformation temperature.
Thermal stress: The stresses in the crystal lattice structure of metals caused by
temperature change. See thermal fluctuations.
Thermal treatment: The heating and cooling of iron and steel, which produces a range
of structures from coarse pearlite to fine martensite. See austenize and martensite.
Thermit welding: Fusion welding utilizing finely divided aluminum and iron oxide
(thermit), principally used for welding rail joints. A mold is constructed on either side of
the rails to be welded and the rails are then superheated (2800° F), which ignites the
thermit. The reaction spreads throughout the mass. The aluminum unites with the oxygen
molecules of iron oxide producing pure iron in the form of superheated (up to 5000° F)
aluminum alloy liquid steel. Discovered in 1896, thermit is produced in refractory lined
crucibles. The process required preheating the rails. Thermit welding is no longer used
for rail welding.
Thermophysical properties: Differences in the allotropic phases of iron and steel due to
the absorption or release of heat and consequent volume changes due to microstructural
deformations (shearing, diffusion, etc.)
Tilt hammer: A variation in the form of the trip (helve) hammer. The tilt hammer first
appeared as illustrations on Greek vases depicting early ironworks. It operates with a gear
mechanism and fulcrum, differing slightly in design from the trip hammer, which has a
revolving fulcrum mechanism (Horsley 1978). Modern lightweight tilt hammers were
designed in the mid-19th century, which operated at higher speeds and facilitated the mass
production of a wide variety of tools and machinery. See helve hammer.
Tin plate: Sheet steel covered with a thin layer of molten tin. See whitesmith.
Topman: In the operation of the blast furnace, the person feeding the furnace with ore,
charcoal, and flux.
Tool: Any instrument of manual operation (Oxford English Dictionary 1975).
Tool and die steel: Another name for tool steel and high speed tool steel. See tool steel.
Tool placement awareness (TPA): Easily learned applied mental discipline that has
been demonstrated to significantly reduce tool misplacement (misplace: to stow with no
hope of retrieval). A bar graph describing the process of misplacement shows the tool
interest curve rising rapidly during a search, sometimes with a parallel rise in blood
pressure, thence to level off during the period of useful possession, only to drop abruptly
when the task is done and the tool is cast aside mindlessly. A fractionally different
approach persuades the user to maintain the high tool interest plateau for a moment past
the period of useful possession, perhaps in that time giving thanks for the privilege of tool
access and only then releasing the tool mindfully to a place where it can be retrieved
efficiently. The key to either frustrating misplacement or efficient retrieval is held in that
moment when hand and tool separate. Think about it, and, when necessity or whim
demands, the reunion will be swift (McLaughlin, David 2008, Liberty Salvage Co.,
Tool steel: 1) In general, any steel with a carbon content at or above 0.5%, which can
then be effectively quenched and tempered to create a more homogenized carbon content.
Modern tool steels used for machinists’ cutting tools are defined as having a carbon
content range of 0.7 – 1.5%. Tool steel is also defined as steel with a carbon content of
0.5 – 1.3%; used for the working parts of a tool (Palmer 1937). Other sources define tool
steel as having up to a 2.0% carbon content. Tool steels may also contain other alloys,
including silicon, manganese, cobalt, vanadium, chromium, and molybdenum. See
classification system for steel, alloy steel, and carbon content of iron and steel. 2) Modern
tool steels are now differentiated from standard steels (see carbon steel classifications)
and are now classified as any steel containing more than 4% of one or more alloys, which
increase their ability to cut steel at high speed, hence the name “high speed tool steel.”
Modern tool steels may contain tungsten, which increases the resistance to the softening
affect of temperature and forms abrasion resistant carbides. Vanadium will increase
forge-ability while also increasing hardness, wear properties, and carbide content.
Molybdenum increases deep hardening and is now considered a cost effective substitute
for tungsten. Chromium increases hardenability and corrosion resistance, and in
conjunction with higher carbon content also increases toughness and wear resistance.
Cobalt high speed tool bits are especially useful for drilling heat resistant alloys and
materials with a Rockwell hardness exceeding 38c. Multiple and diverse combinations of
alloy elements are considered to have a synergistic impact on the efficiency and
durability of the several hundred modern variations of high speed tool steels used as
cutting tools in CNC milling machines and other equipment. See carbon content of steel,
classification of tool steels in Appendix V, Mushet, Robert F., and Taylor-White.
Tough iron: A slang term for the high quality, low phosphorus iron produced by the
bloomery forges of the Forest of Dean in the decades preceding the English Civil War
(1645 – 1653); also used to refer to any high quality low phosphorus wrought iron.
Toughness: The ability of a metal to withstand impact without fracture; the opposite of
brittleness, commonly used to express resistance to sudden shock. Due to its entrained
slag, wrought iron is famous for its tensile strength and toughness. See mechanical
properties of metals.
Tragedy of the round world commons: The unfortunate impact of four centuries of
cascading Industrial Revolutions and a now globalized consumer society on the
vulnerable, nonrenewable finite resources of our biosphere. The impact of innovative flat
world information and communications technologies may exacerbate the tragedy of the
round world commons by diverting our attention from a biosphere in crisis.
Transcrystalline fracture: Fracture that passes through the lattice structure of metals
rather than around the boundaries of crystal structures (intercrystalline fracture); “the
normal type of failure observed in metals” (Shrager 1949, 380).
Transformation: With respect to ferrous metallurgy, changes in the allotropic form of
steel, also called phase change. Transformation mechanisms are either homogenous,
characterized by uniform distribution, as in the fine carbide spheroid microstructures of
cast steel, or by heterogeneous distribution of ferrite-pearlite microstructures in raw steel.
See allotropic forms of iron, microstructure, and transformation temperature.
Transformation induced plasticity (TRIP): Modern term for the study of the
characteristics of bainite reactions, the mechanisms of which are not yet fully understood
Transformation temperature: Temperature levels at which phase change occurs in iron
There are three transformation temperatures, often referred to as critical temperatures,
which are of interest in the heat treatment of steels.
[Eutectoid temperature: 723º C (A1)] The boundary between the ferrite-cementite field
and the austenite-ferrite or austenite-cementite field.
[Alpha-gamma iron transformation temperature for pure iron: 910º C (A3)] The A3 line
represents the boundary between the ferrite-austenite and austenite fields.
[Critical temperature range: The temperature difference between (A1) and (A3) expressed
as (Acm).] The Acm line is the boundary between the cementite-austenite and austenite
The thermal hysteresis [lag] that occurs on heating is indicated by the letter c,
representing the French word chauffage, meaning heating. Similarly, thermal
hysteresis on cooling is indicated by the letter r, representing the French word
refroidissement, meaning cooling. Thus there are two sets of critical temperatures:
Ac1, Ac3, and Accm for heating and Ar1, Ar3, and Arcm for cooling… The faster the rate
of heating, the higher the Ac point: the faster the rate of cooling, the lower the Ar
point. Thus the faster the heating and cooling rates, the larger the difference between
the Ac and Ar points of the reversible equilibrium point A (Sinha 2003, 1.7).
See austenized, critical temperature, and the iron carbon diagrams in Appendix VI.
Transformation time: The amount of time needed to produce various microstructures by
quenching or tempering austenite. Pure martensite is produced by rapid quenching
(cooling) of austenite to a temperature of 220º C in 80 seconds or less, while the actual
transformation occurs in less than one second. Martensite-bainite complexes are formed
with cooling rates of 80 to 2,000 seconds, martensite-ferrite-bainite microstructures have
a transformation time range of 2,000 to 30,000 seconds, and martensite-ferrite-pearlitebainite microstructures have a transformation time range of 30,000 to 100,000 seconds
(69 hours). Very slow cooling, as in the production of cementation steel, produces ferritepearlite microstructures. See the transformation time diagram from Pollack (1977) in
Transition point: Temperature at which changes occur in the allotropic forms of metals.
Transmission electron microscope: See TEM.
Treenail: Wooden pegs, pronounced and often spelled “trunnel,” usually 8 to 14 inches
long, used to secure the framing of a ship. Wooden treenails were superior to iron nails
and spikes because they didn’t rust over long periods of time and swelled when exposed
to moisture after ship launching, thus tightly securing the ship frame constituents.
Trip hammer: A water-powered hammer developed during the medieval period; also
called a helve hammer or drop hammer. The widespread appearance water-powered trip
hammers coincided with development of the blast furnace after 1350 and represented the
first step in more efficient iron production by relieving the bloomsmith of much of the
work of hammering out the slag from the bloom. Operating initially at 50 – 75 blows per
minute, trip (helve) hammers increased in size and speed during the 18th and early 19th
centuries. Joseph Nasmyth invented the steam-powered trip hammer in 1838. In America,
coal- or coke-fired steam hammers made it possible for forges to be located well away
from water power sources, encouraging centralized development of iron production
centers. In the 19th century, large trip hammers as well as smaller tilt hammers played a
central role in the factory system of the mass production of drop-forged low carbon steel
tools. The increasingly powerful hydraulic press has replaced most trip hammers since
1875. See drop-forging, drop hammer, helve hammer, overshot water wheel, shingling,
and tilt hammer.
Trompe: Hydraulic bellows in the form of a water-blowing engine run by air compressed
by falling water. Pipes carry air and water to a receiver where the air is forced into a blast
pipe connected to the tuyère, providing the air for the smelting process. See blast furnace
Trunnel: See treenail.
Trunnel auger: A wormed auger used to cut the holes for wooden trunnels (treenails) to
secure the framing of a ship (in lieu of spikes and bolts). Characterized by double spiraled
flutes, two cutting edges, and two lips, trunnel augers were a common product of a
shipsmith’s forge before the era of the factory system of tool production.
Trydimite: SiO2, noted as a microconstituent in Damascus Wootz steel swords subject to
x-ray phase analysis (Levin 2005).
Tsuba: The hand guard of a Japanese sword.
Tsuchioki: Application of mixtures of adhesive clay to the blades of Japanese swords
prior to preferential tempering. The thickest layer of clay would be applied to the top and
upper sides of the sword, with a much thinner layer applied to the steel cutting edge. The
uniform heating of the blade above the critical temperature resulted in more rapid cooling
of the cutting edge, which, due to preferential tempering, was sharper (because it
contained more martensite) than the softer sword body. See critical temperature,
enclosure, samurai sword, temper, and yaki-modoshi.
Tungsten: Important alloy in alloy and tool steels. If present in amounts of +/- 4%, it
imparts hardness and wear resistance. When present in amounts of about 18%, it imparts
red hardness and hot strength to steel. It forms abrasion resistant particles in tool steel,
promotes carbide formation, and inhibits softening during tempering by facilitating
secondary hardening (Pollack 1977). See the AISI-SAE system of designating carbon and
alloy steels in Appendix IV, alloy steel, Mushet, Robert F., and tool steel.
Tungsten steel: Alloy containing 5 to 7% tungsten. It is used for manufacturing magnets
and in tool steel to facilitate cutting (milling).
Turbine: A machine in the form of a rotary engine that extracts energy from a fluid flow.
The first turbines, as prime movers, were the windmill (an air turbine) and the water
wheel (a water turbine). These were followed by the development of the steam turbine,
gas turbine, and jet engine. See machine and simple machine.
Tuyere (tuyère): The nozzle at the base of any furnace or forge for the admission of the
air produced by a leather bellows or any other air-blast-producing device. The forced air
draught (air blast) needed for the smelting process would enter this nozzle and follow the
tuyère tunnel to the charcoal fuel being burned. The use of the tuyère was the first of the
improvements in furnace design and iron-smelting of the early Iron Age. See blowing
Twinning: Reorientation of lattice structures during plastic deformation of metals. Along
with slip, it is one of the principal forms of crystal deformation. Twinning is one of the
results that occur when “a lamella within a crystal takes up a new orientation related to
the rest of the crystal in a definite symmetrical fashion. The lattice within the twinned
portion is a mirror image of the rest; the plane of symmetry relating one portion to the
other is called the twinning plane” (Barrett 1943, 307). In many cases, twinning involves
rapid slip or sheer along the glide plane, rather than rotation of the planes, and is the
characteristic deformation process that occurs during annealing. Barrett also defines
twinning as the symmetrical reorientation of exactly duplicate lattice structures occurring
rapidly during slip events by the “…shearing movements of the atomic planes over one
another” (Barrett 1943, 308). “…twinning brings slip planes into position for further
deformation” (Barrett 1943, 316). See deformation twinning, lattice structure, and
Ulfberht: Signature of a medieval swordmaker or a family of swordmakers noted on over
100 swords found in a wide ranging number of locations in continental Europe (Williams
Ultra fine microstructures: The fundamental characteristic of ultra high carbon steel
(UHCS); “ultra fine spherical particles of iron carbide embedded in ultra fine spherical
grains of iron” (Sherby 1995, 12).
Ultra high carbon steel (UHCS): Steel with a carbon content of 1.2 - 2.0%. Only ultra
high carbon content steels have the capacity to exhibit characteristics of superplasticity at
high temperatures above ½ of their eutectic.
Ultra low carbon bainitic (ULCB) steel: A modern form of heat-treated steel with a
very low carbon content (0.01 - 0.03%) characterized by toughness and strength;
especially used for piping in Arctic climates (Sinha 2003, 9.31). This steel has the same
carbon content and physical characteristics as wrought iron but has no ferrosilicate in its
Undercool: To cool quenched austenite below its critical temperature but not so low as to
reach the critical temperature needed to form martensite (220º F), i.e. the arresting of the
cooling process; a strategy used to produce steel with bainite microstructures; particularly
useful in the production of hardened tool steels. The generic definition of undercooling is
“the lowering of the temperature of a liquid beyond the freezing temperature and still
maintaining a liquid form” This process results in homogeneous nucleation and is also
known as super cooling (Tom Rahtz/UAH,
http://science.nasa.gov/ssl/msad/dtf/under1.htm). See austenite, bainite, and martensite.
Underground economy: An already flourishing invisible network of artisans, artists,
organic farmers including jewelers, silversmiths, weavers, and born-again ironmongers of
every description. An inevitable social and economic response to the growing economic
power of predatory corporations, both national and multinational, and the gross income
and educational inequality they foster. See klepto-plutocracy.
Undershot water wheel: Water comes underneath the wheel, driving it in a clockwise
direction in contrast to the counterclockwise direction of the overshot water wheel.
Undershot is the oldest form of water wheel. See overshot water wheel.
Unified numbering system: System developed and published by the Society of
Automotive Engineers, Inc. and the American Society for Testing and Materials (1986),
which lists over 3,000 identifier designations for metals and alloys. See Appendix III.
Uniform transformation: The production of high alloy steels with minimal internal
stresses by slow transformation processes, such as normalizing in still air or by cooling
rates, which are slower than those needed to produce martensite. “Oil quenching
produces less rapid change of volume and consequently less distortion than does water
quenching” (Shrager 1949, 157), hence its preferred use in the edge tool forging process.
See normalizing and quench.
Unit cell: Basic unit of the space lattice of the crystal structure of metals that expresses
their allotropic forms. Iron has two forms of temperature-dependent unit cells: the bodycentered cubic structure (BCC) up to 910° C (1670° F) (alpha iron,) and the face-centered
cubic structure (FCC) from 1670° F (910° C) to 2552° F (1400° C) (gamma iron). Above
1552° F, iron reverts to the FCC unit cell structure. A third form of the unit cell is the
close-packed-hexagonal (CPH) space lattice structure, characteristic of non-ferrous
metals, such as cobalt, magnesium and titanium. See allotropic forms, body-centered
cubic structure, close-packed hexagonal structure, and space lattice.
Unit cell parameters: The multiplicity of the patterns of crystal microstructures for
example, in cementite in Wootz steel swords, which may result from the substitution of
the carbide-forming alloys V, Mo, Cr, Mn, and Co for Fe atoms, or Si, S, and B for
carbon atoms within Fe3C structures (Levin 2005).
Upset: To make a piece of iron rod thicker and shorter by hammering. See Bealer (1976).
Vanadium: A rare chemical element (V) occurring in iron, uranium, and lead ores.
Vanadium is a deoxidizer that greatly increases hardenability, is a strong carbide former,
elevates grain coarsening temperature (thus yielding fine grained steel), and resists
tempering by aiding secondary hardening (Pollack 1977). An important tool steel alloy,
vanadium also increases the strength of pearlite by precipitation strengthening of ferrite
and increases the ductility of hypereutectoid steels (Levin 2005). As an important alloy, it
is a very scarce and, thus, expensive metal. See alloys and hardenability.
Venetian steel: Steel produced or available in Venice in the 17th century; noted by
Moxon in 1677 as the highest quality of all the steels available in the 17th century. It is
not currently known what techniques or combinations of techniques the Venetians used to
produce their famed steel. Natural steel from Noricum had been brought down through
Alpine passes to Italy during both the Roman Republic and Roman Empire. Brescian
steel was ubiquitous during the Italian Renaissance, and Wootz steel, the smelting
techniques of which were closely related to those used to produce Brescian steel, would
have been readily accessible to Venetian ironmongers. See Brescian steel, Moxon, and
VG-10 stainless steel: A high quality grade of stainless made in Japan for use by food
and sports cutlers. It is composed of carbon: 1.0%, chromium: 15.0%, molybdenum:
1.0%, vanadium: 0.2%, and cobalt: 1.5% (Erin Casson 2013, personal communication).
Viking sword: Pattern-welded all steel sword blade similar in its layered forging to the
iron and steel pattern-welded Merovingian blades of central Europe (+/-750 AD). The
earliest sword of this type was found in a Roman site in Britain in the 2nd century. It was
the principal weapon of the Vikings and probably locally made. Smith (1960) notes their
sudden disappearance in the 10th century. It is unknown whether the well-traveled
Vikings obtained some of the metalworking skills from Muslim countries making Wootz
steel (Smith 1960).
Walloon process: A process that uses charcoal-fired, open-hearth forges to fine cast iron
into wrought iron from blast furnace pig iron, commonly employed starting in the late
14th century to 1784, when Henry Cort perfected the puddling furnace. Charcoal
protected the bloom of iron from being oxidized prior to its removal for forging. The
Walloon process furnace was used to produce Swedish iron, as well as to fine the pig iron
at the Saugus, MA Ironworks c. 1646 (Gordon 1996). The Walloon furnace produced not
only very low carbon wrought iron (0.02 - 0.08% carbon content) but also a wide range
of malleable iron with a carbon content below that of quenchable steel (0.5% carbon
content). This malleable iron was often made directly into hoes, shovels, and other hand
tools by a blacksmith, such as Joseph Jenks, whose forge was a component of the
integrated ironworks at Saugus. See carbon content of iron and steel, malleable iron,
muck bar, and wrought iron.
Warm-forging: The technique of forging high carbon edge tools and swords at
temperatures below the critical temperature (723º C). Forging at higher temperatures
causes the later embrittlement of steel at room temperature. See cold forging, hot- and
warm-forging, and Wootz steel.
Water bellows: Japanese fan bellows run by a horizontal water wheel, later used in
Korea and China; the main source of power for most Japanese forges in antiquity. See
Watered steel: Etched steel, displaying the pattern derived from the metallurgical
composition of the steel and welding techniques of the smiths, including both their
mechanical (hammering) and thermal (forging) treatment of the sword, knife, or gun
barrel being constructed. The metal surface of the artifact being forged is then watered,
i.e. treated by pickling, i.e. the submerging or covering its surface with such acidic
substances as lemon juice, ferric sulfate, or “acidulated water” (Breant 1823). See, in
particular, chapters 2-5, in Smith’s (1960) classic, A History of Metallography. See
Damascened steel, Japanese swords, and pattern-welding.
Water-hardened steels: Low carbon and low alloy steels that can only be hardened by
quenching in water.
Water-powered drop hammer: Another term for a trip hammer. The drop hammer
became the hydraulic helve hammer of the later 15th century. See trip hammer.
Water quenching: The one quenching method of sufficient speed to give full hardness to
steels with a carbon content of 0.5 to 0.6%.
Weald of Sussex: The region southeast of London, which was, along with the Forest of
Dean, an important iron and steel producing area of Tudor England during the age of the
merchant adventurers. Manganese-laced siderite ores were mined in the Weald before
1600 (and then depleted) and may have attracted the attention of Roman smelters in the
early Iron Age. See Cleere (1985), Forest of Dean, manganese, and ordnance.
Weardale: An important source of iron ore located in County Durham, England, in the
late 17th and early 18th centuries for the brief florescence of the iron and steel industries in
Newcastle and the Derwent Valley in northeast England, 1685 – 1750. Along with the
Weald, a second location of manganese-bearing iron ores, Weardale ore was “…not
greatly dissimilar from the Carinthian ores. From the pig iron smelted from such ores it
would have been possible to produce ‘natural steel’ [German steel] by the continental
method and it should be noted that there was a blast furnace operating on these ores at
Allensford, nearby, from about 1670” (Barraclough 1984a, 64). Barraclough notes that
shortly thereafter (1703) the Hollow Sword Blade Company was, along with most other
forges in England, producing blister steel in a cementation furnace. See German steel,
shear steel, and Weald of Sussex.
Weld: To soften by heat and join together two pieces of metal by hammering, pressure,
or chemical reaction.
Welding: Using heat to join two metal parts together. The earliest ferrous welding
technique is forge or hammer welding, in which the elements to be joined are shaped with
heat and hammer on the anvil (scarfed) and then brought up to welding heat in the forge.
The mating surfaces are treated with flux, often a preparation of borax and silica, to
remove oxides from the joint, and then hammered, rolled, or rammed with sufficient
force to allow the establishment of a molecular bond. Before the end of the 19th century,
three new processes were emerging: oxy-acetylene or gas welding, resistance welding,
and metal arc welding. Of these three, various forms of metal-arc welding have become
the most widely used and the subject of the greatest refinement for industrial applications.
Thus modern welding methods now include gas tungsten arc welding (GTAW) aka TIG,
gas metal arc welding (GMAW) aka MIG, submerged arc welding (SAW), a mechanized
MIG process, and shielded metal arc welding (SMAW) aka “stick” welding. It is this last
technique that is most often referred to as arc welding, using the familiar welding rod,
properly described as an electrode because it conducts electrical current. The process was
advanced considerably by the invention in 1904 of the covered electrode. Before that,
uncoated electrodes produced welds of uncertain properties. The flux coating serves in
several capacities, stabilizing the arc, purifying the weld metal, and protecting the molten
deposit from contact with oxygen and nitrogen in the air. More recent advances in
welding strategies include electron beam welding, laser welding, and hybrid laser-arc
welding, combining laser beam welding with GMAW, allowing deep penetration single
pass butt welds in heavy gauge applications that ordinarily required multi-pass flux-cored
arc welding (FCAW) (McLaughlin, David 2008, Liberty Salvage Co., personal
Welding iron and steel: Joining two pieces of wrought iron, malleable iron, and/or low
carbon steel at temperatures just above their melting point. See scarf weld.
Welding heat: The individual welding temperature necessary for a blacksmith to bring
wrought iron and/or malleable iron and blister steel to their individual welding heats to
facilitate “steeling,” as in the forge welding of edge tools. The welding heat for wrought
iron lies between 2200 – 2700º F (white heat). After reaching that temperature, wrought
iron will give off sparks and droplets of melted metal. With increasing carbon content,
the welding heat of steel drops, cast steel being the most difficult to weld. Steel
containing carbon content in excess of 1.5% cannot be welded.
Weld steel: Term describing an edge tool produced by “steeling” or welding a steel bit or
cutting edge on an iron shaft or haft. In the manufacturing of axes and other edge tools
not made of cast crucible steel, a welded steel cutting edge (bit) was fused (welded) with
the iron components of the tool, hence the name weld steel. Three strategies for welding
steel cutting edges on iron shafted edge tools characterize ax and knife production since
the early Iron Age. The most frequently used welding or “steeling” technique is the
insertion of a steel bit between folded iron, especially for ax-making. The overcoat
method of folding steel around an iron haft is a more recent 18th century ax-making
technique. Scarf welding a steel cutting edge on the side of the iron body of larger offset
broad axes is a third, less common technique of welding steel cutting edges on iron tools.
Weld steel was produced in ancient times as natural steel and, after the advent of blast
furnaces, as German steel (fined cast iron). The most common form of weld steel bar
stock, used between 1700 and 1900, was blister steel derived from the carburization of
wrought or malleable iron bar stock in the cementation furnace. Cast steel produced by
the crucible steel process after 1750 may also have been used as weld steel. Most edge
tools utilizing cast steel as weld steel are usually marked either “cast steel” or “warranted
cast steel.” Blacksmiths working before the development of the cementation furnace
(1650) may have spotted nodules of natural steel accidentally produced in the ironsmelting process, extracted these fragments of steel from the bloom, and welded them
onto iron sockets and ax bodies. See blister steel, bit, cast steel, cementation furnace,
forge welding, scarf welding, steeling, and welding.
Whalecrafters: The New Bedford community of toolmakers who specialized in making
harpoons, as well as edge tools, for the whaling communities of southern New England
(Lytle 1984). The impost records of the New Bedford Customs District, made available
by the New Bedford Whaling Museum, indicate that large quantities of Swedish iron
were imported between 1816, the first year records were kept, and the 1830s to New
Bedford. If not used to make the ductile wrought iron shafts of harpoons, Swedish bar
iron was carburized in as yet undocumented steel (cementation) furnaces to make blister
and shear steel for local edge toolmakers and for whalecrafters who also made steeled
edge tools. After 150 years of making blister steel in England and a century of use in
America, small steel furnaces were a likely component of the 19th century ironworks of
many whalecrafters and edge toolmakers. See cementation furnace and edge tools.
Wheel cutting engine: A hand-operated machine for cutting teeth and gears; first used in
England c. 1670.
Wheellock: A variation of the matchlock gun first produced in 1515 in Nuremburg. The
wheellock was characterized by a flash hole with pyrites. The expensive-to-produce
wheellock was particularly popular with the gentry in Elizabethan England, who used it
for hunting in preference to the unwieldy matchlock arquebus. The wheellock was also
the firearm of choice of continental royalty, nobility, and high-ranking military officers.
The exquisite steel wheellock produced by Austrian-Nuremberg gunsmiths during the
German Renaissance < 1635 was never surpassed in quality and beauty by any other
firearm producing community. The advantage of the costly wheellock was that it could be
fired with one hand. See Arquebus, flintlock, gun barrel iron, gunsmithing, and
White cast iron: “Cast iron having cementite as its principal constituent” (Gordon 1996,
311). Cementite is iron chemically combined with graphite; it therefore contains little or
no free graphite and has very limited commercial application unless it is melted and
annealed into more useful grey cast iron. White cast iron is low in silicon and thus easier
to convert to wrought iron than grey cast iron and, consequently, was the preferred iron
used in the puddling furnace for conversion into wrought iron. It is produced by rapid
cooling in an iron rather than sand mold and can then be annealed by heating to a cherry
red heat for 60 hours to allow crystalline graphite to become free carbon, thereby
producing malleable cast iron. The absence of graphite gives the fracture of white cast
iron a white color. See cast iron, grey cast iron, malleable cast iron, and silicon.
White heart: An uncommon variant form of malleable cast iron in which all the free
carbon within the interior of the casting is converted to chemically combined carbon
during the annealing process producing a hard alloy (Spring 1917, 209-10).
White metal: Metal alloys with a significant tin content, which promotes elasticity and
assists the even distribution of stress loads.
White metal alloy: Babbit alloys used in bearing composition in engines, motors, and
turbines. Originally composed of tin (±89%), copper (±3.5%) and antimony (±3%),
modern bearings composites now include extensive use of lead, aluminum, and bronzebased alloys.
Whitesmith: Metalsmiths who used alloys of iron, zinc, and tin to galvanize metal
products and make domestic utensils, such as teapots, usually by rolling, crimping, or
otherwise shaping their wares; also called a tinsmith. See swage block.
Whitworth steel: A form of fluid, compressed steel that Sir Joseph Whitworth (c. 1862)
adapted from Huntsman's technique of producing cast steel in crucibles. Its brand name
was Wheatsheaf, and it was preferred for making shotgun barrels. Whitworth steel was
later made by the Siemens-Martin (c. 1870) process. See cast steel.
Whitworth thread: The standard screw thread used in England and continental Europe,
which has a 55° angle; named after its inventor, Sir Joseph Whitworth (1792-1871). See
the discussion of Whitworth’s role as an Industrial Revolutionary in Hand Tools in
History: Steel- and Toolmaking Strategies and Techniques before 1870 (Brack 2008).
Widmanstätten structure: The patterns formed by alternating areas of pearlite and
ferrite after rapid cooling of low carbon steel containing large austenite grains. Alois von
Widmanstätten first noted this crystal structure in 1808 on meteorites in the royal mineral
collection in Vienna; the term now refers to artificial structures in annealed steels (Smith
1960, 150) characterized by ferritic/pearlitic plate morphology (Sinha 2003). See
austenite, crystal structure, and Neumann bands.
Wilkinson, John: In the early 1750s, John Wilkinson invented a boring machine to
manufacture precision ground cylinders, which were quickly adapted by Bolton and Watt
in the manufacture of steam engines.
Wire annealing: The softening of cold-hardened or drawn wire by slow heating.
Wootz steel: Another name for Damascus steel, which originated in India in ancient
times and was used for edge tools, swords, and sitar wire (Craddock 1985). An early form
of crucible steel, it was made in +/- 3 kg batches in crucibles, especially in Muslim
communities since at least the early Christian era. Bealer (1976a) suggests Wootz steel
was made with molten cast iron in a manner similar to the Brescian method and was
composed of a mixture of granules of soft iron and carbon steel. Moxon (1975) noted
Wootz steel as one of the principal forms of steel available to toolmakers in the late 17th
century. Smith (1960) indicates that Wootz steel was made in cakes, which were not fully
melted, “but sometimes consisted of an aggregate of unmelted iron granules or little
plates cemented together by once molten cast iron. Such a structure would result from the
standard Indian process of steel making if the temperature were insufficient to melt the
alloy completely. The crucible charge was an iron sponge, sometimes roughly forged into
plates, together with wood for carbonization” (Smith 1960, 21). See crucible steel,
Damascus steel, Moxon, superplasticity, Venetian steel, and Viking sword.
Wootz steel ingot: Ingots produced as disks usually weighing ±2 lb., 4” in diameter, 2”
high, and widely traded to Persia and other western Asian locations (Buchanan 1807).
Wootz steel production process: The exact details of the Wootz steel production process
are unknown, but two strategies have been suggested: 1) the fusion of cast and wrought
iron (Lowe 1990) or 2) the carburization of wrought iron in crucibles packed with
carboniferous materials. With either strategy, ±15 small crucibles were laid in an ash166
filled pit adjacent to a fire pit and buffalo hide bellows provided the blast. Sanskrit texts
written between the 7th and 13th centuries provide a description of the process. The
smelting duration was approximately 24 hours at temperatures ranging from 1300º to
1400º C or higher, which produced a hypereutectoid steel (cc > 0.83%,) and, in some
cases, an ultra high carbon steel (UHCS), with carbon contents ranging from 1% to as
high as 2%. Wootz steel was used in the production of Damascus swords. The
superplasticity of Wootz steel may be due to a combination of unique forging techniques
and the presence of vanadium as a microconstituent (cobalt is also noted) within the
nanotubes of the steel microstructure. The contemporary difficulty in reproducing Wootz
steel may be due to the unavailability of ores containing these microconstituents
Work: “The amount of energy expended when a force is moved through a distance”
(Maiklem 1998, 26).
Work hardening: Hardening of iron and steel by deformation that occurs during
hammering, rolling, drawing, punching, and/or bending of metals at temperatures below
the critical point. See slip interference and stress fields.
Wrought iron: Slag-bearing, malleable iron with low carbon content (0.08 % or less, but
usually within the range of 0.02 - 0.04%) (Aston 1939). Wrought iron does not harden
when cooled suddenly (quenching). Its two principal components are high purity iron
(ferrite) and iron silicate, a glass-like slag with a high silicon content, which is present in
a one inch wrought iron rod in the amount of 250,000 filaments (Aston 1939). Due to its
malleability and ductility, it is easily shaped, threaded, machined, hammered, or stretched
when hot. Its iron silicate content (siliceous slag) gives it unique characteristics,
particularly its resistance to stress concentration (toughness and tensile strength), as well
as its corrosion resistance. Produced in larger quantities with better quality control after
the invention of the puddling (reverbatory) furnace in 1784, the purer wrought iron thus
produced was the key ingredient in producing higher quality cementation and crucible
steel. The slag inclusions in wrought iron aid its corrosion resistance, making it especially
useful in stressful environments where moisture would quickly corrode steel. When
forged across the grain instead of along the grain, loss of strength occurs. Knight (1875)
provides this description of the refining of high quality wrought iron: “Iron sufficiently
pure to be drawn out into bars and welded. . . The iron obtained from [simple furnaces]
was a spongy mass, which was drawn out at intervals by tongs, hammered gently and
cautiously, and then more energetically, to press the particles of iron into contact and
squeeze out the intermixed slag. The mass thus obtained was cut up into smaller pieces,
which were repeatedly heated and hammered till a sound bar of nearly pure iron was
obtained” (Knight 1875, 1377). Utilizing slightly altered methods of refining also
produced malleable iron with a higher carbon content, as well as wrought steel with the
same carbon content as low carbon steel. Malleable iron and wrought steel still contained
significant trace amounts of siliceous slag but, because of the slightly higher carbon
content, were much more suitable for forging common tools, such as shovels, hoes, tongs,
augers, leg vises, and early wagon wrenches, than softer and more ductile wrought iron,
which was more easily deformed. See bloomery, direct process, iron silicate, malleable
iron, muck bar, puddling furnace, and silicon.
Wrought iron and steel sword: The pattern-welded wrought iron and steel sword was a
common form of high quality fighting sword from the early Iron Age to the late 19th
century. The repeated forge welding of interspersed thin layers of tough, ductile, siliconfilament-laced wrought iron between thin layers of sheet steel provided unique qualities
of durability and resistance to fracture. Japanese, Merovingian, and other swordmakers
were experts at using this technique, which is still utilized in the modern age by samurai
swordmakers. The all steel (?) swords of the Vikings and the Wootz steel swords of
Damascus are variations of the usual method of pattern-welding swords. The all
malleable iron sword, also a common form of weapon used during the early Iron Age
until the late medieval period, was a distinctly inferior product. The quality of all three
variations of swordmaking techniques was intimately connected to the skill of the
swordsmith and the number of times each weapon was re-piled and reforged. See
Damascus sword and Japanese samurai sword.
Wrought iron production: Direct process smelting of wrought iron occurs in stages. In a
typical shaft furnace, heating is first used to remove water, and then the ascending gases
begin decomposing iron carbonates at a temperature of 500º C. In lower areas of the
furnace, reduction, which converts the higher oxides Fe3O4 and Fe2O3 to the lower oxide
FeO, begins at a temperature of about 750º C. The production of pure wrought iron in this
idealized furnace thus has the following composition: CO + FeO = Fe + CO2. Successful
smelting of wrought iron is predicated upon maintenance of an adequate CO level in the
furnace material. Rising temperatures in the wrought iron-smelting process at or above
900º C result in the formation of iron carbides, the principal component of raw steel and
cast irons. In blast furnaces, which run much hotter than direct process bloomeries, the
higher temperatures achieved (1600º C) enhance the production of carbon monoxide, the
principal cause of excess carbide formation in a direct process smelting furnace.
Examinations of early Iron Age furnace remains show significant deposits of iron carbide
consistent with the variable but heterogeneous carbon content of most currency bars
recovered from early Iron Age smelting furnaces or the smithies that reforged these
currency bars. Tylecote (1987), provides this riff on the formation of iron carbides during
direct process smelting, thus illustrating the difficulties of smelting pure wrought iron:
At 900 C the carbon would be in solution in the austenite phase of the iron. Under
these conditions the slag would be solid and low in iron as it would be in equilibrium
with the high carbon iron in contact with it. Drops of high carbon iron (in some cases
molten) would then fall down to the hotter parts of the furnace where they would be
oxidized by the blast to lower the carbon content of the metal and raise the iron
content of the slag in equilibrium with it:
Fe3C + O2 3Fe + CO2
2Fe + O2 + SiO2 2FeO.SiO2
Equilibrium is not usually achieved, certainly not over the whole cross-section of the
furnace, so that the result is a rather heterogeneous mixture of high- and low-carbon
areas with an average carbon level that is low. With such a carbon level the iron is
solid (at 1200 C) but the slag becomes molten and runs away leaving a solid iron
bloom with some porosity.
This process can continue until the space between the tuyere and the bottom is full of
metal, slag and charcoal. When this occurs the furnace must be opened or the tuyere
raised and the bloom removed from the bottom. (Tylecote 1987, 151-152)
Tylecote is discussing bloomsmithing in an early Iron Age shaft furnace. Production of
pure wrought iron in such a facility was extremely difficult. Most surviving currency bars
have a heterogeneous carbon content, which would include areas of wrought iron with a
low carbon content, as well as malleable iron and raw steel with a higher carbon and iron
Wrought steel: A high carbon form of wrought iron produced in the puddling furnace or
in fineries, later replaced by Bessemer and Siemens-Martin's open-hearth low carbon
steel. Wrought steel is, in essence, a malleable iron with a higher carbon content than
wrought iron and was forged out of solid iron bar stock. Many leg vises are composed of
wrought steel and were probably made by a blacksmith who specialized in toolmaking.
Wrought steel is also a modern generic term for any rolled or forged steel product,
obscuring its older meaning.
Wüstite: A naturally occurring mineral that is also produced by the smelting of iron in a
highly reducing environment, which, when liquid, is characterized by slowly growing
Yaki-ire: The rapid cooling by water quenching of Japanese steel swords after heating to
the critical temperature (Tc: 1341º F / 723º C), characterized by the appearance of a bright
red-orange color best observed in the darkened environment of the edge toolmaker or
swordsmith. In the case of Japanese sword production, the thickness of the clay enclosure
covering the steel sword during the quenching process determined the cooling rate and
thus the microstructure of the steel sword. See quench, naganita, tsuchioki, and yakimodoshi.
Yaki-modoshi: The further heat treatment of the hard sword blades (tempering) to a
temperature at least 300º F less than the critical temperature, followed by re-quenching to
relieve internal stresses. The degree of hardness or softness of Japanese swords after
rapid quenching was dependent on the thickness of the clay enclosure during the
tempering process. Sword edges covered by a thin layer of clay cooled more quickly and
were thus harder than the softer and more flexible sword bodies. Similar techniques
would have been used by shipsmiths and edge toolmakers who knew the art of edge tool
forging. See kan of the ironmonger, temper, tsuchioki, and yaki-ire.
Yield point: The load per unit area at which deformation or elongation occurs without
further increase in stress.
Zelechovice furnace: Slavic bloomery furnace that was used in the late 8th and early 9th
centuries in the Moravian section of Eastern Europe. Of particular interest with respect to
the issue of direct process natural steel production, these primitive, bowl-type furnaces
were built into the ground and were characterized by a unique bowl cavity at the bottom
of the furnace, in which the bloom of iron was protected from the oxidizing effect of
burning charcoal, while at the same time being covered by the charcoal. Leaving the
bloom of iron within the bowl cavity at the bottom of the furnace adjacent to both the
tuyère and the burning charcoal produced heterogeneous blooms of natural steel. See
Pleiner (1969, 461) for an illustration of the basic design of this early furnace, also
reproduced in volume 6 of the Hand Tools in History series: Steel- and Toolmaking
Strategies and Techniques before 1870 (Brack 2008).
Appendix I: A Guide to the Metallurgy of the
Edge Tools at the Davistown Museum
I. Steelmaking Strategies 1900 BC – 1930 AD
1. Natural Steel: 1900 BC – 1930 AD
Natural steel was made in direct process bloomeries, either deliberately or accidentally, in
the form of occasional nodules of steel (+/- 0.5% carbon content (cc)) entrained in
wrought iron loups. Bloomsmiths deliberately made natural steel for sword cutlers by
altering the fuel to ore ratio in the smelting process, producing heterogeneous blooms of
malleable iron (0.08 to 0.2% cc) and/or natural steel (0.2 to 0.5 cc and higher) or by
carburizing bar or sheet iron submerged in a charcoal fire. Manganese-laced rock ores
(e.g. from Styria in Austria or from the Weald in Sussex, England) facilitated natural
steel production. As a slag constituent, manganese lowered the melting temperature of
slag, facilitating the more uniform uptake of carbon in the smelted iron. The Chalybeans
produced the first documented natural steel at the height of the Bronze Age in 1900 BC,
using the self-fluxing iron sands from the south shores of the Black Sea. Occasional
production of bloomery-derived natural steel edge tools continued in isolated rural areas
of Europe and North America into the early 20th century.
2. German Steel: 1350 - 1900
German steel was produced by decarburizing blast-furnace-derived cast iron in a finery
furnace, and, after 1835, in a puddling furnace. German steel tools are often molded,
forged, or cast entirely of steel, as exemplified by trade and felling axes without an
inserted (welded) steel bit. Such tools were a precursor of modern cast steel axes and
rolled cast steel timber framing tools. German steel shared the world market for steel with
English blister and crucible steel until the mid-19th century.
3. Blister Steel: 1650 - 1900
Blister steel was produced by carburizing wrought iron bar stock in a sandstone
cementation furnace that protected the ore from contact with burning fuel. It was often
refined by piling, hammering, and reforging it into higher quality shear or double shear
steel or broken up and remelted in crucibles to make cast steel. Blister steel was often
used for “steeling” (welding on a steel cutting edge or bit) on axes and other edge tools.
4. Shear Steel: 1700 - 1900
Shear steel was made from refined, reforged blister steel and used for “steeling” high
quality edge tools, such as broad axes, adzes, and chisels, especially by American edge
toolmakers who did not have access to, or did not want to purchase, expensive imported
English cast steel. The use of shear steel was an alternative to imported English cast steel
for making edge tools in America from the late 18th century to the mid-19th century.
5. Crucible Cast Steel: 1750 - 1930
Crucible cast steel was made from broken up pieces of blister steel bar stock, which was
inserted into clay crucibles with small quantities of carboniferous materials (e.g. charcoal
powder). After melting at high temperatures, crucible cast steel was produced in 5 to 25
kg batches and considered to be the best steel available for edge tool, knife, razor, and
watch spring production. Due to lack of heat resistant clay crucibles, extensive
production of high quality crucible cast steel didn’t begin in the United States until after
the Civil War.
6. Brescian Steel: 1350 - 1900?
Brescian Steel was a common Renaissance era strategy used in southern Europe to make,
for example, steel for the condottiers of the Italian city states. Wrought or malleable iron
bar stock was submerged and, thus, carburized in a bath of molten pig iron. Brescian steel
cannot be visually differentiated from German steel or puddled steel, both of which were
produced from decarburizing pig iron.
7. Bulk Processed Steel: 1870 f.
After the American Civil War, a number of new strategies were invented for producing
large quantities of steel, especially low carbon steel, which was required by the rapid
growth of the industrial age and its factory system of mass production. The first
important innovation was Henry Bessemer’s single step hot air blast process, followed by
several variations of the Siemens-Martin open-hearth furnace and electric arc furnaces.
For edge tool production, the electric arc furnace supplanted, and then replaced, crucible
cast steel in the early decades of the 20th century. A few modern drop-forged edge tools
are included in this exhibition as examples of modern bulk process steel producing
Appendix II: Art of the Edge Tool
I. Edge Toolmaking Techniques 1900 BC – 1930 AD
Shaping and Forging by Hand
A. Forge welding: Edge carburizing by heating, followed by hammering and additional
B. Steeling: The welding of a steel bit onto an iron shaft or body
C. Pattern-welding: The welding together of alternating layers of sheet iron and steel,
used by knife and swordmakers; seldom used by edge toolmakers
D. Molding: The shaping of short lengths of hot malleable iron or German steel bar stock
in an iron pattern; sometimes the iron pattern was water-cooled. This method was not
used after blister steel became widely available around 1700.
Shaping and Forging by Machine
E. Rolling: The hot rolling of cast steel into bar stock, and its further shaping by the
formation of sockets, grinding, and further forging, both before and after additional
F. Casting: The hot rolling of cast steel into steel bar stock compatible with its further
shaping in molds or patterns by drop-forging, as in the drop-forging of cast steel axes.
G. Drop-forging: The hydraulic pressing of low carbon steel and malleable iron into tool
forms by using dies as patterns as in the mass production of factory-made hand tools.
Also, its casting in special purpose molds for the production of machinery and
equipment of every conceivable use.
Most hand tools made in the 20th century show no evidence of hand work, but, in a
minority of cases, (e.g. the ax) there is no clear distinction between the hand-forged and
the machine-made tool until the late 20th century. Most edge tools made before 1930 are
“hand-forged” or “forge welded” to some extent, no matter the technique used to “steel”
their edges. The trip hammer and the water wheel are examples of machines that assisted
edge toolmakers in the forging of their tools. The advent of the modern rolling mill
(Henry Cort, 1784) for hot rolling cast steel bar stock did not end the long tradition of
hand-forging an edge tool. When the Collins Ax Factory began drop-forging all steel axes
sometime after 1837, many smaller ax companies continued hand-forging and hand
hammering axes they produced, often with the aid of other machinery, well into the 20th
century. The evolution from hand-forging to machine forging (drop-forging) hand tools
was thus a gradual process. One goal of the creative economy of the post-industrial era is
the revival of handmade hand toolmaking strategies and techniques.
Appendix III: Classification for Metals and
Table 5. Unified Numbering System (UNS) for Metals and Alloys. From Oberg et al. ( 1996, 402)
Machinery’s Handbook: 25th edition: A reference book for the mechanical engineer, designer, manufacturing
engineer, draftsman, toolmaker, and machinist.
A00001 to A99999
C00001 to C99999
D00001 to D99999
E00001 to E99999
F00001 to F99999
G00001 to G99999
H00001 to H99999
J00001 to J99999
K00001 to K99999
L00001 to L99999
M00001 to M99999
N00001 to N99999
P00001 to P99999
R00001 to R99999
S00001 to S99999
T00001 to T99999
W00001 to W99999
Z00001 to Z99999
Aluminum and aluminum alloys
Copper and copper alloys
Specified mechanical property steels
Rare earth and rare earthlike metals and alloys
AISI and SAE carbon and alloy steels (except tool steels)
AISI and SAE H-steels
Cast steels (except tool steels)
Miscellaneous steels and ferrous alloys
Low-melting metals and alloys
Miscellaneous nonferrous metals and alloys
Nickel and nickel alloys
Precious metals and alloys
Reactive and refractory metals and alloys
Heat and corrosion resistant (stainless) steels
Tool steels, wrought and cast
Welding filler metals
Zinc and zinc alloys
Appendix IV: Compositions of AISI-SAE
Standard Carbon Steels
Table 6. From Oberg et al. ( 1996, 407-8) Machinery’s Handbook: 25th edition: A reference book for the
mechanical engineer, designer, manufacturing engineer, draftsman, toolmaker, and machinist.
Nonresulfurized Grades – 1 per cent Mn (max)
Nonresulferized Grades – Over 1 per cent Mn
Free-Machining Grades - Resulfurized
Free-Machining Grades – Resulfurized and Rephosphorized
Appendix V: Classification for Carbon and
Table 7. AISI-SAE System of Designating Carbon and Alloy Steels. From Oberg et al. ( 1996, 406)
Machinery’s Handbook: 25th edition: A reference book for the mechanical engineer, designer, manufacturing
engineer, draftsman, toolmaker, and machinist.
Carbon and alloy steel grades
Plain carbon (Mn 1.00% max)
Resulfurized and rephosphorized
Plain carbon (Mn 1.00% to 1.65%)
Ni 1.25%, Cr 0.65% or 0.80%
Ni 1.25%, Cr 1.07%
Ni 3.50%, Cr 1.50% or 1.57%
Ni 3.00%, Cr 0.77%
Mo 0.20% or 0.25% or 0.25% Mo & 0.042 S
Mo 0.40% or 0.52%
Chromium-molybdenum (Chromoly) steels
Cr 0.50% or 0.80% or 0.95%, Mo 0.12% or 0.20% or 0.25% or
Ni 1.82%, Cr 0.50% to 0.80%, Mo 0.25%
Ni 1.82%, Cr 0.50%, Mo 0.12% or 0.35%, V 0.03% min
Ni 1.05%, Cr 0.45%, Mo 0.20% or 0.35%
Carbon and alloy steel grades
Ni 0.30%, Cr 0.40%, Mo 0.12%
Ni 0.30%, Cr 0.45%, Mo 0.12%
Ni 0.55%, Cr 0.50%, Mo 0.20%
Ni 0.55%, Cr 0.50%, Mo 0.25%
Ni 0.55%, Cr 0.50%, Mo 0.35%
Ni 3.25%, Cr 1.20%, Mo 0.12%
Ni 0.45%, Cr 0.40%, Mo 0.12%
Ni 0.55%, Cr 0.20%, Mo 0.20%
Ni 1.00%, Cr 0.80%, Mo 0.25%
Ni 0.85% or 1.82%, Mo 0.20% or 0.25%
Ni 3.50%, Mo 0.25%
Cr 0.27% or 0.40% or 0.50% or 0.65%
Cr 0.50%, C 1.00% min
Cr 0.28% or 0.50%
Cr 0.80% or 0.87% or 0.92% or 1.00% or 1.05%
Cr 1.02%, C 1.00% min
Cr 1.45%, C 1.00% min
Cr 0.60% or 0.80% or 0.95%, V 0.10% or 0.15% min
W 1.75%, Cr 0.75%
Si 1.40% or 2.00%, Mn 0.65% or 0.82% or 0.85%, Cr 0.00% or
High-strength low-alloy steels
Various SAE grades
Appendix VI: Classification of Tool Steels
Table 8. From Oberg et al. ( 1996, 454) Machinery’s Handbook: 25th edition: A reference book for the
mechanical engineer, designer, manufacturing engineer, draftsman, toolmaker, and machinist.
High-Speed Tool Steels
Hot-Work Tool Steels
Cold-Work Tool Steels
Shock-Resisting Tool Steels S
Special-Purpose Tool Steels L
Water-Hardening Tool Steels W
High-carbon, high-chromium types
Medium-alloy, air-hardening types
Appendix VII: Iron-Carbon Diagrams
The following iron-carbon diagrams reflect only a small portion of the wide variety of
possible interpretations of iron-carbon alloy types and their relationship to carbon
content, temperature, and cooling rate. See, in particular, the transformation time
Schematic iron-carbon diagram
Figure 2 Shrager, M. 1961. Elementary Metallurgy and
Metalography. NY: Dover. pg. 135. Used with permission of Dover.
Iron-carbon phase diagram
Figure 3 Gordon, Robert B. © 1996. American Iron, 1607-1900. pg. 252. The Johns Hopkins
University Press. Reprinted with permission of The Johns Hopkins University Press.
Iron-carbon constitutional diagram 1
Figure 4 Shrager, M. 1961. Elementary Metallurgy and Metalography. NY:
Dover. Figure 20. pg. 35. Used with permission of Dover.
Cooling curve of pure iron diagram
Figure 5 Shrager, M. 1961.
Elementary Metallurgy and
Metalography. NY: Dover. pg. 34.
Used with permission of Dover.
Figure 6 Barraclough, K.C. 1984a. Steelmaking before Bessemer: Blister steel,
the birth of an industry. Volume 1. The Metals Society, London, England. pg.
5. Used with permission from the Institute of Materials, Minerals and Mining.
Figure 7 Used with permission from Serdar Z. Elgun.
Critical temperature: heating versus cooling diagram
Figure 8 Sinha, Anil Kumar. 2003. Physical metallurgy handbook. New
York: McGraw-Hill. pg. 1.8. Reproduced with permission of The McGrawHill Companies.
Alpha-gamma-cementite eutectoid diagram
Figure 9 Sinha, Anil Kumar. 2003. Physical metallurgy handbook. New
York: McGraw-Hill. pg. 1.9. Reproduced with permission of The
Iron-carbon constitutional diagram 2
Figure 10 Shrager, M. 1961. Elementary Metallurgy and Metalography. NY: Dover. pg. 38.
Reproduced with permission from Dover.
Transformation time diagram
Figure 11 Pollack, Herman W. 1977. Materials Science and Metallurgy. Reston, VA: Reston
Publishing Co., Inc. Fig. 8-6 (a), pg. 175.
Appendix VIII: Popular Knife-Makers’ Steels, c.
An early 21st century version of this 1973 excerpt from Latham’s Knives and
Knifemakers would probably contain significant alterations in the form of additional
chromium-vanadium alloy combinations. An unresolved controversial question lingers:
in contrast to the lack of significant improvement in steel for woodworking edge tools
and plane blades, are late 20th century and early 21st century “chromium-vanadium”
knife-makers’ steels superior to 18th and 19th century products?
Figure 12 Latham, Sid. 1973. Knives and Knifemakers. New York: MacMillan. pg. 33.
Appendix IX: Principal Bibliographic Sources
Many of the citations in this bibliography will be encountered scattered through the
general bibliographies of the Hand Tools in History series. They are cited again here
because they are quoted or referenced within the Glossary; they constitute the principal
sources of information on ferrous metallurgy used by the Davistown Museum. Hopefully,
readers of this glossary will find these citations as useful as we have, despite their
obscurity or difficulty to procure through interlibrary loan services. The notation “IS.” at
the end of a citation indicates it is “in stock” in our library.
Please note: a second general bibliography on metallurgy follows the Glossary
bibliography. Many important citations on metallurgy and the history of tools can be
found in the bibliographies to Vol 6: Steel- and Toolmaking Strategies and Techniques
before 1870; Vol 7: Art of the Edge Tool: The Ferrous Metallurgy of New England
Shipsmiths and Toolmakers 1607 - 1882; and Vol 8: The Classic Period of American
Toolmaking, 1827-1930. Please note that volume 8 also includes numerous special topic
bibliographies, including US and New England Toolmakers, Tools of the Trades, and
Collectors’ Guides, Handbooks, and Dictionaries. The Tools of the Trades bibliography
is further subdivided into 64 special topics. The entire collection of the Davistown
Museum’s bibliographic citations is published in hard copy as Special Publication 48:
Davistown Museum: The Complete Bibliographies, which is available online at
Abell, Sir Wescott. 1948. The Shipwright’s Trade. Cambridge: The University Press. IS.
Angell, Marcia. June 23, 2011. The epidemic of mental illness: Why? New York Review
of Books. http://www.nybooks.com/articles/archives/2011/jun/23/epidemic-mentalillness-why/?pagination=false.
Appleton. 1866. Appleton’s dictionary of machines, mechanics, engine-work, and
engineering. vol 1. New York: D. Appleton and Company.
Aston, James and Story, Edward B. 1939. Wrought iron: Its manufacture, characteristics
and applications. Pittsburgh, PA: A. M. Byers Company. IS.
Audel, Theo. 1942. Audels Mechanical Dictionary. NY: Theo Audel and Company. IS.
Bain, Edgar C. 1939. Functions of the alloying elements in steel. Cleveland, OH:
American Society for Metals. IS. http://www.msm.cam.ac.uk/phasetrans/2004/Bain.Alloying/ecbain.html
Baker, William A. 1973. A maritime history of Bath, Maine and the Kennebec region. 2
vols. Bath, ME: Maritime Research Society of Bath. IS.
Barrett, Charles S. 1943. Structure of metals: Crystallographic methods, principles and
data. New York: McGraw-Hill. IS.
Barraclough, K. C. 1984a. Steelmaking before Bessemer: Blister steel, the birth of an
industry. Vol 1. London: The Metals Society.
Barraclough, K. C. 1984b. Steelmaking before Bessemer: Crucible steel, the growth of
technology. Vol 2. London: The Metals Society.
Barraclough, K. C. 1991. Steel in the Industrial Revolution. In The Industrial Revolution
in metals. Day, J. and Tylecote, R. F. eds. London: The Institute of Metals.
Baumeister, Theodore, ed. 1958. Mechanical engineers’ handbook. New York: McGrawHill Book Company.
Bealer, Alex W. 1976. The art of blacksmithing. Edison, NJ: Castle Books.
Bergman, Torbern. 1781. Dissertatio chemica de analysi ferri. Uppsala, Sweden.
Bining, Arthur Cecil. 1933. British regulation of the colonial iron industry. Philadelphia:
University of Pennsylvania Press. IS.
Biringuccio, Vannoccio.  1990. The pirotechnia of Vannoccio Biringuccio: The
classic sixteenth-century treatise on metals and metallurgy. Trans. and Ed. Cyril Stanley
Smith and Martha Teach Gnudi. Mineola, NY: Dover. IS.
Biswas, A. K. 1994. Iron and steel in pre-modern India- a critical review. Indian Journal
of History of Science. 29: 579-610.
Bronson, Bennet. 1986. The making and selling of Wootz, a crucible steel of India.
Brack, H. G. 2005. What needs to be retrieved: The marriage of tools, art and history.
Hulls Cove, ME: Pennywheel Press. IS.
Brack, H. G. 2006. Norumbega reconsidered: Mawooshen and the Wawenoc diaspora.
Hulls Cove, ME: Pennywheel Press. IS.
Brack, H. G. 2008. Art of the edge tool: The ferrous metallurgy of New England
shipsmiths and edge toolmakers. vol. 8. Hand Tools in History Series. Hulls Cove, ME:
Pennywheel Press. IS.
Brack, H. G. 2010. The phenomenology of tools. West Jonesport, ME: Pennywheel Press.
Brack, H. G. 2013. Tools teach: An iconography of American hand tools. Hulls Cove,
ME: Pennywheel Press. IS.
Brain, Jeffery Phipps. 2007. Fort St. George archaeological investigation of the 1607-08
Popham Colony. Occasional Publications of the Maine Archaeological Society. Augusta,
ME: Maine State Museum and Maine Historical Preservation Commission. IS.
Brearley, H. 1933. Steel makers. London: Longmans Green.
Breant, J. R. 1823. Description d’un procede al’aide duquel on obtient une espece d’acier
fondu, sembable a celui des lames damassees Orientales. Bull. Societe d’Encouragement
pour l’Industrie Nationale. 22: 222-227.
Brewington, M. V. 1962. Shipcarvers of North America. Barre: Barre Publishing
Bronson, B. 1986. The making and selling of Wootz, a crucible steel of India.
Archaeomaterials. 1: 13-51.
Buchanan, F. 1807. A journey from Madras through the countries of Mysore, Canara and
Malabar. 3 vols. London.
Camp, J. M. and Francis, C.B. 1919. The making, shaping, and treating of steel.
Pittsburgh, PA: U.S. Steel Corp.
Cias, Witold W. n.d. Phase transformation kinetics and hardenability of medium-carbon
alloy steels. Greenwich, CT: Climax Molybdenum Company. IS.
Cleere, Henry and Crossley, David. 1985. The iron industry of the Weald. Avon:
Leicester University Press. IS.
Climax Molybdenum Co. 1967. Symposium: A transformation and hardenability of
steels: February 27-28th. Sponsored by Climax Molybdenum Company of Michigan and
the University of Michigan, Department of Chemical and Metallurgical Engineering, Ann
Craddock, P. T. 1995. Early metal mining and production. Edinburgh, Scotland:
Edinburgh University Press.
Craddock, P. T. 1998. New light on the production of crucible steel in Asia. Bulletin of
the Metals Museum of the Japan Institute of Metals. 29: 41-66.
Craddock, P. T. and Hughes, M. J. eds. 1985. Furnaces and smelting technology in
antiquity. British Museum Occasional Paper 48. London. IS.
Craddock, P. T. and Lang, eds. 2003. Mining and metal production through the ages.
London: British Museum Press.
Dane, E. Surrey. 1973. Peter Stubs and the Lancashire hand tool industry. Altrincham:
John Sherratt and Son Lt. IS.
Davenport, E. S. and Bain, E. C. 1930. TRANS. AIME (The American Institute of Mining,
Metallurgical and Petroleum Engineers). 117.
Day, Peter. 1995. Michael Faraday as materials scientist, history of materials. Materials
Egerton, W. 1896. Indian and Oriental armour. London.
Faraday, M. 1819. An analysis of wootz or Indian steel. Quarterly Journal of Science,
Literature, and the Arts. 7: 319-30.
Fisher, Douglas A. 1949. Steelmaking in America. New York: US Steel Corp.
Fisher, Douglas Alan. 1963. The epic of steel. New York: Harper & Row. IS.
Fostini, R. V. and Schoen, F. J. 1967. Affects of carbon and austenitic grain size on the
hardenability of molybdenum steels. Paper presented at the Symposium: A
transformation and hardenability of steels, February 27-28th in Ann Arbor, MI. 195-210.
Gardner, J. Starkie. 1892. Victoria & Albert Museum: Ironwork: Part I. From the earliest
times to the end of the mediaeval period. London: Printed under the authority of the
Board of Education.
Ghose, B. N., Bhattacharya, J., Das, N. K., De, R. K., Krishnan, C. S. S. R. and Mohanty,
O. N. 1997. Superplasticity in iron-carbon alloys. Paper presented for ICSAM-97.
Bangalore, India: Indian Institute of Science.
Goodman, W. L. 1964. The history of woodworking tools. New York: David McKay
Gordon, Robert. 1996. American iron, 1607 - 1900. Baltimore: Johns Hopkins University
Gore, Albert. 2006. An inconvenient truth. Movie. Paramount Classics.
Greener, W. W. 1910. The gun and its development. New York: Bonanza Books. IS.
Grossman, M. A. 1935. The principles of heat treatment. Cleveland, OH: American
Society for Metals.
Habraken, L. J. and Economopoulous, M. 1967. Bainitic microstructures in low-carbon
alloy steels and their mechanical properties. Papers presented at the Symposium: A
transformation and hardenability of steels, February 27-28th in Ann Arbor, MI. 69-108.
Hayman, Richard and Horton, Wendy. 2003. Ironbridge: History & guide. Stroud:
Tempus Publishing Ltd.
Heavrin, Charles A. 1998. The axe and man: The history of man’s early technology as
exemplified by his axe. Mendham, NJ: The Astragal Press. IS.
Howe, Henry M. 1890. The metallurgy of steel. New York: Scientific Publishing Co.
Hunter, Louis C. 1979. Waterpower in the century of the steam engine. Vol. 1 of A
history of industrial power in the United States, 1780-1930. Published for the Eleutherian
Mills-Hagley Foundation. Charlottesville, VA: University Press of Virginia.
Hunter, Louis C. 1985. Steam power. Vol. 2 of A history of industrial power in the
United States, 1780-1930. Published for the Eleutherian Mills-Hagley Foundation.
Charlottesville, VA: University Press of Virginia.
Hunter, Louis C. 1991. The transmission of power. Vol. 3 of A history of industrial
power in the United States, 1780-1930. Cambridge, MA: The MIT Press.
Illich, Ivan. 1973. Tools for conviviality. New York: Harper & Row. IS.
Kauffman, Henry J. 1972. American axes: A survey of their development and their
makers. Brattleboro, VT: The Stephen Greene Press. IS.
Kelly, Jack. 2004. Gunpowder: Alchemy, bombards, and pyrotechnics: The history of the
explosive that changed the world. NY: Basic Books.
Kinsman, K. R. and Aaronson, H. I. 1967. Influence of molybdenum and manganese on
the kinetics of the proeutectoid ferrite reaction. Papers presented at the Symposium: A
transformation and hardenability of steels, February 27-28th in Ann Arbor, MI. 39-56.
Klenman, Allen. 1990. Axe makers of North America. Victoria, BC: Whistle Punk Books.
Knight, Edward H. 1877. American mechanical dictionary. Cambridge: Cambridge
University Press. IS.
Kolchin, B.A. 1953. Chernoe Metallurgie v Drevnoi Rusi. Moscow.
La Nice, Susan, Hook, Duncan and Kraddock, Paul. eds. 2007. Metals and mining studies
in Archaeometallurgy. London: Archtype Publications in association with the British
Latham, Sid. 1973. Knives and knifemakers. New York: MacMillan.
Lee, Leonard. 1995. The complete guide to sharpening. Newtown, CT: The Taunton
Levin, A. A., Meyer, D. C., Reibold, M., Kochmann, W., Patzke, N. and Paufler, P. 2005.
Microstructure of a genuine Damascus sabre. Cryst. Res. Technol. 40: 905-16.
Light, John D. 2007. A dictionary of blacksmithing terms. Historical Archaeology. 41:
Liu, K. H., Chan, H., Notis, M. R. and Pigott ,V. C. 1984. Analytical electron microscopy
of early steel from the Bacqah Valley, Jordan. In Microbeam analysis. Romig, A. D. Jr.
and Goldstein, J. I. eds. San Francisco: San Francisco Press, Inc.
Lowe, T. L. 1989. Solidification and the crucible processing of Deccani ancient steel. In
Principles of solidification and materials processing, vol. 2, Trivedi, R., Sekhar, J. A. and
Mazumdar, J. eds. New Delhi: Oxford and IBH Publishing.
Lowe, T. L. 1990. Refractories in high-carbon iron processing: A preliminary study of
Deccani Wootz-making crucibles. In Ceramics and civilization. Kingery, W. D. ed.
Pittsburgh, PA: The American Ceramic Society.
Lytle, Thomas G. 1984. Harpoons and other whalecraft. New Bedford, MA: The Old
Dartmouth Historical Society Whaling Museum.
Lynch, Kenneth. 2007. The armourer and his tools: The Kenneth Lynch tool collection.
Davistown Museum Special Publication 45. Hulls Cove, ME: Pennywheel Press. IS.
Maiklen, Lara, ed. 1998. Ultimate visual dictionary of science. New York: DK
Mehl, R. F. 1938. Symposium on the hardenability of alloy steels. Cleveland, OH:
American Society for Metals.
Mehl, Robert F. and Hagel, W. C. 1956. The austenite-pearlite reaction, progress in
metal physics. vol. 6. Oxford: Pergamon Press.
Mehl, Robert F. and Wells, Cyril. 1937. Constitution of high purity iron-carbon alloys.
Technical Publication No. 798. American Institute of Mining and Metallurgical
Mercer, Henry C.  1975. Ancient carpenters’ tools. Horizon Press for the Bucks
County Historical Society. IS.
Moxon, Joseph.  1989. Mechanick exercises or the doctrine of handiworks.
Morristown, NJ: The Astragal Press.
The first issue of The Doctrine of Handiworks was published in London in
1677, and remains the definitive late Renaissance commentary on
blacksmithing and the sources of steel available in the late 17th century.
Mushet, D. 1804. Experiments on wootz or Indian steel. Philosophical Transactions of
the Royal Society. 95:175.
Needham, J. 1958. The development of iron and steel technology in China. 2 Vols.
London: Newcomen Society.
The definitive survey of steelmaking techniques in China before the modern
Nieh, T. G., Wadsworth, J. and Sherby, O. D. 2005. Superplasticity in metals and
ceramics. Cambridge Solid State Science Series. Cambridge: Cambridge University
Nizolek, T., Benscoter, A. and Notis, M. R. 2007. Metallography and microanalysis of
pattern-welded composite steels. Microsc. Microanal. 13(Suppl 2).
NUCOR. 2007. Certified test report. Auburn, NY: NUCOR Steel Auburn, Inc.
Oberg, Erik, Jones, Franklin D., Horton, Holbrook L. and Ryffel, Henry H. 2000. in
Machinery’s handbook. McCauley, Christopher J., Heald, Riccardo and Hussain,
Muhammed Iqbal eds. New York: Industrial Press Inc.
Oblak, J. M. and Hehemann, R. F. 1967. The structure and growth of Widmanstätten
ferrite. Papers presented at the Symposium: A transformation and hardenability of steels,
February 27-28th in Ann Arbor, MI. 15-38.
Oxford English Dictionary (OED). 1975. Oxford: Oxford University Press.
Palmer, Frank R. 1937. Tool steel simplified: A handbook of modern practice for the man
who makes tools. Reading, PA: The Carpenter Steel Company. IS.
Partington, J. R. 1961. A history of chemistry. New York: St. Martin’s Press.
Paxton, H. W. 1967. The formation of austenite. Papers presented at the Symposium: A
transformation and hardenability of steels, February 27-28th in Ann Arbor, MI. 3-14.
Paynter, Sarah. 2007. Innovations in bloomery smelting in Iron Age and Romano-British
England. In Metals and mining studies in Archaeometallurgy. La Nice, Susan, Hook,
Duncan and Kraddock, Paul eds. 202-10. London: Archtype Publications in association
with the British Museum.
Pense, Alan W. 2000. Iron through the ages. Materials Characterization. 45:353-63.
Perttula, J. 2004. Wootz Damascus steel of ancient Orient. Scandinavian Journal of
Petty, E. R. 1970. Martensite. New York: Longmans.
Piaskowski, Jerzy. 1978. Metallographic examination of two damascene steel blades.
Journal for the History of Arabic Science. 2: 3-30.
Piaskowski, Jerzy. 1982. On the manufacture of high-nickel iron Chalibean steel in
antiquity. In Early Pyrotechnology. Wertime, Theodore ed. Washington: Smithsonian
Institution Press. IS.
Pickering, F. B. 1967. The structures and properties of bainite in steels. Papers presented
at the Symposium: A transformation and hardenability of steels, February 27-28th in Ann
Arbor, MI. 109-132.
Pleiner, Radomir. 1969. Experimental smelting of steel in early medieval furnaces.
Pamatky archaeologicke. 458-487.
Pleiner, Radomir. 1980. Early iron metallurgy in Europe. In The coming of the age of
iron. Wertime, Theodore A. and Muhly, James D. eds. New Haven: Yale University
Pollack, Herman W. 1977. Materials science and metallurgy. Reston, VA: Reston
Publishing Co., Inc. IS.
Rao, K. N. P. 1989. Wootz-Indian crucible steel, feature article. No. 1. Metal News. 11:
Rao, K. N. P., Mukherjee, J. K. and Lahiri, A. K. 1970. Some observations on the
structure of ancient steel from south India and its mode of production. Bulletin of
Historical Metallurgy. 4: 12-4.
de Réaumur, René Antoine Ferchault. 1722. L’art de convertir le fer forgé en acier.
Renfrew, Colin. 1973. Before civilization: The radiocarbon revolution and prehistoric
Europe. London: Cambridge University Press. IS.
Russell, Carl P. 1967. Firearms, traps and tools of the mountain men. New York: Knopf.
Salaman, R. A. 1975. Dictionary of tools used in the woodworking trades, c. 1700-1975.
New York: Charles Scribner’s Sons.
Schmitt, Catherine, Belliveau, Mike, Donahue, Rick and Sears, Amanda. 2007. Body of
evidence – a study of pollution in Maine people. Portland, ME: Alliance for a Clean and
Healthy Maine. IS.
Schubert, John Rudolph Theodore. 1957. The history of the British iron and steel industry
from c. 450 B.C. to A.D. 1775. London: Routledge & Kegan Paul.
Sellens, Alvin. 1990. Dictionary of American hand tools: A pictorial synopsis. Augusta,
KS: Alvin Sellens.
Sherby, Oleg D. 1995a. Damascus steel and superplasticity – Part I: Background,
superplasticity, and genuine Damascus steels. SAMPE Journal. 31:10-7.
Sherby, Oleg D. 1995b. Damascus steel and superplasticity – Part II: Welded Damascus
steels. SAMPE Journal. 31.
Shrager, M. 1961. Elementary metallurgy and metallography. New York: Dover. IS.
Sinha, Anil Kumar. 2003. Physical metallurgy handbook. New York: McGraw-Hill.
Sisco, Anneliese G. trans. 1956. Réaumur’s memoirs on steel and iron. Chicago:
University of Chicago Press.
Smith, Cyril S. 1960. A history of metallography: The development of ideas on the
structure of metals before 1890. Chicago: University of Chicago Press. IS.
Smith, Cyril Stanley, ed. 1968. Sources for the history of the science of steel 1532 - 1786.
Cambridge: The Society for the History of Technology and MIT Press. IS.
Smith, Cyril Stanley. 1983. A search for structure: Selected essays on science, art and
history. Cambridge: MIT Press.
Society of Automotive Engineers, Inc., and American Society for Testing and Materials.
1986. Metals & alloys in the unified numbering system with a description of the system
and a cross index of chemically similar specifications. Warrendale, PA: Society of
Automotive Engineers, Inc.
Spring, Laverne W. 1992. Non-technical chats on iron and steel and their application to
modern industry. Bradley, IL: Lindsay Publications Inc. IS.
Srinivasan, S. and Griffiths, D. 1997. South Indian wootz: evidence for high-carbon steel
from crucibles from a newly identified site and preliminary comparisons with related
finds. Material Issues in Art and Archaeology-V, Materials Research Society Symposium
Proceedings Series. Vol. 462. Pittsburgh.
Srinivasan, Sharada, and Ranganathan, Srinivasa. n.d. India’s legendary ‘Wootz’ steel:
An advanced material of the ancient world. Bangalore, India: National Institute of
Advanced Studies and Indian Institute of Science.
Stanley, Philip E. 1984. Boxwood & ivory: Stanley traditional rules, 1855 - 1975.
Westborough, MA: The Stanley Publishing Co. IS.
Stanley Rule & Level Co. 1975. 1859 Price list of boxwood and ivory rules, levels, try
squares, sliding T bevels, gauges, &c., manufactured by the Stanley Rule and Level
Company, also including the price list of boxwood and ivory rules manufactured by A.
Stanley & Co., New Britain, Conn. Jan. 1855. Fitzwilliam, NH: Ken Roberts Publishing
Stodart, J. 1818. A brief account of Wootz. Asiatic Journal. 5.
Stodart, J. and Faraday, M. 1822. On the alloys of steel. Philosophical Transactions of
the Royal Society of London. 112: 253-70.
Stone, George Cameron. 1999. A glossary of the construction, decoration, and use of
arms and armor in all countries in all times. Mineola, NY: Dover Publications.
Story, Dana. 1995. The shipbuilders of Essex: A chronicle of Yankee endeavor.
Gloucester, MA: Ten Pound Island Book Company.
Tomas, Estanislau. 1999. The Catalan process for the direct production of malleable iron
and its spread to Europe and the Americas. Contributions to Science. 1:225-32.
Tresemer, David. 1996. The scythe book: Mowing hay, cutting weeds, and harvesting
small grains with hand tools. Chambersburg, PA: Alan C. Hood & Co., Inc.
Tweedale, Geoffrey. 1987. Sheffield steel and America: A century of commercial and
technological interdependence, 1830-1930. New York: Cambridge University Press. IS.
Tylecote, Ronald F. 1987. The early history of metallurgy in Europe. London: Longmans
Verhoeven, John D. 1987. Damascus steel, Part I: Indian Wootz steel. Metallography. 20:
Verhoeven, John D. 2001. The mystery of Damascus blades. Scientific American
Magazine. 284: 74-80.
Verhoeven, John D., Baker, H. H., Peterson, D. T., Clark, H. F. and Yater, W. M. 1990.
Damascus steel, part III: The Wadsworth-Sherby mechanism. Materials
Characterization. 24: 205-27.
Verhoeven, John D., Pendray, A. H. and Gibson, E. D. Wootz Damascus steel blades.
Materials Characterization. 37: 9-22.
Wadsworth, J. and Sherby, O. D. 1978. Influence of chromium on superplasticity in ultrahigh carbon steels. Journal of Materials Science. 13: 2645-49.
Wadsworth, J. and Sherby, O. D. 1980. On the Bulat-Damascus steels revisited. Progress
in Materials Science. 25: 35-67.
Wayman, Michael L. 2000. The ferrous metallurgy of early clocks and watches: Studies
in post medieval steel. Occasional Paper Number 136. London: British Museum. IS.
Wertime, Theodore A. 1962. The coming of the age of steel. Chicago: University of
Chicago Press. IS.
Wertime, Theodore A. 1982. Early pyrotechnology. Washington: Smithsonian Institution
Wertime, Theodore A. and Muhly, James D., eds. 1980. The coming of the age of iron.
New Haven: Yale University Press. IS.
Weston, Thomas. 1906. History of the town of Middleboro Massachusetts. New York:
Houghton, Mifflin and Company.
Whitworth, Joseph and Wallis, George. 1854. The industry of the United States in
machinery, manufactures, and useful and ornamental arts compiled from the official
reports of Messrs. Whitworth and Wallis. London: George Routledge & Co.
Williams, Alan. 2007. Crucible steel in medieval swords. In Metals and mining studies in
Archaeometallurgy. La Nice, Susan, Hook, Duncan and Kraddock, Paul eds. London:
Archtype Publications in association with the British Museum.
Zaky, A. R. 1979. Medieval Arab arms, Islamic arms and armour. London.
Appendix X: Metallurgy and Metalworking
The special focus of the Davistown Museum bibliographies in the Hand Tools in History
series is ferrous metallurgy from the early Iron Age to the beginning of the modern era.
Numerous references pertaining to modern iron- and steelmaking technologies are
included in our bibliographies, which are nonetheless not intended to be a complete
survey of important references on this topic.
Aitchison, Leslie. (1960). A history of metals. 2 volumes. Interscience Publishers, NY,
Allen, Richard Sanders. (1992). Connecticut iron and steel from Black Sea sands. Journal
of the Society for Industrial Archeology. 18(1/2). pg. 129-132.
Alling, George W. (1903). Points for buyers and users of tool steel. D. Williams, New
Arnold, J. O. (1898). The micro-chemistry of cementation. Journal of Iron and Steel
Institute. Part II. pg. 185-194.
Aston, James and Story, Edward B. (1939). Wrought iron: Its manufacture,
characteristics and applications. A. M. Byers Company, Pittsburgh, PA. IS.
Bancroft, W. E. (1946). Salt baths for hardening high speed steel. Metal Progress. pg.
Barraclough, K. C. (October 1971). Puddled steel: A forgotten chapter in the history of
steelmaking. J. Iron Steel Inst. 209. pg. 785-789.
Barraclough, K. C. (December 1971). Puddled steel: The technology. J. Iron Steel Inst.
209. pg. 952-957.
Barraclough, K. C. (1974). The production of steel in Britain by the cementation and
crucible processes. Historical Metallurgy. 8. pg. 103-111.
Barraclough, K. C. (1976). The development of the cementation process for the
manufacture of steel. Post-Medieval Archaeology. 10. pg. 65-88.
Barraclough, K. C. (1978). A crucible steel melter’s logbook. Historical Metallurgy. 12.
Barrett, Charles S. (1943). Structure of metals: Crystallographic methods, principles and
data. McGraw-Hill, New York, NY.
Batra, R.C. (1994). Consideration of microstructural changes in the study of adiabatic
shear bands. Research Triangle Park, NC: U.S. Army Research Park. X.
Bauerman, H. (1891). Elements of metallurgy. 3rd edition. Phillips, J.A., ed. London,
Baylis, B. (1866). On puddling -- by a practical puddler. Published privately, London,
Bell, Isaac Lowthian. (1872). Chemical phenomena of iron smelting: An experimental
and practical examination of the circumstances which determine the capacity of the blast
furnace, the temperature of the air, and the proper condition of the materials to be
operated upon. D. Van Nostrand, NY, NY.
Bell, Isaac Lowthian. (1878). On the separation of phosphorus from pig iron. Journal of
Iron and Steel Institute. 1. pg. 17-34, 34-37.
Bell, Isaac Lowthian. (1884). Principles of the metallurgy of iron and steel. Newcastle,
Bell Telephone System. Principles of zone melting. Monograph 2000.
Bell Telephone System. Ultrapure metals produced by zone melting technique.
Bell Telephone System. Continuous multistage separation by zone melting. Monograph
Bell Telephone System. Single crystals of exceptional quality by zone leveling.
Bergman, Torbern. (1781). Dissertatio chemica de analysi ferri. Uppsala, Sweden.
Extracts from this work (A Chemical Essay on the Analysis of Iron) are reprinted
in English in C. S. Smith’s Sources for the history of the science of steel 1532 1786.
Bessemer, Henry, Sir. (August 13, 1856). The manufacture of iron (steel) without fuel.
Cheltenham Meeting of the British Association [of iron makers].
A complete copy of this paper may be found on page 156 of Sir Henry Bessemer,
F.R.S. an autobiography. http://books.google.com/books?id=XOAAAAAYAAJ&dq=bessemer+%22The+manufacture+of+malleable+iron+without+
Bethlehem Steel Company. (1944). Properties of frequently used carbon and alloy steels.
Bethlehem Steel Company. (1944). Steel in the making. Bethlehem, PA.
Bethlehem Steel Company. (1942). Tool steel treaters’ guide. Bethlehem, PA.
Bezis-Selfa, John. (2004). Forging America: Ironworkers, adventurers and the Industrial
Revolution. Cornell University Press, Ithaca, NY.
Birch, Alan. (1952). Midlands iron industry during the Napoleonic wars. Edgar Allen
News. 31. pg. 231-233.
Boucher, Jack E. (1964). Of Batsto and bog iron. The Batsto Citizens Committee, Batsto,
Brearley, Harry. (February 2, 1924). Stainless steel: The story of its discovery. Sheffield
Brearley, Harry. (1941). Knotted string: An autobiography of a steel-maker. Longmans.
Brearley, Harry. (1946). Talks about steel making. American Society for Metals,
Brownlie, D. (1930). The history of the cementation process of steel manufacture.
Journal of Iron and Steel Institute. CXXI, Part I. pg. 455-464, 474.
Bullens, D. K. (1938/1939). Steel and its treatment. 2 vols. John Wiley and Sons, Inc.,
New York, NY.
Camp, J. M. and Francis, C. B. (1919). The making, shaping, and treating of steel.
Campbell, H. H. (1907). The manufacture and properties of iron and steel. Hill
Publishing Co., NY, NY.
Campbell, H. H. (1896). The manufacture and properties of structural steel. Scientific
Publishing Co., NY, NY.
Campbell, H. L. (date unknown). Metal casings. John Wiley and Sons, Inc., New York,
Carlberg, Per. (July 1958). Early industrial production of Bessemer steel at Edsken.
Journal of the Iron and Steel Institute. 189. pg. 201-204.
Carpenter, H. C. H. and Robertson, J. M. (1930). The metallography of some ancient
Egyptian implements. Journal of Iron and Steel Institute. CXXI, Part I. pg. 417-448.
Carpenter Steel Company. (1944). Carpenter matched tool steel manual. Seventh edition.
The Carpenter Steel Company, Reading, PA. IS.
Chandler, Harry. (1999). Metallurgy for the non metallurgist. ASM International,
Materials Park, OH.
Charles, J. A. (1975). Where is the tin? Antiquity. 49. pg. 19-24.
Christian, J. W. (1965). Physical properties of martensite and bainite. Iron and Steel
Clarke, E.B. (1914). Electric furnaces for steelmaking. TAES. 25. pg. 139-159.
Coghlan, Herbert H. (1956). Notes on prehistoric and early iron in the Old World.
Occasional Papers on Technology. 8. Oxford University Press. pg. 134-165.
Colby, A. L. (1903). Nickel steel: Its properties and applications. Proceedings of the
American Society of Testing Materials. 3. pg. 141-168.
Conner, William G. (1921-1922). The carbonizing of steel parts. In: Transactions of
American Society for Steel Treating. Volume II. pg. 148.
Cottrell, Alan Howard. (1967). An introduction to metallurgy. Edward Arnold, London.
Craddock, Paul T. (date unknown). The manufacture and properties of iron and steel.
McGraw-Hill Book Co., New York, NY.
Craddock, P. T., Ed. (1998). 2000 years of zinc and brass. British Museum Occasional
Paper 50, London, England.
Crossley, D. W. (1981). Medieval iron smelting. In: Medieval industry. Crossley, D.W.
Ed. CBA Research Report. no. 40. Council for British Archaeology, London, UK. pg. 2941.
Crookes, W. and Rohrig, E. A. (1870). A practical treatise on metallurgy. New York,
Davis, James J. (1922). The Iron puddler. Bobbs-Merrill, Indianapolis, IN.
Dichmann, C. (n.d.). The basic open-hearth steel process. Constable & Co., Ltd.,
Dixon, George F. (2004). A blacksmith’s craft. Blue Moon Press, Huntingdon, PA.
Ducoff-Barone, Deborah. (1983). Marketing and manufacturing: A study of domestic
cast iron articles produced at Colebrookdale furnace, Berks County, Pennsylvania, 17351751. Pennsylvania History. 50. pg. 20-37.
Elam, C. F. (1935). The distortion of metal crystals. Oxford.
Ellingham, H. J. T. (1944). The physical chemistry of process metallurgy. Journal of the
Society of Chemistry and Industry. 63. pg. 125.
Espelund, Arne. (1997). The “Evenstad” process-description, excavation, experiment and
metallurgical evaluation. In: Norbach, Lars Chr., ed., Early iron production-archaeology,
technology and experiments. Technical Report Nr. 3. The Historical-Archaeological
Experimental Centre, Lejre, Denmark. pg. 47-58.
Espelund, Arne. (1997). Ironmaking in Trondelag during the Roman and Pre-Roman Iron
Age. In: Norbach, Lars Chr., ed., Early iron production-archaeology, technology and
experiments. Technical Report Nr. 3. The Historical-Archaeological Experimental
Centre, Lejre, Denmark. pg. 103-114.
Evenstad, O. (1968). A treatise on iron ore and the process of turning it into iron and
steel. Bull. HMG. Translated by N.L. Jensen. 2(2). pg. 61-5.
Fairbairn, William. (1865). Iron: Its history, properties and processes of manufacture.
Adam and Charles Black, Edinburgh.
Fennimore, Donald L. (1996). Metalwork in early America: Copper and its alloys from
the Winterthur collection. Henry Francis du Pont Winterthur Museum, Winterthur, DL.
Finley, M. I. (Sept 1970). Metals in the ancient world. Journal of the Royal Society of
Flather, D. (1901-1902). Crucible steel: Its manufacture and treatment. Proc. Staffs. Iron
Steel Inst., pg. 55-82.
Forsythe, Robert. (1908). The blast furnace and the manufacture of pig iron: An
elementary treatise for the use of the metallurgical student and the furnaceman. D.
Williams Co., NY, NY.
Fruehan, R. J. (1998). The making, shaping, and treating of steel. 11th edition. Vol. 2
Steelmaking and refining volume. AISE Steel Foundation, Pittsburgh, PA.
Fulford, Michael, Sim, David, Doig, Alistair, and Painter, Jon. (2005). In defence of
Rome: A metallographic investigation of Roman ferrous armour from northern Britain.
Journal of Archaeological Science. 32. pg. 241-150. IS.
Fuller, John, Sr. (1894). Art of coppersmithing: A practical treatise on working sheet
copper into all forms. David William, NY, NY. Reprinted in 1993 by Astragal Press,
Mendham, NJ. IS.
Gale, Walter Keith Vernon. (1963/1964). Wrought iron: A valediction. Transactions of
the Newcomen Society. 36. pg. 1-11.
Gale, Walter Keith Vernon. (1964/1965). The rolling of iron. Transactions of the
Newcomen Society. 37. pg. 35-46.
Gale, Walter Keith Vernon. (1979). The black country iron industry. Metals Society,
Gardner, John. (March 1970). Cast steel. The Chronicle. 23(1). pg. 6, 16. IS.
Gilmer, H. (1953). Birth of the American crucible steel industry. Western Pennsylvania
Historical Mag. XXXVI. pg. 19-34.
Giolitti, Frederico. (1915). The cementation of iron and steel. Translated from the Italian
by Richards, Joseph W. and Rouiller, Charles A. McGraw-Hill, New York, NY.
Gledhill, J. M. (1904). The development and use of high speed steel. Journal of Iron and
Steel Institute. II. pg. 127-167.
Gledhill, J. M. (1904). High speed tool steel. Engineering Review. pg. 405-411.
Goodale, S. L. (1920). Chronology of iron and steel. Pittsburgh, PA.
Gordon, Robert B. (1983). Material evidence of the development of metalworking
technology at the Collins Axe Factory. IA: The Journal of the Society for Industrial
Archeology. 9. pg. 19-28.
Gordon, Robert B. (1988). Strength and structure of wrought iron. Archeomaterials. 2.
Gordon, Robert B. (2001). A landscape transformed: The ironmaking district of
Salisbury, Connecticut. Oxford University, New York, NY.
Gordon, Robert B. and Raber, Michael S. (1984). An early American integrated
steelworks. IA: The Journal of the Society for Industrial Archeology. 10(1). pg. 17-34.
Gray, R. D. (1979). Alloys and automobiles. Indianapolis.
Greenwood, William Henry. (1870). A manual of metallurgy. G. P. Putnam’s sons, New
Greenwood, William Henry. (1902). Steel and iron: Comprising the practice and theory
of the several methods pursued in their manufacture, and of their treatment in the rolling
mills, the forge and the foundry. Cassell and Co., Ltd., London.
Greenwood, William Henry. (1907). Iron: Its sources, properties, and manufacture.
Revised and partially rewritten by A. Humboldt Sexton. David McKay, Publishers,
Grossmann, Marcus Aurelius. (1935). Principles of heat treatment. United States Steel
Corp. The Haddon Craftsmen, Inc., Scranton, PA. IS.
Grossman, M. A. and Bain, E. C. (1931). High-speed steel. New York, NY.
Guillet, L. (1905). Les aciers speciaux, 2 Vols. Paris, FR.
Guthrie, R. I. L. and Stubbs, P. (1973). Kinetics of scrap melting in baths of molten pig
iron. Canadian Metallurgical Quarterly. 12(4). pg. 465-473.
Hackney, W. (1874/1875). The manufacture of steel. Proc. Inst. Civil Eng. xlii. pg. 2-68.
Hadfield, R. A. (1888). Manganese steel. Journal of the Iron and Steel Institute of Japan.
33. pg. 41-77.
Hadfield, R. A. (1888). Manganese and its applications in metallurgy. Proc. Inst. Civil
Eng. cxiii. pg. 1-59.
Hadfield, R. A. (1889). On manganese steel. Journal of the Iron and Steel Institute. II.
Hadfield, R. A. (1889). On alloys of iron and silicon. Journal of the Iron and Steel
Institute. II. pg. 222-242.
Hadfield, R. A. (1892). Alloys of iron and chromium. Journal of the Iron and Steel
Institute. II. pg. 49-131.
Hadfield, R. A. (1894). The early history of crucible steel. Journal of the Iron and Steel
Institute of Japan. II. pg. 224-238.
Hadfield, R. A. (1898/1899). Alloys of iron and nickel. Proc. Inst. Civil Eng. CXXVIII.
Hadfield, Robert. (January 1912). On Sinhalese iron and steel of ancient origin.
Proceedings of the Royal Society of London. Series A, Containing Papers of a
Mathematical and Physical Character. 86(584). pg. 94-100. X.
Hadfield, Robert Abbott, Sir. (1925). Metallurgy and its influence on modern progress,
with a survey of education and research. Chapman & Hall, London.
Hadfield, Robert A., Sir. (1931). Faraday and his metallurgical researches with special
reference to their bearing on the development of alloy steels. Chapman & Hall, London.
Hall, J. H. (April 3, 1913). The Manufacture of crucible steel. Iron Trades Review. pg.
Hall, J. H. (April 10, 1913). The Manufacture of crucible steel. Iron Trades Review. pg.
Harbord, Frank William and Hall. (1918). The metallurgy of steel. C. Griffin & Co.,
Hasluck, Paul N., ed. (1904). Metalworking: A book of tools, materials, and processes for
the handyman. Cassell and Company Ltd., London. Reprinted in 1994 by Lindsay
Hatch, Charles E. Jr. and Gregory, Thurlow Gates. (1962) The first American blast
furnace, 1619 - 1622. Virginia Magazine of History and Biography. 70. pg. 259 - 296.
Hatfield, William Herbert. (1926). Comparison of permanent magnet steels. J. Sci.
Instrum. 3. pg. 234-235.
Hatfield, William Herbert. (1928). The application of science to the steel industry.
Printed by Evangelical Publishing House, Cleveland.
Hatfield, William Herbert. (1928). Cast iron in the light of recent research. Charles
Griffin & Co., London.
Hatfield, William Herbert. (1938). Research in the iron and steel industry. Institute of
Chemistry of Great Britain and Ireland, London.
Hatfield, William Herbert. (1942). Lecture on rust-, acid- & heat-resisting steels.
Institute of Chemistry of Great Britain and Ireland, London.
Hibbard, Henry Deming. (1916). Manufacture and uses of alloy steels. G.P.O.,
Hiles, J. and Mott, R. A. (1944). The mode of combustion of coke. Fuel. 23(6). pg. 154171.
Howe, H. M. (1890). The metallurgy of steel. The Scientific Publishing Co, NY, NY.
Hubbard, Howard G., ed. (November, 1937). Metal alloys. The Chronicle. 2(2). pg. 13.
This article continues over several issues: 2(2), pg. 13; 2(3), pg. 20; (2) 4, pg. 30;
2(5), pg. 39; 2(7), pg. 52.
The information on the alloys is extracted from: Mackenzie’s Five Thousand
Receipts in All the Useful and Domestic Arts, Kay's edition, Philadelphia, 1829.
“Bronze. Melt in a clean crucible 7 pounds of pure copper: when fused, throw into
it 3 pounds of tin. These metals will combine, forming bronze, which, from the
exactness of the impression which it takes from a mould, has, in ancient and
modern times, been generally used in the formation of busts, medals, and statues.”
“Bell metal. Melt together 6 parts of copper, and 2 of tin: These proportions are
the most approved for bells throughout Europe, and in China. In the union of the
two metals above mentioned, the combination is so complete, that the specific
gravity of the alloy is greater than that of the two metals combined.” pg. 30.
Huddleston, Jerry and Stutzenberger, Fred. (July 2006). Damascene: Part I. Muzzle
Blasts. 67(11). pg. 61-64. X.
Huddleston, Jerry and Stutzenberger, Fred. (August 2006). Damascene: Part II. Muzzle
Blasts. 67(12). pg. 61-64. X.
Hyde, Charles. (1977). Technological change in the British iron industry, 1700-1870.
Princeton University Press, Princeton, NJ.
International Correspondence Schools. (1916). Gauges, jigs, dies, tempering, heat
treatment, blacksmithing and forging. I.C.S. Reference Library, International Textbook
Company, Scranton, NY.
Ishihara, Y. (1958). Progress of special steelmaking in Japan. Symposium on Production
of Alloy Steels (Jamshedpur). pg. 172-175.
Jeans, J. S. (1880). Steel: Its history, manufacture, properties and uses. London.
Jefferson, T. B. and Woods, Gorham. (1954). Metals and how to weld them. The James F.
Lincoln Arc Welding Foundation, Cleveland, OH. IS.
Johannsen, Otto. (1924). Geschichte des eisens; im auftrage des Vereins deutscher
eisenhüttenleute gemeinverstñdlich dargestellt, von dr. Otto Johannsen. Verlag
Stahleisen m. b. h., Düsseldorf.
History of iron.
Kashchieva, Elena, Tsaneva, Svetila, Dimitriev, Yanko and Kirov, Roumen. (2003).
Microstructure and chemical composition of Thracian medallions with enamel in
millefiori technique found in Bulgaria. Journal of Non-Crystalline Solids. 323: 137-142.
Kauffman, Henry J. (n.d.). Early American copper, tin and brass: Handcrafted
metalware from colonial times. Astragal Press, Mendham, NJ.
Kauffman, Henry J. (1948). Coppersmithing in Pennsylvania: Being a treatise on the art
of the eighteenth century coppersmith, together with a description of his products and his
establishments. Pennsylvania German Folk Lore Society, Allentown, PA.
Kauffman, Henry J. (1966). Early American ironware: Cast and wrought. Weathervane
Books, NY, NY.
Kauffman, Henry J. (1966). Metalworking trades in early America. The Charles E. Tuttle
Co., Inc. Reprinted in 1995 by Astragal Press, Mendham, NJ. IS.
Kauffman, Henry J. (1968). American Copper & Brass. T. Nelson, Camden, NJ.
Reprinted in 1979 by Bonanza Books, NY, NY. IS.
Kauffman, Henry J. (December 1969). Cast steel. The Chronicle. 22(4). pg. 49-50. IS.
Kauffman, Henry J. (1970). The American pewterer: His techniques & his products. T.
Nelson, Camden, NJ.
Kayser, J. F. (March 11, 1927). Practical crucible steel making. Iron and Coal Trades
Review. pg. 396-397.
Kayser, J. F. (March 18, 1927). Practical crucible steel making. Iron and Coal Trades
Review. pg. 438-439.
Kemp, Emory L. (1993). The introduction of cast and wrought iron in bridge building.
IA: The Journal of the Society for Industrial Archeology. 19(2), pg. 5-16.
Kester Solder Company. (1948). Solder and soldering technique: A condensed industrial
manual. Kester Solder Company, Chicago, IL. IS.
Killick, D. J. and Gordon, R. B. (1987). Microstructures of puddling slags from Fontley,
England and Roxbury, Connecticut, U.S.A. Journal of Historical Metallography Society.
21. pg. 28-36.
Landrin, H. C. (1868). Treatise on steel: Comprising its theory, metallurgy, properties,
practical working, and use. Translation of original French done by A. A. Fesquet. Henry
Carey Baird, Philadelphia, PA.
Lankford, William T., Jr., Samways, N. L., Craven, R. F., McGannon, H. E., eds. (1985).
The making, shaping and treating of steel, 10th ed. United States Steel Co., Herbick &
Held, Pittsburgh, PA
Laughlin, Ledlie I. (1940). Pewter in America. 2 vols. Houghton Mifflin, Boston, MA.
Leever, Sylvia. (October 2003). Late medieval iron making, the bloomery process: A
treatise on the making of iron in a bloomery and on the quality of the armour made from
such iron. TUDelft: Delft, Materials Science and Engineering. Delft University of
Technology, Delft, NL. IS.
Light, John D. (1987). Blacksmithing technology and forge construction. Technology and
Culture. 28(3). pg. 658-665.
Light, John D., and Wylie, William N. (1986). A guide to research in the history of
blacksmithing. Research Bulletin. No. 243, Parks Canada, Ottawa, Canada.
Lister, Raymond. (1966). The craftsman in metal. A. S. Barnes and Company, NY, NY.
Longmuir, P. (1905). Practical metallurgy: Iron and steel. London.
Louis, H. (1879). On the chemistry of puddling. J. Iron Steel Inst. 1. pg. 219-226.
Lynch, John. (1957). Metal sculpture: New forms new techniques. The Viking Press, NY,
Markham, Eward Russell. (1903). The American steel worker. The Derry-Collard
Company, NY, NY.
Martinez, M. A., Abenojar, J., Mota J. M. and Calabres, R. (2006). Ultra high carbon
steels obtained by powder metallurgy. Materials Science Forum. 530-531: 328.33.
Maryon, Herbert. (1961). Early near eastern steel swords. AJA. 65. pg. 173-84.
Masse, H. J. L. J. (1911). Chats on old pewter. T. Fisher Unwin, London, UK.
McCreight, Tim and Bsullak, Nicole. (2001). Color on metal: 50 artist share insights and
techniques. Guild Publishing, Shamper’s Bluff, New Brunswick, Canada.
McCreight, Tim and Kazan, Katie. (2007). Metalsmith’s book of boxes and lockets.
Brynmorgan Press, Brunswick, ME.
Mehl, Robert Franklin. (1948). A brief history of the science of metals. Sponsored jointly
by the Institute of Metals Division, AIME and the Seeley W. Mudd Memorial Fund,
American Institute of Mining and Metallurgical Engineers, NY, NY.
Mehl, R. F. (1965). On the Widmannstatten structure. In: The Sorby centennial
symposium on the History of Metallurgy. Smith, C. S., Gordon and Breach Science
Meilach, Dona and Seiden, Don. (1966). Direct metal sculpture: Creative techniques and
appreciation. Crown Publishers Inc., NY, NY. IS.
Metal Powder Industries Federation. (2007). Advances in powder metallurgy and
particulate materials: Proceedings of the 2007 International Conference on Powder
Metallurgy & Particulate Materials, May 13-16, Denver, Colorado. Princeton, NJ:
Metallurgical Society. (1961). History of iron and steelmaking in the United States:
Publication in one book of a series of historical articles that have appeared in Journal of
Metals, 1956-1961. American Institute of Mining, Metallurgical, and Petroleum
Engineers, NY, NY.
Misa, Thomas J. (1995). A nation of steel. London.
Moldenke, Richard George Gottlob. (1910). The production of malleable castings: A
practical treatise on the processes involved in the manufacture of malleable cast iron.
Penton Pub. Co., Cleveland, OH.
Moldenke, Richard George Gottlob. (1917). The principles of iron founding. McGrawHill Book Co., NY, NY.
Moldenke, Richard George Gottlob. (1927). Malleable casting. International Textbook
Co., Scranton, PA.
Morton, G. R., and Brit, R. G. (1974). The Present day production of wrought iron.
Journal of the Historical Metallurgy Society. 8. pg. 96-102.
Nosek, Elzbieta M. (1985). The Polish smelting experiments in furnaces with slag pits.
In: Craddock, P.T. and Hughes, M.J., Eds. Furnaces and smelting technology in antiquity.
British Museum Occasional Paper 48, London, England. IS.
Neilson, William G. (July 24, 1867). Manufacture of wrought iron direct from the ore.
Bulletin of the Iron and Steel Association. 26.
Notis, M. and Shugar, A.(2003). Roman shears: Metallography, composition, and a
historical approach to Investigation. Proceedings of the Archaeometallurgy in Europe
Conference, Milan, Italy Sept 24-26 2003. 1. pg. 109-118. X.
Nuwer, Michael. (October 1988). From batch to flow: Production technology and workforce skills in the steel industry, 1880-1920. Technology and Culture. 29. pg. 808 - 838.
Oberg, Erik, Jones, Franklin D., Horton, Holbrook L. and Ryffel, Henry H. (
1996). Machinery’s Handbook: 25th edition: A reference book for the mechanical
engineer, designer, manufacturing engineer, draftsman, toolmaker, and machinist.
Industrial Press Inc., NY, NY. IS.
Osborn, Henry Stafford. (1869). The metallurgy of iron and steel: Theoretical and
practical: In all its branches; with special reference to American materials and
processes. H.C. Baird, Philadelphia, PA.
Overman, Frederick. (1851). The manufacture of steel: Containing the practice and
principles of working and making steel. A. Hart, Philadelphia, PA
Overman, Frederick. (1852). A treatise on metallurgy; comprising mining, and general
and particular metallurgical operations, with a description of charcoal, coke, and
anthracite furnaces, blast machines, hot blast, forge hammers, rolling mills, etc., etc. D.
Appleton, NY, NY.
Overman, Frederick. (1854). The manufacture of iron, in all its various branches.
Including a description of wood-cutting, coal digging, and the burning of charcoal and
coke; the digging and roasting of iron ore, the building and management of blast
furnaces, working by charcoal, coke, or anthracite; the refining of iron. Also a
description of forge hammers, rolling mills, blast machines, hot blast, etc. etc. To which
is added an essay on the manufacture of steel. H. C. Baird, Philadelphia, PA.
Overman, Frederick. (1894). The manufacture of steel: Containing the practice and
principles of working and making steel. H.C. Baird, Philadelphia, PA.
Palmer, Frank R. (1937). Tool steel simplified: A handbook of modern practice for the
man who makes tools. The Carpenter Steel Company, Reading, PA. IS.
Palmer, Frank R., Luerssen, George V. and Pendleton, Joseph S., Jr. (1978). Tool steel
simplified. Fourth Edition. Chilton Company, Radnor, PA. IS.
Parr, J.G. (1972). The sinking of the Ma Robert: An excursion into mid nineteenth
century steelmaking. Technology and Culture. 13(2). pg. 209-225.
Parsons, Sam Jones. (1909). Malleable cast iron. Van Nostrand, NY, NY.
Partington, J. R. (1961). A history of chemistry. St. Martin's Press, NY, NY.
Percy, J. (1864). Metallurgy: Iron and steel. London.
Percy, J. (1877). On the cause of the blisters on “Blister steel”. Journal of the Iron and
Steel Institute. II. pg. 460-463.
Perttula, Juha. 2001. Reproduced wootz Damascus steel. Scandinavian Journal of
Perttula, Juha. 2004. Wootz Damascus steel of ancient orient. Scandinavian Journal of
Phillips, J. Arthur. (1874). Elements of metallurgy: A practical treatise on the art of
extracting metals from their ores. C. Griffin and Company, London, UK.
Piaskowski, J. (1972). Criteria for determining a technology of bloomery iron products.
Archaeologia Polona. 17(1). pg. 7-45.
Pleiner, Radomir. (1969). Iron working in ancient Greece. National Technical Museum,
Pleiner, Radomir. (1980). Early iron metallurgy in Europe. In: The Coming of the Age of
Iron. Wertime, Theodore A. and Muhly, James D., eds. Yale University Press, New
Haven, CT. IS.
Piley, J. (1889). Alloys of nickel and steel. Journal of the Iron and Steel Institute. I. pg.
Pollack, Herman W. (1977). Materials science and metallurgy. Reston Publishing Co.,
Inc., Reston, VA.
Pruemmer, R. A., Balakrishna Bhat, T., Siva Kumar, K. and Hokamoto, K. (2006).
Explosive compaction of powders and composites. Enfield: Science Publishers.
Raquenet, A., Ed. (2010). Artistry in iron: 183 designs, includes CD-ROM. Dover
Read, T. T. (1934). Metallurgical fallacies in archaeological literatur. AJA. 38. pg. 382.
Richardson, H. C. (1934). Iron, prehistoric and ancient. AJA. 38(4). pg. 574.
Ricketts, J. A. (2001). History of Ironmaking. Association for Iron & Steel Technology
(AIST), Warrendale, PA.
Robb, Frances C. (1993). Cast aside: The first cast-iron bridge in the United States. IA:
The Journal of the Society for Industrial Archeology. 19(2). pg. 48-62.
Roberts, G. A., Hamaker, J. C., and Johnson, A. R. (1962). Tool steels. American Society
for Metals, Cleveland, OH.
Sabadasz, Joel. (1992). The development of modern blast furnace practice: The
Monongahela Valley furnaces of the Carnegie Steel Company, 1872-1913. IA: The
Journal of the Society for Industrial Archeology. 18(1/2). pg. 94-105.
Sauveur, A. (1910). The metallography and heat treatment of iron and steel. Cambridge,
Schaur, R. Title unknown. Stahl und Eisen. 49. pg. 489-498.
Scoffern, J. et al. (1857). The useful metals and their alloys. London, UK.
Seely, Bruce E. (1981). Blast furnace technology in the mid-19th century: A case study
of the Adirondack Iron and Steel Company. IA: The Journal of the Society for Industrial
Archeology. 7(1). pg. 27-54.
Semiatin, S. L. and Lahoti, G. D. (1981). The forging of metals. Scientific American.
245(2). pg. 98-106.
Seymour, Lindsay, J. (1964). Iron and brass implements of the English and American
house. Carl Jacobs, Bass River, MA.
Shrager, M. (1949). Elementary Metallurgy and Metallography. Reprinted in 1961 by
Dover, NY. IS.
Siemens, C. W. (1862). On a regenerative gas furnace. Proc. Inst. Mech. Eng. pg. 21-44.
Siemens, C. W. (1868). On the regenerative gas furnace as applied to the manufacture of
cast steel. J. Chem. Soc. pg. 279-310.
Siemens, C. W. (1873). On smelting iron and steel. J. Chem. Soc. pg. 661-678.
Slaager, Goud. (1978). The gold beater, a miscellany. Unpublished, prepared for the
February 1978 meeting of the Early Trades and Crafts Society. IS.
Smith, C. S. (1964). The discovery of carbon in steel. Technology and Culture. 5(2). pg.
Smith, C. S. (1965). The Sorby centennial symposium on the history of metallurgy.
Gordon and Breach Science Publishers, NY.
Smith, J. B. (n.d.). Wire manufacture and uses. John Wiley & Sons, NY, NY.
Smith, Robert E. (1939). Units in etching, spinning, raising, and tooling metal. Edited by
E. H. Mattingly. The McCormick-Mathers Publishing Company, Wichita, KS. IS.
Smith, Robert E. (1951). Etching, spinning, raising and tooling metal. McKnight &
McKnight Publishing Company, Bloomington, IL. IS.
Snelus, G. J. (1879). On the removal of phosphorus and sulphur during the Bessemer and
Siemens-Martin processes of steel manufacture. Journal of the Iron and Steel Institute. I.
Sorby, H. C. (1886). On the application of very high powers to the study of the
microscopial structure of steel. Journal of the Iron and Steel Institute of Japan. I. pg.
Sorby, H. C. (1887). The microscopical structures of iron and steel. Journal of the Iron
and Steel Institute of Japan. 33. pg. 255-288.
Spring, Laverne W. (1917). Non-technical chats on iron and steel and their application
to modern industry. Frederick A. Stokes Company, NY, NY. Reprinted in 1992 by
Lindsay Publications Inc., Bradley, IL. IS.
A surprisingly comprehensive overview of ferrous metallurgy and a museum
Recommended for visitors to the Davistown Museum’s Center for the Study of
Early Tools library.
Frequently cited in our Glossary of Ferrous Metallurgy Terms.
Stansfield, Alfred. (1907). The electric furnace. The Canadian Engineer, Toronto.
Steines, Adolph. (2002). Moving metal: The art of chasing and repoussé. Blue Moon
Press, Huntingdon, PA.
Translated from German.
Stodart, J. and Faraday, M. (1822). On the alloys of steel. Philos. Trans. R. Soc. 112. pg.
Stoughton, B. (1923). The metallurgy of iron and steel. McGraw-Hill Book Co., NY, NY.
Straub, H., Tarmann, B. and Plöckinger, E. (1965). Experiments on smelting in Norictype furnaces. Kantner Museums Schriften 35.
Swank, James M. (1892). History of the manufacture of iron in all ages and particularly
in the United States from colonial times to 1891. Philadelphia, PA. IS.
Swank, James M. (1897). The manufacture of iron in New England. In: The New England
states. Davis, William, ed. D.H. Hurd and Co., Boston, MA.
Tabor, D. (1951). The hardness of metals. Clarendon Press, Oxford, England.
Taylor, F. S. (1954). Some metallurgical processes of the early 16th century. TNS. 29. pg.
Taylor, F. W. (1906). On the art of cutting metals. American Society of Mechanical
Engineers, New York, NY.
Temple, Robert K. G. (1988). Cast iron and steel manufacture. The UNESCO Courier.
Terekhova, N. N. (1974). Cast iron production technology of the Mongols in the Middle
Ages. Sov. Arch. (1). pg. 69-78.
Thälen, L. (1973). Notes on the ancient iron currency bars of Northern Sweden and the
nickel alloys of some archaeological objects. Early Med. Stud. 5. pg. 24-41.
Tholander, E. (1979). A study of the technology behind nickel-alloyed prehistoric steel.
Proc. 5th Atlantic Colloq., Dublin. M. Ryan, Ed. pg. 317-34.
Tomtlund, J.-E. (1973). Metallographic investigation of 13 knives from Helgö. Early
Med. Stud. 5. pg. 42-63.
Turner, Thomas Henry. (1895). The metallurgy of iron and steel: Being one of a series of
treatises on metallurgy written by associates of the Royal School of Mines. RobertsAusten, W.C. Ed. Charles Griffin, London, UK.
Turner, Thomas. (1900). The metallurgy of iron. C. Griffin and Co., London, UK.
Tweedale, Geoffrey. (1987). Sheffield steel and America: A century of commercial and
technological interdependence, 1830-1930. Cambridge University Press, NY, NY. X.
Tweedale, Geoffrey. (1995). Steel city: Entrepreneurship, strategy, and technology in
Sheffield 1743-1993. Oxford University Press, Oxford, UK.
Tylecote, R. F. (1965). Iron smelting in pre-industrial communities. JISI. 203. pg. 340221
Tylecote, R. F. (1981). Medieval smith and his methods. In: Medieval industry. D.W.
Crossley, ed. CBA Research Report, No. 40. Council for British Archaeology, London,
Tylecote, R. F., Austin, J. N. and Wraith, A. E. (1971). The mechanism of the bloomery
process in shaft furnaces. JISI. 209. pg. 342-364.
Tylecote, Ronald F. and Cherry, John. (1970). The 17th century bloomery at Muncaster
Head. Transactions of the Cumberland and Westmorland Antiquarian Society. 70. pg. 69109.
Tylecote, R. F. and Clough, R. E. (1983). Recent bog-iron ore analysis and the smelting
of pyrite nodules. Offa. 40. pg. 115-118.
Tylecote, R. F. and Merkel, J. F. (1985). Experimental smelting techniques:
Achievements and future. In: Furnaces and smelting technology in antiquity. Craddock,
P. T. and Hughes, M. J., eds. British Museum Occasional Paper 48, London, England. IS.
Tyler, P. M. (February 10, 1921). High speed steel manufacture in Sheffield. Iron Age.
United States Steel Corporation. (1957). The making, shaping and treating of steel. 7th
edition. US. Steel Corp., Pittsburgh, PA.
Victoria and Albert Museum. (1913). Old English pattern books of the metal trades.
Victoria and Albert Museum, London, England.
Villars, P. and Calvert, L. D. (1991). Pearson’s handbook of crystallographic data for
intermetallic phases. vols. 1-4. American Society for Metals, Metals Park, OH.
Wakelin, David H. ed. (1999). The making, shaping, and treating of steel. Vol. 1
Ironmaking volume. AISE Steel Foundation, Pittsburgh, PA.
Wanklyn, M. D. G. (1973). Iron and steelworks in Coalbrookdale 1645. Shropshire
Newsletter. 44. pg. 3-6.
Wedel, Ernst von. (1960). The history of die forming. Metal treatment and drop forging.
27. pg. 401-408.
Wertime, Theodore A. (1962). The coming of the age of steel. Chicago, IL. IS.
Wertime, T. A. (1964). Man’s first encounter with metallurgy. Science. 146. pg. 12571267. 159. pg. 927-935.
Wertime, Theodore A. and Muhly, James D., eds. (1980). The coming of the age of iron.
Yale University Press, New Haven, CT. IS.
West, Thomas Dyson. (1902). Metallurgy of cast iron: Complete exposition of the
processes involved in its treatment, chemically and physically, from the blast furnace
through the foundry to the testing machine. Cleveland Print. and Pub. Co., Cleveland,
Whitaker, P. and Williams, T. H. (1969). Examination of a north Indian sword in the
collection of the Pitt-Rivers Museum, Oxford and experiments in the forging of low
carbon strip. Bull. HMG. 3(2). pg. 39-45.
Williams, A. R. (1976). Ancient steel from Egypt. Journal of Archaeological Science. 3.
Wilson, A. J. C., ed. (1992). International tables for crystallography. Vol C. Kluwer
Academic Publishers, Boston, MA.
Wolf, Fridolin. (2006). The abcs of blacksmithing. Blue Moon Press, Huntingdon, PA.
Woodworth, Joseph Vincent. (1903). Hardening, tempering, annealing and forging of
steel: A treatise on the practical treatment and working of high and low grade steel.
N.W. Henley & Co., NY, NY. IS.
Woodworth, Joseph Vincent. (1905). American tool making & interchangeable
manufacturing: A treatise upon the designing, constructing, use, and installation of
tools,jigs, fixtures ... and labor-saving contrivances. N.W. Henley & Co., NY, NY.
Woodworth, Joseph Vincent. (1911). Drop forging, die sinking and machine forming of
steel: Modern shop practices, processes, methods, machines, tools and details. Munn &
Co., NY, NY. IS.
Wright, J. (1907). Electric furnaces and their industrial applications. NY, NY.
Wynne, E. J. and Tylecote, R. F. (1956). An experimental investigation into primitive
iron smelting technique. Journal of the Iron and Steel Institute.
Zastrow, Nancy B. (2004). Lives shaped by steel: Celebrating east coast outdoor metal
artists. Iron Artists, Silver Springs, MD.
Zastrow, Nancy B. (2010). Passion and power: Metal artists in western U.S. Copper
Heron, Silver Springs, MD.
Zapffe, Carl A. (Oct. 14, 1948). Who discovered stainless steel? Iron Age. CLXII.